Toward the Systematic Design of Complex Materials from Structural Motifs

by

Tess Eleonora Smidt

A dissertation submitted in partial satisfaction of the requirements for the degree of Doctor of Philosophy

in

Physics

in the

Graduate Division

of the

University of California, Berkeley

Committee in charge:

Professor Jeﬀrey B. Neaton, Chair Professor Ramamoorthy Ramesh Professor Kristin Persson

Spring 2018 The dissertation of Tess Eleonora Smidt, titled Toward the Systematic Design of Complex Materials from Structural Motifs, is approved:

Chair Date

Date

Date

University of California, Berkeley Toward the Systematic Design of Complex Materials from Structural Motifs

Copyright 2018 by Tess Eleonora Smidt 1

Abstract

Toward the Systematic Design of Complex Materials from Structural Motifs by Tess Eleonora Smidt Doctor of Philosophy in Physics University of California, Berkeley Professor Jeﬀrey B. Neaton, Chair

With ﬁrst-principles calculations based on density functional theory, we can predict with good accuracy the electronic ground state properties of a ﬁxed arrangement of nuclei in a molecule or crystal. However, the potential of this formalism and approach is not fully utilized; most calculations are performed on experimentally determined structures and stoi- chiometric substitutions of those systems. This in part stems from the diﬃculty of system- atically generating 3D geometries that are chemically valid under the complex interactions existing in materials. Designing materials is a bottleneck for computational materials ex- ploration; there is a need for systematic design tools that can keep up with our calculation capacity. Identifying a higher level language to articulate designs at the atomic scale rather than simply points in 3D space can aid in developing these tools. Constituent atoms of materials tend to arrange in recognizable patterns with deﬁned symmetry such as coordination polyhedra in transition metal oxides or subgroups of organic molecules; we call these structural motifs. In this thesis, we advance a variety of systematic strategies for understanding complex materials from structural motifs on the atomic scale with an eye towards future design. In collaboration with experiment, we introduce the harmonic honeycomb iridates with frustrated, spin-anisotropic magnetism. At the atomic level, the harmonic honeycomb iri- dates have identical local geometry where each iridium atom octahedrally coordinated by oxygen hosts a Jeff = 1/2 spin state that experiences interactions in orthogonal spin direc- tions from three neighboring iridium atoms. A homologous series of harmonic honeycomb can be constructed by changing the connectivity of their basic structural units. Also in collaboration with experiment, we investigate the metal-organic chalcogenide assembly [AgSePh]∞ that hosts 2D physics in a bulk 3D crystal. In this material, inor- ganic AgSe layers are scaﬀolded by organic phenyl ligands preventing the inorganic lay- ers from strongly interacting. While bulk Ag2Se is an indirect band gap semiconductor, [AgSePh]∞ has a direct band gap and photoluminesces blue. We propose that these hy- brid systems present a promising alternative approach to exploring and controlling low- dimensional physics due to their ease of synthesis and robustness to the ambient environ- 2 ment, contrasting sharply with the diﬃculty of isolating and maintaining traditional low- dimensional materials such as graphene and MoS2. Automated density functional theory via high throughput approaches are a promising means of identifying new materials with a given property. We automate a search for fer- roelectric materials by integrating density functional theory calculations, crystal structure databases, symmetry tools, workﬂow software, and a custom analysis toolkit. Structural distortions that occur in the structural motifs of ferroelectrics give rise to a switchable spontaneous polarization. In ferroelectrics lattice, spin, and electronic degrees of freedom couple leading to exotic physical phenomena and making them technologically useful (e.g. non-volatile RAM). We also propose a new neural network architecture that encodes the symmetries of 3D Euclidean space for learning the structural motifs of atomic systems. We describe how these networks can be used to speed up important components of the computational materials discovery pipeline and generate hypothetical stable atomic structures. Finally, we conclude with a discussion of the materials design tools deep learning may enable and how these tools could be guided by the intuition of materials scientists. i

To Mom and Dad ii

Contents

Contents ii

List of Figuresv

List of Tables xv

1 Introduction1 1.1 Harmonic Honeycomb Iridates...... 3 1.2 Metal-organic Chalcogenide Assemblies (MOChAs) ...... 7 1.3 Ferroelectrics ...... 8 1.4 Deep learning for atomic systems ...... 11

2 Methods 13 2.1 Density Functional Theory ...... 13

3 Realization of a three-dimensional spin-anisotropic harmonic honeycomb iridate 17 3.1 Introduction ...... 17 3.2 Results ...... 18 3.3 Discussion ...... 23 3.4 Methods ...... 26

4 Ab initio Studies of Structural and Energetic Trends in the Harmonic Honeycomb Iridates 28 4.1 Introduction ...... 28 4.2 Calculation Details ...... 29 4.3 DFT Results ...... 31 4.4 Conclusion ...... 38

5 Silver Benzeneselenolate is a Self-Assembling Direct-Gap Metal-Organic Chalcogenide Assembly 43 5.1 Introduction ...... 43 5.2 Results and Discussion ...... 44 iii

5.3 Conclusions and Prospects ...... 51

6 An Automatically Curated First-Principles Database of Ferroelectrics 52 6.1 Background and Summary ...... 52 6.2 Methods ...... 54 6.3 Data Records ...... 65 6.4 Technical Validation and Veriﬁcation ...... 67 6.5 Usage Details ...... 76

7 Tensor Field Networks: Rotation- and Translation-Equivariant Neural Networks for 3D Point Clouds 79 7.1 Motivation ...... 79 7.2 Related work ...... 80 7.3 Representations and equivariance ...... 81 7.4 Tensor ﬁeld network layers ...... 83 7.5 Demonstrations and experiments ...... 88 7.6 Future work ...... 93

8 Outlook 95

Bibliography 98

A Appendix for Realization of a three-dimensional spin-anisotropic har- monic honeycomb iridate 121

B Appendix for Ab initio Studies of Structural and Energetic Trends in the Harmonic Honeycomb Iridates 138

C Appendix for Silver Benzeneselenolate is a Self-Assembling Direct-Gap Metal-Organic Chalcogenide Assembly 143 C.1 General Information ...... 144 C.2 Miscible Gram-Scale Synthesis of [AgSePh]∞ ...... 144 C.3 Immiscible Interface Synthesis of [AgSePh]∞...... 144 C.4 Fluorescence Imaging Methods ...... 145 C.5 Calculation Methods ...... 145 C.6 Calculation Details ...... 146

D A prototypical ferroelectric: BaTiO3 155

E Appendix for An Automatically Curated First-Principles Database of Ferroelectrics 157 iv

F Isotropy Subgroups: How to check if two structure are continuously deformable 163

G A brief primer on deep learning 167

H Appendix for Tensor Field Networks 169 H.1 Proofs of general equivariance propositions ...... 170 H.2 Motivating point convolutions ...... 170 H.3 Proof of equivariance of point convolution layer ...... 171 H.4 Details for gravitational accelerations and moment of inertia tasks . . . . . 173 H.5 Proof of weighted point-averaging layer equivariance ...... 174 H.6 Missing point task accuracies and MAE by epoch ...... 175 v

List of Figures

1.1 The splitting of 5d orbitals for iridium atoms octahedrally coordinated by oxygen atoms. Crystal ﬁeld splitting breaks the degeneracy of the 5d orbitals into a two-dimensional manifold Eg and a three-dimensional manifold T2g. Spin-orbit coupling further splits the T2g manifold with Leff = 1 into Jeff = 1/2 and Jeff = 3/2 states...... 5 1.2 In the harmonic honeycomb iridates, the IrO6 edge-share with three nearest neigh- bors, forming three orthogonal planes deﬁned by the Ir-O-Ir bonds. These planes are indicated with blue, red, and green shading. The Ir ions are indicated by the circles while the oxygens (not shown) lie on the edges of the polyhedra...... 6 1.3 MOChAs can host inorganic structures of varying dimensionality and topology, from sheets and tubes (2D), to chains and rings (1D), to individual clusters (0D). 7 1.4 Diﬀerent transition metals and organic ligands form MOChAs with various co- ordinations and topologies. (Top to Bottom) adamantane + copper give a nan- otube structure made of triangular coordination polygons, carborane + lead give a chiral 1D chain of seesaw coordination polyhedra, carborane + mercury give a non-chiral 1D chain of seesaw coordination polyhedra...... 9 1.5 Top) Three methods for making MOChAs: immiscible layered strategy, gram- scale bulk synthesis, and wafer-scale gas phase deposition. Middle row). Crystals produced from each method. Bottom row) All three methods produce diﬀerent crystal morphologies but uniform emission energy...... 9 1.6 a) A ferroelectric is a material with a spontaneous polarization that is switchable by applying an external electric ﬁeld. b) The free energy written in terms of polarization has a double well, each well representing stable, switchable polar structures. c) A plot of the polarization of a ferroelectric versus the application of an electric ﬁeld will produce a hysteresis loop...... 10 1.7 A network with 3D translation- and 3D rotation-equivariance allows us to identify chemical motifs in any location or orientation using the same ﬁlters...... 12 vi

H 3.1 Single crystal of 1 -Li2IrO3 and the Ir lattice structure. (A) Single crystal oriented to beh paralleli to the crystallographic axes shown in (C), (B) 3D view and (C) projection in the ab plane. In (B) gray shading emphasizes the Ir (purple balls) honeycomb rows that run parallel to the a b diagonals, alternating upon moving along the c-axis. For simplicity only Li ions± (grey balls) located in the center of Ir honeycombs are shown. In (B) and (C) the rectangular box indicates the unit cell. Comparing (A) and (C) we note that the 70◦ angle between honeycomb rows is evident in the crystalline morphology. . .∼ ...... 19 3.2 The temperature dependence of the single-crystal magnetic suscepti- bility along the three principal crystalline directions. The inset shows 1/χ for all three axes χa, χb, and χc. The dashed line indicates the slope of the inverse Curie-Weiss susceptibility for a paramagnet with eﬀective moment of 1 µeff = 1.6µB, close to that expected of an Ir Jeff = /2 state if g-factor anisotropy is ignored. All three components of susceptibility show strong deviation from Curie-Weiss behavior as a function of temperature...... 20 3.3 Temperature dependence of the magnetic anisotropy. (A) Each Ir is sur- rounded by one of two planar, triangular environments indicated by blue and red shaded triangles, located at 35◦ either side of the b-axis. (B) The anisotropy of the magnetic susceptibility as∼ measured by torque and the diﬀerences in (SQUID) susceptibilities (grey lines) are shown as a function of temperature for all three crystallographic directions. An anomaly indicates the onset of magnetic order at TN = 38 K. (C) The ratios of the anisotropic susceptibility tend to simple fractional values dictated by the g-factor anisotropy of the local planar iridium environment. (D) sin(2θ) ﬁts to the anisotropy αbc illustrating the change of sign at 75K...... 22 ∼ H 3.4 Low temperature magnetic properties of the 1 -Li2IrO3. (A) The Ir-O2- Ir planes deﬁning three orthogonal directions of theh spin-exchange,i one parallel to bˆ and the other two parallel to aˆ cˆ, labelled + and (aˆ is the unit vector along a). This connects to the notation± used to describe the− Kitaev Hamiltonian in SI III. (B) Torque signal τ divided by the applied magnetic ﬁeld H at a temperature of 1.5 K, illustrating a linear low-ﬁeld dependence and a kink at H∗, which is strongly angle dependent (colors correspond to angles shown in (D)). (C) Magnetization vs magnetic ﬁeld applied along the b-axis at a temperature of ∗ 15 K. (D) & (E) The angle dependence θab/ac of the kink ﬁeld H of the ordered state (full circles, left axes) with respect to the crystallographic axes a, b and c. ∗ H is correlated to the magnetization anisotropy αij (open circles, right axes) indicating a common moment at H∗ in all ﬁeld orientations...... 24 vii

3.5 Introducing the harmonic honeycomb series. (A) Two kinds of c-axis bonds H (black links) in the harmonic honeycomb family N -Li2IrO3 are shown, one linking within a honeycomb plane (for example blueh toi blue, top) and one that rotates between honeycomb planes (for example red to blue, bottom). For undis- torted octahedra, these links are locally indistinguishable, as can be observed by the local coordination of any Ir atom (also see Figure 3.3A). (B) These building blocks can be used to construct a series of structures. The end members include the theoretical N = 0 ‘hyper-honeycomb’ [160, 127, 146] and the N = layered honeycomb [189]. Here N counts the number of complete honeycomb∞ rows in a section along the c-axis before the orientation of the honeycomb plane switches. 25 4.1 (a) Conventional unit cells of H 0 , H 1 , H 2 , and H [174]. H , H 0 , H 1 , and H 2 have 2, 4, 8, andh i 12 formulah i h i units inh∞i their primitiveh∞i unit cell,h i respectively.h i h Membersi of the harmonic honeycomb series have identical local geometry, only varying in the connectivity of their basic structural units, orthog- onal edge-sharing iridium oxide octahedra. The two growth or bonding planes are normal to a + b and a b, where a and b are the orthorhombic lattice vectors (in- dicated by the axes at− the bottom left). The harmonic honeycomb pattern builds along the orthorhombic c direction. Compared to Li2IrO3 structures, Na2IrO3 structures have greater distortion of iridium oxide octahedra and larger volume. (b-e) Exaggerated distortions in the harmonic honeycombs. (b-c) Two parallel faces of each iridium oxide octahedron twist opposite to each other. These faces are parallel to the growth plane. (c) Which faces twist changes at twisting bonds. (b) A bond that preserves the bonding plane. (c) A “twist” bond that changes the bonding plane. (d) The octahedra also compress along their twist axis. (e) The twisting and compression of the octahedra cause Ir-O-Ir bond angles to in- crease from their ideal 90◦ and the angle between bonding planes to be close to the undistorted value of arccos(1/3) 70.5◦...... 39 4.2 Non-magnetic density of states normalized by the number of formula units per unit cell for Li2IrO3 and Na2IrO3 harmonic honeycomb structures. Density of states is similar across the series...... 40 H H 4.3 PBE+SOC+U density of states of Li2IrO3 and Na2IrO3 for non- h∞i h∞i magnetic (all magnetic moments ﬁxed at zero µB) and ferromagnetic (along the H b direction or H 0 c direction) magnetic orders are shown in (a). A gap opensh∞i in the density ofh statesi of both systems with a non-zero magnetic order. Diﬀerences in the Li2IrO3 and Na2IrO3 density of states are caused by distortions of the local environment more so than change in volume. Li2IrO3 and Na2IrO3 structures have Ir-O-Ir bond angles of 94◦ and 100◦, respectively...... 40 viii

4.4 Plots of ratio of relaxed lattice parameters vs doping for PBE+U where U=0,1.5,3.0,6.0. The discontinuity indicates that when PBE gives asymmetric Ir-Ir bonds below a given Na doping. The discontinuity in the lattice parameters shifts toward more Li doping with increasing U, demonstrating that the performance of the func- tional is sensitive to localization of iridium 5d orbitals and closeness of iridium atoms...... 41 4.5 Plots of Ir-Ir bond lengths and Ir-O-Ir bond angles as a function of Na doping of H 0 Li2IrO3 for PBE+U and PBE+SOC+U (U = 3 eV). While SOC is not suf- ﬁcienth i to prevent discontinuities in bond length relaxations, it does give uniform bond length ( < 0.01 A)˚ and bond angles ( < 1.5 degree) for all relaxations. Note, if U = 3 eV± is used for Li concentration±< 15% and U = 1.5 eV for Li

concentration < 15% there is no dicontinuity. (Li1−xNax)2 IrO3 is metallic for U = 1.5 eVand 0.1 < x < 0.2%. According to VCA, the distortion is not linear in doping...... 42

5.1 a) The monoclinic unit cell of solid silver benzeneselenolate contains two complete layers of hybrid chalcogenide 2D polymer. Silver is coordinated tetrahedrally by four selenium atoms. b,c) The multilayered structure isolates inorganic layers via the benzene moieties oriented above and below the silver selenide polymer layer. D) A single isolated layer has a thickness of 1.4 nm, each containing two layers of phenyl rings and one layer of silver selenolate. Silver is represented as the grey spheres, selenium in dark orange, and carbon in black. Aromatic rings are accented in blue...... 45 5.2 a) A chartreuse deposit of silver benzeneselenolate forms at an immiscible liquid- liquid interface of organic and aqueous solutions of diphenyl diselenide and sil- ver nitrate, respectively. b) Crystals of [AgSePh]∞ recovered have typical edge lengths between 1 and 4 microns. b) Scanning electron micrograph of a silver ben- zeneselenolate silver crystal reveals the layered structure of the crystal. Individual layers are resolved in high-resolution SEM images. c) Atomic force microscopy reveals highly uniform [AgSePh]∞ (001) terraces with measured step heights at 1.4 nm...... 46 5.3 a) Confocal micrographs showing the color uniformity of photoluminescence in [AgSePh]∞. b) A single, intense emission of the solid at 467 nm is attributed to a direct-gap electronic transition. c,d) Optical and confocal micrographs of [AgSePh]∞ showing ﬂuorescence scanning confocal images of several individual crystals of nearly the same size. e) Distribution of the intensity from 157 indi- vidual crystals plotted as a function of the area of the crystal and f) aspect ratio. The Pearson’s r-value for each set of data was calculated by using linear least squares ﬁtting (solid line); for both the plots of area (r-value of 0.07) and aspect ratio (r-value of 0.1) the Pearson’s r-values indicate no correlation with intensity. Images are false colored according to emission wavelength...... 48 ix

5.4 a) DFT-HSE band structure and density of states of bulk [AgSePh]∞. See sup- porting information Figure C.6 for details. Band color signiﬁes the fractional contribution of states centered on inorganic (Ag and Se, orange) and organic (C and H, black) atoms in the crystal. The total density of states is shown in gray. b) DFT-HSE band structure of a single layer of [AgSePh]∞ c) DFT-HSE band structure of a single layer of [AgSePh]∞ with the phenyls replaced by hydrogen. The hydrogen positions have been relaxed with PBE; see supporting information Figure C.5. The near-band edge character remains relatively unchanged when the phenyls are replaced by hydrogen, suggesting that the degree of 2D quantum conﬁnement is unchanged by 3D crystallization. d) The Brillouin zone for the primitive cell of [AgSePh]∞. The path in the Brillouin zone used for the band structure is identiﬁed by orange lines and k-point labels...... 49 5.5 Depictions of side and top views of [AgSePh]∞ with overlain charge density maps. The DFT-HSE computed valence band maximum (VBM) and conduction band minimum (CBM) at Γ are accented in yellow and blue, respectively. The minimal but non-negligible participation of carbon in the CBM state suggests tailoring of electronic properties via synthetic modiﬁcation of ligand...... 50

6.1 Diagram of entire automated ferroelectric search workﬂow. Databases are shown as purple cylinders. Processes are shown as rectangles: blue designates pro- cesses used to identify and perform ab initio calculations, green designates post- processing and validation, and orange designates the web-interface. Arrow di- rections indicate the ﬂow of information. For example, the Workﬂow Database provides information to the Computing Resources for which calculations to com- pute and the Workﬂow Database is updated as calculations complete or errors occur on the Computing Resources...... 56 6.2 Diagram of DFT workﬂow written with atomate and Fireworks. Blue and red boxes denote initial nonpolar and polar structures, respectively, green boxes de- note DFT calculations, orange rhombuses denote decision steps, and purple el- lipses denote exit steps...... 60 6.3 Polarization curves for BaTiO3 along the [001] versus distortion from nonpolar to polar structure. Due to the change in lattice parameters and volume across the distortion, the quantum of polarization along the [001] direction is diﬀerent for each structure. This causes the spontaneous polarization for diﬀerent branches to diﬀer. The branch that starts at zero is the corrected branch. The branch that starts near -600 µC/cm2 is the data from VASP. Note, while in this speciﬁc case, the calculated polarization values for all interpolations were on the same branch, this is not usually the case...... 62 x

6.4 A visual demonstration of the same branch polarization algorithm demonstrated in 1D (rather than 3D) using BaTiO3. As mentioned in Figure 6.3, VASP returns polarizations all along the branch starting at -600 µC/cm2. However, to better demonstrate the algorithm, we will suppose that the values for the polarization for each interpolation are those circled in red. In the ﬁrst panel, we move the nonpolar polarization to be on the branch closest to zero. In the second panel, we move the ﬁrst interpolated polarization to be on the branch closest to the adjusted nonpolar polarization. In the third panel, we move the second interpolated polarization to be on the branch closest to the adjusted ﬁrst interpolation polarization. If the algorithm ﬁnishes successfully, the adjusted polarizations will on the same branch. 64 6.5 The polarization reconstruction for CrO3 with workﬂow ID wfid 1484694851.899452. The polarization along the b lattice parameter is incorrectly reconstructed because the diﬀerent polarization branches are closer than the change in polarization be- tween structure interpolations. To correctly reconstruct this polarization with our existing algorithm, more structure interpolations would be needed between the nonpolar and polar structures...... 65 6.6 Legend for Figure 6.7...... 70 6.7 Validated ferroelectric candidates from our search. Spontaneous polarization plot- ted against nonpolar-polar energy diﬀerence, maximum atomic distortion, PBE band gap, and energy of polar structure above lowest energy polymorph reported in the Materials Project...... 71 6.8 Distortion candidate point group relations...... 72 6.9 Diagrams of polarization magnitude vs. point group...... 72 6.10 Experimental vs. Calculated polarizations for ferroelectric materials in the Landolt- B¨ornsteinseries. Note, the plot is log-log. We give colored regions to show which experimental values are within 25, 50, and 75 of calculated values. . . . . 76 ± ± ± (l) 7.1 Example of Vacm representing two point masses with velocities and accelerations. Colored brackets indicate the a (point), c (channel), and m (representation) in- (l) dices. (l) is the key for the Vacm dictionary of feature tensors...... 84 7.2 Network diagram for learning gravitational accelerations and moment of inertia tensor. The input tensor has indices [channels, points, representation]. The input for the gravitational acceleration and moment of inertia tasks are point mass scalars, therefore the representation index is 1-dimensional. Convolution ﬁlters are indicated by blocks marked F and Clebsch-Gordan tensors are indicated by CG. The numbers along the arrows for the representation index indicate the l of that arrow, with CG blocks combining the input and ﬁlter ls to generate output of a speciﬁc l...... 89 7.3 Radial function learned by l = 1 ﬁlter for gravity toy dataset. Minimum radial cutoﬀ distance of 0.5 is chosen for randomly sampled points such that there are enough samples generated near the minimum distance...... 90 xi

7.4 3D Tetris shapes. Blocks correspond to single points. The third and fourth shapes from the left are mirrored versions of each other...... 90 7.5 Network diagrams for shape classiﬁcation task showing how information ﬂows between tensors of diﬀerent order. Clebsch-Gordan tensors are implied in the arrows indicating convolutions. The numbers above the self-interactions indi- cate the number of channels. Individual convolutions, indicated by arrows, each produce a separate tensor, and concatenation is performed after the convolutions. 91 7.6 A hypothetical example input and output of the missing point network. (A) A benzene molecule with hydrogen removed (B) The relative output vectors pro- duced by the network, with arrows shaded by the associated probabilities. . . . 92

A.1 X-ray diﬀraction pattern in the (hk0) (top) and (h1l) (bottom) planes. Raw data (AB) is well reproduced by calculations (CD) for the Cccm structure (Table A.1), in contrast an F ddd (hyper-honeycomb) structure (EF) can only explain the existence of less than half of the observed diﬀraction peaks...... 122 A.2 Observed diﬀraction intensities plotted against those calculated in the reﬁned (A) Cccm (Table A.1) and (B) F ddd structural models. The dashed lines indi- cate 1:1 agreement between data and model and error bars reﬂect the intensity uncertainties after averaging the observed intensities of reﬂections expected to be equivalent under orthorhombic symmetry. The three families of reﬂections discussed in the text are plotted as diﬀerent symbols/colors (black circles, red squares, and blue triangles). Note that the F ddd model predicts zero intensity at the observed (odd, odd, even) reﬂections and largely overestimates the intensities of (odd, odd, odd) peaks...... 123 A.3 Crystal structure models described in the text, (A) Cccm (Table A.1) and (B) F ddd, large brown balls - Ir, medium light gray balls - Li, small gray balls - O. . 124 A.4 Preliminary measurements of the change in the lattice parameters along the crys- tallographic a, b and c direction on cooling below the magentic transition at TN. We do not observe any changes in the crystallographic symmetry, but the elastic response in each direction is highly anisotropic, with the b-axis changing roughly 10 times more that the a-axis...... 125 A.5 The magnetic anisotropy extracted from the low ﬁeld slope of the torque sig- nal τ/µ0H, similar to that shown in Figure 3.4 B, taken for rotations through the three principal crystallographic planes and at diﬀerent temperatures. The anisotropy is shown in units of µB per Ir, for (A) the χa χb, (B) χa χc and (C) − − χb χc. The only change of sign in the anisotropy is in (A) and an enlargement of this− scale is shown in Figure 3D of the main text to emphasize this...... 126 xii

A.6 Torque signal taken at magnetic ﬁelds up to 35 T at the National High magnetic Field Laboratory. The ﬁeld H∗ is extremely clear at all angles. At angles away from the principal axes the torque signal is very clearly linear and follows a sin 2θ dependence described by equation A.4. The larger asymmetry in this data set compared to that measured in the superconducting magnet, is due to the larger ﬁeld gradient experienced by the sample...... 127 A.7 (A) The two choices of edge shared bonds give rise to two kinds of links that are locally indistinguishable. These deﬁne two bonding planes (see Figure 3A of the ◦ main text) that are an angle φo 70 apart. (B) Links along the c-axis can either keep the same (S-links) or rotate∼ (R-links) the honeycomb planes...... 128 A.8 The harmonic honeycomb family is rich in structural possibilities that tune sym- metry (depending on whether the number of NR and NS links is odd or even) and dimensionality (the extent of the NS links). This table summarizes this ob- servation. Note we assume that the IrO6 octahedra have ideal cubic symmetry. Complex distortions may create systems of lower symmetry than that indicated. 129

B.1 Non-magnetic and ferromagnetic c band structures of relaxed unit cells of Li2IrO3 H and Na2IrO3 1 with PBE+SOC+U with path through k-space show at the bottom of (a).h Whilei the non-magnetic band structure is metallic (b), a gap opens up between j = 1/2 states with a magnetic order (d). The density of states H for Li2IrO3 and Na2IrO3 1 (and likewise for the entire harmonic honeycomb series) is dominated by oxygenh i p and iridium d orbitals (c and e)...... 140

C.1 Powder X-Ray diﬀractogram of [AgSePh]∞ overlapping the diﬀractogram calcu- lated from Cuthbert et al. providing positive identiﬁcation for silver benzenese- lenolate.28 ...... 147 C.2 Larger [AgSePh]∞ crystal sizes, having dimensions in excess of 20 µm, are ob- served in the gram-scale-reaction product...... 147 C.3 Additional micrographs of [AgSePh]∞. Detail of step edges of the layered system down to single layer step edges are evident in the SEM micrographs...... 148 C.4 Single particles of [AgSePh]∞ were selected from confocal microscopy images and their spectra were compared. Color was invariant regardless of size and aspect ratio. Thickness had no discernable eﬀect but the precise thicknesses of crystals can be inferred only from total intensity. 100 isolated crystals were selected for this representation...... 149 C.5 HSE band structures for bulk and single-layer [AgSePh]∞ and single layer [AgSePh]∞ with the phenyls replaced with hydrogens Dashed lines show the Fermi level (at 0 eV) and the HSE band gap for bulk and single-layer [AgSePh]∞. Color of band signiﬁes the fraction of band occupations by inorganic atoms (Ag and Se) ver- sus organic atoms (C and H). Bulk and single layer HSE band structures look identical. Single layer and hydrogen truncated AgSe look similar for Ag and Se dominated bands with small changes to the band gap and mobilities...... 149 xiii

C.6 HSE, PBE, and df2 band structures for bulk [AgSePh]∞ Dashed lines show the Fermi level. Color of band signiﬁes the fraction of band occupations by inorganic atoms (Ag and Se) versus organic atoms (C and H). Band occupations and shape remain similar across these three levels of theory. N, N1 and Z are along the primitive lattice vectors a , b and c , respectively...... 150 C.7 Parameters of Ag lattice used∗ ∗ in relaxation∗ table...... 150

D.1 BaTiO3 is the quintessential ferroelectric. BaTiO3 has a cubic perovskite crystal structure at high temperatures. Both the barium and titanium are octahedrally coordinated by oxygen. Octahedra of similar center element share corners. . . . 155 D.2 BaTiO3 goes through three phase transition as temperature is lowered: P m3¯ (221) P 4mm (99) Amm2 (38) R3m (160). The red arrows in the diagram indicate→ the direction→ of the spontaneous→ polarization due to the displacement of the titanium atom and associated rearrangement of the oxygen atoms[273, 125]. 156

F.1 Symmetry checks for isotropy subgroups the BaTiO3phase transition P m3¯m (221) → R3m (160). a) cubic and rhombohedral BaTiO3 structures. b) The maximal subgroup relations of the of the point group 4/m32¯ /m (abbreviated as m3¯m), modiﬁed from Figure 7.1 in [179] and reproduced with permission. The nonpolar point group (4/m32¯ /m) is highlighted in green and the polar point group (3m) is highlighted in red. The point groups highlighted in blue (43¯ m and 32¯ /m) are the maximal subgroups between the nonpolar and polar point groups. c) A table, generated using the BCS tool CELLSUB (http://www.cryst.ehu.es/cryst/ cellsub.html)[29], of the indices of the maximal polar subgroups of the cubic space group P m3¯m with k-index of 1. We have highlighted those in red that correspond to subgroups shown in Figure D.2 d) A table of the possible transfor- mation matrices for diﬀerent chains of maximal subgroup from the nonpolar (221) to polar space group (160) for a group-subgroup index of 8. This table was gen- erated using the BCS tool (http://www.cryst.ehu.es/cryst/symmodes.html) SYMMODES[56]. This transformation matrix is used to transform the lattice and Wyckoﬀ positions...... 165 F.2 Wyckoﬀ splitting for BaTiO3 from the cubic phase to tetragonal phase. While the cubic phase has 3 symmetrically unique positions, the tetragonal phase has 4. 166 F.3 Once we have possible transformation matrices for the group-subgroup relation of a given index that give the proper Wyckoﬀ splitting, we transform the nonpolar lattice to the polar symmetry setting and compare to the polar lattice. If the lattices match within a generous tolerance of 3 Aand˚ 10 degrees, we then check the distance the atoms have move during the distortion...... 166

G.1 Diagrams for example neural networks a) Diagram for an arbitrary function f. b) A one-layer fully-connected network. c) A two-layer fully-connected network. d) A diagram for backpropogation through a fully-connected network...... 168 xiv

H.1 Condition for layer rotation equivariance...... 171 H.2 Filter equivariance equation...... 172 H.3 Equivariance of Clebsch-Gordan coeﬃcients. Note that each D may refer to a diﬀerent irreducible representation...... 173 H.4 Diagrammatic proof of point convolution rotation equivariance...... 174 H.5 Radial function learned by l = 0 and l = 2 ﬁlters for moment of inertia toy dataset. The ﬁlters learn the analytical radial functions. For a collection of randomly generated point sets, the mean minimum distance is the average of the minimum distance between points in each point set. Distances smaller than the mean minimum distance might not have been seen by the network enough times to correct the radial ﬁlter...... 175 H.6 Accuracy of missing point task by epoch of training ...... 177 H.7 Distance MAE of missing point task by epoch of training ...... 177 xv

List of Tables

4.1 Comparison of experimental and DFT (PBE+SOC+U) lattice parameters and H H Wyckoﬀ positions for Li2IrO3 and Na2IrO3. Experimental Li2IrO3 structure is reﬁned fromh∞i powder diﬀractionh∞i data [190]. Position tolerance re- quired to symmetrize DFT structures obtained from PBE+SOC+U is given below Wyckoﬀ positions...... 32 4.2 Comparison of experimental and DFT (PBE+SOC+U) lattice parameters and H H Wyckoﬀ positions for 0 Li2IrO3 and 0 Na2IrO3. Position tolerance re- quired to symmetrize DFTh structuresi obtainedh i from PBE+SOC+U is given below Wyckoﬀ positions...... 33 4.3 Comparison of experimental and DFT (PBE+SOC+U) lattice parameters and H H Wyckoﬀ positions for 1 Li2IrO3 and 1 Na2IrO3. Position tolerance re- quired to symmetrize DFTh structuresi obtainedh i from PBE+SOC+U is given below Wyckoﬀ positions...... 34 4.4 Comparison of experimental and DFT (PBE+SOC+U) lattice parameters and H H Wyckoﬀ positions for 2 Li2IrO3 and 2 Na2IrO3. Position tolerance re- quired to symmetrize DFTh structuresi obtainedh i from PBE+SOC+U is given below Wyckoﬀ positions...... 35

6.1 Results obtained by applying our workﬂow to the Materials Project database. indicates “in Materials Project database at time of search”. Boxes relate num-† bers by symmetry conditions, DFT calculations, and validation processes. Rows separated by a single line give the sum of the numbers given below it in the same box...... 57 6.2 Key, value data type, and value description for distortion.json entries. . . . 68 6.3 JSON keys, value data type, and value description for distortion dictionary of distortion.json entries...... 68 6.4 Key, value data type, and value description for workflow data.json entries. . . 69 xvi

6.5 Comparison of this work to other ab initio studies of ferroelectric perovskites. indicates the reference being compared to used the Local Density Approxi- mation† (LDA) functional in their calculations. LDA results tend to be smaller than results calculated with PBE (which we use in this work) due to smaller predicted lattice parameters by LDA than PBE. The workﬂow ids for entries in the table are (1) wfid 1476040944.53976 (2) wfid 1476040944.53976 and wfid 1476040947.794782 (3) wfid 1476040956.832394 (4) wfid 1476040982.95148 (5) wfid 1476041128.167316 (6) wfid 1476040384.215156 (7) wfid 1476040759.946834 (8) wfid 1484445148.273011 (9) wfid 1484445014.628732 (10) wfid 1476040851.179557...... 77

7.1 Performance on missing point task ...... 93

H A.1 Fractional atomic coordinates for 1 -Li2IrO3 extracted from single-crystal x- ray data at 300 K (Cccm space group,h i a = 5.9119(3) A,˚ b = 8.4461(5) A,˚ c = 17.8363(10) A,˚ Z = 16). All sites are fully occupied and Li positions are ﬁxed to nominal values such that edge-sharing IrO6 and LiO6 octahedra form a near- hexagonal arrangement in both (a + b, c) and (a b, c) planes. The isotropic displacement parameter U for Li is also ﬁxed to a value− in the range found for the other atoms. Values in brackets show standard deviations in the ﬁtted parameters.130

H H B.1 Lattice parameters for various levels of theory for 1 and Li2IrO3 and H H h i h∞i 1 and Na2IrO3 . All calculations for a given structure type are initalized withh i identicalh∞i magnetic order. U = 1.5 eV. The percentage diﬀerence between the relaxed and experimental lattice parameter is indicated by the color of the cell.138 B.2 Total energy (eV) for constrained collinear magnetic orders on relaxed Li2IrO3 structures...... 139 B.3 Total energy (eV) for constrained collinear magnetic orders on relaxed Na2IrO3 structures...... 139 B.4 Bond lengths and angles for experimental and theoretical structures...... 139 B.5 Table of total energy, Ir-Ir bond lengths, and Ir-O-Ir bond angles for Li2IrO3. . . 140 B.6 Table of total energy, Ir-Ir bond lengths, and Ir-O-Ir bond angles for Na2IrO3. . 140 B.7 Table of total energy, Ir-Ir bond lengths, and Ir-O-Ir bond angles for experimen- tally synthesized harmonic honeycomb iridates...... 141 H B.8 1 Li2IrO3 PBE+SOC+U lattice parameters for varying U. All calculations areh i initialized with the same magnetic order. The ﬁnal magnetizations are not identical to one another. For PBE+SOC+U(0.25 eV) and PBE+SOC, the ex- perimental lithium iridate structure is metallic. The relaxed PBE+SOC+U(0.25 eV) and PBE+SOC structures have gaps and relax to non-magnetic ground states.141 B.9 PBE+SOC+U for various initial magnetizations. All relaxations have a mag- netic order. Magnetic orders were initialized with magnetic moments of 1 Bohr magneton on each iridium atom...... 141 xvii

B.10 PBE+U for various initial magnetizations. Calculations initialized with as a non- magnetic state relax to be non-magnetic and have similar lattice parameters to a non spin-polarized calculation.: ...... 142

C.1 Calculated eﬀected masses at the direct gap of bulk, single and hydrogen-truncated [AgSePh]∞ The eﬀective masses at the direct gap are similar for bulk and single layer [AgSePh]∞ and [AgSePh]∞ truncated with hydrogens. Only two principle directions are given for 2D single layer calculations...... 148 C.2 Relaxation Wyckoﬀ tables:Lattice and Wyckoﬀ position parameters for one phenyl conﬁguration of Cuthberts crystal structure and DFT relaxations of that conﬁg- uration...... 151 C.3 Wyckoﬀ table for experimental structure of [AgSePh]∞. Lattice and Wyckoﬀ position parameters for one phenyl conﬁguration of Cuthberts crystal structure. 151 C.4 Wyckoﬀ table for LDA Relaxation of experimental structure of [AgSePh]∞. Lat- tice and Wyckoﬀ position parameters for one phenyl conﬁguration of Cuthberts crystal structure relaxed with LDA...... 152 C.5 Wyckoﬀ table for PBE Relaxation of experimental structure of [AgSePh]∞. Lat- tice and Wyckoﬀ position parameters for one phenyl conﬁguration of Cuthberts crystal structure relaxed with PBE...... 153 C.6 Wyckoﬀ table for df2 Relaxation of experimental structure of [AgSePh]∞. Lat- tice and Wyckoﬀ position parameters for one phenyl conﬁguration of Cuthberts crystal structure relaxed with df2...... 154

E.1 Table of calculated versus experimentally measured polarizations as given in the Landolt-B¨ornstein- Group III: Condensed Matter - Ferroelectrics and Related Substances [227, 228, 229]...... 158 E.2 New high-quality candidates ...... 159 E.3 New high-quality candidates ...... 160 E.4 Known high-quality candidates ...... 161 E.5 Known high-quality candidates ...... 162

H.1 Performance on missing point task by atom type ...... 176 xviii

Acknowledgments

To my advisor Prof. Jeﬀ Neaton, thank you for making sure I was always asking scientif- ically important questions and supporting me even when I wanted to do something strange. Thank you for always having a smile when I walk through your oﬃce door, for being a role model for how to handle immense responsibility with composure and joviality, and for fos- tering a supportive research environment where we are held to high-standards of scientiﬁc merit, eﬀective communication, and personal integrity. Thank you to my collaborators: Kim A. Modic, Itamar Kimchi, Nicholas P. Breznay, Alun Biﬃn, Sungkyun Choi, Roger D. Johnson, Radu Coldea, Pilanda Watkins-Curry, Gregory McCandless, Julia Y. Chan, Felipe Gandara, Z. Islam, Ashvin Vishwanath, Arkady Shekhter, Ross D. McDonald, and James G. Analytis (Chapter3), Sinead M. Griﬃn (Chapter 4), Mary S. Collins, Behzad Rad, Paul D. Ashby, and J. Nathan Hohman (Chapter 5), Sebastian E. Reyes-Lillio and Anubhav Jain (Chapter 6), and Nathaniel Thomas, Steve Kearnes, Lusann Yang, Li Li, Kai Kohlhoﬀ, and Patrick Riley (Chapter 7). Thank you to those who helped edit this thesis: Nate, Sean, Ben, Alejandro, Sinead, and Stephanie. My research was supported in part by a National Science Foundation Graduate Research Fellowship under Grant No. DGE 1106400, the Materials Project funded by the U.S. Depart- ment of Energy, Oﬃce of Science, Oﬃce of Basic Energy Sciences, Materials Sciences and Engineering Division under Contract No. DE-AC02-05-CH11231: Materials Project pro- gram KC23MP, the Molecular Foundry at Lawrence Berkeley National Lab, the Laboratory Directed Research and Development Program of Lawrence Berkeley National Laboratory under U.S. Department of Energy Contract No. DE-AC02-05CH11231, and an internship at Google. This research used resources of the National Energy Research Scientiﬁc Computing Center, a DOE Oﬃce of Science User Facility supported by the Oﬃce of Science of the U.S. Department of Energy under Contract No. DE-AC02-05CH11231. Additional calculations were conducted at the High Performance Computing clusters at Lawrence Berkeley Lab. To my labmates, for the many “team-building exercises” at Celia’s and Free House and conversations around the red couch. To my housemates, for giving me a relaxing and sup- portive space to come home to and for sharing many laughs over bottles of wine. To my graduate school compatriots and close friends, for your company during the ups and downs, many shared tasty meals, conversations about life, the universe, and everything, and always being up for silliness and mischief. You all have made my life outrageously interesting. To Meg, for everything you do for us Neatonians. I can never repay you with enough pickles, though I will try. To Marisa and Aricay, for wrangling Jeﬀ’s unruly schedule. To Nate Hohman, Jeﬀ Urban, and Anubhav Jain, for helping me ﬁnd my research voice. To Aimee and Tahnee, for always being a source of creative inspiration and absurdity. Thank you for all the airport pick ups and pilgrimages to Old Town and Extraordinary Desserts1. To Adrian, for teaching me how to have an astronaut mentality and for 10 years of beginning of the semester lunches. To the triumvirate of extraordinarily classy gentlemen,

1To the reader: If you are in San Diego, you MUST go to this restaurant. xix

Commodore Sukrit, King Philipp and Admiral of the Fleet Benjamin, for their exquisite tastes for the ﬁner things of life and marvelous wit. To Yasaman, for being my companion in condensed matter physics and deep learning at Berkeley and at Google and for all the bunny pictures. To Grandma Sally, for your perspective, compassion, understanding, love, and all the penguins. Sean, for getting me to repeatedly lift heavy things and bringing out my inner 5-year old. Nate, for pushing me and thinking so carefully about what things in this world need the most doing. I treasure our adventures and walks in conversation. Mom and Dad, for raising me to believe I could do anything and for always being there to share in my successes and comfort me through the rough patches. 1

Chapter 1

Introduction

Humanity’s increasing ability to manipulate matter across length scales has been one of the most inﬂuential factors in developing new technologies. Yet as far as we have come, we are still far from mastering arbitrary forms of matter at one of its most fundamental controllable level – atoms. Material synthesis and characterization remain laborious and resource-intensive processes; thus, it is important to prioritize eﬀorts toward existing and newly-discovered materials that show the greatest promise for new phenomena and techno- logical applications. In order to eﬃciently identify the most promising materials, we must understand how speciﬁc atomic arrangements give rise to desirable properties and use avail- able means to predict arrangements with high likelihood of being synthesized. The invention of the transistor, a technology made possible by the scientiﬁc understanding of solid state physics, has precipitated an exponential increase in computational power since the mid-20th century. Now in turn, the multidisciplinary process of materials discovery increasingly relies on computational methods. We can now rapidly screen materials for desirable properties by searching materials databases and performing high-throughput ﬁrst- principles calculations. This approach has led to the identiﬁcation of new functional materials that have been subsequently conﬁrmed in the lab [58, 277, 268]. However, this model of computational materials discovery is limited to the structures we can provide to our ﬁrst- principles methods. How can we systematically design materials to expand our search beyond the structures stored in databases? For atomic systems (crystals, materials, molecules, proteins, etc), quantum mechanics provides an ultimate design constraint. The electronic and nuclear interactions in materials lead to laws that set rules for the possible geometries atoms can adopt. How these quantum mechanical rules dictate the resulting atomic conﬁgurations is central to this thesis. The design space of stable atomic systems is much more limited than all possible ar- rangements of points in 3D space. Atoms in materials form geometric patterns and simple recurring arrangements. In inorganic crystals, we often identify units comprised of transi- tion metal atoms coordinated by atoms such as oxygen or sulfur that form simple polyhedra such as tetrahedra or octahedra. For molecules, we identify subgroups that are prevalent in organic chemistry such as phenyl groups (benzene) and hydroxyl groups (OH−). These CHAPTER 1. INTRODUCTION 2 recurrent collections of atoms in a ﬁxed structure that we deﬁne as structural motifs are the building blocks of atomic systems. This thesis explores a variety of systematic strategies for understanding and designing complex materials from structural motifs on the atomic scale. These approaches for designing materials combine geometric, chemical, and physical intuition with calculations based on quantum theory (density functional theory) and symmetry analysis. The primary features of structural motifs in materials are their geometry and topology: the shape of the motifs and how the motifs connect or otherwise relate to each other. For example, a transition metal atom may be octahedrally coordinated by oxygen but this coor- dination may be distorted away from the Platonic ideal. This distortion can greatly impact the electronic properties resulting from this motif. These octahedral motifs can connect to each other in various ways. They can share corners (as they do in Perovskites), edges (as they do in the Harmonic Honeycomb Iridates in Chapters 3 and 4) or faces (as they do in Corundum). For many systems, there is no unique way to meaningfully partition an atomic structure into structural motifs and some may be more useful in speciﬁc contexts than oth- ers. By breaking a structure into components that enable complex phenomena, we may be able to systematically design motifs and connectivities that lead to desirable properties, expediting our ability to explore the space of possible materials. Some material classes share structural motifs but diﬀer in the way those motifs connect. In the Chapters 3 and 4, we closely analyze how edge-sharing three-fold coordinated IrO6 octahedra in the harmonic honeycomb iridates leads to exotic magnetism. We propose an inﬁnite series of homologous structures that share the same basic structural units but diﬀer in their connectivity. We suggest this class of complex correlated systems can be better understood using a series of homologous structures with an identical local structure but diﬀerent connectivity. In other material classes, structural motifs are deﬁned by interactions between two diverse starting ingredients, enabling a range of geometries and connectivities. In Chapter 5, we explore metal-organic chalcogenide assemblies (MOChAs), bulk hybrid materials with low- dimensional inorganic structures that are scaﬀolded by organic ligands. In MOChAs, the formation of motifs is driven by the possible oxidation states of a transition metal and the packing of chalcogenide (S, Se, or Te) bonded organic molecules around that transition metal. These motifs connect through supramolecular assembly to form low-dimensional organic structures. In the case of silver benzene selenolate ([AgSePh]∞), the end product is a bulk system with two-dimensional electronic properties. We show how MOChAs lend themselves to geometric analysis and design. In structural phase transitions the geometry of motifs may change while the topology of those motifs is maintained. Ferroelectrics are materials that undergo a structural transition that results in the appearance of a spontaneous polarization that can be switched due to the energetic adjacency of degenerate low-symmetry states. In Chapter 6 we demonstrate how symmetry analysis, density functional theory calculations, and post-processing analysis can be automated to search for ferroelectric candidates, identifying several previously-unknown ferroelectric candidates. We discuss the use of isotropy subgroups for relating structures via CHAPTER 1. INTRODUCTION 3

symmetric distortions. Ideally, we want a means to automate the understanding of materials from their atomic structure. However, it is diﬃcult to hand-code, using physical and chemical intuition, all possible structural motifs. Deep learning is a machine learning method in which multiple layers of neural networks are trained using the backpropogation algorithm to learn important features of large datasets. These techniques have revolutionized computer vision, a ﬁeld that previously used hand-crafted features to create models to identify objects in images. Deep learning models now exceed human performance on a variety of image classiﬁcation tasks [94]. In materials informatics, it is currently common practice to hand-featurize atomic structures when building machine learning models of material properties because we lack a natural method of encoding these structures for neural networks [36, 279, 33]. If deep learning techniques can be adapted for atomic systems, they could be used to learn what structural motifs are chemically stable and give rise to desirable properties. In the Chapter 7, we present a new type of neural network architecture that can naturally handle 3D geometry and the mathematical objects that characterize physical systems. We contrast this network to existing work that focuses on creating input representations of atomic systems compatible with existing networks invented in computer vision or throwing out geometric information. The remainder of this chapter gives an overview of the material systems, phenomena, and computational techniques described in later chapters.

1.1 Harmonic Honeycomb Iridates

The harmonic honeycomb iridates (A2IrO3 for A Na,Li) are a class of structures with exotic anisotropic quantum magnetism. At the atomic level,∈ the harmonic honeycomb iridates form a class of structures with identical local geometry that diﬀer in the connectivity of basic structural units. Some structures in this series have been synthesized while others have yet eluded experimental synthesis eﬀorts. In these materials, electron correlation, spin-orbit coupling, and crystal ﬁeld eﬀects have comparable energy scales. The result is anistropic magnetism that originates from a single spin on each iridium in a Jeff = 1/2 state. Due to their geometry and spin, these materials may exhibit magnetic interactions de- scribed by the Kitaev model, an analytically solvable Hamiltonian that gives rise to a quan- tum spin liquid. Even as the temperature approaches absolute zero, quantum spin liquids have disordered spin states - the spins never order but rather transition between energetically degenerate conﬁgurations.

Energy levels of a single IrO6 octahedra

The dominant structural motif in harmonic honeycomb iridates are IrO6 octahedra. The 5d orbitals of the iridium atoms are split due to the presence of the oxygen atoms into a 2 2 2 2 2 two-fold degenerate manifold containing the x y and 2z x y d orbitals called Eg − − − CHAPTER 1. INTRODUCTION 4

and a three-fold degenerate manifold containing the xy, yz, and zx d orbitals called T2g. Since the Eg orbitals are closer to the oxygen atoms than the T2g orbitals and the oxygen atoms have a negative valence, the Eg orbitals are higher and the T2g orbitals are lower in energy, see the center of Figure 1.1. The energy diﬀerence between these orbitals due to the presence of the oxygen is called the crystal ﬁeld splitting. Experimentally, octahedrally coordinated iridates have crystal ﬁeld splitting, ∆CF 3 eV [96]. ≈ In the presence of large crystal ﬁeld splitting, the mixing of Eg and T2g is too energetically expensive to occur. The matrix elements of the angular moment operator L = (Lx,Ly,Lz) on the T2g orbitals are identical to those of the p orbitals modulo a minus sign, therefore the T2g orbitals have Leff = 1 [239]. The corresponding matrix elements for Eg mixing is zero therefore Eg orbitals have Leff = 0 and are said to be “quenched”[239]. As iridium is a heavy element, its electrons experience a large potential well from iridium’s nucleus and the energy scales involved begin to be comparable to the energy of the electron. Thus, the coupling between spin and orbital momentum, proportional to (Z4/n3)L S where Z is the atomic number and n is the principal quantum number, becomes a non-negligible· term of the Hamiltonian [47]. Spin and orbital angular momentum no longer commute and the quantum states of the electrons are eigenstates of total angular moment, J = L + S. The T2g orbitals have Leff = 1. Since 1 1/2 = 1/2 3/2, the T2g orbitals split into two ⊗ ⊕ manifolds, a two-fold degenerate Jeff = 1/2 manifold and a four-fold degenerate Jeff = 3/2 manifold, see the right of Figure 1.1. If the operator L S acts on the T2g orbitals with spin · components, we ﬁnd that the Jeff = 1/2 are λSO higher in energy and Jeff = 3/2 are λSO/2 lower in energy [239]. λSO in iridates is close to 0.5 eV [96], for a total splitting of 0.75 eV. ≈ Iridium has 9 5d electrons and in the harmonic honeycomb iridates, iridium takes a +4 oxidation state. The energy of Hund’s coupling is smaller than the crystal ﬁeld splitting energy (JH 0.25 eV ∆CF 3.0 eV [271]), so the 5 remaining Ir electrons ﬁll the T2g ≈ ≈ manifold such that Jeff = 3/2 is ﬁlled and Jeff = 1/2 is half ﬁlled. Since the Jeff = 1/2 is half ﬁlled, we would expect the iridates to be metallic. However, d orbitals are more localized than s or p orbitals and electrons experience repulsion from electrons in other d orbitals. This repulsion can be described by the Hubbard model in which there is competition between a hopping interaction with coeﬃcient t and the repulsion term with coeﬃcient U [114, 114]. As U/t 0, the system is metallic and as U/t the system is insulating. This eﬀect is large in→ 3d systems (with U 5 eV) where orbitals→ ∞ are more tightly bound with little overlap and small in 5d orbitals (≈U 1.5 2 eV in iridates) which are more diﬀuse, therefore overlapping more [167, 116]. Despite≈ the− eﬀect being small, this results in the two Jeff = 1/2 states being further split, preventing a metallic state. When a gap in the electronic states at the Fermi level is cause by Hubbard repulsion, a material is said to be a Mott insulator. The Mott gap in the honeycomb iridates is 0.4 eV [96]. ≈ CHAPTER 1. INTRODUCTION 5

Figure 1.1: The splitting of 5d orbitals for iridium atoms octahedrally coordinated by oxygen atoms. Crystal ﬁeld splitting breaks the degeneracy of the 5d orbitals into a two-dimensional manifold Eg and a three-dimensional manifold T2g. Spin-orbit coupling further splits the T2g manifold with Leff = 1 into Jeff = 1/2 and Jeff = 3/2 states.

Interaction of edge-sharing IrO6 octahedra Magnetic interactions arise primarily from exchange symmetry, the requirement that wave- functions of electrons must be antisymmetric under the exchange of any two electrons [48]. The Hamiltonian for the coupling of two spins can be written as ASi Sj, where A is a constant, [49]. The simplest extension of this interaction to the case of· many electrons is given by the Heisenberg model [48], X HH = JijSi Sj, (1.1) ij · where ij denotes neighbors. However, in general the magnetic Hamiltonian can have higher- order terms. Given two IrO6 octahedra sharing a single edge, there is a plane deﬁned by the iridium centers and the two oxygen atoms the iridium share (which we will call the Ir-O-Ir bond plane). The magnetic iridium atoms interact via their shared oxygen through superexchange [48]. Given ideal octahedral geometry, there are two identical Ir-O-Ir bond exchange paths for the isotropic terms. The Jeff = 1/2 states destructively interfere along these paths causing the isotropic Heisenberg interaction to disappear, leaving a weak anisotropic interaction due to Hund’s coupling [118]. This is called the Quantum Compass Model. Assuming the Ir-O-Ir bonds are in the xy-plane, the Hamiltonian further simpliﬁes to CHAPTER 1. INTRODUCTION 6

Figure 1.2: In the harmonic honeycomb iridates, the IrO6 edge-share with three nearest neighbors, forming three orthogonal planes deﬁned by the Ir-O-Ir bonds. These planes are indicated with blue, red, and green shading. The Ir ions are indicated by the circles while the oxygens (not shown) lie on the edges of the polyhedra.

z z Hij = JzSi Sj . (1.2)

The IrO6 octahedra in harmonic honeycomb iridates edge-share with three nearest neigh- bor octahedra. These neighbors are maximally far apart from one another such that the three planes deﬁned by the shared oxygen and central iridium atoms are orthogonal to each other, shown in Fig. 1.2. This gives a 3-fold orthogonal Quantum Compass Model known as the Kitaev Model, that is

X γ γ HK = Kγ S S . (1.3) − i j hiji where < ij > denotes, nearest neighbor iridium atoms that form a bonding plane perpen- dicular to γ. Due to distortion of the IrO6 octahedra, the magnetism of the harmonic honeycomb iridates is described by a Kitaev-Heisenberg model, where the distorted Ir-O-Ir exchange paths prevent complete destructive interference of the isotropic magnetic interaction. In Chapter 3, we present the discovery of the ﬁrst 3D harmonic honeycomb iridate and characterize its anisotropic magnetism. In Chapter 4 we compute the ground state structures of select members of the harmonic honeycomb homologous series with density functional theory-based methods (varying U and testing sensitivity to SOC) and investigate the eﬀect of the alkali metal (Li or Na) on the distortion of IrO6 octahedra. CHAPTER 1. INTRODUCTION 7

Figure 1.3: MOChAs can host inorganic structures of varying dimensionality and topology, from sheets and tubes (2D), to chains and rings (1D), to individual clusters (0D).

1.2 Metal-organic Chalcogenide Assemblies (MOChAs)

Metal-organic chalcogenides assemblies (MOChAs) are self-assembled hybrid crystals where low-dimensional transition metal chalcogenide structures are scaﬀolded by organic ligands [267]. Depending on the choice of organic ligand, the electronic structure near the Fermi level may be entirely dominated by the inorganic structure or inﬂuenced by the organic ligand. Due to the intrinsically insulating nature of many organic ligands, the geometry of MOChAs can be designed to yield bulk materials with low-dimensional electronic properties. Electrons restricted in one or more dimensions have properties that diﬀer from electrons in the bulk due to quantum conﬁnement and the lack of screening by neighboring atoms. This is one of the driving motivations for research in modern nanoscience. Two examples of this are graphene and MoS2; both form 2D sheets as well as nan- otubes. Graphene, a single layer of graphite, is the prototypical low-dimensional material comprised of an atomically-thin 2D hexagonal lattice of carbon atoms. While graphite is a semi-metal, graphene is a so-called Dirac semi-metal where electrons near the Fermi level behave relativistically. Layered transition metal dichalcogenides are comprised of edge shar- ing coordination polyhedra. These materials (e.g. MoS2) are semiconductors and undergo an indirect-to-direct bandgap transition when exfoliated to a monocrystalline single-layer. In both these examples, the bulk material is comprised of monolayers bonded by van der Waals interactions and the low-dimensional properties are only present in an isolated mono- layer. Low-dimensional materials are often laborious to synthesize, isolate, and keep clean. MOChAs present an alternative approach to realizing materials with low-dimensional prop- erties and to exploring low-dimensional phenomena. In contrast to isolated low-dimensional materials, MOChAs self-assemble at near room temperature and are robust to an ambient environment. CHAPTER 1. INTRODUCTION 8

The synthesis of MOChAs is highly modular allowing for various combinations of metals, chalcogenides, and organic ligands to be readily explored. MOChAs are synthesized using a metal salt or metal wafer and organic groups attached via a dichalcogen bond (R-E-E-R) where R represents any organic ligand and E = S, Se, Te. The reaction between the metal ion and the organochalcogen drives molecular self-assembly, resulting in the formation of supramolecular hybrid structures. There are three primary synthetic routes for achieving self-assembly of these structures, shown in Figure 1.5: immiscible layered strategy, gram- scale bulk synthesis, and wafer-scale gas phase deposition. With care, it is possible to produce millimeter-scale single-crystals of spontaneously self-assembled hybrid compounds. With metal-organic chalcogenides, we can harness the variety of geometry of organic molecules to tune the electronic properties of low-dimensional transition metal chalcogenide structures. Changing ligands and inorganic composition can yield diverse crystal geometries or variations of similar structures, see Figure 1.4. Using MOChAs style synthesis, we can make low-dimensional transition metal chalco- genide structures of materials that do not form layered materials or other low-dimensional structures in the bulk. In Chapter 5, we focus on one such example, silver benzene selenolate, [AgSePh]∞ where the subscript denotes the bulk material is comprised of many van der ∞ Waals bonded layers of AgSePh. Bulk Ag2Se is an indirect band gap semiconductor com- prised of four- and ﬁve-fold selenium coordinated silver atoms; the coordination polyhedra edge-share along all three crystal lattice directions. In contrast, [AgSePh]∞ is comprised of 2D sheets of silver tetrahedrally coordinated by selenium with the sheets scaﬀolded by phenyl groups. Additionally, [AgSePh]∞ is a direct band gap semiconductor that photoluminesces blue light. In Chapter 5, we describe multiple synthetic avenues for creating [AgSePh]∞ and study the quantum conﬁnement of its layers using photoluminescence measurements and density functional theory.

1.3 Ferroelectrics

When structural motifs are distorted, new electronic properties can arise that were previously forbidden by symmetry. One such property is ferroelectricity. Ferroelectric materials display couplings between magnetic, electronic, and lattice degrees of freedom, leading to exotic phenomena and making them technologically useful. Macroscopically, a ferroelectric material has a spontaneous polarization that is switchable by an applied electric ﬁeld [152] (see Figure 1.6a). At the atomic scale, ferroelectric switching is a structural transition between energetically degenerate structures with a spontaneous polarization resulting from the displacements of charged atoms. Phenomenologically, these degenerate ferroelectric structures arise from the symmetry breaking of higher-symmetry structure without a spontaneous polarization. Materials can only host a spontaneous polarization if they have a space group symmetry with a polar point group. Out of the 32 crystallographic point groups, 10 are polar (1, 2, m, mm2, 3, 3m, 4, 4mm, 6 and 6mm). The remaining point groups are nonpolar. A crystal with a nonpolar CHAPTER 1. INTRODUCTION 9

Figure 1.4: Diﬀerent transition met- Figure 1.5: Top) Three methods for mak- als and organic ligands form MOChAs ing MOChAs: immiscible layered strat- with various coordinations and topolo- egy, gram-scale bulk synthesis, and wafer- gies. (Top to Bottom) adamantane + scale gas phase deposition. Middle row). copper give a nanotube structure made of Crystals produced from each method. triangular coordination polygons, carbo- Bottom row) All three methods produce rane + lead give a chiral 1D chain of see- diﬀerent crystal morphologies but uni- saw coordination polyhedra, carborane + form emission energy. mercury give a non-chiral 1D chain of see- saw coordination polyhedra.

symmetry has a center of symmetry such that no vector quantity (such as a polarization vector) can be compatible with the crystal symmetry. The high-symmetry structure that cannot host a spontaneous polarization belongs to a nonpolar space group; we call it the nonpolar structure.1 The ferroelectric lower-symmetry structures belong to a polar space group; we call these degenerate structures the polar structures. See Appendix D for a concrete example of a prototypical ferroelectric, BaTiO3. In Chapter 6, we use this symmetry criterion to ﬁnd compatible pairs of nonpolar-polar structures to search for new ferroelectrics that may host new physics or be technologically useful.

1It is common in the ferroelectric literature for it to be said the high-symmetry structure is required to have centrosymmetry, meaning having inversion symmetry; this is not necessarily correct. Nonpolar is a more general symmetry criterion. All point groups with inversion symmetry are nonpolar, but there are chiral, nonpolar point groups without inversion symmetry (222, 422, 622, 32, 23, and 432). CHAPTER 1. INTRODUCTION 10

Figure 1.6: a) A ferroelectric is a material with a spontaneous polarization that is switchable by applying an external electric ﬁeld. b) The free energy written in terms of polarization has a double well, each well representing stable, switchable polar structures. c) A plot of the polarization of a ferroelectric versus the application of an electric ﬁeld will produce a hysteresis loop.

The structural transition from the nonpolar structure to one of multiple possible polar structures can be due to a phonon mode becoming “soft”, meaning it has become non- restorative, with decreasing temperature. In order to break the symmetries forbidding a spontaneous polarization to arise in the higher-symmetry nonpolar structure, the phonon mode itself must have a polar symmetry. One can search for ferroelectric materials by computing the phonon band structure for nonpolar structures and identifying polar phonon modes with negative energies. This method was used by Ref. [86] to search for ferroelectric candidates. For our work in Chapter 6, we use a search method motivated by the Landau theory of phase transitions[60]. Near the structural phase transition between the high-symmetry non- polar and low-symmetry polar structure, the free energy can be expanded using polarization, P , (in this case treated as 1D) as an order parameter as the following:

1 2 1 4 1 6 F = a0(T Tc)P + bP + cP EP, (1.4) 2 − 4 6 − where a0, b, c are constants, T is temperature, Tc is the critical temperature of the phase transition, and E is the electric ﬁeld. Below a critical temperature Tc, the free energy of a ferroelectric expressed in terms of polarization has (in the case of a 1D polarization) a double well, with each well represent- ing a stable, switchable structure with a spontaneous polarization (see Figure 1.6b). This transition is second order if the coeﬃcient b is positive, and ﬁrst order if it is negative [60]. In Chapter 6, we search for nonpolar-polar structure pairs that satisfy the symmetry requirements of Landau theory. In addition to the high(low)-symmetry structures being nonpolar(polar), we additionally require that they are continuously deformable into each other. This means that they satisfy group-subgroup relations and the polar structure must belong to an isotropy subgroup of the nonpolar structure; we go into detail about these CHAPTER 1. INTRODUCTION 11 symmetry requirements in Chapter6 and Appendix F. We then compute the polarization of structures along the distortion between nonpolar and polar structure in order to recover the spontaneous polarization. We must use intermediate structures to recover this quantity because polarization for a periodic system is deﬁned on a lattice; it is not a single well-deﬁned quantity and depends on the choice of unit cell [254]. It is the change in the polarization between the nonpolar and polar structure that is well-deﬁned [205]. If one follows the change in the polarization value on the polarization lattice as it moves throughout the ferroelectric distortion, one can deﬁne a single-valued change in the spontaneous polarization that does not depend on the choice of unit cell. This deﬁnition of polarization is compatible with what is seen experimentally. Experi- mentally, the polarization of a ferroelectric is not measured directly but instead determined by switching the polarization of a given sample with an external electric ﬁeld and measuring the current that results from the polarization switching [153]. If one then plots the inte- grated current divided by the surface area of the sample (to obtain units of [charge]/[area] in common units (µCoulomb/cm2).) as a function of electric ﬁeld, one obtains a plot of the polarization versus electric ﬁeld. This plot will have a hysteresis loop due to the switching. An ideal hysteresis loop would have a simple rectangular loop; above the critical electric ﬁeld that is suﬃcient to oppose the existing polarization, the polarization would instantaneously switch to the opposite polarization. However, experimentally measured hysteresis loops look more like Figure 1.6c. The speciﬁc shape of the hysteresis loop is determined by the inter- actions of the ferroelectric domains (domains with diﬀerently oriented polarizations) inside a macroscopic material [153]. In Chapter 6, we design an automated workﬂow for ﬁnding ferroelectric candidates by harnessing symmetry analysis to ﬁnd nonpolar-polar structure pairs and calculating the spontaneous polarization of these candidates using density functional theory calculations of intermediate structures between the nonpolar and polar structures. This workﬂow has been open-sourced and contributed to the atomate python package [165]. The data resulting from our ﬁrst ferroelectric search using this workﬂow on the Materials Project databases[124] has been made publicly available at http://blondegeek.github.io/ferroelectric_search_ site/.

1.4 Deep learning for atomic systems

Deep learning is a promising technique for expediting existing tools and creating new capa- bilities in computational materials exploration. It could potentially compute the properties of materials in an order of magnitude less time and propose hypothetical structures from experimentally known motifs. One of the challenges with applying deep learning techniques to materials and atomic systems generally is creating neural networks capable of operating on and producing the data types relevant to materials, such as 3D geometric conﬁgurations. The community has approached this challenge in two ways: designing specialized input representations of atomic systems to use with existing neural network architecture [32, 33, CHAPTER 1. INTRODUCTION 12

Figure 1.7: A network with 3D translation- and 3D rotation-equivariance allows us to identify chemical motifs in any location or orientation using the same ﬁlters.

36, 236, 92] and inventing new networks more tailored toward atomic structures [126, 83, 89, 222, 221]. These approaches have been used to predict properties of small molecules and crystals with chemical accuracy [202, 215, 62, 221] and to generate new molecules for applications such as drugs and devices [92]. However, these techniques either do not generalize to all types of atomic systems (molecules, crystals, polymers, nanocrystals, proteins, etc) or they throw out potentially useful geometric information. For example, Ref. [92] uses string representa- tions of the topology of molecular graphs, called SMILES strings, as input to their network [262]. This input representation is not appropriate for material systems because materials have much more ambiguous bonding structures and a topological representation does not in- clude any geometric information about the positions of the atoms. Ref. [126, 83, 89, 222, 221] use pairwise distances to encode atomic structures. Other rotation-invariant geometric in- formation, such as bond angles can also be included, however this becomes expensive to encode. Ideally, a neural network would use the atomic positions of the atomic system we are investigating and structural motifs could be identiﬁed at diﬀerent locations and orientations within an example without the need for data augmentation, see Figure 1.7. In Chapter 7, we present a universal framework for deep learning on atomic systems that can naturally handle 3D geometry and features of physical systems. We call this framework tensor ﬁeld networks. 13

Chapter 2

Methods

2.1 Density Functional Theory

The research presented in this dissertation uses density functional theory to understand the electronic structure of experimentally realized materials, evaluate hypothetical structures, and relate changes in the geometry of an atomic system to changes in its electronic properties. Density functional theory (DFT) is a technique that has made quantum mechanical properties feasible to calculate for a wide variety of atomic systems, tens to thousands of atoms in size. Modern DFT relies on the Kohn-Sham equations which are solved self- consistently; expedient linear algebra libraries; and a generous application of compute power to calculate electronic properties. The many body Schr¨odingerEquation in the Born-Oppenheimer approximation can be written as:

ˆ h ˆ ˆ ˆ i HΨ = T + Vext + Vint + EII Ψ = EΨ, (2.1) ˆ ˆ where T is the kinetic energy operator, Vext is potential energy associated with the nuclei, Vint describes the electron-electron interactions, EII is the classical interaction between nuclei, and E is the energy [162]. While such an equation is simple to write down, it is compu- tationally infeasible to solve for more than tens of particles because the complexity scales exponentially with the number of particles [132]. Density functional theory (DFT) formalism relies on two theorems, known as the Hohenberg- ˆ Kohn theorems [109]. First, for a given system, Vext(r) and thus the total energy of a system is a functional of the ground state charge density, n(r), expressed as Z E[n(r)] = drVext(r)n(r) + F [n(r)] + EII , (2.2) where F [n(r)] includes kinetic energy and electron-electron interactions. Second, the density that minimizes the total energy is the ground state charge density. These two theorems have signiﬁcant consequences; combined they imply the ground state total energy of a system CHAPTER 2. METHODS 14 of interacting electrons and nuclei is determined by the ground state electron density. We only need to know the energy functional E[n(r)] to solve for the ground state charge density variationally[163]. While a wavefunction has 3N variables, a charge density has only 3 (one for each spatial dimension). The greatly reduced number of degrees of freedom needed to describe the total energy and density of interacting many-body systems makes DFT a potentially powerful approach compared to more expensive wavefunction based methods. While the Hohenberg-Kohn theorem proves the existence of a universal functional, it does not provide a way to determine this functional.1 Fortunately, soon after the appearance of the Hohenberg-Kohn theorem in 1964, Kohn and Sham found a way to map the many-problem to that of a single electron in an external potential of non-interacting electrons in 1965 [133]. In this formulation, solving for the ground state charge density of this eﬀective non-interacting system leads to the same ground state charge density of the true interacting many-body system; the ground state wavefunctions of the eﬀective non-interacting system, obtained from the Kohn-Sham equations are used to determine ground state charge density of the many-body system. More explicitly, the Kohn-Sham approach reformulates the Hohenberg- Kohn expression for the ground state functional as: Z EKS = TS[n] + drVext(r)n(r) + EHartree[n] + EII + EXC [n] (2.3)

where TS[n] is the kinetic energy of non-interacting electrons, EHartree[n] is the mean-ﬁeld Coulomb interaction energy of the electron density, and EXC [n] is the exchange-correlation functional. The ﬁrst three terms of this equation are known and can be straightforwardly solved for. The EXC [n] term expresses the diﬀerence in kinetics and potential of an in- teracting versus a non-interacting system, which is readily seen in the following expression [163],

D ˆE D ˆ E EXC [n] = T TS[n] + Vint EHartree[n], (2.4) − − and is in general unknown.

Density functionals

A major success of DFT is that approximate forms of EXC have been developed that have been very eﬀective. Diﬀerent density functionals will treat exchange and correlation, EXC [n] diﬀerently. In this dissertation we use the LDA, PBE, and HSE functionals; these functionals are deﬁned below. In the local density approximation (LDA), one uses the exact exchange of a homogeneous electron gas as calculated from quantum Monte Carlo calculations [133]. The EXC for the LDA depends linearly on the charge density,

1Even if we were handed the universal functional, it may still be too expensive to feasibly compute. CHAPTER 2. METHODS 15

Z LDA homogen. EXC [n] = dr n(r)XC (n(r)). (2.5) Despite its simplicity, LDA has been successful at describing many material systems. The generalized gradient approximation (GGA) has lead to a class of functionals that depend on the charge density and its gradient, Z EGGA[n] = drGGA(n(r), n(r)). (2.6) XC XC ∇ The functional by Perdew, Burke and Ernzerhof (PBE) is a speciﬁc functional based on the GGA that is widely used [193]. GGAs can improve on the LDA for certain classes of systems. Neither LDA nor GGA treat van der Waals dispersion interactions, a nonlocal cor- relation eﬀect. LDA tends to overbind and PBE tends to underbind, resulting in structures that tend to have smaller and larger lattice parameters than experiment, respectively. Both LDA and PBE generally underestimate band gaps. Hybrid functionals include a diﬀerent fraction of exact Fock exchange. Range-separated hybrid functionals can include a fraction of exact exchange at short and long range. The exchange and correlation functional by Heyd, Scuseria, and Ernzerhof (HSE) includes a fraction of exact exchange for short range interactions and GGA exchange for longer range interactions distances and can be written as

EHSE = aEHF,SR(ω) + (1 a)EPBE,SR(ω) + EPBE,LR + EPBE (2.7) XC X − X X C , where a is 0.25 and ω, the range separation parameter, is 0.2 [140]. Fortuitously, HSE tends to give better band gaps than LDA and PBE, due to the inclusion of some amount of exact exchange, but for accurate band gaps one needs to go beyond DFT to an excited state formalism such as many body perturbation theory. Practically, one arrives at the ground state electron density through a self-consistent approach. For a given arrangement of nuclei, a starting guess for the charge density is made based on atomic orbitals. This charge density is then used to generate Vext(r) and Ψi(r). We then update the wavefunctions based on the solutions of the Kohn-Sham equations. We repeat until the ground state energy and forces converge to desired values, typically 10−3eV and 10−2 eV/A.˚

Plane waves and pseudopotentials To represent wavefunctions, one needs a basis set. In this dissertation, we focus on crystal systems so we use plane-waves. The plane-wave basis depends on the crystallographic lattice parameters of the input unit cell and an energy cutoﬀ Ecutoﬀ. For a given Ecutoﬀ, all plane- waves satisfying the following equation are included 2 h¯ 2 G + k < Ecutoﬀ, (2.8) 2me | | CHAPTER 2. METHODS 16 where G is a reciprocal lattice vector and k is a vector in reciprocal space. For many systems, including those described in this thesis, it is computationally expensive to treat all electrons independently. Like all electrons, the wavefunctions of core electrons must be orthogonal to one another. Because core electrons exist in a rather conﬁned region near the nucleus, this requires core electron wavefunctions to oscillate and deﬁnes their nodal structure. To accurately describe these core wavefunctions, one must use a basis that has a resolution comparable to these oscillations, which can be hundredths of Angstroms. For example, for Ecuttoﬀ = 520 eV, the resolution is approximately a tenth of an Angstrom.

2 2 h¯ 1 −11 520 eV (2.9) 2me 1.2 10 meters ≈ × To achieve a resolution of approximately a hundredth of an Angstrom, Ecutoﬀ would have to be increased a hundred fold. Moreover, core electrons are highly localized and well-separated in energy from valence electrons, which are crucial to determining structural and electronic properties. Therefore, it is a good approximation to freeze them into an eﬀective core and neglect core degrees of freedom in solving the Kohn-Sham equations. Thus, rather than treating core electrons directly, we use pseudopotentials which combine the nuclear and core electron contributions and create a smooth potential.

Treating on-site correlations associated with localized electrons with Hubbard U In general, the most commonly used exchange-correlation functionals for the solid state, LDA and PBE, are most eﬀective where the electron density is nearly uniform. Electrons in the Kohn-Sham DFT formalism neglecting exact exchange eﬀectively experience spurious interactions with their contribution to the charge density when the many-body system is cast as an eﬀective potential. This creates additional unphysical delocalization of the electron density; this can be highly problematic when describing more tightly bound d and f orbitals of transition-metals [164]. A computationally inexpensive approach that can improve treatment of such systems is to introduce a Hubbard U parameter penalizing electrons occupying the same site [26]. However, the value of U is usually empirically set; the use of U means the functional now depends on the density and occupation and the manner in which U is typically introduced leads to double counting errors, which can be serious in some cases [164]. Hybrid functionals such as HSE remove the need for such a parameter by including some amount of exact exchange. We use Hubbard U parameters in Chapters 4, 5 and 6 to treat materials comprised of transition-metals. 17

Chapter 3

Realization of a three-dimensional spin-anisotropic harmonic honeycomb iridate

The work described in this chapter has been published as Ref. [172].

Spin and orbital quantum numbers play a key role in the physics of Mott insulators, but in most systems they are connected only indirectly — via the Pauli exclusion principle and the Coulomb interaction. Iridium-based oxides (iridates) introduce strong spin-orbit coupling directly, such that the Mott physics has a strong orbital character. In the layered honeycomb iridates this is thought to generate highly spin-anisotropic magnetic interactions, coupling the spin orientation to a given spatial direction of exchange and leading to strongly frustrated magnetism. Here we report a new iridate structure that has the same local connectivity as the layered honeycomb and exhibits striking evidence for highly spin-anisotropic exchange. The basic structural units of this material suggest that a new family of three-dimensional structures could exist, the ‘harmonic honeycomb’ iridates, of which the present compound is the ﬁrst example.

3.1 Introduction

Quantum spin systems are characterized by small moments where the spin orientation is decoupled from the crystal lattice, in contrast to Ising-like spin systems that often apply to higher spin states. In the Heisenberg model describing spin-isotropic exchange between neigboring spins, spatial anisotropies of the exchange suppress long-range order [170], but do not lead to anisotropy of the magnetic susceptibility. Striking examples of this are quasi- 1D and -2D systems where the exchange diﬀers by orders of magnitude for neighbors along distinct crystallographic directions [234, 91]. The spin-orbit interaction introduces magnetic anisotropy by coupling the spin to the symmetry of the local orbital environment. Although CHAPTER 3. REALIZATION OF A THREE-DIMENSIONAL SPIN-ANISOTROPIC HARMONIC HONEYCOMB IRIDATE 18 in spin-1/2 systems the crystal ﬁeld does not introduce single-ion anisotropy (due to Kramer’s protection of the spin-1/2 doublet), it can — via spin-orbit — introduce spin-anisotropies in the g-factor and in the exchange interactions. The strength of the spin-orbit coupling varies by orders of magnitude between the 3d and 5d transition metals. In the former, quenching of the orbital moment decouples the orbital wavefunction from the spin, giving a g-factor anisotropy that is typically small and an even smaller spin-anisotropy. For example, spin- 1/2 copper in a tetragonal crystal ﬁeld has a g-factor anisotropy of order 10%, whereas the spin-anisotropy of exchange is of the order of 1% [91]. The stronger spin-orbit coupling of the 5d transition metals is known to give rise to larger magnetic anisotropies. In materials with edge-shared IrO6 octahedra, spin-anisotropy of the exchange between neighboring eﬀective spin-1/2 states is enhanced by the interference of the two exchange paths across the planar Ir-O2-Ir bond. Jackeli and Khaliullin (JK) suggested that in the honeycomb iridates this may lead to extreme spin-anisotropy of the exchange coupling, where in the limiting case, the only non-vanishing interaction is for the spin component normal to the Ir-O2-Ir plane [119, 59, 3]. In the honeycomb lattice, such an interaction couples diﬀerent orthogonal spin components for the three nearest neighbors; no single exchange direction can be simultaneously satisﬁed, leading to strong frustration. It is the possibility of engineering spin-anisotropy coupled to spatial exchange pathways that has spurred intense scientiﬁc research, particularly in connection to the search for quantum spin-liquids [130, 119, 59, 3]. However, whether the spin-anisotropic exchange interaction that is coupled to the Ir-O2-Ir bonding plane is realized in such materials remains an intense subject of scientiﬁc debate [233, 3, 63, 97], highlighting the need for the discovery of new materials with related structures and strongly anisotropic exchange interactions. We have synthesized single crystals of a new polytype of Li2IrO3 in which we reveal the eﬀect of the spin-anisotropy of exchange from the temperature dependence of the anisotropic magnetic susceptibility.

3.2 Results

Crystal structure

Single crystals of Li2IrO3 were synthesized as described in Methods. As shown in Figure 3.1A, the crystals are clearly faceted and typically around 100 100 200µm3 in size. In contrast to the monoclinic structure of the layered iridate, we ﬁnd× that× these materials are orthorhombic and belong to the non-symmorphic space group Cccm, with lattice parameters a = 5.9119(3) A,˚ b = 8.4461(5) A,˚ c = 17.8363(10) A˚ (see Appendix A for details of the crystallography). The structure (shown in Figure 3.1B and C) contains two interlaced honeycomb planes, the orientation of which alternate along the c axis. The x-ray reﬁnement (see Appendix A and Figures A.1-A.4) is consistent with fully stoichiometric Li2IrO3. In 4+ 5 this case the Ir oxidation state is Ir (5d ), ﬁxing the eﬀective Ir local moment Jeﬀ = 1/2, which is consistent with the magnetic properties of our crystals (see Figure 3.2). In CHAPTER 3. REALIZATION OF A THREE-DIMENSIONAL SPIN-ANISOTROPIC HARMONIC HONEYCOMB IRIDATE 19

H Figure 3.1: Single crystal of 1 -Li2IrO3 and the Ir lattice structure. (A) Single crystal oriented to be parallel to theh i crystallographic axes shown in (C), (B) 3D view and (C) projection in the ab plane. In (B) gray shading emphasizes the Ir (purple balls) honeycomb rows that run parallel to the a b diagonals, alternating upon moving along the c-axis. For simplicity only Li ions (grey balls)± located in the center of Ir honeycombs are shown. In (B) and (C) the rectangular box indicates the unit cell. Comparing (A) and (C) we note that the 70◦ angle between honeycomb rows is evident in the crystalline morphology. ∼ addition, highly-sensitive single-crystal susceptibility and torque measurements (see below) observe sharp anomalies at the transition to magnetic order, with no measurable variability in this transition temperature between many crystals measured, indicating that the observed magnetic order is well-formed and intrinsic to the crystals. This suggests that if present, Li vacancy disorder is small, because such vacancies will to lead non-magnetic Ir5+ 5d4[52], whose presence is expected to give rise to spin-glass behavior [25] which we do not observe. Taken together, our experiments indicate that our crystals are representative of the high- H H purity, stoichiometric limit. We denote the crystal structure 1 -Li2IrO3, where 1 refers to the single, complete oneycomb row. h i h i H High temperature magnetic anisotropy As can be seen in Figure 3.2, the raw magnetic susceptibility shows a magnetic anomaly at 38 K, most likely reﬂecting the bipartite nature of the structure, which alleviates the magnetic frustration. Due to the smallness of our samples and sensitivity to sample misalignment, the anisotropy at high temperatures could not be quantitatively resolved to high accuracy using SQUID magnetometry. To do so, we utilized torque magnetometry, which exclusively probes magnetic anisotropy (see discussion in Appendix A) and is suﬃciently sensitive to measure single crystals of 10µm dimensions. Torque magnetometry was measured by attaching an oriented single∼ crystal to a piezoresistive micro-cantilever [183] that measures mechanical CHAPTER 3. REALIZATION OF A THREE-DIMENSIONAL SPIN-ANISOTROPIC HARMONIC HONEYCOMB IRIDATE 20

0.06

600 0.05 400 1/ 0.04 200

0 /Ir) 0 50 100 150 200 250 300 B 0.03

( T (K)

a 0.02 b c 0.01

0.0 0 50 100 150 200 250 300 T (K)

Figure 3.2: The temperature dependence of the single-crystal magnetic suscepti- bility along the three principal crystalline directions. The inset shows 1/χ for all three axes χa, χb, and χc. The dashed line indicates the slope of the inverse Curie-Weiss sus- ceptibility for a paramagnet with eﬀective moment of µeff = 1.6µB, close to that expected of 1 an Ir Jeff = /2 state if g-factor anisotropy is ignored. All three components of susceptibility show strong deviation from Curie-Weiss behavior as a function of temperature. stress as the crystal ﬂexes the lever to try to align its magnetic axes with the applied ﬁeld. The mechanical strain is measured as a voltage change across a balanced Wheatstone Bridge and can detect a torque signal on the order of 10−13 Nm. The lever only responds to a torque perpendicular to its long axis and planar surface. As a result, the orientation of the crystal on the lever (determined by x-ray measurements and the diamond shaped morphology) deﬁnes the plane of rotation in ﬁeld and which principal components of anisotropy, αij (i, j a, b, c) are measured. To achieve this the cantilever was mounted on a cryogenic goniometer∈ to allow rotation of the sample with respect to magnetic ﬁeld without thermal cycling. The low temperature anisotropy was conﬁrmed on several similar sized single crystals. To measure αij = χi χj between 1.5 K and 250 K, three discrete planes of rotation for the same crystal were used.− A magnetically anisotropic material experiences a torque when its magnetization is not aligned with the applied magnetic ﬁeld; the deﬂection of the cantilever in a uniform magnetic CHAPTER 3. REALIZATION OF A THREE-DIMENSIONAL SPIN-ANISOTROPIC HARMONIC HONEYCOMB IRIDATE 21 ﬁeld is hence a direct measure of the magnetic anisotropy, ~τ = M~ H~ . At small ﬁelds, where the magnetic response is linear, the magnetic anisotropy is captured× by a susceptibility tensor Mi = χijHj. For an orthorhombic crystal, the magnetic axes coincide with the crystallographic directions, deﬁning χa,b,c. For example, for rotations in the b-c plane, the anisotropic magnetization (Mb,Mc) = (χbHb, χcHc) creates a torque

2 (χb χc)H sin2θ τa = − (3.1) 2 where θ is the angle between a crystallographic axis (c in this case) and the applied magnetic ﬁeld. The geometry of the lattice is intimately connected to the magnetic anisotropy. Speciﬁ- cally, we note that the angle φ0 between the honeycomb strips (see Figure 3.1C) is ﬁxed by the geometry of the edge shared bonding of the IrO6 octahedra (see Figures 3.3A). For cubic 1 ◦ octahedra cos φ0 = /3, namely φ0 70 , as shown in Figure 3.3A. The magnetic axes can be uniquely identiﬁed from a complete≈ angular dependence of the torque measurements, with the amplitude of the sin2θ dependence being proportional to the magnetic anisotropy αij. The observed magnetic axes are independent of temperature between 300 K and 1.5 K. The magnetic anisotropy, shown as data points in Figure 3.3B agrees well with the diﬀerences in the low temperature susceptibility data (grey lines in Figure 3.3B). At temperatures that are high relative to the exchange interaction energy scale, we expect that only the g-factor aﬀects the magnetic anisotropy. We ﬁnd that the ratio of the anisotropic susceptibilities αij/αjk asymptotically approach simple fractions at high temperature (above 100 K, see Figure 3.3C). Speciﬁcally, each Ir is in a three-fold local planar environment with∼ (almost) equidistant neighbors and thus the Ir g-factor anisotropy can be captured by ascribing each honeycomb plane susceptibility components parallel, χk and perpendicular, χ⊥ to the plane (consider Figure 3.3A). This uniaxial local iridium environment combined with the relative 1 orientation of the iridium planes, cos φ0 = /3, constrains the three components of suscepti- bility at high temperature to be equally spaced; 2χb = χa + χc (see Appendix A) and the 1 1 anisotropy ratios to be αba/αac = /2, αbc/αac = /2, αbc/αab = 1, just as we observe. This observation places constraints on the− ordering of the principal components of the g-factor at all temperatures.

Reordering of the principal magnetic axes The striking reordering of the principal components of susceptibility revealed in torque and SQUID magnetometry, is associated with a strong deviation from Curie-Weiss behavior as the temperature is lowered: αbc changes sign at T 75 K (Figure 3.3 D and Figures A.5-A.6). This is in stark contrast to spin-isotropic Heisenberg≈ exchange systems where the low tem- perature susceptibility reﬂects the g-factor anisotropy observed at high temperatures, even in the presence of spatially-anisotropic exchange [91]. The change of sign of αbc arises because χb softens, becoming an order of magnitude greater than χa and 5 χc (Figure 3.2 and 3.3B). As a result, the susceptibility cannot be parameterized by a∼ Curie-Weiss× temperature: CHAPTER 3. REALIZATION OF A THREE-DIMENSIONAL SPIN-ANISOTROPIC HARMONIC HONEYCOMB IRIDATE 22

A 50 B

40 -3

) x10 30 -1 T

-1 20 f.u.

B 10 µ ( ij

c α 0

-10 b ~70º αba αbc αac

0 50 100 150 200 250 a T (K) 6 C D

1 -3 3

1 ) x10 /2 -1 T

0 -1 0 ratio f.u. α

1 B - /2 µ (

αba/αac bc 52K α -3 -1 60K αbc/αac 75K 100K αbc/αab -6 50 100 150 200 -45 0 45

T (K) θbc (°)

Figure 3.3: Temperature dependence of the magnetic anisotropy. (A) Each Ir is surrounded by one of two planar, triangular environments indicated by blue and red shaded triangles, located at 35◦ either side of the b-axis. (B) The anisotropy of the magnetic susceptibility as measured∼ by torque and the diﬀerences in (SQUID) susceptibilities (grey lines) are shown as a function of temperature for all three crystallographic directions. An anomaly indicates the onset of magnetic order at TN = 38 K. (C) The ratios of the anisotropic susceptibility tend to simple fractional values dictated by the g-factor anisotropy of the local planar iridium environment. (D) sin(2θ) ﬁts to the anisotropy αbc illustrating the change of sign at 75K. ∼ the linear extrapolation of all three components of inverse susceptibility to the temperature axis depends strongly upon the temperature range considered. Between 50–150 K the ex- trapolation of all three components of inverse susceptibility is negative, consistent with the CHAPTER 3. REALIZATION OF A THREE-DIMENSIONAL SPIN-ANISOTROPIC HARMONIC HONEYCOMB IRIDATE 23 absence of net moment in the ordered state. However, at higher temperatures (200–300 K) the inverse susceptibilities 1/χb, 1/χc extrapolate to positive temperature intercepts (see Fig- ure 3.2) indicating a ferromagnetic component to the interactions. Above 200 K, 1/χ the 1 Curie-Weiss slope gives µeff 1.6µB, consistent with a Jeff = /2 magnetism. ≈ The observed ten fold increase in χb cannot be driven by the g-factor of the local iridium environment, whose geometric constraints are temperature independent (see Appendix A). The temperature dependence of χb must therefore arise from spin-anisotropic exchange. We note that all the c-axis bonds have the Ir-O2-Ir plane normal to the b-axis, whether they preserve or rotate between the two honeycomb orientations (see the full structure in Figure A.3A and a schematic in Figure 3.4A - green shading indicate the Ir-O2-Ir planes). This is the only Ir-O2-Ir plane that is normal to a crystallographic axis. This coupling of the spin-anisotropy to the structure, provides evidence for spin-anisotropic exchange across the c-axis links, and by extension should be present in all Ir-O2-Ir exchange paths. This likely arises from the interfering exchange mechanism suggested by JK in the context of the Kitaev model (see Appendix A).

Low temperature magnetic properties

The softening of χb is truncated at 38 K by a magnetic instability. Within the ordered state, the magnetization increases linearly with applied ﬁeld (Figure 3.4C, τ/H in 3.4B and Figure A.6). At suﬃciently high magnetic ﬁelds H∗, the magnetization kinks abruptly. This ∗ corresponds to an induced moment of 0.1µB. Above H , the ﬁnite torque signal reveals that the induced moment is not co-linear≈ with the applied ﬁeld, consistent with the ﬁnite slope observed at these ﬁelds in Figure 3.4C. This shows that in the phase above H∗ the induced magnetization along the ﬁeld direction is not yet saturated (the value is well below 1 the expected saturated Ir moment of 1µB for Jeff = /2). The angular dependence of both the slope of the linear regime and the kink∼ ﬁeld H∗, exhibit an order of magnitude anisotropy with ﬁeld orientation (Figure 3.4D and 3.4E). Such strong anisotropy in a spin-1/2 system highlights the strong orbital character arising from the spin-orbit coupling, again in contrast to spin-1/2 Heisenberg anti-ferromagnetism [91].

3.3 Discussion

There is a very interesting connection between the layered honeycomb Li2IrO3 and the H polytype studied here. The 1 -Li2IrO3 is distinguished by its c-axis bond, which either preserves or rotates away fromh ai given honeycomb plane (see Figure 3.5A and Figure A.7); in the case that all the bonds preserve the same plane, the resulting structure is the layered honeycomb system. Further polytypes can be envisioned by tuning the c-axis extent of the honeycomb plane before switching to the other orientation (see Figure 3.5B). We denote H H each polytype N -Li2IrO3, where N refers to the number of complete honeycomb rows (see Figure 3.5Bh andi Figure A.8), andh thei family as the “harmonic”-honeycombs, so named CHAPTER 3. REALIZATION OF A THREE-DIMENSIONAL SPIN-ANISOTROPIC HARMONIC HONEYCOMB IRIDATE 24

6 A B

3 ) -1 + 0

- Nm T b -9 -3 H (10 /

- + τ

-6 H*

5 10 15

µ0 H (T)

[100] [010] [001] [100] 0.15 30

C D E b 1

τ /

a H

2 (10 ) b a

-1 0.10 20 -9 (T) f.u. H* 0 T Nm B H* H*

M ( µ 0.05 10

-2 )

-1 0.00 0 1 2 3 4 0 45 90 -45 0 45 90

µ0 H (T) θab (°) θac (°)

H Figure 3.4: Low temperature magnetic properties of the 1 -Li2IrO3. (A) The h i ˆ Ir-O2-Ir planes deﬁning three orthogonal directions of the spin-exchange, one parallel to b and the other two parallel to aˆ cˆ, labelled + and (aˆ is the unit vector along a). This connects to the notation used to± describe the Kitaev Hamiltonian− in SI III. (B) Torque signal τ divided by the applied magnetic ﬁeld H at a temperature of 1.5 K, illustrating a linear low-ﬁeld dependence and a kink at H∗, which is strongly angle dependent (colors correspond to angles shown in (D)). (C) Magnetization vs magnetic ﬁeld applied along the b-axis at a ∗ temperature of 15 K. (D) & (E) The angle dependence θab/ac of the kink ﬁeld H of the ordered state (full circles, left axes) with respect to the crystallographic axes a, b and c. ∗ H is correlated to the magnetization anisotropy αij (open circles, right axes) indicating a common moment at H∗ in all ﬁeld orientations. CHAPTER 3. REALIZATION OF A THREE-DIMENSIONAL SPIN-ANISOTROPIC HARMONIC HONEYCOMB IRIDATE 25

Figure 3.5: Introducing the harmonic honeycomb series. (A) Two kinds of c-axis H bonds (black links) in the harmonic honeycomb family N -Li2IrO3 are shown, one linking within a honeycomb plane (for example blue to blue, top)h i and one that rotates between honeycomb planes (for example red to blue, bottom). For undistorted octahedra, these links are locally indistinguishable, as can be observed by the local coordination of any Ir atom (also see Figure 3.3A). (B) These building blocks can be used to construct a series of structures. The end members include the theoretical N = 0 ‘hyper-honeycomb’ [160, 127, 146] and the N = layered honeycomb [189]. Here N counts the number of complete honeycomb rows in a section∞ along the c-axis before the orientation of the honeycomb plane switches.

H to invoke the periodic connection between members. The layered compound, -Li2IrO3 H h∞i [189] and the hypothetical hyper-honeycomb structure, 0 -Li2IrO3 [127] are the end mem- bers of this family (see also SI IV). The edge-sharing geometryh i of the octahedra preserves the essential ingredients of the Kitaev model and this is universal for this family of polytypes. Each structure is a material candidate for the realization of a 3D spin liquid in the pure H Kitaev limit (see Appendix A and for 0 -Li2IrO3 see Refs. [160, 146, 127]). Finally, we speculate on the consequencesh i and feasibility of making other members of H H H the N -Li2IrO3 family. Both the layered -Li2IrO3 and the 1 -Li2IrO3 are stable structures,h i implying that intermediate membersh∞i may be possible underh appropriatei synthesis conditions. The building blocks shown in Figure 3.5A connect each member of the harmonic honeycomb series in a manner that is analogous to how corner sharing octahedra connect the Ruddlesden-Popper (RP) series. Indeed, despite the fact that members of the RP family are locally identical in structure, they exhibit a rich variety of exotic electronic states; including superconductivity and ferromagnetism in the ruthenates [169, 99], multiferroic behavior in the titanates [37], collosal magnetoresistance in the manganites [171] and high temperature CHAPTER 3. REALIZATION OF A THREE-DIMENSIONAL SPIN-ANISOTROPIC HARMONIC HONEYCOMB IRIDATE 26 superconductivity in the cuprates [148]. The harmonic honeycomb family is a honeycomb analogue of the RP series, and its successful synthesis could similarly create a new frontier in the exploration of strongly spin-orbit coupled Mott insulators.

3.4 Methods

Synthesis

Powders of IrO2 (99.99% purity, Alfa-Aesar) and Li2CO3 (99.9% purity, Alfa-Aesar) in the ratio of 1:1.05, were reacted at 1000◦C, then reground and pelletized, taken to 1100◦C and cooled slowly down to 800◦C. The resulting pellet was then melted in LiOH in the ratio of ◦ ◦ H 1:100 between 700-800 C and cooled at 5 C/hr to yield single crystals of 1 -Li2IrO3. The crystals were then mechanically extracted from the growth. Single crystal x-rayh i reﬁnements were performed using a Mo-source Oxford Diﬀraction Supernova diﬀractometer. Please see Appendix A for a detailed analysis.

Magnetic measurements Two complementary techniques were used to measure the magnetic response of single crystals H of 1 -Li2IrO3; a SQUID magnetometer was employed to measure magnetization and a piezoresistiveh i cantilever to directly measure the magnetic anisotropy. The magnetization measurements were performed in a Cryogenic S700X. Due to the size of the single crystals, the high temperature magnetization was near the noise ﬂoor of the experiment. Nevertheless, SQUID measured anisotropies at high temperatures were close to those measured by torque, with absolute values of χa(300K) = 0.0021µB/T f.u. and χb = 0.0024µB/T f.u.. Curie-Weiss ﬁts to the linear portion of the susceptibility yielded an eﬀective moment of µeff = 1.6(1)µB, 1 consistent with Jeff = /2 magnetism. However, the SQUID resolution was not adequate to determine the susceptibilities anisotropy at high temperature to the accuracy we required (see Figure 3.2 ). To resolve the magnetic anisotropy throughout the entire temperature range, we employed torque magnetometry, where a single crystal could be precisely oriented. Although the piezoresistive cantilever technique is sensitive enough to resolve the anisotropy of a 50µm3 single crystal, and hence ordering of susceptibilities at high temperature, the absolute∼ calibration of the piezoresistive response of the lever leads to a larger systematic error than in the absolute value of the susceptibility measured using the SQUID at low temperature. To reconcile these systematic deﬁciencies in both techniques, the torque data was scaled by a single common factor of the order of unity, for all ﬁeld orientations and temperatures, so as to give the best agreement with the diﬀerences between the low temperature susceptibilities as measured using the SQUID. The rescaled torque data was thus used to resolve the magnetic anisotropy at high temperature where the susceptibility is smallest. Torque magnetometry was measured on a 50 100 40µm3 single crystal (5.95 10−9 mol Ir) employing a piezoresistive micro-cantilever× [183]× that measures mechanical stress× as CHAPTER 3. REALIZATION OF A THREE-DIMENSIONAL SPIN-ANISOTROPIC HARMONIC HONEYCOMB IRIDATE 27 the crystal ﬂexes the lever to try to align its magnetic axes with the applied ﬁeld. The mechanical strain is measured as a voltage change across a balanced Wheatstone Bridge and can detect a torque signal on the order of 10−13 Nm. Torque magnetometry is an extremely sensitive technique and is well suited for measuring very small single crystals. The cantilever was mounted on a cryogenic goniometer to allow rotation of the sample with respect to magnetic ﬁeld without thermal cycling. The lever only responds to a torque perpendicular to it’s long axis and planar surface, such that the orientation of the crystal on the lever and the plane of rotation in ﬁeld could be chosen to measure the principal components of anisotropy, αij. The low temperature anisotropy was conﬁrmed on several similar sized single crystals. However to measure αij = χi χj between 1.5 K and 250 K, three discrete planes of rotation for the same crystal were used.− When remounting the sample to change the plane of rotation, care was taken to maintain the same center of mass position of the crystal on the lever to minimize systematic changes in sensitivity. Magnetic ﬁelds were applied using a 20 T superconducting solenoid and a 35 T resistive solenoid at the National High Magnetic Field Laboratory, Tallahassee, FL. 28

Chapter 4

Ab initio Studies of Structural and Energetic Trends in the Harmonic Honeycomb Iridates

Edge-sharing iridates present an exciting opportunity to study the competition of Mott insulator physics and strong spin-orbit coupling. These interactions also make these materials a challenge to study computationally. Harmonic honeycomb iridates are a recently discovered homologous series of stoichiometrically identical structures that host anisotropic magnetism and exotic spin ordering. We use density functional theory (DFT) to investigate structural and energetic trends in Li2IrO3 and Na2IrO3 harmonic honeycomb iridates. We predict the formation energies and distortion of as-yet unsynthesized series members to be degenerate for identical composition. We also demonstrate that DFT can accurately predict the structure of Li2IrO3 harmonic honeycomb iridates, but only if we account for strong spin-orbit coupling and electron-electron correlation at the level of a Hubbard U in these materials.

4.1 Introduction

Iridates have the ingredients believed to be necessary to host a spin-liquid state: crystal ﬁeld splitting to create low spin states, strong spin-orbit interactions to couple spin and lattice degrees of freedom, and frustrated lattices to foster anisotropic magnetic interactions [35]. Systems as complex as iridates, it is invaluable to have a series of structures one can compare and tune to understand the ingredients driving local and long-range interactions. The harmonic honeycomb iridates are a recently discovered series of crystal structures that are three-dimensional analogs to the two-dimensional honeycomb lattice [172]. The materials are spin-orbit Mott insulators, where strong spin-orbit coupling and electronic correlation result in the opening of a gap [172, 242, 45, 44]. Like iridates on kagome, hy- perkagome, pyrochlore and honeycomb lattices, the harmonic honeycombs are geometrically frustrated which may give rise to new physics leading to a spin liquid state [35]. Direct CHAPTER 4. AB INITIO STUDIES OF STRUCTURAL AND ENERGETIC TRENDS IN THE HARMONIC HONEYCOMB IRIDATES 29 evidence of bond-directional interactions in layered honeycomb Na2IrO3, suggest that a spin liquid state may be achievable in the harmonic honeycomb iridates if anisotropic interactions can be tuned through structural distortions or chemical substitutions [115]. The harmonic honeycomb structures are pictured in Figure 4.1. We use H # to designate a particular structure, where # is the number of rows of completed hexagonsh i along the orthorhombic c direction between alternating bonding planes. Single crystals of Li2IrO3 H H H H 0 , Li2IrO3 1 , and Na2IrO3 and polycrystalline samples of Li2IrO3 have beenh i synthesizedh [190i , 231, 172, 242].h∞i The magnetic order and anisotropy of these materialsh∞i is sensitive to distortion and structure dimensionality 1. Not yet synthesized members may have the environment necessary to host exotic phases and can lend important clues to understand these materials’ complex magnetic interactions. Using density functional theory (DFT), we investigate whether as-yet unsynthesized members are energetically favorable and examine variations in magnetically relevant bond lengths and angles across the series. We ﬁnd we can accurately predict these values by including spin-orbit coupling and Hubbard U-type corrections for Ir 5d orbitals in our cal- culations. Li2IrO3 is more sensitive to the inclusion of these interactions than Na2IrO3 due the Ir-Ir bond lengths being 5% shorter in Li2IrO3 than Na2IrO3 . We use the virtual crystal approximation (VCA) to demonstrate this sensitivity. Our calculations indicate the harmonic honeycombs of Li2IrO3 are nearly degenerate in formation energy for various spin-orderings, likewise for Na2IrO3. For a given alkali, the diﬀerence in energetics between phases corresponding to early members of this series do not exceed 20 meV per formula unit, small compared to the growth temperature of these materials of approximately 1300 K (112 meV). Thus, the lack of experimental evidence of other structures may not be an issue of energetics but of kinetics or growth conditions. For a given alkali, there is no notable change of Ir-Ir bond length or Ir-O-Ir bond angles across the relaxed harmonic honeycomb series. According to Ref. [120], the strength of local anisotropic interactions is sensitive to distortions of the iridium oxide octahedra. Since our calculations show that for a given composition these distortions are uniform across the series, diﬀerences in magnetism of the harmonic honeycomb iridates for a given alkali may indicate sensitivity to long-range structure. Our calculations suggest that the harmonic honeycomb iridates may provide a path for understanding and tuning long-range interactions.

4.2 Calculation Details

Our DFT calculations are performed using the Vienna Ab initio Software Package (VASP) with a plane wave basis [135, 137, 136]. We use the generalized gradient approximation

1 H H H Li2IrO3 0 , 1 and have been measured or postulated to have incommensurate spiral mag- h i h i h∞i H netic orders [44, 45, 209]. Na2IrO3 has a comparatively simple, commensurate “zigzag” collinear h∞i H H order [155, 64, 270]. The magnetic anisotropy of Li2IrO3 0 and 1 dramatically reorders below the h i h i H spin ordering temperature while the magnetic anisotropy of polycrystalline Li2IrO3 and single crystal H h∞i Na2IrO3 do not exhibit this change across their transition temperature [172, 242, 231, 233, 55]. h∞i CHAPTER 4. AB INITIO STUDIES OF STRUCTURAL AND ENERGETIC TRENDS IN THE HARMONIC HONEYCOMB IRIDATES 30 functional of Perdew, Burke, and Ernzerhof (PBE) [193], PAW pseudopotentials [46, 138] and an energy cutoﬀ of 520 eV. Monkhorst k-point meshes of 9x9x5, 9x9x3, 9x9x1, and 9x9x9 are used for the H 0 , H 1 , H 2 and H structures, respectively. Relaxations are performed with spin-orbith i couplingh i h andi Hubbardh∞i U corrections to localized Ir 5d states following the approach in Ref. [81], unless otherwise speciﬁed, and allow unconstrained non- collinear magnetism as described in Ref. [108, 107]. When including these interactions during optimizations, non-collinear spin and structural contributions to the total energy have to be calculated iteratively, making these calculations computationally expensive. Unit cell and ionic position relaxations are initialized with idealized harmonic honeycomb structures, where iridium oxide octahedra are undistorted such that Ir-O-Ir bond angles are 90◦ and all Ir-Ir bond lengths are taken to be equal and derived from average experimental values. Relaxations are not restricted to the spacegroup of the initial structure since spinor wavefunctions used in relativistic calculations transform under the appropriate spin space- group determined by the magnetic order [217]. Previous studies of the harmonic honeycomb iridates do not indicate structural transitions at low temperature [172, 233, 64]. Thus, we report re-symmetrized relaxed structures for ease of comparison using the Materials Project Python package (pymatgen) [187]. We conﬁrm that there is no signiﬁcant change in total energy between the relaxed and re-symmetrized structures. Relaxation results are converged such that Hellmann-Feynman forces on individual atoms in any direction are less than 0.01 eV/A,˚ the energy diﬀerence between self-consistent electronic steps is less than 10−5 eV, and that the absolute value of the external pressure, computed as the trace of the stress tensor, is less than 0.5 kB. When referring to the level of theory of the calculation, we will use abbreviations to denote the functional used (in this case, PBE) and whether not spin-orbit coupling (SOC) and a Hubbard U correction to the 5d iridium orbitals (U) is included. To relax the series for structural and energetic comparisons, we use PBE+SOC+U. The values for onsite U correction used in studying iridates spans from 0 to 4 eV, with most calculations using U = 1.5 - 3 eV [168, 272, 184, 155, 161, 150]. We ﬁnd that lattice H parameters, bond angles, and bond lengths of 1 Li2IrO3 are insensitive to U provided that U was at least 0.5 eV. We use U = 1.5 eV for allh i calculations, unless otherwise speciﬁed, to ensure that our calculations maintain a gap during relaxations and permit total energy comparisons between series members. Lattice parameters, bond lengths, and distortions of PBE+SOC+U relaxations are insensitive to inital magnetic conﬁguration. Because of this, we initialized structural relaxations with a randomized spin ordering with a normalized magnetic moment of 1 µB per Ir. To evaluate diﬀerent approximations to DFT for these systems, we compare (i) the ratio of lattice parameters, (ii) Ir-Ir bond lengths, and (iii) Ir-O-Ir bond angles with experimental values where possible. The ﬁrst two metrics inform us whether there has been an anisotropic relaxation of the unit cell. Experimentally synthesized structures have Ir-Ir bond lengths that vary by less than 0.01 A.˚ Thus, deviations from this trend indicate inaccuracies of a give approximation. ± The third metric is a direct measurement of the distortion of the iridium oxide octahedra, see Figure 4.1(b-e). The distortion mode of experimental structures from idealized harmonic CHAPTER 4. AB INITIO STUDIES OF STRUCTURAL AND ENERGETIC TRENDS IN THE HARMONIC HONEYCOMB IRIDATES 31 honeycomb lattices is identical across the series for both Li2IrO3 and Na2IrO3 and preserves the spacegroup of the undistorted structure. The amplitude of the distortion is greater in Na2IrO3 than Li2IrO3 . The distortion is dominated by displacements of oxygen and alkali atoms and changes in the Ir-O-Ir bond parameterize the distortion of the iridium oxide octahedra.

4.3 DFT Results

Tables 4.1, 4.2, 4.3, and 4.4 show lattice parameters and Wyckoﬀ positions for Li2IrO3 and H H H H Na2IrO3 , 0 , 1 , and 2 relaxed with PBE+SOC+U(=1.5 eV). h∞i h i h i h i The lattice parameters for Li2IrO3 and Na2IrO3 structures relaxed with PBE+SOC+U diﬀer <2% from experimental values, out-performing other approximations tested. Our re- H H sults for PBE+SOC+U for Na2IrO3 and Li2IrO3 agree with VASP GGA+SOC+U calculations in Ref. [161], where U =h∞i 3.0 eV. Ref. [161] similarlyh∞i noted that GGA+SOC+U gave better agreement with lattice parameters than GGA. From our structural relaxations of the atomic positions and volume of idealized unit cells H H H H of 0 , 1 , 2 and Li2IrO3 and Na2IrO3, for a given alkali, we ﬁnd no notable changeh i of bondh i lengthsh i andh∞i bond angles across the series. The distortion of the Ir-O-Ir bond angle is driven by the choice of alkali metal (Li or Na). The ratio of the radii of sodium and iridium is further from unity than the ratio of radii of lithium and iridium, thus causing greater distortion of the oxygen octahedra. Experimentally, angles between 92 97◦ are H H − seen in Li2IrO3 0 and Li2IrO3 1 . Our calculations ﬁnd angular variations of only one h i ◦h i ◦ degree around average values of 94 for Li2IrO3 and 100 for Na2IrO3. The uniformity of distortion and bond lengths across the series results in similar band structures and densities of states for members of identical composition. For example, Fig- ure 4.2 shows very little variation in the non-magnetic band structure and density of states across the series 2. A non-vanishing magnetic order is required to open up a gap in the harmonic honeycomb iridates. Figure 4.3 shows the nonmagnetic and ferromagnetic along c H H density of states of Na2IrO3 and Li2IrO3 relaxed with PBE+SOC+U. While the non-magnetic band structureh∞i is metallic, a magnetich∞i order is able to open the gap for both H structures. Comparingh∞i the total formation energy of members of the series is challenging due to the complexity of incommensurate magnetic orders. In this chapter, we restrict our comparison to simple collinear orders: ferromagnetic and N´eelantiferromagnetic (nearest neighbors have opposite magnetization) along H 0 lattice parameters a, b, and c and non-magetic. These magnetic orders map identically andh i unambiguously on inequivalent structures. We apply a penalty term to the total energy functional to constrain the spin direction for a given order as described in Ref. [158] and implemented in VASP. For Ir, we used the an integration sphere of radius 1.423 A,˚ equalling the Wigner-Seitz radius for elemental Ir.

2Band structures of the harmonic honeycombs can be found in the S.I. CHAPTER 4. AB INITIO STUDIES OF STRUCTURAL AND ENERGETIC TRENDS IN THE HARMONIC HONEYCOMB IRIDATES 32 ◦ h∞i c z 0 0 γ 0.5 0.5 ˚ A 5.67 H 0.206 0.792 90.00 ◦ 0 0 0 y b β 9.54 0.160 0.333 0.817 109.33 PBE+SOC+U ◦ 3 olerance: 4.4E-03 T a 0 0 0 x α 0.5 5.51 IrO 0.252 0.295 2 90.00 Na ◦ h∞i c z 0 0 γ 0.5 0.5 5.61 H 0.211 0.796 90.00 ◦ 0 0 0 y b β 9.39 0.160 0.333 0.822 109.04 eriment [ 64 ] Exp ◦ a 0 0 0 x α 0.5 5.43 0.252 0.289 90.00 ◦ c z 0 0 γ 0.5 0.5 ˚ A 5.16 0.234 0.764 90.00 ◦ 0 0 0 y b β structure is reﬁned from powder diﬀraction data]. [ 190 Position 9.03 0.161 0.333 0.826 3 109.78 IrO PBE+SOC+U ◦ 2 olerance: 5.1E-03 3 T a 0 0 0 x α 0.5 5.22 IrO 0.252 0.268 90.00 2 Li ◦ h∞i c z 0 0 γ 0.5 0.5 H 5.12 0.241 0.788 90.00 ◦ . Experimental Li 0 0 0 y b 3 β 8.93 0.191 0.333 0.816 109.76 eriment [ 190 ] IrO 2 ◦ Exp Na a 0 0 0 x α 0.5 5.16 0.248 0.256 90.00 h∞i H 8i 8j 2a 4g 2d 4h Site (12) and 3 tom Ir1 O1 O2 C2/m IrO Spacegroup: A 2 Li1/Na1 Li2/Na2 Li3/Na3 able 4.1: Comparison of experimental and DFT (PBE+SOC+U) lattice parameters and Wyckoﬀ positions for Li tolerance required to symmetrize DFT structures obtained from PBE+SOC+U is given below Wyckoﬀ positions. T CHAPTER 4. AB INITIO STUDIES OF STRUCTURAL AND ENERGETIC TRENDS IN THE HARMONIC HONEYCOMB IRIDATES 33 h 0 i H ◦ c z γ ˚ A 18.99 0.880 0.046 0.709 0.125 0.034 90.00 3 IrO ◦ 2 y b β Na 9.10 90.0 0.125 0.125 0.125 0.125 0.352 h 0 i H PBE+SOC+U ◦ olerance: 5.1E-03 T a x α 6.48 0.125 0.125 0.125 0.831 0.647 90.00 ◦ c z γ ˚ A 17.99 0.877 0.045 0.708 0.125 0.038 90.00 ◦ y b β 8.55 90.0 0.125 0.125 0.125 0.125 0.364 PBE+SOC+U ◦ olerance: 2.3E-02 3 T a x α 5.96 0.125 0.125 0.125 0.863 0.633 90.00 IrO 2 Li ◦ h 0 i c z γ H 17.79 0.875 0.042 0.709 0.125 0.039 90.00 ◦ y b β 8.43 90.0 0.125 0.125 0.125 0.125 0.367 eriment [ 45 ] Exp ◦ . Position tolerance required to symmetrize DFT structures obtained from PBE+SOC+U is 3 a x α 5.89 0.125 0.125 0.125 0.856 0.622 90.00 IrO 2 Na 16e 16g 16g 16g 32h Site h 0 i (70) H and tom Ir1 O1 O2 Fddd 3 Spacegroup: A Li1/Na1 Li2/Na2 IrO 2 able 4.2: Comparison of experimental and DFT (PBE+SOC+U) lattice parameters and Wyckoﬀ positions for Li T given below Wyckoﬀ positions. CHAPTER 4. AB INITIO STUDIES OF STRUCTURAL AND ENERGETIC TRENDS IN THE HARMONIC HONEYCOMB IRIDATES 34 h 1 i H ◦ c z 0 0 γ 0.5 ˚ A 0.25 19.02 0.330 0.245 0.920 0.084 0.166 0.092 0.159 90.00 3 IrO ◦ 2 0 y b β Na 0.5 0.5 0.5 9.10 0.50 0.25 0.25 0.25 90.0 0.523 0.252 0.273 h 1 i H PBE+SOC+U ◦ olerance: 1.1E-02 T a 0 x α 0.5 0.5 0.5 6.48 0.75 0.75 0.25 0.729 0.706 0.044 0.478 90.00 ◦ c z 0 0 γ 0.5 ˚ A 0.25 18.02 0.331 0.248 0.920 0.083 0.167 0.087 0.163 90.00 ◦ 0 y b β 0.5 0.5 0.5 8.53 0.50 0.25 0.25 0.25 90.0 0.510 0.252 0.260 PBE+SOC+U ◦ olerance: 2.6E-02 3 T a 0 x α 0.5 0.5 0.5 5.96 0.75 0.75 0.25 0.742 0.737 0.014 0.493 90.00 IrO 2 Li ◦ h 1 i c z 0 0 γ H 0.5 0.25 0.25 17.84 0.333 0.917 0.084 0.167 0.087 0.163 90.00 ◦ 0 y b β 0.5 0.5 0.5 0.5 8.45 0.25 0.25 0.25 90.0 0.515 0.262 0.262 eriment [ 172 ] ◦ Exp . Position tolerance required to symmetrize DFT structures obtained from PBE+SOC+U is a 0 x α 3 0.5 0.5 0.5 5.91 0.75 0.75 0.25 0.773 0.722 0.006 0.487 90.00 IrO 2 Na 8i 8l 8j 4c 8g 8k 8k 8k 4d Site 16m 16m h 1 i (66) H and Ir1 Ir2 O1 O2 O3 O4 tom Cccm 3 Spacegroup: A La1/Na1 La2/Na2 La3/Na3 La4/Na4 La5/Na5 IrO 2 able 4.3: Comparison of experimental and DFT (PBE+SOC+U) lattice parameters and Wyckoﬀ positions for Li T given below Wyckoﬀ positions. CHAPTER 4. AB INITIO STUDIES OF STRUCTURAL AND ENERGETIC TRENDS IN THE HARMONIC HONEYCOMB IRIDATES 35 h 2 i H ◦ c z γ ˚ A 57.07 0.873 0.042 0.433 0.485 0.708 0.652 0.097 0.986 0.930 0.072 0.011 0.905 0.292 0.125 90.00 3 IrO ◦ 2 y b β Na 9.10 90.0 0.125 0.125 0.125 0.125 0.125 0.125 0.125 0.125 0.125 0.102 0.102 0.102 0.124 0.125 h 2 i H PBE+SOC+U ◦ olerance: 1.0E-03 T a x α 6.48 0.125 0.125 0.125 0.125 0.125 0.125 0.125 0.125 0.125 0.896 0.896 0.897 0.919 0.919 90.00 ◦ c z γ ˚ A 54.12 0.874 0.042 0.432 0.485 0.708 0.652 0.097 0.986 0.931 0.013 0.071 0.904 0.292 0.125 90.00 3 IrO ◦ 2 y b β Li 8.52 90.0 0.125 0.125 0.125 0.125 0.125 0.125 0.125 0.125 0.125 0.115 0.116 0.117 0.123 0.125 h 2 i H PBE+SOC+U ◦ olerance: 1.9E-0.2 T a x α 5.96 0.125 0.125 0.125 0.125 0.125 0.125 0.125 0.125 0.125 0.881 0.882 0.883 0.891 0.890 90.00 16e 16g 16g 16g 16g 16g 16g 16g 16g 16g 32h 32h 32h 32h Site (66) . Position tolerance required to symmetrize DFT structures obtained from PBE+SOC+U is 3 tom Ir1 Ir2 Ir3 O1 O2 O3 O4 O5 Cccm IrO Spacegroup: A 2 Li1/Na1 Li2/Na2 Li2/Na3 Li3/Na4 Li4/Na5 Li5/Na6 Na h 2 i H and 3 IrO 2 able 4.4: Comparison of experimental and DFT (PBE+SOC+U) lattice parameters and Wyckoﬀ positions for Li T given below Wyckoﬀ positions. CHAPTER 4. AB INITIO STUDIES OF STRUCTURAL AND ENERGETIC TRENDS IN THE HARMONIC HONEYCOMB IRIDATES 36

The total moment on each site depends on the magnetic order and ranges from 0.2-0.4 µB for Li2IrO3 and 0.14-0.26 µB for Na2IrO3. For a given magnetic order, the magnetic moment per site varies less than 0.02 µB across the series, thus we do not constrain the magnitude of the magnetic moments. The magnetic moment per site for Li2IrO3 structures has been H measured to be 0.471 µB for 0 [45]. Ref. [270] measured the magnetic moment per site H h i for Na2IrO3 to be 0.22 µB. h∞i Our iridium site magnetic moments for Na2IrO3 are approximately 0.1 µB smaller than those calculated in Ref. [166]. In VASP, an integration sphere radius is deﬁned for each atomic species in the calculation. Any magnetic moment within that radius is then projected onto local atomic orbitals for a given site. Thus, the diﬀerences between Ref. [166] and our calculations of the local magnetic moment may be due to integration scheme. There is also an additional 10% contibution from the oxygen sites, as expected for itenerant magnetism, which we do not add to the total Ir magnetic moment. We do agree with Ref. [166] that we see roughly a halving of Ir magnetic moments between ferromagnetic and antiferromagnetic orders. The reason for the disparity between the magnetic moments calculated for Li2IrO3 and experiment may be due to the fact that we are imposing magnetic structures (ferromagnetic and N´eelantiferromagnetic) that are not the ground state (incommensurate spiral). As shown in Ref. [166], the magnitude of magnetic moment per iridium site is sensitive to magnetic order. The relaxed Li2IrO3 structures vary by less than 5 meV and the relaxed Na2IrO3 struc- tures vary by less than 20 meV, respectively. None of the Li2IrO3 or Na2IrO3 structures are calculated to be signiﬁcantly lower in energy in comparison to other series members. H Na2IrO3 0 is lower in energy for these particular spin orders in comparison to the other series members.h i Without comparing magnetic ground states, it may be diﬃcult to diﬀeren- tiate whether DFT predicts an energetic favorite or if the structures are degenerate. Total energy diﬀerences between collinear orders do not provide substantial insight into the ground state magnetic orders due to their simplicity compared to experimentally measured ground states. However, the diﬀerences in total energy between calculated magnetic orders is small, varying less that 10 meV for a given structure. Tables of total energies for given magnetic orders are included in the Appendix B.

Importance of SOC and U for relaxations We determine the sensitivity of our structural relaxations to the level of theory used in our DFT calculations by performing relaxations of idealized structures of Li2IrO3 and Na2IrO3 with diﬀerent levels of theory (PBE, PBE+U, PBE+SOC, PBE+SOC+U). We ﬁnd that for Li2IrO3, it is necessary to use PBE+SOC with U 0.5 eV to obtain structures with Ir-Ir ≥ bond lengths compatible with experiment. In contrast, Na2IrO3 structures are less sensitive to changes in the level of theory; however, PBE+SOC+U gives the best agreement with experiment. CHAPTER 4. AB INITIO STUDIES OF STRUCTURAL AND ENERGETIC TRENDS IN THE HARMONIC HONEYCOMB IRIDATES 37

Li2IrO3 relaxations with PBE+SOC+U(<0.5 eV), PBE+SOC, PBE+U(=0,1.5,3,6 eV), and PBE result in asymmetric Ir-Ir bond lengths (diﬀering as much as 0.5 A),˚ disparate Ir-O-Ir bond angles and nonmagnetic orders as the lowest energy magnetic order by at least 100 meV per formula unit. 3D Li2IrO3 structures when relaxed with these levels of theory, compress along the orthorhombic c lattice direction which opens a gap in the nonmagnetic H band structure, see Table B.1 for converged lattice parameters for Li2IrO3 and Na2IrO3 1 H h i for a given level of theory. Relaxations of Li2IrO3 with these levels of theory resulted in structures that could not be symmetrized back intoh∞i C2/m, even with a symmetry tolerance of 1 A.˚ We believe the cause of this anisotropic compression in these cases is due to the need to break the degeneracy of the t2g 5d-orbitals In Na2IrO3 the ratio of Na and Ir atomic radii are suﬃciently diﬀerent as to induce large distortions. In this case, the octahedra are suﬃciently distorted as to easily break the degeneracy of the t2g 5d-orbitals. Since, Li and Ir have more similar radii, there is less distortion from purely electrostatic forces so distortion is additionally incurred through bending of the opposite atoms of the octahedra. This distortion easily induces a gap in Li2IrO3 band structure. The distortion lessens as levels of theory are introduced that break the t2g degeneracy.

Virtual Crystal Approximation

We attribute the diﬀerence in sensitivity of Li2IrO3 and Na2IrO3 to level of theory to the diﬀerences in average Ir-Ir separation; in particular, the Ir-Ir sites, which are bridged by oxygen atoms, are 5% further apart for Na2IrO3 than in Li2IrO3. This larger separation for Na2IrO3 in this case reduces superexchange interactions through a delocalization of the Ir 5d electrons via decreased hybridization with O p electrons, reducing the importance of Hubbard U and SOC corrections to spin-polarized PBE calculations. We test this hypothesis by performing relaxations of H 0 with “hybrid” Li-Na atoms to approximate idealized doping (by continuously changing theh i alkali atomic radius) using the Virtual Crystal Approximation (VCA) implemented in VASP. VCA uses a linear combination of existing pseudopotentials to create a “new” atom, mimicking a solid solution with a given stoichiometry. For example, if one wishes to calculate the structure of 50% Li and 50% Na, each alkali metal site would be occupied 50% by a Li atom and 50% by a Na atom. During a relaxation, the linear combination of the forces experienced on a given site by the diﬀerent occupying atomic species is used to calculate the next structure. VCA approximates isotropic doping – meaning that all sites are equally likely to be re- placed by the substituting ion. Experimentally, this is known to not be the case for the harmonic honeycomb iridates. Ref. [161] investigated the change of lattice parameters and H preference of cation substitution in (Na1−xLix)2IrO3 and ﬁnd that Li atoms anisotrop- ically replace cation sites, causing localh∞i distortions. Thus, our VCA calculations should not be considered predictions of lattice parameters and bond lengths for doped materials. Ref. [213] measured that for approximately equivalent Ir-Ir bond lengths, changes in the Ir-O-Ir bond angle due to distortion (or disorder) from doping can have a dramatic eﬀect on CHAPTER 4. AB INITIO STUDIES OF STRUCTURAL AND ENERGETIC TRENDS IN THE HARMONIC HONEYCOMB IRIDATES 38 magnetic order. We perform VCA calculations with PBE+U(=0,1.5,3,6 eV) and PBE+SOC+U(=3 eV) H 3 on idealized (Li1−xNax)2 IrO3 0 . For PBE+U for both (Li1−xNax)2 IrO3, we ﬁnd a sharp doping transition at whichh thei H 0 c axis collapses, resulting in asymmetric Ir-Ir bonds. This transition moves closer andh i closer to pure Li doping with increasing U, in- dicating that it is sensitive to the localization of the Ir 5d orbitals, see Figure 4.4. For H Li2IrO3 0 , PBE+U(=6 eV) gives Ir-Ir bond lengths that diﬀer by greater than 0.1 Awhile˚ PBE+SOC+U(=3h i eV) gives Ir-Ir bond lengths that diﬀer by less than 0.01 A,˚± see Figure 4.5. ±

We also performed VCA calculations with PBE+U(=0,1.5) on idealized (Li1−xNax)2 RhO3 H 0 and saw similar discontinuities in plots of the Ir-Ir bond lengths as a function of dop- h i ing. These discontinuities occurred at lower doping that for (Li1−xNax)2 IrO3 but showed the same shift to lower doping when a higher Hubbard U correction was applied.

4.4 Conclusion

Despite the complexity of the harmonic honeycomb iridates, our calculations accurately re- produce experimental structures and predict yet to be synthesized series members by includ- ing spin-orbit coupling and using Hubbard U corrections for iridium 5d orbitals. Including these interactions is crucial for accurately calculating properties of Li2IrO3, although less so than Na2IrO3. Using these calculations, we assess trends in formation energetics and struc- tural distortion in the harmonic honeycomb iridates. These studies provide concrete insight helpful to experimental eﬀorts. Our calculations demonstrate the importance of systemat- ically testing the level of ab initio theory needed to accurately capture basic properties of complex material systems. The workﬂow we present can be used for future ab initio studies to investigate the eﬀects of strain and pressure on the magnetism of the harmonic honeycomb iridates.

3PBE+SOC+U(=1.5 eV) was insuﬃcient to produce symmetric Ir-Ir bonds for 5% Na and 10% Na so we used U=3.0 eV CHAPTER 4. AB INITIO STUDIES OF STRUCTURAL AND ENERGETIC TRENDS IN THE HARMONIC HONEYCOMB IRIDATES 39

(a) (b)

(c)

(d)

(e)

Li / Na Ir O

Figure 4.1: (a) Conventional unit cells of H 0 , H 1 , H 2 , and H [174]. H , H 0 , H 1 , and H 2 have 2, 4, 8, and 12 formulah unitsi h ini theirh i primitiveh∞i unit cell, respectively.h∞i h i Membersh i of theh i harmonic honeycomb series have identical local geometry, only varying in the connectivity of their basic structural units, orthogonal edge-sharing iridium oxide octa- hedra. The two growth or bonding planes are normal to a + b and a b, where a and b are the orthorhombic lattice vectors (indicated by the axes at the bottom− left). The har- monic honeycomb pattern builds along the orthorhombic c direction. Compared to Li2IrO3 structures, Na2IrO3 structures have greater distortion of iridium oxide octahedra and larger volume. (b-e) Exaggerated distortions in the harmonic honeycombs. (b-c) Two parallel faces of each iridium oxide octahedron twist opposite to each other. These faces are parallel to the growth plane. (c) Which faces twist changes at twisting bonds. (b) A bond that preserves the bonding plane. (c) A “twist” bond that changes the bonding plane. (d) The octahedra also compress along their twist axis. (e) The twisting and compression of the octahedra cause Ir-O-Ir bond angles to increase from their ideal 90◦ and the angle between bonding planes to be close to the undistorted value of arccos(1/3) 70.5◦. CHAPTER 4. AB INITIO STUDIES OF STRUCTURAL AND ENERGETIC TRENDS IN THE HARMONIC HONEYCOMB IRIDATES 40 DOS (states/eV/f.u.)

Energy (eV) Figure 4.2: Non-magnetic density of states normalized by the number of formula units per unit cell for Li2IrO3 and Na2IrO3 harmonic honeycomb structures. Density of states is similar across the series.

: 30 Nonmagnetic 25 20 15 10 5 0 Ferromagnetic 12

DOS (states/eV) 8 4 0 -1 0 1 Energy (eV) H H Figure 4.3: PBE+SOC+U density of states of Li2IrO3 and Na2IrO3 for non- h∞i h∞i H magnetic (all magnetic moments ﬁxed at zero µB) and ferromagnetic (along the b direction or H 0 c direction) magnetic orders are shown in (a). A gap opens in the densityh∞i h i of states of both systems with a non-zero magnetic order. Diﬀerences in the Li2IrO3 and Na2IrO3 density of states are caused by distortions of the local environment more so than ◦ ◦ change in volume. Li2IrO3 and Na2IrO3 structures have Ir-O-Ir bond angles of 94 and 100 , respectively. CHAPTER 4. AB INITIO STUDIES OF STRUCTURAL AND ENERGETIC TRENDS IN THE HARMONIC HONEYCOMB IRIDATES 41

U = 0 eV U = 1.5 eV U = 3.0 eV U = 6.0 eV a/c

U = 0 eV U = 1.5 eV U = 3.0 eV U = 6.0 eV b/c

Li (% Na) Na Figure 4.4: Plots of ratio of relaxed lattice parameters vs doping for PBE+U where U=0,1.5,3.0,6.0. The discontinuity indicates that when PBE gives asymmetric Ir-Ir bonds below a given Na doping. The discontinuity in the lattice parameters shifts toward more Li doping with increasing U, demonstrating that the performance of the functional is sensitive to localization of iridium 5d orbitals and closeness of iridium atoms. CHAPTER 4. AB INITIO STUDIES OF STRUCTURAL AND ENERGETIC TRENDS IN THE HARMONIC HONEYCOMB IRIDATES 42

(Å) without SOC with SOC Ir1-Ir1 (bond 1)

Ir-Ir Bond Length Ir1-Ir1 (bond 2)

without SOC with SOC

(degrees) Ir1-O2-Ir1 Ir1-O1-Ir1 Ir-O-Ir Bond Angle

Li (% Na) Na Figure 4.5: Plots of Ir-Ir bond lengths and Ir-O-Ir bond angles as a function of Na doping H of 0 Li2IrO3 for PBE+U and PBE+SOC+U (U = 3 eV). While SOC is not suﬃcient to preventh i discontinuities in bond length relaxations, it does give uniform bond length ( < 0.01 A)˚ and bond angles ( < 1.5 degree) for all relaxations. Note, if U = 3 eV is used for± Li concentration < 15% and U± = 1.5 eV for Li concentration < 15% there is no dicontinuity.

(Li1−xNax)2 IrO3 is metallic for U = 1.5 eVand 0.1 < x < 0.2%. According to VCA, the distortion is not linear in doping. 43

Chapter 5

Silver Benzeneselenolate is a Self-Assembling Direct-Gap Metal-Organic Chalcogenide Assembly

Silver and diphenyl diselenide self-assemble into a blue-luminescent excitonic semiconducting crystalline hybrid lamellar van der Waals solid, silver benzeneselenolate ([AgSePh]∞). Each composite layer of the vdW solid is itself comprised of an ultrathin silver selenide layer having 2D connectivity and a supramolecular lattice of ordered phenyl rings. We ﬁnd that the material has a strong blue photoluminescence at 467 nm. Density functional theory calculations imply signiﬁcant quantum conﬁnement of electronic carriers within inorganic layers. Three synthetic preparations for [AgSePh]∞ in diﬀerent scales and form factors were developed.

5.1 Introduction

Single monolayers separated from layered van der Waals solids, like transition metal dichalco- genides (TMDs, e.g. MoS2), usually exhibit semiconducting properties that are distinct from that of the bulk crystalline solid. For example, TMD monolayers possess direct band gaps and high electron mobilities, whereas their bulk crystalline counterparts are typically indirect band gap semiconductors [159, 88, 53, 43]. These and other interesting physical phenomena emerge from single layers due to quantum conﬁnement and enhanced electron- electron interactions, and provide a variety of opportunities for technological exploitation [251, 220, 151, 54, 156]. However, the need to isolate monolayers from bulk crystals com- plicates their use in practical technology. Hybrid coordination polymers that combine an inorganic semiconducting polymer with a supramolecular matrix comprised of the covalently linked organic sidegroups have been considered as an alternate route for the preparation of CHAPTER 5. SILVER BENZENESELENOLATE IS A SELF-ASSEMBLING DIRECT-GAP METAL-ORGANIC CHALCOGENIDE ASSEMBLY 44 low-dimensional materials, with the inclusion of covalently linked ligands serving to isolate inorganic material systems [80, 111, 113, 112, 237, 260, 267, 252, 102, 143]. Here, we report that one such hybrid coordination polymer, silver benzeneselenolate ([AgSePh]∞, where the inﬁnity subscript denotes a bulk crystal as opposed to a single monolayer), is a direct-gap semiconductor that expresses fully isolated 2D semiconduct- ing properties in the bulk crystal. This compound exhibits a deep blue photoluminescence (467 nm) consistent with a direct-gap semiconductor. We developed two accessible-synthetic- routes to the single-crystal product: a single-step immiscible-interface method and a one-pot reaction with gram-scale yield, showcasing the ease at which this hybrid chalcogenide ma- terial is made by using commercially available small molecule precursor and mild reaction conditions. We will discuss our synthetic route, optical characterization of the direct gap semiconductor transition, and our companion density functional theory calculations. We then employ crystal engineering by way of design of discrete organic diselenide ligands and assemble them into analogous crystalline metal-organic chalcogenide assemblies. We ﬁnd the properties of each are consistent with a propose that variance of organic ligand shape in the silver organoselenolate system presents a straightforward route towards the preparation of synthetically tailorable, self-assembling 2D materials from small molecule building blocks.

5.2 Results and Discussion

Synthesis and Characterization of [AgSePh] ∞ The chemistry of metal organochalcogenolates[78, 68] present a rich chemical infrastructure for preparing layered, crystalline supramolecular assemblies. Silver, like many soft transition metals, can adopt a wide array of coordination geometries[219] while accommodating a broad variety of organic ligands. For example, both aryl and n-alkyl thiols assemble with silver into layered crystalline Ag-S 2D coordination polymers[191, 70, 110]. Selenium analogs of these compounds are less explored, in part because the use of harsh, odorous, or highly reactive selenium reagents is not ideal. Previous methods used to synthesize both discrete complexes and coordination polymers occur via chalcogenolysis, through cleavage of the Se-H bond[182], or the isolation of the reactive selenolate salt (-SeR)[50]. Corrigan and coworkers ﬁrst reported the synthesis and single-crystal X-ray structure for a coordination polymer [AgSePh]∞ (Fig. 5.1) in 2002, during an eﬀort to form silver selenolate polynuclear clusters, using a selenium lithiate as precursor[69]. The 2D lamellar structure of this product was characterized; however the application for this coordination polymer had not yet presented itself, as the interest in low-dimensional TMDs arrived only later. We prepare single crystals of [AgSePh]∞ via crystallization between two immiscible sol- vents, water and toluene, at room temperature [267]. We employ the reagent diphenyl diselenide, a nonodorous, solid organoselenium source. This is dissolved in toluene (3 mM) and layered over a solution of silver nitrate in H2O (3 mM). Cleavage of the diselenide by silver ion appears spontaneous, and coordination polymerization is restricted to the liquid- CHAPTER 5. SILVER BENZENESELENOLATE IS A SELF-ASSEMBLING DIRECT-GAP METAL-ORGANIC CHALCOGENIDE ASSEMBLY 45

Figure 5.1: a) The monoclinic unit cell of solid silver benzeneselenolate contains two com- plete layers of hybrid chalcogenide 2D polymer. Silver is coordinated tetrahedrally by four selenium atoms. b,c) The multilayered structure isolates inorganic layers via the benzene moieties oriented above and below the silver selenide polymer layer. D) A single isolated layer has a thickness of 1.4 nm, each containing two layers of phenyl rings and one layer of silver selenolate. Silver is represented as the grey spheres, selenium in dark orange, and carbon in black. Aromatic rings are accented in blue. liquid interface. Crystallization occurs readily without stirring over 1-3 days, with product manifesting as an opaque ﬁlm, chartreuse in color, pinned between the two solvent layers (Fig 2a). The structure is conﬁrmed by matching the powder X-Ray diﬀractogram of both products to the theoretical pattern derived from the known crystal structure (See support- ing information, Figure C.1). Alternatively, a one-pot synthesis using triphenylphosphine to stabilize silver nitrate in tetrahydrofuran, similarly yields crystalline [AgSePh]∞ in high speciﬁcity at a gram scale with crystalline product dimensions in excess of tens of microns. The one-pot product contains considerably larger and thicker crystals relative to the immis- cible layer approach, at the cost of increased polydispersity. Products produced by both routes are otherwise indistinguishable by the characterization methods employed above. CHAPTER 5. SILVER BENZENESELENOLATE IS A SELF-ASSEMBLING DIRECT-GAP METAL-ORGANIC CHALCOGENIDE ASSEMBLY 46

Figure 5.2: a) A chartreuse deposit of silver benzeneselenolate forms at an immiscible liquid- liquid interface of organic and aqueous solutions of diphenyl diselenide and silver nitrate, respectively. b) Crystals of [AgSePh]∞ recovered have typical edge lengths between 1 and 4 microns. b) Scanning electron micrograph of a silver benzeneselenolate silver crystal reveals the layered structure of the crystal. Individual layers are resolved in high-resolution SEM images. c) Atomic force microscopy reveals highly uniform [AgSePh]∞ (001) terraces with measured step heights at 1.4 nm.

The ﬁlm is harvested by drawing a silicon wafer through the liquid-liquid interface at an angle. The precipitate adheres readily to silicon substrate. A layer of single crystals of [AgSePh]∞, each having edge lengths of 1-5 µm and a typical thickness of 100-200 nm, are shown in Figure 5.2b. Features of the crystal surface are examined by SEM and AFM in Figure 5.2c-d. The prominent 001 plane of the silver benzeneselenolate crystal is visible in Figure 5.2c as the large ﬂat face. The smaller faces correspond to 010 and 100 facets, corresponding to exposed edges of the 2D hybrid crystalline polymer. Scanning electron microscopy resolves the individual molecular step edges, corresponding to the thickness of a single silver benzeneselenolate sheet (Fig. 5.2b). Atomic force microscopy (AFM) conﬁrms the expected 1.4 nm step height of the (001) crystallographic plane. AFM images of these outermost layers of the [AgSePh]∞ crystal further reveal that the exposed terraces are vir- tually defect free over hundreds of nanometers, with no molecular vacancies are observed in our images at this scale.

Optical Characterization of the Semiconductor Direct-Gap We note comparisons to two-dimensional TMDs, such as MoS2, with some important dis- tinctions due to the presence of the intervening organic groups and metal-metal interactions. MoS2 is a layered indirect band gap semiconductor in the bulk, but has a direct band gap and high charge carrier mobilities as a single layer [159]. Similar to most TMD van der Waals (vdW) solids[248], adjacent 2D layers of silver benzeneselenolate are covalently de- coupled. Unlike the TMD solids, the vdW coupling is strongest between the organic ligands, rather than between neighboring AgSe planes. As the transition metal chalcogenide layer is chemically decoupled from its neighboring layers, the bulk hybrid silver benzeneselenolate CHAPTER 5. SILVER BENZENESELENOLATE IS A SELF-ASSEMBLING DIRECT-GAP METAL-ORGANIC CHALCOGENIDE ASSEMBLY 47 system might be expected to be electrically decoupled as well, thereby exhibiting properties associated with monolayer-TMDs rather than with bulk-TMD systems. To test this hypoth- esis, we measured the photoluminescence (PL) spectroscopically and microscopically, and the results are shown in Figure 5.3. On excitation with shorter wavelength light (380 nm), a single PL peak is observed at 2.65 eV, or 467 nm, a deep blue. To determine if the crystal size aﬀects the PL color or intensity, we imaged single crystals by confocal microscopy using a 405 nm laser. Measuring the emission spectra, we ﬁnd that each single crystal has an emission peak at 467 nm, consistent with the ensemble measurement (Figure 5.3, Figure C.4, Materials and Methods). Moreover, we observe no correlations between emission intensity and crystal aspect ratio or surface area (Figure 5.3e,f). The analysis at the single particle level suggests that the photoluminescence intensity is not dependent on the lateral size dimensions of the crystal at the microscale. Instead, emission intensity correlates with number of layers, or crystal thickness. Although absolute crystal thickness is not directly measured in this experiment, relative thicknesses may be inferred by visual inspection using the optical microscope (Figures 5.3c-d).

Band Structure Calculations To understand the origin of the electronic properties of this system, we performed density functional theory (DFT) calculations with the VASP code [135, 137, 136, 138] using the hybrid functional of Heyd, Scuseria, and Ernzerhof (HSE), which includes approximate short- range exchange and correlation eﬀects important for a balanced treatment of delocalized sp valent and localized d and π states in [AgSePh]∞. Using experimental lattice parameters and atomic positions, we perform calculations on the following periodic structures: 1) bulk [AgSePh]∞, 2) single-layer [AgSePh]∞, and 3) a single-layer [AgSePh]∞ with the phenyls replaced by hydrogen atoms. We use 1) and 2) to demonstrate that the layers of [AgSePh]∞ are eﬀectively electrically isolated and 3) to illustrate the impact of the ligand on the electronic structure. Our DFT band structures and density of states for these systems are summarized in Figure 5.4. Our computed band structures of bulk and single layer [AgSePh]∞ are indistinguishable, demonstrating that the layers of bulk [AgSePh]∞ are electrically isolated. Within DFT-HSE, bulk and single layer [AgSePh]∞ have a direct band gap at Γ of 2.4 eV, in good agreement with the measured photoluminescence, despite the fact that DFT is not expected to yield quantitative gaps on formal grounds. To obtain quantitative optical gaps and spectra, a more advanced treatment of exchange and correlation eﬀects, including electron-hole interactions, is required in addition to our calculations, e.g., the use of ab initio many-body perturba- tion theory (MBPT) within the GW approximation and the Bethe-Salpeter equation (BSE) approach[101, 211, 212]. The lowest-lying DFT-HSE conduction band of bulk [AgSePh]∞ is highly dispersive in plane, with electron eﬀective masses of 1.13 me and 0.44 me, respec- tively, at Γ (Figure C.6). Bands exhibit signiﬁcantly less dispersion perpendicular to the AgSe planes and along the stacking direction of [AgSePh]∞, with an electron eﬀective mass CHAPTER 5. SILVER BENZENESELENOLATE IS A SELF-ASSEMBLING DIRECT-GAP METAL-ORGANIC CHALCOGENIDE ASSEMBLY 48

Figure 5.3: a) Confocal micrographs showing the color uniformity of photoluminescence in [AgSePh]∞. b) A single, intense emission of the solid at 467 nm is attributed to a direct- gap electronic transition. c,d) Optical and confocal micrographs of [AgSePh]∞ showing ﬂuorescence scanning confocal images of several individual crystals of nearly the same size. e) Distribution of the intensity from 157 individual crystals plotted as a function of the area of the crystal and f) aspect ratio. The Pearson’s r-value for each set of data was calculated by using linear least squares ﬁtting (solid line); for both the plots of area (r-value of 0.07) and aspect ratio (r-value of 0.1) the Pearson’s r-values indicate no correlation with intensity. Images are false colored according to emission wavelength. CHAPTER 5. SILVER BENZENESELENOLATE IS A SELF-ASSEMBLING DIRECT-GAP METAL-ORGANIC CHALCOGENIDE ASSEMBLY 49

Figure 5.4: a) DFT-HSE band structure and density of states of bulk [AgSePh]∞. See supporting information Figure C.6 for details. Band color signiﬁes the fractional contribution of states centered on inorganic (Ag and Se, orange) and organic (C and H, black) atoms in the crystal. The total density of states is shown in gray. b) DFT-HSE band structure of a single layer of [AgSePh]∞ c) DFT-HSE band structure of a single layer of [AgSePh]∞ with the phenyls replaced by hydrogen. The hydrogen positions have been relaxed with PBE; see supporting information Figure C.5. The near-band edge character remains relatively unchanged when the phenyls are replaced by hydrogen, suggesting that the degree of 2D quantum conﬁnement is unchanged by 3D crystallization. d) The Brillouin zone for the primitive cell of [AgSePh]∞. The path in the Brillouin zone used for the band structure is identiﬁed by orange lines and k-point labels.

of 18.7 me, reﬂecting weak (although non-negligible) interplanar coupling and indicating signiﬁcantly lower mobility along the [001] direction. The electronic structure of bulk and single layer [AgSePh]∞ near the valence and conduc- tion band edges is dominated by contributions from silver selenide. Figure shows isosurfaces of the square of the wavefunction for the bulk [AgSePh]∞ conduction band minimum and valence band maximum states at the Γ point. While the state at the valence band maximum exhibits directional bonding associated with Ag 4d and Se 3p character, the conduction band minimum is more delocalized, featuring signiﬁcant Ag 5s character. As can be seen in Figure 5.5, the phenyl group p states contribute minimally to band edge states with valence band maximum and conduction band minimum isosurface density visible only on the carbon atoms adjacent to the AgSe layer. The calculated density of states shows a separation of bands having organic (phenyl) and inorganic (Ag and Se) character near the band gap. The phenyl π and π∗ states are largely grouped at energies well below and above the Ag- and Se-rich valence and conduction band edges, respectively, consistent with the relatively large benzene gap (Figure 5.4) and minimal carbon character at the band edges. Indeed, replacing the phenyl groups with hydrogen leads CHAPTER 5. SILVER BENZENESELENOLATE IS A SELF-ASSEMBLING DIRECT-GAP METAL-ORGANIC CHALCOGENIDE ASSEMBLY 50

Figure 5.5: Depictions of side and top views of [AgSePh]∞ with overlain charge density maps. The DFT-HSE computed valence band maximum (VBM) and conduction band minimum (CBM) at Γ are accented in yellow and blue, respectively. The minimal but non-negligible participation of carbon in the CBM state suggests tailoring of electronic properties via syn- thetic modiﬁcation of ligand. to small changes in band gap and in-plane eﬀective masses compared to the phenylated layer (Table C.1, Figure C.5). The relative alignment of the organic and inorganic states suggests an opportunity to tune the near-band edge character of each component via ligand choice. A ligand with a smaller band gap, such as pentacene, could contribute states hybridizing with those of silver selenide at the band edge. Thus, it may be possible to tune electronic properties of this system, as well as the coupling between layers, by ligand design. The use of ligands has been successfully used to tune the optoelectronic properties of quantum dots[216], we can apply the same principles to metal-organic crystalline systems described here. Previous experiments and ab initio MBPT calculations on TMDs have established large exciton binding energies[199], novel screening eﬀects[253], and trion formation[42]. Given the similarity of its atomic structure to that of 2D TMDs, and the added presence of the phenyl ligands, such excited state phenomena are also likely to emerge from this silver selenide system and will be explored in future work. CHAPTER 5. SILVER BENZENESELENOLATE IS A SELF-ASSEMBLING DIRECT-GAP METAL-ORGANIC CHALCOGENIDE ASSEMBLY 51 5.3 Conclusions and Prospects

Coordination polymers are often treated as kinetic side products en route to more elab- orate, discrete organometallic clusters. However, the incorporation of organic side groups with inorganic polymers presents a straightforward approach to combine the chemical variety of organic chemistry with the compelling transport phenomena exhibited by 2D materials. Using metal-directed self-assembly, we synthesized silver benzeneselenolate, a material that expresses 2D semiconducting phenomena in its as-crystallized bulk state. The phenyl rings additionally appear to eﬃciently isolate the inorganic layers from one another, enabling the material to display monolayer-like properties in the bulk, and without need for exfoliation. The organization of this material is consistent with that of a multilayered single-crystal supramolecular quantum well. The 2.65 eV peak emission is attributed to a direct-gap tran- sition. The straightforward synthesis from convenient reagents makes silver benzeneseleno- late a notable candidate for studying high-binding-energy excitonic physics in as-synthesized crystalline 2D materials. Crystal engineering applied to such low-dimensional semiconducting coordination poly- mers is accessible because of the robustness of silver/chalcogen coordination reactions. Be- cause any ligand shape and composition can be varied over a broad range, molecular side group diversiﬁcation enables a straightforward route to band level engineering between the organic and inorganic with ligand selection[274]. In this example, the inclusion of covalently attached ligands considerably alter the properties of the 2D AgSe-R polymer in compari- son to Ag2Se, which is a small bandgap near-infrared emitter[216, 276]. Using coordination polymers as the basis for 2D material systems opens synthetic avenues to the investigation of semiconducting inorganic systems that are not preexisting in nature, due to the variety of coordination geometries inherent to transition metals and the practically limitless design available through selection of organic ligands. 52

Chapter 6

An Automatically Curated First-Principles Database of Ferroelectrics

Ferroelectric materials have a wide-range of technological applications including non-volatile memory and optoelectronics. In this chapter, we integrate density functional theory, crystal structure databases, symmetry tools, workﬂow software, and a custom analysis toolkit to build a library of known and proposed ferroelectrics. With our automated workﬂow, we screen over 17,000 candidate structure pairs from the Materials Project structure database using symmetry relations between nonpolar and polar structures to generate a dataset of 239 ferroelectric candidates. Results are automatically parsed, stored in a database, and accessible via a web interface showing distortion animations and plots of polarization and total energy as a function of distortion. We provide the candidates found using our workﬂow on the Materials Project structure database. We benchmark these candidates against exper- imental data and other ab initio results. The data is available on FigShare and github. We also contribute our workﬂow and analysis code to the open-source python packages atomate and pymatgen so others can conduct their own symmetry driven searches for ferroelectrics and other phenomena.

6.1 Background and Summary

High-throughput screening of material databases integrated with ﬁrst principles calculations has been increasingly successful in the discovery of new functional materials [268, 61, 71]. A remaining challenge is that while all the individual components for performing high- throughput searches exist, the infrastructure needed to connect and automate all the nec- essary components is still under development. In particular, the identiﬁcation and curation of ferroelectrics has been an active area of research for the past half-century [154, 255, 2]. A ferroelectric material has a spontaneous polarization that is switchable between two or CHAPTER 6. AN AUTOMATICALLY CURATED FIRST-PRINCIPLES DATABASE OF FERROELECTRICS 53 more states by an applied electric ﬁeld [152, 201]. Ferroelectrics are technologically useful, used in tunable capacitors and non-volatile RAM, and display couplings between magnetic, electronic, and lattice degrees of freedom [152, 201]. Ferroelectricity arises from a structural phase transition. This phase change results in the appearance of a spontaneous polarization [152]. In a conventional ferroelectric, the high-symmetry structure is nonpolar and the low-symmetry structure is polar, permitting a spontaneous polarization. The atomic structure distorts such that the new structure has a subset of the symmetries of the original structure, satisfying the requirements of a second- order phase transition [60]. Abrahams ﬁrst proposed searching for pairs of nonpolar and polar structures related by symmetry to ﬁnd ferroelectric candidates. In the late 1980s, he performed some of the earliest searches for ferroelectrics in crystallographic database using symmetry criteria [6, 7]. More recently, similar automated searches for new ferroelectric candidates have used symmetry arguments to identify nonpolar reference structures for existing polar materials [57, 117, 139]. Other papers have used a combination of group theoretic and ﬁrst-principles calculations to propose ferroelectric candidates [241, 194, 235]. Bennett et al proposed using high throughput calculations to perform high-throughput substitution calculations on known classes of ferroelectrics [39, 40, 41]. Recent work used high-throughput phonon calculations to identify ferroelectric from polar, soft phonon modes [86]. However, previous works have focused on a limited number of compounds or families of compounds using few symmetry conditions. Furthermore, predictions were based on limited experimental data due to the screening approach, leading to predictions diﬃcult to test experimentally. With shrinking computing costs, high-throughput material searches using density functional theory are on the rise. Ferroelectric databases and systematic screening of properties such as small band gaps, large polarizations, large volume expansion, high critical temperatures and coupling to magnetic and/or topological degrees of freedom may lead to new functional materials and potentially new physical phenomena [87]. In this chapter, we integrate density functional theory (DFT), crystal structure databases, symmetry tools, workﬂow software, and a custom analysis toolkit to build a workﬂow capable of generating libraries of known and proposed ferroelectrics. This workﬂow is general and can be performed on any crystal structure dataset. We present the results from perform- ing this workﬂow on the Materials Project database of inorganic crystal structures [124]. We screen over 17,000 candidates using symmetry relations between nonpolar and polar structure pairs. We identify 239 ferroelectric candidates, 183 being classiﬁed as high-quality candidates by a stringent validation process. 78 of these high-quality candidates are known (anti)ferroelectrics or previously proposed, and 105 are new. Using the workﬂow developed here, this is the ﬁrst automatically-curated ab initio dataset of diverse, multi-class known and new ferroelectrics calculated with a standardized method that permits straightforward comparison. This dataset can be used to develop new tools and criteria for studying ferro- electricity across diverse materials systems. In addition our code for conducting this search has been contributed to the open-source python packages atomate and pymatgen so others can conduct searches of their own and build directly on this work. CHAPTER 6. AN AUTOMATICALLY CURATED FIRST-PRINCIPLES DATABASE OF FERROELECTRICS 54 6.2 Methods

Ferroelectricity from First-Principles The spontaneous polarization is not a direct observable; one can only measure the change in a material’s spontaneous polarization switching between two stable conﬁgurations [208]. Applying an electric ﬁeld to a ferroelectric leads to a hysteresis loop in a plot of the polar- ization versus applied electric ﬁeld. The half of the change in polarization is deﬁned as the spontaneous polarization at a given ﬁeld and temperature; the extrapolation of this quantity to zero ﬁeld is the spontaneous polarization [152]. The spontaneous polarization can be directly predicted using ab initio methods. We identify ferroelectrics as materials possessing two structural phases: a high-symmetry nonpolar structure and a low-symmetry polar structure that can support a polarization [128]. We automatize a search for compounds supporting two such phases and then compute the polarization diﬀerence between the two structures. The polar and nonpolar symmetry criteria stems from the following. As a consequence of structural periodicity, the polarization of a crystal is a lattice vector. This means the polarization, P, of a crystal is only deﬁned modulo a “quantum of polarization”, [208, 238],

X eRi P = P + n , (6.1) 0 i Ω i∈{a,b,c}

where e is the charge of the electron, ni is an integer, Ri is a lattice vector, and Ω is the unit cell volume. In three dimensions, the only space groups compatible with leaving a 3D lattice vector invariant under its symmetry operations are those with polar point groups. Out of the 32 crystallographic point groups, 10 are polar; these polar point groups can keep points along speciﬁc lines (point groups 2, 3, 4, 6, mm2, 4mm, 3m, 6mm), planes (point group m), or all points in 3D space (point group 1) ﬁxed [152]. All other point groups are nonpolar. We deﬁne polar structures as crystal structures with a polar space group, which is composed of a polar point group plus translations, likewise for nonpolar structures. To recover a smooth polarization path, we ensure the nonpolar structure must be con- tinuously deformable into the polar structure along a path that preserves the symmetry of the polar structure. We then perform calculations of multiple structures along the distortion path to compute the Berry phase polarization, which can be compared to the experimentally measured spontaneous polarization.

Antiferroelectrics Antiferroelectrics, in contrast to ferroelectrics, exhibit double hysteresis loops in polarization versus electric-ﬁeld measurements [200]. The ﬁeld-induced phase transition is caused by energetically competing nonpolar and polar phases separated by a ﬁrst order phase transition. The nonpolar phase is often refereed to as “anti-polar” to distinguish it from the nonpolar CHAPTER 6. AN AUTOMATICALLY CURATED FIRST-PRINCIPLES DATABASE OF FERROELECTRICS 55 reference structure. Symmetry conditions for antiferroelectrics are described in Ref. [247]. For completeness, to ﬁnd anti-ferroelectrics using ab initio techniques one would ideally ﬁnd the reference nonpolar phase, the antipolar phase and the polar phase. However, one can also ﬁnd antiferroelectric candidates by the same method as used to ﬁnd ferroelectrics. In this case, the antipolar structure should be found to be lower in energy than the polar structure.

Workﬂow overview We ﬁrst describe the general workﬂow diagram shown in Figure 6.1. The complete workﬂow involves the passing of data between many separate calculations. To create an automated ferroelectric search, we automate the following tasks:

1. Identifying candidate materials possessing nonpolar-polar structure pairs related by a group-subgroup symmetry relation.

2. Performing DFT calculations of changes in total energy, band gap, and polarization across the nonpolar-polar distortion.

3. Post-processing calculation data to compute the spontaneous polarization.

4. Validating the calculation quality for each ferroelectric candidate.

5. Creating an interface for viewing the results for all candidates.

We start by choosing a crystal structure database on which to perform the search (see Structure Selection Symmetry Analysis) and perform a symmetry analysis to ﬁnd candidate materials possessing nonpolar-polar structure pairs related by a continuous symmetry defor- mation. Any such pairs found to satisfy the symmetry criteria are stored in the Distortion Database as being deformable by symmetry. This criteria includes the following: The polar structure belongs to a space group that is a subgroup of the space group of the nonpo- lar structure. There exists a transformation matrix between the nonpolar structure in its high-symmetry setting to the low-symmetry setting of the polar structure. We then prepare a workﬂow to perform DFT calculations on the candidate pairs to extract the changes in the band gaps, total energies, and polarization of the distortion (see Computational Methods). These workﬂows are stored in a Workﬂow Database that is then accessed by our Computing Resources where the calculations are performed. Then, the information stored in the Distortion, Workﬂow, and Calculation Databases is used together to post-process quantities such as the spontaneous polarization and vali- date the candidates using experimental and previous ab initio results (see Post-processing and Spontaneous Polarization Values and Veriﬁcation of computational methodology). The information needed to assess the quality and properties of the candidates is then added to the Candidate Database where it can be accessed by our web Interface for viewing the CHAPTER 6. AN AUTOMATICALLY CURATED FIRST-PRINCIPLES DATABASE OF FERROELECTRICS 56

Figure 6.1: Diagram of entire automated ferroelectric search workﬂow. Databases are shown as purple cylinders. Processes are shown as rectangles: blue designates processes used to identify and perform ab initio calculations, green designates post-processing and validation, and orange designates the web-interface. Arrow directions indicate the ﬂow of information. For example, the Workﬂow Database provides information to the Computing Resources for which calculations to compute and the Workﬂow Database is updated as calculations complete or errors occur on the Computing Resources. candidates in aggregate (see Graphical Interface). We ﬁnally validate the candidates to en- sure the polarization and energy proﬁle across the nonpolar-polar distortion are smooth and continuous. In the sections below, we describe in detail the methods used for creating an automat- ically curated dataset of ferroelectrics from the Materials Project database [124]. The Ma- terials Project database is largely based on structures from the Inorganic Crystal Structure Database (ICSD) and also includes hypothetical structures created through stoichiometric substitution. The results from applying our workﬂow are described below and summarized in Table 6.1. We note that the workﬂow we create is modular and open-source, so it can be readily adapted and applied by others, expanding the search for ferroelectrics and multifer- roics. CHAPTER 6. AN AUTOMATICALLY CURATED FIRST-PRINCIPLES DATABASE OF FERROELECTRICS 57

Table 6.1: Results obtained by applying our workﬂow to the Materials Project database. indicates “in Materials Project database at time of search”. Boxes relate numbers by symmetry† conditions, DFT calculations, and validation processes. Rows separated by a single line give the sum of the numbers given below it in the same box. Structures† 67,000 Polar structures† ∼15,000 Distinct polar formula† ∼10,000 Nonpolar-polar pairs ∼17,000 ∼

Symmetry Distinct nonpolar-polar pairs formula 1,600 Pairs with continuous transformation ∼ 414 Pairs with metallic endpoints 86 Pairs with metallic interpolations 40 Pairs with calculation errors 49 DFT Pairs that completed successfully 239 High-quality ferroelectric candidates 183 Known ferroelectrics in high-quality candidates 78 alid.

V New ferroelectrics in high-quality candidates 105

Structure Selection The input to our workﬂow is a collection of a candidate nonpolar-polar structure pairs. There are several methods that can be used to create candidate nonpolar-polar structure pairs. For example, one can apply a polar distortion to an existing nonpolar structure or create a nonpolar reference structure for an existing polar structure. For this dataset, we require both the nonpolar and polar structures to exist in the Materials Project database. To search for compatible nonpolar-polar structure pairs in the Materials Project dataset, we ﬁnd structures that are in space groups that satisfy group-subgroup relations with a nonpolar high-symmetry space group and a polar low-symmetry space group. We also require that the number of sites in the nonpolar structure are less than or equal to the number of sites in the polar structure. We perform this query using is using pymatgen, spglib, and the Materials Project API [188, 250, 186]. We give the number of structures resulting from this query in the top box of Table 6.1. At the time of this search, the Materials Project database has approximately 67,000 struc- tures, approximately 15,000 of which are polar. We ﬁnd approximately 17,000 nonpolar-polar structure pairs. These pairs contain approximately 1,600 materials out of the approximately 10,000 distinct polar compositions in the Materials Project database. All other polar com- positions in the Materials Project do not have symmetry compatible nonpolar candidates in the database. We note that it is possible to propose hypothetical nonpolar reference struc- tures for these polar candidates using group theoretic methods or large symmetry tolerances [57, 117, 139, 86]; this is left for future work. CHAPTER 6. AN AUTOMATICALLY CURATED FIRST-PRINCIPLES DATABASE OF FERROELECTRICS 58 Naming Conventions We use the formula name output by the pymatgen alphabetical formula method for the Composition class (with spaces and 1s removed) to output consistent formulas for our can- didates. This method orders elements in such a way that does not match conventions in the literature. For example, we use O3PbTi where the standard in the literature is PbTiO3. Compositions printed by pymatgen also diﬀer from those used in mineralogy, such as for boracite, lawsonite and many other minerals in our dataset. In our dataﬁles, we also provide formula name output by the pymatgen reduced formula method for the Composition class which sorts elements by electronegativity.

Symmetry Analysis The automated nature of our ferroelectric search relies on strict symmetry criteria. As described in the Structure Selection section, we pre-screen our candidate nonpolar-polar structure pairs using the symmetry tools in pymatgen and spglib to ensure that these pairs already satisfy basic group-subgroup relationships. We then use symmetry tools provided by the Bilbao Crystallographic Server (BCS) to impose the symmetry criteria described in the Workﬂow Overview [31, 28, 30]. BCS has a freely available web interface for accessing a wide variety of symmetry tools. We create python scripts to automate interaction with and scrape returned data from BCS to perform our symmetry checks using the python package mechanize. We use the BCS Structure Relations tool to obtain a transformation matrix connecting two group-subgroup related structures [225, 243, 240]. More details on this process are given in Appendix F. The Structure Relations tool checks for the following: 1.1 Compatible group-subgroup index relations. The index of a group-subgroup relation indicates how many ferroelectric domains (distinct polar structures) arise from the symmetry breaking of the high-symmetry structure. 1.2 There exists a path of maximal subgroups between the high symmetry structure and low symmetry structure. 1.3 The Wyckoﬀ position splitting of the high symmetry structure is compatible with the Wyckoﬀ positions of the low symmetry structure. 1.4 The lattice of the high-symmetry structure in the low-symmetry setting must be within a certain tolerance of the lattice of the low-symmetry structure 1.5 Each atom in the high symmetry structure in the low symmetry setting can be paired to an atom in the low symmetry structure such that no atom pairs are greater than a given tolerance apart. Structure Relations takes Crystallographic Information Files (CIFs) high-symmetry and low-symmetry structures and tolerance threshholds as arguments. We use a lattice tolerance CHAPTER 6. AN AUTOMATICALLY CURATED FIRST-PRINCIPLES DATABASE OF FERROELECTRICS 59 of 3 A˚ and 10◦ for lattice parameters and angles, respectively. For the present work, we also use a maximum pairing distance of 1.5 A,˚ since few ferroelectrics have a distortion that results in any atom being displaced by more than 1.5 A.˚ Out of the 17,000 structure pairs that we test with Structure Relations, 414 are found to be deformable by symmetry with maximum distortion less than or equal to 1.5 A.˚

Symmetry precision Symmetry precision is a tolerance factor used to assess whether an atom is equivalent to another after a symmetry operation up to a maximum distance. A symmetry precision between 10−1 and 10−5 A˚ is typically used. In the Materials Project database, a symmetry tolerance of 10−1 A˚ is used for the reported space group stored in the database. We use this tolerance to generate CIFs sent to BCS Structure Relations. We evaluated how varying the symmetry tolerance changes the resolved space group for all the structures in the Materials Project. We were able to determine this −1 eﬃciently by using binary search on a log10 scale for a maximum symmetry tolerance of 10 A˚ and minimum tolerance of 10−5 A.˚ Out of the 67,000 structures we checked, 50,000(75%) of structures were resolved into one distinct space group for the entire symmetry precision range. For additional discussion about the sensitivity of symmetry precision on resulting space groups in the search for ferroelectrics, see Refs. [86, 224].

DFT calculation details We perform spin polarized DFT calculations using the Vienna Ab initio Software Package (VASP) [135, 137, 136]. We use the generalized gradient approximation functional of Perdew, Burke, and Ernzerhof (PBE) [193]. Our calculations use PAW pseudopotentials with an energy cutoﬀ of 520 eV for the plane-wave basis [46, 138]. We use the Berry phase method from Ref. [129, 254, 205, 206, 207] as implemented in VASP to calculate the electronic part of the macroscopic polarization. We calculate the ionic part of the macroscopic polarization using the point charge dipole moment for each atom in the unit cell, see the calc ionic function in pymatgen.analysis.ferroelectricity. polarization for details. We use the default parameters VASP input deﬁned in pymatgen (and used by Materials Project) and atomate [122, 121,1]. For details on these parameters, see the documentation for pymatgen.io.vasp.sets.MPStaticSet. We use a Hubbard U correction to localize d states of select oxides and ﬂuorides following the approach in Ref. [81]. To see the guidelines for which compounds we apply a U, see Ref. [124, 122, 121, 1]. We use a reciprocal k-point density of 50 for structural relaxations and 100 for static and polarization calculations. We use total energy convergence criteria of 5 10−5 eV per atom for the electronic self-consistent loop and 5 10−4 eV/Aper˚ atom for the× ionic relaxation loop for structural relaxations. × CHAPTER 6. AN AUTOMATICALLY CURATED FIRST-PRINCIPLES DATABASE OF FERROELECTRICS 60

Figure 6.2: Diagram of DFT workﬂow written with atomate and Fireworks. Blue and red boxes denote initial nonpolar and polar structures, respectively, green boxes denote DFT calculations, orange rhombuses denote decision steps, and purple ellipses denote exit steps. CHAPTER 6. AN AUTOMATICALLY CURATED FIRST-PRINCIPLES DATABASE OF FERROELECTRICS 61 LDA is commonly used for polarization calculations because most known ferroelectrics are oxides and LDA tends to more accurately describe oxides. However, generalized gradient approximation (GGA) functionals such as PBE tend to generally perform better than LDA across a wider range of materials. We use PBE to compare to calculations in the Materials Project. We expect PBE and PBE+U to underestimate the band gap. Our results are in line with the typical overestimation of PBE for the lattice parameters, and therefore, we expect a similar overestimation of the polarization.

Scientiﬁc workﬂow packages We construct the scientiﬁc workﬂows to perform the structural relaxations and calculations of energy, band gap, and polarization using the FireWorks and atomate python packages [123, 165]. FireWorks is built for managing computational scientiﬁc workﬂows. atomate is built for constructing workﬂows for multiple computational material science codes such as VASP. atomate uses FireWorks classes to build modules for performing common VASP calculations such as structural relaxations and self-consistent calculations of total energy. atomate also provides a framework for building custom modules, which we use to build our structural interpolations and polarization calculations modules.

DFT workﬂow We perform the DFT workﬂow shown in Figure 6.2 for the 414 candidates with maximum distortions that do not exceed 1.5 A˚ and have structures returned from BCS that were able to be converted to pymatgen Structures objects. We use a maximum distortion cutoﬀ of 1.5 A˚ because a distortion larger than this cutoﬀ tends to be unphysical. For each structure pair, we begin with the nonpolar structure in the low symmetry setting (obtained from BCS Structure Relations in the Symmetry Analysis step) and the polar structure. We use the nonpolar structure transformed into the low symmetry setting so we can perform structure interpolations and polarization calculations across similar lattices. We perform relaxations of the unit cell and atomic positions of both of these structures two times, similar to what Materials Project performs on its database entries. We then ﬁx the relaxed nonpolar and polar structures and perform a self-consistent calculation to compute the total energy and band gap. If either the nonpolar structure or polar structure is found to be metallic, which we deﬁne as having a band gap of less than 10 meV, we stop the workﬂow for that candidate. If the polar and nonpolar structures are both not metallic, we compute the polarizations of both structures. 31 of the 414 structure pairs were found to have a metallic nonpolar structure but insulating polar structure, 2 were found to have a metallic polar structure but insulating nonpolar structure, and 51 were found to have both metallic polar and nonpolar structures. 2 additional structures have at least a metallic nonpolar structure, but these workﬂows were halted before the polar structures had their band gaps computed. CHAPTER 6. AN AUTOMATICALLY CURATED FIRST-PRINCIPLES DATABASE OF FERROELECTRICS 62

Figure 6.3: Polarization curves for BaTiO3 along the [001] versus distortion from nonpolar to polar structure. Due to the change in lattice parameters and volume across the distortion, the quantum of polarization along the [001] direction is diﬀerent for each structure. This causes the spontaneous polarization for diﬀerent branches to diﬀer. The branch that starts at zero is the corrected branch. The branch that starts near -600 µC/cm2 is the data from VASP. Note, while in this speciﬁc case, the calculated polarization values for all interpolations were on the same branch, this is not usually the case.

We compute the total energy, band gap, and polarization of eight linear interpolations of the nonpolar to polar structures. We found eight interpolations to be suﬃcient for recon- structing a continuous same branch polarization for at least 75% of our candidates. Unlike the previous step where a metallic calculation causes the workﬂow to stop, we instead allow interpolations to be metallic but in such cases do not attempt to calculate the polarization of that structure. 40 candidates were found to have metallic interpolations. The DFT workﬂow is labeled as complete when all polarization calculations along the path have completed or have been skipped in the case of metallic interpolation.

Post-processing Spontaneous Polarization Values Only polar space groups are compatible with polarization vectors of arbitrary length. Non- polar space groups are also compatible with a polarization vector, but the polarization vector modulo quantum of polarization along each lattice direction must be zero or a half quantum. If we can ﬁnd a reference nonpolar structure that is suﬃciently similar to our polar struc- CHAPTER 6. AN AUTOMATICALLY CURATED FIRST-PRINCIPLES DATABASE OF FERROELECTRICS 63 ture, we can calculate the polarization of several interpolations between this initial reference nonpolar and ﬁnal the ferroelectric, polar structure. This structure is used as a means to calculate the spontaneous polarization, it is not necessary for the nonpolar structure to exist for the polar material to be ferroelectric or for us to calculate a valid polarization. Starting with the nonpolar structure, we can calculate its polarization which is either zero or a half quantum of polarization along the three lattice directions. Then we perform the same calculation for the ﬁrst interpolation, and then the next, until we arrive at the ﬁnal polar structure. If we have a suﬃcient number of interpolations between our structures, we will have hopefully traced out smooth, continuous paths in polarization space. Subtracting the vectors at the nonpolar beginning and the polar ending of these paths will give us the spontaneous polarization vector. We perform the following steps to recovering the same branch polarization. We ﬁrst construct a periodic lattice for each interpolation with lengths and angles corresponding to the quantum of polarization along each lattice direction; this corresponds to the second term of the polarization equation given in the section Ferroelectricity from ﬁrst-principles. For calculating polarization, the lengths of the lattice vectors are divided by the volume of the unit cell and multiplied by conversion factors for electron charge and length scale. Because our polar and nonpolar structures can have diﬀerent lattices, the quantum of polarization along the a, b, and c lattice parameters can diﬀer for each structure. See Figure 6.3 for an example for BaTiO3. Our algorithm for adjusting the polarizations to be on the same branch is depicted in Figure 6.4. First, we take the nonpolar polarization, and choose the image of the polarization value in the nonpolar polarization lattice that is closest to Cartesian coordinates (0,0,0) which is one corner of the unit cell. The value of the nonpolar polarization along a, b, and c can either be zero or a half-quantum. Then, we ﬁnd the image the of the ﬁrst interpolation polarization value (using the ﬁrst interpolation lattice) that is closest to the Cartesian coordinates (since lattices may diﬀer) of the moved nonpolar polarization value. We continue this process until we get to the polar polarization. This algorithm will ﬁnd the polarization path with the smallest diﬀerence between po- larizations of subsequent interpolations. This can cause the algorithm to ﬁnd the incorrect same branch polarization in cases where the change in polarization between interpolations is larger than the quantum of polarization between branches. One example of this failure mode is polarization resolved for CrO3 with workﬂow ID wfid 1484694851.899452, see Figure 6.5. In this example, the algorithm chooses a discontinuous path that has a smaller spontaneous polarization of 79.9 µC/cm2 in red. However, the most continuous path uses the last three interpolations in the branch shown with a dashed red line give a polarization of 124.7 µC/cm2.

Graphical Interface To view the ferroelectric candidate data in aggregate, we create an interactive web site for viewing polarization and total energy plots, animations of the distortion, and other CHAPTER 6. AN AUTOMATICALLY CURATED FIRST-PRINCIPLES DATABASE OF FERROELECTRICS 64

Figure 6.4: A visual demonstration of the same branch polarization algorithm demonstrated in 1D (rather than 3D) using BaTiO3. As mentioned in Figure 6.3, VASP returns polar- izations all along the branch starting at -600 µC/cm2. However, to better demonstrate the algorithm, we will suppose that the values for the polarization for each interpolation are those circled in red. In the ﬁrst panel, we move the nonpolar polarization to be on the branch closest to zero. In the second panel, we move the ﬁrst interpolated polarization to be on the branch closest to the adjusted nonpolar polarization. In the third panel, we move the second interpolated polarization to be on the branch closest to the adjusted ﬁrst inter- polation polarization. If the algorithm ﬁnishes successfully, the adjusted polarizations will on the same branch. data. The interface consists of two main pages: 1) a page containing a sortable table of ferroelectric candidates organized by category (whether the candidate had a polarization resolved and if so with what conﬁdence) and 2) individual candidate pages that show energy and polarization plots, distortion animations, and other data speciﬁc to that candidate. This interface is available at https://blondegeek.github.io/\penalty\z@{}ferroelectric_ search_site/.

Code Availability The Vienna Ab Initio Software Package (VASP) used to perform DFT calculations is a proprietary code. The Bilbao Crystallographic Server (BCS) is freely available on-line at http://www.cryst.ehu.es. Fireworks, atomate, and pymatgen are python packages ac- cessible on GitHub. Fireworks and atomate are released under a modiﬁed BSD (Berkeley Software Distribution) License. pymatgen is released under a MIT (Massachusetts Institute of Technology) License. Both MIT and BSD licenses are open-source and permit both com- mercial and non-commercial use. Our workﬂow code is included in atomate version 0.6.7 and our analysis code is available in pymatgen since v4.7.4. CHAPTER 6. AN AUTOMATICALLY CURATED FIRST-PRINCIPLES DATABASE OF FERROELECTRICS 65

Figure 6.5: The polarization reconstruction for CrO3 with workﬂow ID wfid 1484694851.899452. The polarization along the b lattice parameter is incor- rectly reconstructed because the diﬀerent polarization branches are closer than the change in polarization between structure interpolations. To correctly reconstruct this polarization with our existing algorithm, more structure interpolations would be needed between the nonpolar and polar structures.

Our code for recovering the same branch polarization from polarization calculations has been contributed to pymatgen under the pymatgen.analysis.ferroelectricity mod- ule. Our code for the DFT and polarization analysis workﬂows for performing polarization calculations has been contributed to atomate under the atomate.vasp.workflows.base. ferroelectric module. We also release a python package to automate interaction with several BCS’s tools used in this search called bilbaocrystapi. We also provide code for the interface that we used to view our candidates in aggregate. The web interface for the current work is hosted at http://blondegeek.github.io/ferroelectric_search_site/. The code for the interface can be found at http://github.com/blondegeek/\penalty\z@ {}ferroelectric_search_site.

6.3 Data Records

This dataset is available as two JSON ﬁles deposited in FigShare (doi:10.6084/m9.ﬁgshare.6025634 and doi:10.6084/m9.ﬁgshare.5048425) and our GitHub repository (http://github.com/ blondegeek/ferroelectric_search_site). We also provide an interface for viewing the dataset at http://blondegeek.github.io/ferroelectric_search_site. The JSON ﬁles provide details of the symmetry analysis performed for each candidate and data generated by DFT calculations and post-processing from the workﬂow. CHAPTER 6. AN AUTOMATICALLY CURATED FIRST-PRINCIPLES DATABASE OF FERROELECTRICS 66 VASP input and output ﬁles for each candidate are provided as a zip ﬁle on FigShare. The title of the zip ﬁle includes the workﬂow ID to correlate the VASP ﬁles to information in the JSON ﬁles provided.

File format We contribute the following data:

1. JSON ﬁle with information describing all nonpolar-polar structure pairs with group- subgroup relations compatible with a second-order phase transition in the Materials Project determined with BCS Structure Relations and used in this search. See Tables 6.2 and 6.3 for details.

2. JSON ﬁle with information on workﬂow status of each calculated candidate and cal- culation details extracted from VASP inputs and outputs. This includes total energy, band gap, polarization, post-processed information and validation criteria for candi- dates with completed calculation. See Table 6.4 for details.

3. Zipped folders with the VASP INCAR, KPOINTS, OUTCAR, and POSCAR ﬁles.

Properties For each candidate we provide an initial nonpolar-polar pair of structures, including the nonpolar structure in the nonpolar, high-symmetry setting and polar, low-symmetry setting. We also provide the displacements of each atom and other metrics provided by BCS Structure Relations. For each successful calculation, we provide the structure used for calculation, the ionic and electronic polarization computed by VASP, the ionic polarization computed via the method of point charges, the energy and energy per atom of the structure, and other com- monly computed quantities such as total magnetization, magnetization per atom, forces, and stresses. We also give details as to which calculations (out of the 22 computed) for a given candidate were completed. For each set of completed calculations we also provide, the recovered spontaneous polar- ization using the algorithm described in the Method section and spline data characterizing the smoothness of the recovered polarization and energy trend across the nonpolar-polar distortion.

Graphical representation of results In Figure 6.7, we partition the high-quality candidates into known and new ferroelectrics and further partition those ferroelectrics into subclasses. In 6.7 we see that known and new ferroelectric candidates are well mixed along the metrics of nonpolar-polar structure energy CHAPTER 6. AN AUTOMATICALLY CURATED FIRST-PRINCIPLES DATABASE OF FERROELECTRICS 67 diﬀerence, distortion maximum between nonpolar and polar structures, PBE band gap of polar structure, and energy above hull. In the middle of Figure 6.7, the high performers denoted with red triangles are the perovskite family. Perovskites dominate the ferroelectric literature and we recover many known perovskite ferroelectrics in this search: LiNbO3, AlBiO3, BiInO3, KNbO3, BaO3Ti, Bi2Nb2O9Pb, Bi2O9SrTa2, NaNbO3, Bi4O12Ti3, CdO3Ti, O3PbTi, Bi2MoO6, HfO3Pb, O3PbZr and Ca3Mn2O7. Other classes identiﬁed in the middle of Figure ?? are the organic (NH4)2SO4 family in blue, boracites in green and structures already proposed by theory to be ferroelectric in purple. These show that there are many known and proposed ferroelectrics in the literature with polarizations of 10 µC/cm2 or less. In the bottom row of Figure 6.7, we categorize new ferroelectric candidates into diﬀerent trending compositions or structure types. There are several candidates containing ﬂuorides, oxocarbons, and hydroxyl groups. We highlight these candidates because they are very diﬀerent in composition from oxide ferroelectrics most common in the literature. We also point out some hypothetical non-magnetic hexagonal manganite-like structures found in the Materials Project database that have polarizations of approximately 10 µC/cm2 and half- quantum nonpolar polarizations. In Figure 6.8, we show trends in the number of deformation candidates with given nonpo- lar point group - polar point group transitions. Each space group is comprised of translation and point group symmetry. There are 32 point groups; polar point groups are shown in red and nonpolar in blue. The thickness and color of line connecting nonpolar and polar point groups indicate the number of structures in the dataset with a deformation between those point groups. Point group transitions that correspond to orthorhombic structures such as mmm mm2, monoclinic structures such as 2/m 2 or 2/m m, and hexagonal 6/mmm →6mm are most prevalent. → → In Figure→ 6.9, we show polarization of ferroelectric candidates plotted by polar point group, similar to the plot of piezoelectric tensor magnitudes in Ref. [71]. The majority of candidates have polarization less than 5 µC/cm2, shown on the right. The high performers in point group 4mm are perovskites with a reference structure with in point group m 3m. The darkness of a radial cell is proportional to the the number of candidates in that region− of the plot. For example, there are many candidates with polar point groups 2 and mm2 that have polarizations within 25 µC/cm2.

6.4 Technical Validation and Veriﬁcation

Veriﬁcation of computational methodology Several checks are needed to ensure our automated calculations have completed satisfactorily and the information automatically extracted from them is reliable. CHAPTER 6. AN AUTOMATICALLY CURATED FIRST-PRINCIPLES DATABASE OF FERROELECTRICS 68 entries. entries. distortion.json JSON ﬁle data dictionary of distortion.json distortion Project Id Project Id Project computed band gap. Project computed band gap. pertaining to distortion between nonpolar and polar structure. ids are used to generate cid in workﬂow id number, if available id number, if available osition with elements sorted by electronegativity. information as directly outputinformation by as Bilbao directly Crystallographic output Serverinformation by website as Bilbao directly Crystallographic output Server by website Bilbao Crystallographic Server website olar space group, integer between 1 and 230 olar space group from Bilbao Crystallographic Server, integer between 1 and 230 of lattice distortion (S) is the spontaneous strain (sum of the squared eigenvalues um distortion distance between nonpolar and polar structure. um distortion distance between nonpolar and polar structure. olar space group, integer between 1 and 230 olar space group from Bilbao Crystallographic Server, integer between 1 and 230 olar structure in high-symmetryolar setting structure in low-symmetry setting measure of compatibility (∆) (Bergerhoﬀ et al. 1998) koﬀ splitting pairing between high symmetry and low symmetry structures. Description These Comp Materials Materials ICSD ICSD P Nonp P Nonp Details Materials Materials olar structure in low-symmetry setting able of low-symmetry setting of Wyckoﬀ position, the string “(x, y, z)”, species, distor- Description Nonp Nonp P Structure Structure Structure T Wyc Maxim Degree Maxim The tion in x, y, and z, and the magnitude of distortion of the strain tensor divided by 3). jectid.ObjectId de de de ype T bson.ob unico unico unico ﬂoat ﬂoat ﬂoat ﬂoat ﬂoat ﬂoat dict ﬂoat ﬂoat de de de de de de de of pymatgen.Structure of pymatgen.Structure of pymatgen.Structure ype able 6.2: Key, value data type, and value description for T dict dict dict unico unico unico list list unico unico unico unico T spacegroup gap spacegroup olar gap ula setting pre id icsd spacegroup band olar w w form p nonp id icsd spacegroup band symm lo pre lo symm pre id Key high high dmax high low distortion pairings s dav delta high low polar nonpolar polar polar nonpolar nonpolar polar nonpolar bilbao bilbao distortion pretty Key able 6.3: JSON keys, value data type, and value description for T CHAPTER 6. AN AUTOMATICALLY CURATED FIRST-PRINCIPLES DATABASE OF FERROELECTRICS 69 onds to the ionic . calc corresp tries. en distortion.json entries . in dmax data.json workflow in Bohr magnetons per atom per static calculation computed structures band minimum per static calculation computed structures max distortion distance. Compare to forces per atom per static calculation computed structures Project Id Project Id projected onto spd orbitals per atom per static calculation computed structures in eV for eachper static atom calculation in structure eV for each static calculation structure of workﬂow denoted by FireWorks. alphanumeric portion of the string after cid calculation structures. Fully complete workﬂows have 10. tensor per static calculation computed structures id numbers, if available. id numbers, if available. branch polarization along a, b, and c for each polarization calculation structure. osition with elements sortedosition alphabetically. with elements sorted by electronegativity. olar space group, integer between 1 and 230. olar structure as referenced in distortion JSON ﬁle jump between spline and data for polarization along a, b, and c. jump between spline and data for energy per atom. ber of relaxation calculations performed. Fully complete workﬂowsber have of 2. static calculations performed. Fully complete workﬂowsber have of 10. polarization calculations performed. Fully complete workﬂows have 10. workﬂow id. task labels of the relaxation calculations performed. task labels of the static calculations performed. task labels of theCartesian polarization norm calculations of performed. thevector recovered along spontaneous a, polarization. b, and c of the recovered spontaneous polarization vector. with keys of specieswith and keys values of of species ZVAL in and number values of of electrons. Hubbard U correction in eV pairs. of band gaps in eV for static calculation computed structures erage jump between spline and data for for polarization along a, b, and c. erage jump between spline and data for energy per atom. w electron polarization perw polarization ionic calculation polarization structure per fromw polarization VASP ionic calculation polarization structure per from polarization VASP calculation structure from alence band maximum per static calculation computed structures olar space group, integer between 1 and 230. olar structure as referenced in distortion JSON ﬁle olarization quanta along a, b, and c lattice vectors for each polarization calculation otal magnetization in Bohr magnetons per static calculation computed structures Description The The Status Comp Comp Materials Materials ICSD ICSD P Nonp P Nonp Static Num The Num The Num The The The Ra Ra Ra P Same Max Av Energy Energy Max Av Calculated dict dict Conduction V stress Charges Magnetization T Cartesian list bson.objectid.ObjectId used in the distortion database structure jectid.ObjectId de de de de de de de of dicts of pymatgen.Structure of pymatgen.Structure of pymatgen.Structure of ﬂoats of ﬂoats of strs of strs of strs of ﬂoats of list of ﬂoats of list of ﬂoats of list of ﬂoats of list of ﬂoats of list of ﬂoats of ﬂoats of ﬂoats of ﬂoats of ﬂoats of ﬂoats of ﬂoats of list of ﬂoats of list of dictof of list ﬂoats of ﬂoats of ﬂoats of list of ﬂoats of ﬂoats ype T bson.ob unico unico unico unico unico unico unico list list ﬂoat ﬂoat dict dict List ﬂoat list ﬂoat list ﬂoat list ﬂoat list list list list list list list list list list ﬂoat ﬂoat ﬂoat dict dict list list list list list list list list jumps jumps spline asp othness v able 6.4: Key, value data type, and value description for els norm T els max smo spline lab ula ta othness distance lab olarization olarization els ids structure hange hange p p form atom atom atom len task c c quan max smo ula h olarization olarization lab max len task ids structure er er er p p olar status id icsd spacegroup p p p form len task id icsd spacegroup olar branc magnetization dict p nonp electron ionic ionic olarization id Key wﬁd nonpolar polar relaxation cid workﬂow nonpolar polar static polarization polarization polarization raw raw raw zval charges alphabetical pretty polar orig structures relaxation static polarization polarization energies energies energies energies calculated vbms stresses magnetization bandgaps nonpolar orig polarization hubbards cbms total same forces p CHAPTER 6. AN AUTOMATICALLY CURATED FIRST-PRINCIPLES DATABASE OF FERROELECTRICS 70

Figure 6.6: Legend for Figure 6.7.

Testing smoothness of energy and polarization trends with distortion We want to ﬂag any ferroelectric candidates whose calculations cannot be used to reliably assess the quality of the candidate. For example, if the trend in total energy is not continuous, we cannot be conﬁdent that we can extract a meaningful polarization trend. Similarly, if the same branch polarization is not continuous, we can not be conﬁdent that an accurate spontaneous polarization has been determined. To assess the smoothness of trends in polarization and energy across a distortion, we use UnivariateSplines from scipy.interpolate. We use cubic splines for ﬁtting polarizations and quartic splines for ﬁtting total energies. We use the default smoothness parameter of 1.0. With this default, quartic splines sometimes fail for steep double wells. These splines can be generated using the Polarization class in pymatgen.analysis.ferroelectricity. polarization. We found 13 materials to have several discontinuities in total energy (even when these calculations resulted in smooth polarizations). These materials were transition metal oxides, ﬂuorides, carbonates, orthosilicates, and phosphates with alkali metals (Li, Na, and Ba for these speciﬁc examples), many being Li-ion battery cathode candidates. The transition metals in these materials (Co, Cr, Fe, Mn, Ni, V) can take multiple oxidation states. Because these discontinuities in energy were coincident with discontinuities in the total magnetization, we believe the cause of these jumps were caused by the transition metal species changing oxidation state through the distortion. To mitigate this, one might be able to constrain the total magnetization for each interpolation based on the interpolation of the initial nonpolar magnetization and ﬁnal polar magnetization.

Metallic endpoints and metallic interpolations Workﬂows that have either polar or nonpolar structures that are calculated to be metallic are halted. In the workflow data.json, these workﬂows are designated by a workflow status of “DEFUSED”. 86 structures have metallic endpoints. These candidates do not have in- terpolation calculations performed. Occasionally, interpolations between two nonmetallic CHAPTER 6. AN AUTOMATICALLY CURATED FIRST-PRINCIPLES DATABASE OF FERROELECTRICS 71

Figure 6.7: Validated ferroelectric candidates from our search. Spontaneous polarization plotted against nonpolar-polar energy diﬀerence, maximum atomic distortion, PBE band gap, and energy of polar structure above lowest energy polymorph reported in the Materials Project. CHAPTER 6. AN AUTOMATICALLY CURATED FIRST-PRINCIPLES DATABASE OF FERROELECTRICS 72

Figure 6.8: Distortion candidate point group relations.

Figure 6.9: Diagrams of polarization magnitude vs. point group. CHAPTER 6. AN AUTOMATICALLY CURATED FIRST-PRINCIPLES DATABASE OF FERROELECTRICS 73 structures are metallic. Out of our 239 completed workﬂows, 40 of them had metallic in- terpolation structures. If any interpolation along the path from nonpolar to polar structure is metallic, the quality of automated analysis cannot be guaranteed. We include these candidates in our dataset, but they are noted as having a “polarization len” of less than 10 or do not have a “polarization change norm” (in cases where some of the interpolated polarizations are None). If a candidate has a “polarization len” equal to 10 and have a “polarization change norm”, all polarization calculations completed successfully.

Comparison of Materials Project to Relaxed Structures Two structural relaxation steps are already performed on all structures in the Materials Project. We perform additional relaxations of the unit cell and atomic positions to ensure total energy convergence. We found only less than 5% (10%) of our relaxed structures have lattice parameter diﬀerences that diﬀered larger than 3% (1%) from the original Materials Project structures. Because we perform relaxations of nonpolar structures transformed to the low symmetry polar setting, we compare the relaxed nonpolar structure to the low symmetry transformed structure output by BCS of the nonpolar structure from Materials Project.

Known and New Ferroelectrics In any high-throughput search, there are calculations that complete perfectly and some that require further scrutiny to understand. We deem high-quality candidates as calculations where the polarization and total energy trends are smooth and continuous according to a max diﬀerence between the data and ﬁtting spline to be 10−1 µC/cm2 for the spline ﬁt to the same branch adjusted polarization and 10−2 eV for spline ﬁt to the energy trend versus distortion. Out of the 239 candidates, 183 pass through our stringent validation that ensures the polarization and energy trends across the ferroelectric distortion are smooth and continuous. The remaining candidates are still valid candidates; we recommend checking the polarization and energy trends by eye as the algorithms used for analysis may not have been able to reliably recover the spontaneous polarization in these cases. The only factor that distinguishes known ferroelectrics from new ferroelectrics in our workﬂow is whether or not a given ferroelectric candidate is present in the literature. Thus, we perform a literature review by hand for every considered candidate. We leave automating such literature searches to future work. We ﬁnd out of 183 high quality candidates, 78 are known or previously proposed and 105 are new ferroelectric candidates. In Figure 6.7, we plot nonpolar-polar total energy diﬀerence, maximum distortion dis- tance, PBE band gap, and energy diﬀerence between the polar structure and lowest energy polymorph reported in the Materials Project of known and proposed and new ferroelectric candidates versus the calculated spontaneous polarization. The legend for these is in Figure 6.6. We also provide tables of the new candidates in Tables E.2 and E.3 and of the known candidates in Tables E.4 and E.5. CHAPTER 6. AN AUTOMATICALLY CURATED FIRST-PRINCIPLES DATABASE OF FERROELECTRICS 74 As seen in the top of Figure 6.7, there are no trends in these quantities that distinguish known versus new ferroelectrics. The plots in the middle of Figure 6.7 demonstrate the variety of known ferroelectric candidates that we are able to recover, from perovskites and boracites to candidates in the organic (NH4)2SO4 family and proposed by theory. The plots at the bottom of Figure 6.7 show categories of new ferroelectric candidates we ﬁnd in the Materials Project, some from previously known ferroelectric classes such as hexagonal manganite-like structures and surprising categories such as ﬂuorides, crystals containing oxocarbons, and crystals containing hydroxyl groups. We elaborate on these categories of known and new ferroelectrics in the Graphical representation of results.

Validation through comparison to hand-curated list of ferroelectrics in the Pauling File database The Pauling File is a materials database accessible through SpringerMaterials [2]. In this database, there are materials tagged as ferroelectric and antiferroelectric. We use these tagged entries to estimate how many known (anti)ferroelectrics make it through our workﬂow. In the Pauling Files, there are 955 distinct compositions tagged as (anti)ferroelectric, 306 of which are pure (not doped) compositions. Out of 306 pure compositions, 95 of those compositions are included in the Materials Project as polar materials. This does not necessarily mean that the Materials Project database contains the same ferroelectric polar structure as referenced in the Pauling Files, simply that there exists a polar structure in the Materials Project with the same composition as a tagged ferroelectric or antiferroelectric in the Pauling Files. 57 of these compositions have nonpolar-polar structures in the Materials Project, 42 of which are found to be deformable by BCS Structure Relations. 33 of the 42 are successfully identiﬁed by the workﬂow to have smooth polarizations. Out of the 9 candidates that did not successfully make it through the workﬂow, 6 of them (BiFeO3, CrO3Y, Eu2GeSe4,O3W, CuLa2O4, Cl3CoTl) had metallic endpoints, 2 candidates (MnO3Y and Br3MnRb) had metallic interpolation structures, and for 1 candidate (Ge3O11Pb5), there was a problem converting the BCS provided structures into a pymatgen Structure objects. This suggests that the primary impact to the robustness of our workﬂow is the level of DFT used; since PBE tends to underestimate band gaps, several of these candidates are experimentally insulating but are metallic in our calculations.

Validation through comparison to experimental measurements in Landolt-B¨ornsteinseries Experimentally measured polarizations depend greatly on the quality of the sample and method used to measure the spontaneous polarization. For many ferroelectrics, there are ex- perimental polarization measurements that have been made across decades that vary greatly depending on these factors. For example, measurements of single crystal BiFeO3 in 1970 2 found the polarization to be less than 6.1 µC/cm [244]. Thin ﬁlms of BiFeO3 were measured to have a polarization 50-90 µC/cm2 [259] in 2003. Then, ﬁrst-principles calculations pre- CHAPTER 6. AN AUTOMATICALLY CURATED FIRST-PRINCIPLES DATABASE OF FERROELECTRICS 75

2 sented in 2005 predicted the polarization of single crystal BiFeO3 to be 90-100 µC/cm [180]. These ﬁrst-principles results motivated further experimental investigation. Multiple teams 2 studying ceramic BiFeO3 found a small spontaneous polarization of less than 10 µC/cm attributed to the high-conductivity of their samples causing a leakage current [196, 196]. Subsequent measurements of single crystal BiFeO3 which conversely have high-resistivity permitted measuring a polarization that was in agreement with ﬁrst-principle calculations [145]. We compare our calculated polarizations to ferroelectric materials referenced in the Landolt-B¨ornstein- Group III Condensed Matter - Ferroelectrics and Related Substances [227, 228, 229, 230]. This series classiﬁes hundreds of ferroelectrics into a 72 class numbering scheme. We note that polarization values for ferroelectrics in the Landolt-B¨ornsteinseries volumes 36A, 36B and 36C may be superseded by more recent experimental measurements. Plots of calculated vs. experimental spontaneous polarizations are shown in Figure 6.10 and tabulated in Table E.1. For experimental polarizations greater than 10 µC/cm2, the majority of experimental polarizations are between 25% and -50% of those that we calculate. The exceptions are NaNbO3 and Bi2O9SrTa2, which are calculated to have polarizations much greater than their experimental values, and the polarization of Bi4O12Ti3 which is calculated to be much lower than the experimental value. The multiple entries of a given formula on the plot indicate multiple calculations in our dataset for the same compound. Compounds with polarizations of less than or equal to 1 µC/cm2 are not shown on the plot given the log-log scale. For polarizations less than 5 µC/cm2, we see our calculations capture the general trends of the experimental polarizations. We ﬁnd that the PBE functional we use for our DFT calculations overestimates polariza- tions. This is partially due to unit cells relaxed with PBE having larger than experimental volumes and thus larger distortions.

Validation through comparison to DFT calculated polarizations DFT calculated values for the ferroelectric polarization depends heavily on the structures and functional used in the calculation. For example, we relax the full geometry of our endpoint structures. Other references constrain the relaxed polar unit cell to have the same volume as the experimental structure. One such example is [27]; these calculated polarizations will be systematically smaller than ours due to PBE optimized structures having larger than experimental lattice parameters. We compare to literature where a fully optimized (unit cell, volume, and atomic positions) relaxation procedure is used. The ferroelectric ﬁrst-principles literature is largely dominated by studies of perovskites. We compare to calculations for the following perovskites: BaTiO3, PbTiO3, LiNbO3, SrBi2Ta2O9, BiAlO3, CdTiO3, Ca3Mn2O7, BiFeO3, and YMnO3. These comparisons are summarized in Table 6.5. We ﬁnd our calculations in excellent agreement with the literature that use comparable methods, the only exception being BiFeO3, and YMnO3. CHAPTER 6. AN AUTOMATICALLY CURATED FIRST-PRINCIPLES DATABASE OF FERROELECTRICS 76

Figure 6.10: Experimental vs. Calculated polarizations for ferroelectric materials in the Landolt-B¨ornsteinseries. Note, the plot is log-log. We give colored regions to show which experimental values are within 25, 50, and 75 of calculated values. ± ± ±

BiFeO3 candidates (of which there are 3) are found to have a metallic nonpolar structure and YMnO3 candidates (of which there are 4) are found to have metallic intermediate struc- tures by our workﬂow and thus do not have computed polarizations in this dataset. Ref. [275] notes diﬃculties in calculating polarizations for these structures due to LDA and PBE underestimating the gap. They attempt to calculate these polarizations at the level of PBE using a Hubbard U correction of 2 eV and 7.5 eV for the Fe in BiFeO3 and Mn in YMnO3, re- spectively. They are successful in calculating the polarization of BiFeO3, but YMnO3 is still metallic in their PBE calculations even with the Hubbard U correction. We used a Hubbard U correction of 5.3 eV for Fe and 3.9 eV for Mn. See [1] for elaboration on how Hubbard U’s are chosen in our workﬂow. We have a metallic nonpolar structure for BiFeO3 and several metallic interpolations for YMnO3, thus we do not obtain the spontaneous polarization of either.

6.5 Usage Details

In this chapter, we present 414 nonpolar-polar structure pairs in the Materials Project database that are compatible with a second-order phase transition as ferroelectric candi- dates and perform DFT calculations of total energy, band gap and polarization for these structures pairs. This dataset oﬀers the ﬁrst opportunity to compare many known and new ferroelectrics CHAPTER 6. AN AUTOMATICALLY CURATED FIRST-PRINCIPLES DATABASE OF FERROELECTRICS 77

Table 6.5: Comparison of this work to other ab initio studies of ferroelectric perovskites. indicates the reference being compared to used the Local Density Approximation (LDA) functional† in their calculations. LDA results tend to be smaller than results calculated with PBE (which we use in this work) due to smaller predicted lattice parameters by LDA than PBE. The workﬂow ids for entries in the table are (1) wfid 1476040944.53976 (2) wfid 1476040944.53976 and wfid 1476040947.794782 (3) wfid 1476040956.832394 (4) wfid 1476040982.95148 (5) wfid 1476041128.167316 (6) wfid 1476040384.215156 (7) wfid 1476040759.946834 (8) wfid 1484445148.273011 (9) wfid 1484445014.628732 (10) wfid 1476040851.179557.

2 Formula and a (A)˚ b (A)˚ c (A)˚ Ps (µC/cm ) Space Group

BaTiO3 Ref. [257] 4.005 - 4.210 43.5 (99) Ref. [275] 4.000 - 4.216 47 This work (1) 4.001 - 4.216 46.3 This work (2) 4.000 - 4.225 47.1 PbTiO3 Ref. [275] 3.844 - 4.767 125.5 (99) This work (3) 3.867 - 4.600 117.2 LiNbO3 Ref. [275] 5.203 - 14.11 84.4 (161) This work (4) 5.216 - 14.11 84.1 SrBi2Ta2O9 Ref. [269] 5.55 5.55 25.10 34.1 (36) This work (5) 5.599 5.612 25.509 37.0 † CdTiO3 Ref. [144] 5.2498 5.3870 7.5699 21 (26) This work (6) 5.402 5.524 7.693 37.0 † CdTiO3 Ref. [144] 5.2392 5.3777 7.6192 29 (33) This work (7) 5.359 5.494 7.813 34.8 † BiAlO3 Ref. [34] 3.84 (cubic) - - 75.6 (161) This work (8) 3.845 - - 81.1 † Ca3Mn2O7 Ref. [38] - - - 5 (36) This work (9) 19.476 5.332 5.377 5.6 This work (10) 19.457 5.334 5.380 5.9 CHAPTER 6. AN AUTOMATICALLY CURATED FIRST-PRINCIPLES DATABASE OF FERROELECTRICS 78 side by side with the same methodology. We believe by setting strict criteria for ferroelec- tricity and casting a wide-net using high-throughput searches, we will ﬁnd candidates that challenge and advance our understanding of ferroelectric phenomena. As seen in our can- didates, there may be many candidate ferroelectrics waiting to be discovered that defy our expectations. This dataset will be useful for creating new tools and criteria for analyzing diverse ferroelectrics. The infrastructure provided by the Bilbao Crystallographic Server, FireWorks, pymatgen, and atomate is crucial to being able to perform these types of searches eﬃciently. Thus, we also provide our code and data for these searches with the hope they will lower the barrier for others to perform similar searches. Our code for performing structural interpolations and polarization calculations has been incorporated into the pymatgen and atomate packages. We also release a python package to automate interaction with several BCS’s tools used in this search. We also provide code for the interface that we used to view our candidates in aggregate. The workﬂow we have presented can be extended to any crystal structure database, experimental and hypothetical. Several small modiﬁcations can be made to this workﬂow to extend the scope of these searches. The same DFT workﬂow can be used to screen any experimentally measured polar structure by generating nonpolar reference structures with BCS Pseudosymmetry[57]. This workﬂow can also be adapted to perform species substitutions and ﬁnd symmetry relations between structure types, classes of structures that share space group, Wyckoﬀ positions, and other lattice similarities. 79

Chapter 7

Tensor Field Networks: Rotation- and Translation-Equivariant Neural Networks for 3D Point Clouds

The work described in this chapter was submitted to the 2018 International Conference on Machine Learning with the pre-print available as Ref. [246].

We introduce tensor ﬁeld networks, which are locally equivariant to 3D rotations, transla- tions, and permutations of points at every layer. 3D rotation equivariance removes the need for data augmentation to identify features in arbitrary orientations. Our network uses ﬁlters built from spherical harmonics; due to the mathematical consequences of this ﬁlter choice, each layer accepts as input (and guarantees as output) scalars, vectors, and higher-order tensors, in the geometric sense of these terms. We demonstrate how tensor ﬁeld networks learn to model simple physics (Newtonian gravitation and moment of inertia), classify simple 3D shapes (trained on one orientation and tested on shapes in arbitrary orientations), and, given a small organic molecule with an atom removed, replace the correct element at the correct location in space.

7.1 Motivation

Convolutional neural networks are translation-equivariant, which means that features can be identiﬁed anywhere in a given input. This capability has contributed signiﬁcantly to their widespread success. In this chapter, we present a family of networks that enjoy much richer equivariance: the symmetries of 3D Euclidean space. This includes 3D rotation equivariance (the ability to identify a feature in any 3D rotation and its orientation) and 3D translation equivariance. There are three main beneﬁts. First, this is more eﬃcient than data augmentation to obtain 3D rotation-invariant output, making computation and training less expensive. This CHAPTER 7. TENSOR FIELD NETWORKS: ROTATION- AND TRANSLATION-EQUIVARIANT NEURAL NETWORKS FOR 3D POINT CLOUDS 80 is signiﬁcantly more important in 3D than 2D. Without equivariant ﬁlters like those in our design, achieving an angular resolution of δ would require a factor of (δ−1) more ﬁlters in 2D but (δ−3) more ﬁlters in 3D.1 Second, a 3D rotation- and translation-equivariantO network can identifyO local features in diﬀerent orientations and locations with the same ﬁlters, which is helpful for interpretability. Finally, the network naturally encodes geometric tensors (such as scalars, vectors, and higher-rank geometric objects), mathematical objects that transform predictably under geometric transformations such as rotation. Here, and in the rest of this chapter, the word “tensor” refers to geometric tensors, not generic multidimensional arrays. Our network diﬀers from a traditional CNN in three ways:

• We operate on point clouds using continuous convolutions. Our layers act on 3D coordinates of points and features at those points.

• We constrain our ﬁlters to be the product of a learnable radial function R(r) and a (l) spherical harmonic Ym (ˆr).

• Our ﬁlter choice requires the structure of our network to be compatible with the algebra of geometric tensors.

We call these tensor ﬁeld networks because every layer of our network inputs and outputs tensor objects: scalars, vectors, and higher-order tensors at every geometric point in the network. Tensor ﬁelds are ubiquitous in geometry, physics, and chemistry. Our motivation was to design a universal architecture for deep learning on atomic systems (such as molecules or materials), but our network design is quite general. We expect tensor ﬁeld networks to be useful in many tasks involving 3D geometry. For example, tensor ﬁeld networks could be used to process 3D images in a rotation- and translation-equivariant way. We mention other potential applications in Section 7.6. In this chapter, we explain the mathematical conditions such a 3D rotation- and translation- equivariant network must satisfy, provide several examples of equivariant compatible network components, and give examples of tasks that this family of networks can uniquely perform.

7.2 Related work

Our work builds upon Harmonic Networks [265], which uses discrete convolutions and ﬁlters composed of circular harmonics to achieve 2D rotation equivariance, and SchNet [221], which presents a rotation-invariant network using continuous convolutions. The mathematics of rotation equivariance in 3D is much more complicated than in 2D because rotations in 3D do not commute; that is, for 3D rotation matrices A and B, AB = BA in general (see Ref. [204] for more about the mathematics of tensors under 3D rotations).6 Ref. [65] introduce Spherical CNNs, which are equivariant models on spherical spaces. Our network diﬀers from this work

1This is because the manifold of orthonormal frames at a point in 2D (the group O(2)) has dimension 1 and in 3D (O(3)) has dimension 3. CHAPTER 7. TENSOR FIELD NETWORKS: ROTATION- AND TRANSLATION-EQUIVARIANT NEURAL NETWORKS FOR 3D POINT CLOUDS 81 because it is equivariant to all the symmetries of 3D Euclidean space, both 3D rotation and translation, and because it directly operates on more general data types, such as points. SchNet can be emulated by our network by only using L = 0 ﬁlters. Harmonic Networks is the 2D discretized analog of our 3D network. Our network and Spherical CNNs share much of the same mathematical underpinnings but diﬀer in the learnable parameters for rotation-equivariant ﬁlters. Additionally, while Spherical CNNs use one convolution center, we use many. Many other authors have investigated the problems of rotation equivariance in 2D, such as [278, 93, 149]. Typically these work by looking at rotations of a ﬁlter and diﬀer in exactly which rotations and how that orientation information is preserved (or not) higher in the network. Other authors have dealt with similar issues of invariance or equivariance under par- ticular input transformations. G-CNNs [66] create invariance with ﬁnite symmetry groups (unlike the continuous groups in this work). Ref [65] use spherical harmonics and Wigner D- matrices but only address spherical signals (two dimensional data on the surface of a sphere). Ref. [134] use tensor algebra to create neural network layers that extend Message Passing Neural Networks [89], but they are permutation group tensors (operating under permutation of the indices of the nodes) not geometric tensors. The networks presented in Ref. [197, 198] operate on point clouds and use symmetric func- tions to encode permutation invariance. Ref. [198] employ a randomized sampling algorithm to include pooling in the network. These networks do not include rotation equivariance. Other neural networks have been designed and evaluated on atomic systems using nuclei centered calculations. Many of these capture 3D geometry just by including the pairwise distance between atoms (e.g. SchNet [222] and the graph convolutional model from Ref. [83]). Our work notably draws from SchNet [222] for the point convolutions, radial functions, and self-interaction layers. All models that rely only on pairwise distances or angles between points have the weakness (unlike this work) that they can not distinguish between chiral inputs (e.g. left hand and right hand), which have identical pairwise distances but are diﬀerent shapes in 3D. The other major approach to modeling 3D atomic systems is to voxelize the space [258, 51, 249]. In general, these are subject to signiﬁcant expense, no guarantees of smooth transformation under rotation, and edge eﬀects from the voxelization step. An introduction to the concepts of steerability and equivariance in the context of neural networks can be found in Ref. [67], which focuses on discrete symmetries.

7.3 Representations and equivariance

A representation D of a group G is a function from G to square matrices such that for all g, h G, ∈ D(g)D(h) = D(gh) CHAPTER 7. TENSOR FIELD NETWORKS: ROTATION- AND TRANSLATION-EQUIVARIANT NEURAL NETWORKS FOR 3D POINT CLOUDS 82 A function : (for vector spaces and ) is equivariant with respect to a group G and group representationsL X → Y DX and DY ifX for all gY G, ∈ DX (g) = DY (g) L ◦ ◦ L Invariance is a type of equivariance where DY (g) is the identity for all g. We are concerned with the group of symmetry operations that includes isometries of 3D space and permutations of the points. Composing equivariant networks 1 and 2 yields an equivariant network 2 1 (proof in AppendixH). Therefore, proving equivarianceL L for each layer of a network isL suﬃcient◦ L to prove (up to numerical accuracy) that a whole network is equivariant. Furthermore, if a network is equivariant with respect to two transformations g and h, then it is equivariant to the composition of those transformations gh (by the deﬁnition of a representation). This implies that demonstrating permutation, translation, and rotation equivariance individually is suﬃcient to prove equivariance of a network to the group (and corresponding representations) containing all combinations of those transformations. As we describe shortly, translation and permutation equivariance are manifest in our core layers, so we will focus on demonstrating rotation equivariance. Tensor ﬁeld networks act on points with associated features. A layer takes a ﬁnite set L S of vectors in R3 and a vector in at each point in S and outputs a vector in at each point in S, where and are vectorX spaces. We write this as Y X Y

(~ra, xa) = (~ra, ya) L 3 where ~ra R are the point coordinates and xa , ya are the feature vectors (a being an indexing∈ scheme over the points in S). (To simplify∈ X ∈ the Y formulas here, we are assuming that inputs and outputs are at the same points in R3, but this is not necessary.) This combination of R3 with another vector space can be written as R3 , where refers to the direct sum operation, where vectors in each space are concatenated⊕ X and matrices⊕ acting on each space are combined into a larger block diagonal matrix. We now describe the conditions on for equivariance with respect to diﬀerent input transformations. L

Permutation equivariance

Condition: σ = σ L ◦ P P ◦ L where σ(~ra, xa) := (~rσ(a), xσ(a)) and σ permutes the points to which the indices refer. AllP of the layers that we will introduce in Section 7.4 are manifestly permutation- equivariant because we only treat point clouds as a set of points, never requiring an imposed order like in a list. In our implementation, points have an array index associated with them, but this index is only ever used in a symmetric way. CHAPTER 7. TENSOR FIELD NETWORKS: ROTATION- AND TRANSLATION-EQUIVARIANT NEURAL NETWORKS FOR 3D POINT CLOUDS 83 Translation equivariance

Condition: ~ = ~ L ◦ Tt Tt ◦ L where ~t(~ra, xa) := (~ra + ~t, xa). This condition is analogous to the translation equivariance conditionT for CNNs. It is possible to use a more general translation equivariance condition, where the operator on the right-hand side of the equation also acts upon the representation subspace, but we will not consider that in this chapter. Y All of the layers in Section 7.4 are manifestly translation-equivariant because we only ever use diﬀerences between two points ~ri ~rj (for indices i and j). − Rotation equivariance The group of proper 3D rotations is called SO(3), which is a manifold that can be parametrized by 3 numbers (see Ref. [95]). Let DX be a representation of SO(3) on a vector space (and X DY on ). Acting with g SO(3) on ~r R3 we write as (g)~r, and acting on x gives DXY(g)x. ∈ ∈ R ∈ X Condition: (7.1) (g) DX (g) = (g) DY (g) L ◦ R ⊕ R ⊕ ◦ L X X where (g) D (g) (~ra, xa) = (g)~ra,D (g)xa . (For layers in this chapter, only the R ⊕ R action of DY (g) on that will be nontrivial, so we will use a convention of omitting the R3 layer output in ourY equations.) The key to attaining local rotation equivariance is to restrict our convolution ﬁlters to have a particular form. The features will have diﬀerent types corresponding to whether they transform as scalars, vectors, or higher tensors. To make our analysis and implementation easier, we decompose representations into irreducible representations. The irreducible representations of SO(3) have dimensions 2l + 1 for l N (including l = 0) and can be chosen to be unitary. We will use the term “rotation order”∈ to refer to l in this expression. The rotation orders l = 0, 1, 2 correspond to scalars, vectors, and symmetric traceless matrices, respectively. The group elements are represented by D(l), which are called Wigner D-matrices (see Ref. [90]); they map elements of SO(3) to (2l + 1) (2l + 1)-dimensional complex matrices. We could× additionally have equivariance with respect to O(3), the group of 3D rotations and mirror operations (a discrete symmetry). We would augment our convolution using the method for obtaining equivariance with respect to discrete symmetries described in Ref. [67]. We discuss this a bit more in Section 7.5.

7.4 Tensor ﬁeld network layers

At each level of a tensor ﬁeld network, we have a ﬁnite set S of points in R3 with a vector in a representation of SO(3) (that has been decomposed into a direct sum of irreducible CHAPTER 7. TENSOR FIELD NETWORKS: ROTATION- AND TRANSLATION-EQUIVARIANT NEURAL NETWORKS FOR 3D POINT CLOUDS 84

(l) Figure 7.1: Example of Vacm representing two point masses with velocities and accelerations. Colored brackets indicate the a (point), c (channel), and m (representation) indices. (l) is (l) the key for the Vacm dictionary of feature tensors. representations) associated with each point. This is essentially a ﬁnite version of a tensor ﬁeld, which was our inspiration for this network design. At each point, we can have multiple instances of l-rotation-order representations corre- sponding to diﬀerent features of that point. We will refer to these diﬀerent instances as (l) channels. We implement this object Vacm as a dictionary with key l of multidimensional arrays each with shapes [ S , nl, 2l + 1] (where nl is the number of channels with represen- tation l) corresponding to|[point,| channel, representation index]. See Figure 7.1 for an example of how to encode a simple system in this notation. We will describe tensor ﬁeld network layers and prove that they are equivariant. To prove that a layer is equivariant, we only have to prove rotation equivariance for a given rotation order. This requires showing that when the point cloud rotates and the input features are transformed, the output features transform accordingly. (All of these layers will be manifestly permutation-invariant and translation-equivariant.)

Point convolution This layer is the core of our network and builds upon the pointwise convolutions in [221]. We start by considering the action of a general pointwise ﬁlter transformation X Fc(~ra ~rb)Vbc − b∈S Note that our design is strictly more general than standard convolutional neural networks, which can be treated as a point cloud S of a grid of points with regular spacing.

Spherical harmonics and ﬁlters To design a rotation-equivariant point convolution, we want rotation-equivariant ﬁlters. The (l) 2 spherical harmonics, Ym : S C (where m can be any integer between l and l), are an orthonormal basis for functions→ on the sphere. These functions are equivariant− to SO(3); CHAPTER 7. TENSOR FIELD NETWORKS: ROTATION- AND TRANSLATION-EQUIVARIANT NEURAL NETWORKS FOR 3D POINT CLOUDS 85 that is, they have the property that for g SO(3) andr ˆ S2, ∈ ∈ (l) X (l) (l) Y ( (g)ˆr) = D 0 (g)Y 0 (ˆr). m R mm m m0 For our ﬁlters to also be rotation-equivariant, we restrict them to the following form:

(lf ,li) (lf ,li) (lf ) Fcm (~r) = Rc (r)Ym (ˆr)

where li and lf are non-negative integers corresponding to the rotation order of the input and (lf ,li) the ﬁlter, respectively; Rc : R≥0 R are learned functions; andr ˆ and r are the direction unit vector and magnitude of ~r, respectively.→ Filters of this form inherit the transformation property of spherical harmonics under rotations because R(r) is a scalar in m. This choice of ﬁlter restriction is analogous to the use of circular harmonics in Ref. [265] (though we do not have an analog to the phase oﬀset because of the non-commutativity of SO(3)).

Combining representations using tensor products Our ﬁlters and layer input each inhabit representations of SO(3) (that is, they both carry l and m indices). In order to produce output that we can feed into downstream layers, we need to combine the layer input and ﬁlters in such a way that the output also transforms appropriately (by inhabiting a representation of SO(3)). A tensor product of representations is a prescription for combining two representations l1 (l1) (l2) (l1) (l2) and l2 to get another representation l1 l2. If u l1 and v l2, then u v l1 l2 and ⊗ ∈ ∈ ⊗ ∈ ⊗ l1 l2 X X (l,m) (u v)(l) = C u(l1)v(l2) ⊗ m (l1,m1)(l2,m2) m1 m2 m1=−l1 m2=−l2 where C are called Clebsch-Gordan coeﬃcients (see Ref. [98]). Note that l is any integer between l1 l2 and (l1 + l2) inclusive, and m is any integer between l and l inclusive. The crucial| − | property of the Clebsch-Gordan coeﬃcients that we need− to prove equivari- ance of this layer is

X (l0,m0) (l1) (l2) C 0 0 D 0 (g)D 0 (g) (l1,m1)(l2,m2) m1m1 m2m2 0 0 m1,m2 0 (7.2) X (l) (l0,m0) = D 0 (g)C m0m0 (l1,m1)(l2,m2) 0 m0 (see, for example, Ref. [204]).

Layer deﬁnition Filters inhabit one representation, inputs another, and outputs yet another. We need the Clebsch-Gordan coeﬃcients to combine inputs and ﬁlters in such a way that they yield the desired output representation: CHAPTER 7. TENSOR FIELD NETWORKS: ROTATION- AND TRANSLATION-EQUIVARIANT NEURAL NETWORKS FOR 3D POINT CLOUDS 86

(lO) (lI ) ~ra,V LacmO acmI X (l ,m ) X (l ) := C O O F (lF ,lI )(~r )V I (7.3) (lF ,mF )(lI ,mI ) cmF ab bcmI mF ,mI b∈S where ~rab := ~ra ~rb and the subscripts I, F , and O denote the representations of the input, − ﬁlter, and output, respectively. A point convolution of an lF ﬁlter on an lI input yields outputs at 2 max(lI , lF )+1 diﬀerent rotation orders lO (one for each integer between lI lF | − | and (lI + lF ), inclusive), though in designing a particular network, we may choose not to calculate or use some of those outputs. Using the equivariance of the ﬁlter F and the property of the Clebsch-Gordan coeﬃcients Equation 7.2, we can show the rotation equivariance of point convolutions, Equation 7.1 (detailed proof in Appendix H, Section H.3): (lO) X (lI ) (lI ) acm (g)~ra, Dm m0 (g)Vacm0 L O R I I I m0 I (7.4) X (lO) (lO) (lI ) = D 0 (g) 0 ~ra,Vacm mOmO acmO I 0 L mO This aspect of the design, and this proof of its correctness, is the core of our result.

Scalars (l = 0) and vectors (l = 1) In this section, we attempt to demystify Wigner D-matrices, spherical harmonics, and Clebsch-Gordan coeﬃcients by stating their values for a real representation of l = 0 (scalars) and l = 1 (vectors). (It can sometimes be simpler to use a complex representation, but we can always use a basis change to convert between real and complex versions.) The corresponding objects for l > 1 are more complicated. The Wigner D-matrices are D(0)(g) = 1 D(1)(g) = (g), R where are the usual rotation matrices on R3. The spherical harmonics are R Y (0)(ˆr) 1 Y (1)(ˆr) rˆ ∝ ∝ The Clebsch-Gordan coeﬃcients are just the familiar ways to combine scalars and vectors: For 1 1 0, ⊗ → (0,0) C δij (1,i)(1,j) ∝ which is the dot product for 3D vectors. For 1 1 1, ⊗ → (1,i) C ijk (1,j)(1,k) ∝ which is the cross product for 3D vectors. The 0 0 0 case is just regular multiplication of two scalars, and 0 1 1 and 1 0 1 corresponds⊗ → to scalar multiplication of a vector. ⊗ → ⊗ → CHAPTER 7. TENSOR FIELD NETWORKS: ROTATION- AND TRANSLATION-EQUIVARIANT NEURAL NETWORKS FOR 3D POINT CLOUDS 87 Self-interaction We follow Ref. [222] in using point convolutions to scale feature vectors elementwise and using self-interaction layers to mix together the components of the feature vectors at each point. Self-interaction layers are analogous to 1x1 convolutions, and they implicitly act like l = 0 (scalar) types of ﬁlters: X (l) (l) Wcc0 Vac0m c0 In general, each rotation order has diﬀerent weights because there may be diﬀerent numbers of channels nl corresponding to that rotation order. For l = 0, we may also use biases. Putting a self-interaction layer after a one-hot encoding input is the same as the embedding layer described in Ref. [222]. The weight matrix W is a scalar transform with respect to the representation index m, so the D-matrices commute with W , straightforwardly implying that this layer is equivariant. Equivariance for l = 0 is straightforward because D(0) = 1.

Concatenation The most general way to combine incoming channels of the same rotation order before the next point convolution layer is to concatenate along the channel axis (increasing the number of input channels), then apply a self-interaction layer. This concatenation operation is equivariant because concatenation does not aﬀect the representation index.

Nonlinearity Our nonlinearity layer acts as a scalar transform in the l spaces (that is, along the m dimension). For l = 0 channels, we can use (0) (0) (0) η Vac + bc (0) (0) for some function η : R R and biases bc . For l > 0 channels, our nonlinearity has the form → η(l) V (l) + b(l)V (l) k kac c acm where η(l) : R R can be diﬀerent for each l and → s (l) X (l) 2 V ac := Vacm k k m | | (It may be necessary to regularize this norm near the origin for this layer to have desirable diﬀerentiability properties.) Note that D(g)V = V k k k k because D is a unitary representation. Therefore, this layer is a scalar transform in the representation index m, so it is equivariant. CHAPTER 7. TENSOR FIELD NETWORKS: ROTATION- AND TRANSLATION-EQUIVARIANT NEURAL NETWORKS FOR 3D POINT CLOUDS 88 Global pooling A global pooling operation that we use in our demonstrations is summing the feature vectors over each point. This operation is equivariant because D-matrices act linearly.

7.5 Demonstrations and experiments

We chose experiments that are simple enough to be easily understandable yet suggestive of richer problems. They each highlight a diﬀerent aspect of our framework. Each of these tasks is either unnatural or impossible in existing frameworks. We have focused on understanding how to construct and train these models in controlled tasks because of the complexity of the architecture. In future work, we will apply our network to more complicated and useful tasks. In these tasks, we used radial functions identical to those used in Ref. [221]: We used radial basis functions composed of Gaussians, and two dense layers are applied to this basis vector. The number, spacing, and standard deviation of the Gaussians are hyperparameters. We used a shifted softplus activation function log(0.5ex + 0.5) for our radial functions and nonlinearity layers. We implemented our models in TensorFlow [5]. Our code is available at https://github.com/tensorfieldnetworks/tensorfieldnetworks

Tensor outputs: acceleration vectors in Newtonian gravity and moment of inertia tensor Network types: 0 1 and 0 0 2 To demonstrate→ the simplest→ non-trivial⊕ tensor ﬁeld networks, we train networks to calcu- late acceleration vectors of point masses under Newtonian gravity and the moment of inertia tensor at a speciﬁc point of a collection of point masses. These tasks only require a single layer of point convolutions to demonstrate. Furthermore, we can check the learned radial functions against analytical solutions. The acceleration of a point mass in the presence of other point masses according to Newtonian gravity is given by X mn ~ap = GN rˆnp − r2 n6=p np

where we deﬁne ~rnp := ~rn ~rp. (We choose units where GN = 1, for simplicity.) The moment of inertia− tensor is used in classical mechanics to calculate angular mo- mentum. Objects generally have diﬀerent moments of inertia depending on which axis they rotate about, and this is captured by the moment of inertia tensor (see Ref. [142]): X h i Iij = mp (~rp ~rp)δij (~rp)i(~rp)j p · − CHAPTER 7. TENSOR FIELD NETWORKS: ROTATION- AND TRANSLATION-EQUIVARIANT NEURAL NETWORKS FOR 3D POINT CLOUDS 89

Figure 7.2: Network diagram for learning gravitational accelerations and moment of inertia tensor. The input tensor has indices [channels, points, representation]. The input for the gravitational acceleration and moment of inertia tasks are point mass scalars, therefore the representation index is 1-dimensional. Convolution ﬁlters are indicated by blocks marked F and Clebsch-Gordan tensors are indicated by CG. The numbers along the arrows for the representation index indicate the l of that arrow, with CG blocks combining the input and ﬁlter ls to generate output of a speciﬁc l.

The moment of inertia tensor is a symmetric tensor, so it can be encoded using a 0 2 representation. (AppendixH contains a more detailed explanation of how to go from⊕ irreducible representations to matrix tensor representation.) For both of these tasks, we input to the network a set of random points with associated random masses. (Details of about how these points are generated and about the hyperpa- rameters for our radial functions are given in Appendix H.) For the moment of inertia task, we also designate a diﬀerent special point at which we want to calculate the moment of inertia tensor. Our networks are simple: for learning Newtonian gravity, we use a single l = 1 convolution with 1 channel; for learning the moment of inertia tensor, we use a single layer comprised of l = 0 and l = 2 convolutions with 1 channel each. See Figure 7.2 for a diagram of these networks. We use elementwise summed L2 losses for the diﬀerence of the acceleration vectors and for the diﬀerence of the moment of inertia tensor. We get excellent agreement with the Newtonian gravity inverse square law after a 1,000 training steps and with the moment of inertia tensor radial functions after 10,000 steps. In Figure 7.3, we show that the single radial ﬁlter is able to learn the 1/r2 law for gravitational accelerations. (Related ﬁgures for the moment of inertia task can be found in Appendix H.) We could have obtained equivariant accelerations by using a pure l = 0 network to predict the gravitational potential φ : R3 R, a scalar ﬁeld, and then taking derivatives of φ with respect to the point coordinates→ to obtain the forces and accelerations (as in, CHAPTER 7. TENSOR FIELD NETWORKS: ROTATION- AND TRANSLATION-EQUIVARIANT NEURAL NETWORKS FOR 3D POINT CLOUDS 90

Figure 7.3: Radial function learned by l = 1 ﬁlter for gravity toy dataset. Minimum radial cutoﬀ distance of 0.5 is chosen for randomly sampled points such that there are enough samples generated near the minimum distance.

Figure 7.4: 3D Tetris shapes. Blocks correspond to single points. The third and fourth shapes from the left are mirrored versions of each other.

e.g., Ref. [222]). However, many important vector quantities, such as magnetic ﬁelds in electromagnetism, cannot be derived from scalar ﬁelds.

Shape classiﬁcation Network type: 0 0 In three dimensions,→ there are 8 unique shapes made of 4 adjacent cubes (up to trans- lations and rotations); see Figure 7.4. We call these shapes 3D Tetris, and represent them using points at the center of each cube. We demonstrate the rotation equivariance of our network by classifying 3D Tetris pieces in the following way: During training, we input to the network a dataset of shapes in a single orientation, and it outputs a classiﬁcation of which shape it has seen. To demonstrate the equivariance of the network, we test the network with shapes from the same dataset that have been rotated and translated randomly. Our network performs perfectly on this task. We use a 3-layer network that includes the following for every layer: all possible paths CHAPTER 7. TENSOR FIELD NETWORKS: ROTATION- AND TRANSLATION-EQUIVARIANT NEURAL NETWORKS FOR 3D POINT CLOUDS 91

Figure 7.5: Network diagrams for shape classiﬁcation task showing how information ﬂows be- tween tensors of diﬀerent order. Clebsch-Gordan tensors are implied in the arrows indicating convolutions. The numbers above the self-interactions indicate the number of channels. Indi- vidual convolutions, indicated by arrows, each produce a separate tensor, and concatenation is performed after the convolutions.

with l = 0 and l = 1 convolutions, a concatenation (if necessary), a self-interaction layer, and a rotation-equivariant nonlinearity. We only use the l = 0 output of the network since the shape classes are invariant under rotation and hence scalars. To get a classiﬁcation from the l = 0 output of the network, we sum over the output of all points (global pooling).

Chirality There are two shapes in 3D Tetris that are mirrors of each other. Any network that relies solely upon distances (such as SchNet) or angles between points (such as ANI-1 [236]) cannot distinguish these shapes. Our network can. A tensor ﬁeld network that contains a path with an odd number of odd-rotation-order ﬁlters has the possibility of detecting local changes in handedness. This is because

Y (l)( ~r) = ( 1)lY (l)(~r). − − A tensor ﬁeld network that does not include such paths will be invariant to mirror symmetry. As an example, a 0 0 network can correctly classify all 3D Tetris shapes except for the chiral shapes. The smallest→ network that can classify chiral shapes must include the path 0 1 1 1 1 1 0 (superscripts correspond to ﬁlter rotation order), which yields the vector −→ −→ −→ triple product F~1 (F~2 F~3) of the ﬁlter vectors F~i for each layer. This combination picks up a minus sign under· × mirror operations.

Missing point Network type: 0 0 1 → ⊕ CHAPTER 7. TENSOR FIELD NETWORKS: ROTATION- AND TRANSLATION-EQUIVARIANT NEURAL NETWORKS FOR 3D POINT CLOUDS 92

Figure 7.6: A hypothetical example input and output of the missing point network. (A) A benzene molecule with hydrogen removed (B) The relative output vectors produced by the network, with arrows shaded by the associated probabilities.

In this task, we randomly remove a point from a shape and ask the network to replace that point. This is a ﬁrst step toward general isometry-equivariant generative models for 3D point clouds. We output an array of scalars, a special scalar, and one vector at each point. The vector, ~δa, indicates where the missing point should be relative to the starting point ~ra (both direction and distance) and the array of scalars indicates the point type. The special scalar is put through softmax and used as a probability pa measuring the conﬁdence in that point’s vote. We aggregate votes for location using a weighted sum: X pa(~ra + ~δa) a (See AppendixH for a proof that this is translation-equivariant.) This scheme is illustrated in Figure 7.6. We train on molecular structures for this task because molecules can be comprised of a small number of atoms (making the task computationally easy to demonstrate) and because precise positions are important for chemical behavior. We trained on structures in the QM9 dataset, a collection of 134,000 molecules with up to nine heavy atoms (C, N, O, F); including hydrogens, there are up to 29 atoms per molecule [203]. Our network is 3 layers deep, with 15 channels per rotation order at each layer. The input features to the network are a one-hot encoding of atom types at each point. We use 2-layer radial functions with 4 Gaussians with centers evenly spaced from 0 to 2.5 angstroms and variance that is half of the spacing. Most covalent bonds are 1-2 angstroms in length, so our radial functions are smaller than the diameter of the molecules of the QM9 dataset. We train on a 1,000 molecule subset of molecules that have 5 to 18 atoms. In a single epoch, we train on each molecule in the training set (1,000 molecules with 5-18 atoms) with CHAPTER 7. TENSOR FIELD NETWORKS: ROTATION- AND TRANSLATION-EQUIVARIANT NEURAL NETWORKS FOR 3D POINT CLOUDS 93

Table 7.1: Performance on missing point task

Accuracy (%) Number of Distance Atoms ( 0.5 A˚ predictions MAE in A˚ and≤ atom type) 5-18 (train) 15863 91.3 0.16 19 19000 93.9 0.14 23 23000 96.5 0.13 25-29 25356 97.3 0.16 one randomly selected atom deleted (1,000 examples total per epoch). We then test the network on a random selection of 1,000 molecules with 19 atoms, 1,000 molecules with 23 atoms, and 1,000 molecules with 25-29 atoms. For each epoch during training, we use each molecule once and randomly remove one atom. During evaluation, for each molecule, we make a prediction for every possible atom that could be removed. For example, for a molecule with 10 atoms, we will generate 10 predictions, each with a diﬀerent atom missing. This is why the number of predictions is larger than the number of molecules. We deﬁne an accurate placement of the missing atom position to be within 0.5 angstroms of the removed atom position with the correct atom type according to argmax of the returned atom type array. We choose the 0.5 angstrom cutoﬀ because it is smaller than the smallest covalent bond, a hydrogen-hydrogen bond which has a length of 0.7 angstroms. We present the accuracy of our predictions in Table 7.1. We train for 225 epochs and show comparable prediction accuracy on the test sets of 19, 23, and 25-29 atoms as the training set of 5-18 atoms. We include a breakdown of the accuracy and distance mean absolute error (MAE) in the Appendix H. Our network is most accurate for carbon and hydrogen missing atoms (over 90%), moder- ately accurate for oxygen and nitrogen (about 70-80%), and not accurate for ﬂuorine atoms (since there are only 50 examples in our training set, they might not be seen during training due to random selection of the missing atom).

7.6 Future work

We have explained the theory of tensor ﬁeld networks and demonstrated how they work on simple examples. We hope that tensor ﬁeld networks can be applied to a wide range of phenomena: In the context of atomic systems, we hope to train networks to predict properties of large and heterogeneous systems, learn molecular dynamics, calculate electron densities (as inputs to density functional theory algorithms), and hypothesize new stable structures. Ultimately, we hope to design new useful materials, drugs, and chemicals. CHAPTER 7. TENSOR FIELD NETWORKS: ROTATION- AND TRANSLATION-EQUIVARIANT NEURAL NETWORKS FOR 3D POINT CLOUDS 94 For more general physics, we see potential applications in modeling complex ﬂuid ﬂows, analyzing detector events in particle physics experiments, and studying conﬁgurations of stars and galaxies. We see other applications in 3D perception, robotics, computational geometry, and bioimaging. 95

Chapter 8

Outlook

In this thesis, we have understood the properties of a variety of atomic systems in terms of their structural motifs. We have classiﬁed these motifs based on their geometry, topology, and symmetry. We have also investigated potential methods for learning to identify struc- tural motifs and relating those motifs to electronic properties using custom neural network architectures equivariant to 3D rotations and translations. While we have focused in this work on going from structural motifs to properties, the more challenging question is can we do the inverse? A holy grail of computational materials discovery is a tool that, given desired mate- rial properties, can automatically generate corresponding atomic structures that host those properties [280]. However, before this tool can be feasible, we need an algorithm capable of generating stable atomic structures, regardless of properties. Such an algorithm does not currently exist. High-throughput computational materials discovery pipelines are bottlenecked by our ability to systematically propose new structures. Generally, structures fed to high-throughput searches are already experimentally known or are just element substitutions of existing ma- terials. Current approaches to computational materials discovery often presuppose that a material already exists and is awaiting identiﬁcation. In contrast to this assumption, syn- thesis eﬀorts (such as those at Berkeley Lab, including the Molecular Foundry and the Energy Sciences Area) regularly yield materials that diﬀer substantially from the structures in databases of previously known materials. An algorithm that could generate stable atomic structures could in the process learn a representation of the structural motifs atomic systems can host. This representation could be used as an ab initio materials map and as a similarity metric for comparing diverse atomic systems. There are many similarity metrics that exist for speciﬁc classes of material systems, especially molecules, but they cannot naturally be stitched together. Furthermore, these metrics do not necessarily allow for algebra on the metric – interpolations in metric space cannot necessarily be converted back into meaningful structures. Genetic algorithms have been proposed as a means to generate hypothetical atomic structures, but they are generally constrained to explore a restricted space of structures CHAPTER 8. OUTLOOK 96

[261, 195, 157, 181]. Furthermore, it is diﬃcult to understand why a given structure is generated by these algorithms. With deep learning techniques specialized to deal with 3D geometry, we can learn a similarity metric out of the wealth of structural data, we already have available. Ref. [92], which focuses on molecules, demonstrates that learning such a representation is possible, although more work is needed to train a network on broader classes of atomic systems. A computational tool that could generate new atomic-scale geometries would greatly accelerate materials discovery and innovation. This approach would also aid in resolving atomic structures from experimental data (such as data generated by users of the ALS) by reducing the time it takes to characterize new structures. MOChA style synthesis is amenable to combinatorial exploration through use of automated robotic synthesis. To better explore this synthesis space, it would be advantageous to have speciﬁc structures in mind to synthesize and quickly assess the relative structural stability and electronic properties of such structures. While hypothetical structures and density functional theory calculations in and of themselves cannot readily suggest speciﬁc synthetic pathways, due to the modularity of MOChA style synthesis, often just having components in mind gives direction to a synthetic search. Existing tools will play an important role in creating structure generating algorithms. Contributors to the python package atomate have already started the process of building recipes for reliably calculating speciﬁc material properties with minimal user input [165]. These recipes are rapidly feeding databases of density functional theory calculations and will serve as crucial datasets for statistical methods. Deep learning techniques can expedite the calculation of properties traditionally computed with density functional theory and enable ab initio molecular dynamics for large systems (exceeding thousands of atoms) [89, 223]. It would also be very helpful to have open-source tools with modern APIs to transform and relate structures through symmetry. Bilbao Crystallographic Server and ISOTROPY are excellent tools. However, the fact that there is no open-source version of these codes and that they do not have modern APIs makes them diﬃcult to modify and include for speciﬁc materials search eﬀorts, including high-throughput ﬁrst-principles workﬂows. Having easier access to these tools would make it much simpler to expand the automated ferroelectric workﬂow described in Chapter 6 by including nonpolar structures derived polar structures and vice versa. In parallel with automated methods, we need better human-guided design tools to ar- ticulate the relationships of atomic systems. While software like Avogadro can help a user articulate a speciﬁc atomic system and test its feasibility, these tools do not make the intuitive leap that one atomic structure can imply many others, such as was the case in Chapters 3 [100]. This is the diﬀerence between design of individual systems to systematic design. Para- metric models used in mechanical design could be immensely useful here if we can combine them with fast methods for testing the chemical feasibility of atomic structures. The pop- ularity of Foldit, a video game built on the protein folding software Rosetta, demonstrates that it is possible to create interactive environments where quantitative chemical insights can be translated into tools that harness human visual intuition [131]. CHAPTER 8. OUTLOOK 97

New tools are needed to bring us closer to the systematic design of atomic systems. These tools are emerging with the conﬂuence of open-source software, robotic tools for synthesis and characterization, decreasing computational costs, systematized high-throughput ﬁrst- principles calculations, and rapidly evolving deep learning techniques. 98

Bibliography

[1] Materials Project Calculation Guide. https://materialsproject.org/docs/ calculations. [2] Pauling ﬁle multinaries edition – 2012 in springermaterials. Copyright 2016 Springer- Verlag Berlin Heidelberg & Material Phases Data System (MPDS), Switzerland & National Institute for Materials Science (NIMS), Japan.

[3] Zigzag Magnetic Order in the Iridium Oxide Na2IrO3. [4] CS231n: Convolutional Neural Networks for Visual Recognition, 2018.

[5] M. Abadi, A. Agarwal, P. Barham, E. Brevdo, Z. Chen, C. Citro, G. S. Corrado, A. Davis, J. Dean, M. Devin, S. Ghemawat, I. Goodfellow, A. Harp, G. Irving, M. Is- ard, Y. Jia, R. Jozefowicz, L. Kaiser, M. Kudlur, J. Levenberg, D. Man´e,R. Monga, S. Moore, D. Murray, C. Olah, M. Schuster, J. Shlens, B. Steiner, I. Sutskever, K. Tal- war, P. Tucker, V. Vanhoucke, V. Vasudevan, F. Vi´egas, O. Vinyals, P. Warden, M. Wattenberg, M. Wicke, Y. Yu, and X. Zheng. TensorFlow: Large-scale machine learning on heterogeneous systems, 2015. Software available from tensorﬂow.org.

[6] S. C. Abrahams. Structurally Based Prediction of Ferroelectricity in Inorganic Mate- rials with Point Group 6mm. Acta Crystallographica Section B, B44:585–595, 1988.

[7] S. C. Abrahams. Structurally based predictions of ferroelectricity in seven inorganic materials with space group Pba2 and two experimental conﬁrmations. Acta Crystal- lographica Section B, 45(3):228–232, 1989.

[8] M. Adachi, Y. Akishige, T. Asahi, K. Deguchi, K. Gesi, K. Hasebe, T. Hikita, T. Ikeda, Y. Iwata, M. Komukae, et al. BaTiO3 (cubic)[F] Survey, 1A-10. In Oxides, pages 1–9. Springer, 2001.

[9] M. Adachi, Y. Akishige, T. Asahi, K. Deguchi, K. Gesi, K. Hasebe, T. Hikita, T. Ikeda, Y. Iwata, M. Komukae, et al. CdTiO3, 1A-9. In Oxides, pages 1–12. Springer, 2001.

[10] M. Adachi, Y. Akishige, T. Asahi, K. Deguchi, K. Gesi, K. Hasebe, T. Hikita, T. Ikeda, Y. Iwata, M. Komukae, et al. KNbO3 [F], 1A-2. In Oxides, pages 1–70. Springer, 2001. BIBLIOGRAPHY 99

[11] M. Adachi, Y. Akishige, T. Asahi, K. Deguchi, K. Gesi, K. Hasebe, T. Hikita, T. Ikeda, Y. Iwata, M. Komukae, et al. LiNbO3 [F] References, 2A-1. In Oxides, pages 1–14. Springer, 2001.

[12] M. Adachi, Y. Akishige, T. Asahi, K. Deguchi, K. Gesi, K. Hasebe, T. Hikita, T. Ikeda, Y. Iwata, M. Komukae, et al. NaNbO3 [(F) A], 1A-1. In Oxides, pages 1–36. Springer, 2001.

[13] M. Adachi, Y. Akishige, T. Asahi, K. Deguchi, K. Gesi, K. Hasebe, T. Hikita, T. Ikeda, Y. Iwata, M. Komukae, et al. PbHfO3 [(A)], 1A-16. In Oxides, pages 1–14. Springer, 2001.

[14] M. Adachi, Y. Akishige, T. Asahi, K. Deguchi, K. Gesi, K. Hasebe, T. Hikita, T. Ikeda, Y. Iwata, M. Komukae, et al. PbTiO3 [F], 1A-11. In Oxides, pages 1–77. Springer, 2001.

[15] M. Adachi, Y. Akishige, T. Asahi, K. Deguchi, K. Gesi, K. Hasebe, T. Hikita, T. Ikeda, Y. Iwata, M. Komukae, et al. PbZrO3 [A], 1A-15. In Oxides, pages 1–60. Springer, 2001.

[16] M. Adachi, Y. Akishige, T. Asahi, K. Deguchi, K. Gesi, K. Hasebe, T. Hikita, T. Ikeda, Y. Iwata, M. Komukae, et al. Bi4Ti3O12 [F], 9A-15. In Oxides, pages 1–26. Springer, 2002.

[17] M. Adachi, Y. Akishige, T. Asahi, K. Deguchi, K. Gesi, K. Hasebe, T. Hikita, T. Ikeda, Y. Iwata, M. Komukae, et al. Cr3B7O13Cl [F, A], 18A-2. In Oxides, pages 1–34. Springer, 2002.

[18] M. Adachi, Y. Akishige, T. Asahi, K. Deguchi, K. Gesi, K. Hasebe, T. Hikita, T. Ikeda, Y. Iwata, M. Komukae, et al. Mg3B7O13Cl [F], 18A-1. In Oxides, pages 1–37. Springer, 2002.

[19] M. Adachi, Y. Akishige, T. Asahi, K. Deguchi, K. Gesi, K. Hasebe, T. Hikita, T. Ikeda, Y. Iwata, M. Komukae, et al. Mn3B7O13I, 18A-20. In Oxides, pages 1–9. Springer, 2002.

[20] M. Adachi, Y. Akishige, T. Asahi, K. Deguchi, K. Gesi, K. Hasebe, T. Hikita, T. Ikeda, Y. Iwata, M. Komukae, et al. PbBi2Nb2O9 [(F)], 9A-10. In Oxides, pages 1–7. Springer, 2002.

[21] M. Adachi, Y. Akishige, T. Asahi, K. Deguchi, K. Gesi, K. Hasebe, T. Hikita, T. Ikeda, Y. Iwata, M. Komukae, et al. SbNbO4 [F,(A)], 5A-2. In Oxides, pages 1–9. Springer, 2002. BIBLIOGRAPHY 100

[22] M. Adachi, Y. Akishige, T. Asahi, K. Deguchi, K. Gesi, K. Hasebe, T. Hikita, T. Ikeda, Y. Iwata, M. Komukae, et al. Sr2Ta2O7 [F], 8A-6. In Oxides, pages 1–16. Springer, 2002.

[23] M. Adachi, Y. Akishige, T. Asahi, K. Deguchi, K. Gesi, K. Hasebe, T. Hikita, T. Ikeda, Y. Iwata, M. Komukae, et al. SrBi2Ta2O9 [F], 9A-12. In Oxides, pages 1–4. Springer, 2002.

[24] A. Altomare, G. Cascarano, C. Giacovazzo, A. Guagliardi, M. C. Burla, G. Polidori, and M. Camalli. SIR92 – a program for automatic solution of crystal structures by direct methods. Journal of Applied Crystallography, 27(3):435, Jun 1994.

[25] E. C. Andrade and M. Vojta. Magnetism in spin models for depleted honeycomb-lattice iridates: Spin-glass order towards percolation. arXiv:1309.2951 [cond-mat], Sept. 2013.

[26] V. I. Anisimov, J. Zaanen, and O. K. Andersen. Band theory and mott insulators: Hubbard u instead of stoner i. Phys. Rev. B, 44:943–954, Jul 1991.

[27] R. Armiento, B. Kozinsky, M. Fornari, and G. Ceder. Screening for high-performance piezoelectrics using high-throughput density functional theory. Phys. Rev. B, 84:014103, Jul 2011.

[28] M. I. Aroyo, A. Kirov, C. Capillas, J. M. Perez-Mato, and H. Wondratschek. Bilbao crystallographic server. II. representations of crystallographic point groups and space groups. Acta Crystallographica Section A Foundations of Crystallography, 62(2):115– 128, mar 2006.

[29] M. I. Aroyo, J. M. Perez-Mato, C. Capillas, E. Kroumova, S. Ivantchev, G. Madariaga, A. Kirov, and H. Wondratschek. Bilbao crystallographic server: I. databases and crystallographic computing programs. Zeitschrift f¨urKristallographie - Crystalline Materials, 221(1), jan 2006.

[30] M. I. Aroyo, J. M. Perez-Mato, C. Capillas, E. Kroumova, S. Ivantchev, G. Madariaga, A. Kirov, and H. Wondratschek. Bilbao Crystallographic Server: I. Databases and crystallographic computing programs. Zeitschrift f¨urKristallographie - Crystalline Materials, 221(1), jan 2006.

[31] M. I. Aroyo, J. M. Perez-Mato, D. Orobengoa, E. Tasci, G. de la Flor, and A. Kirov. Crystallography online: Bilbao Crystallographic Server. Bulg. Chem. Commun., 43(2), jan 2011.

[32] N. Artrith and A. Urban. An implementation of artiﬁcial neural-network potentials for atomistic materials simulations: Performance for tio2. Computational Materials Science, 114(Supplement C):135 – 150, 2016. BIBLIOGRAPHY 101

[33] N. Artrith, A. Urban, and G. Ceder. Eﬃcient and accurate machine-learning interpo- lation of atomic energies in compositions with many species. Phys. Rev. B, 96:014112, Jul 2017.

[34] P. Baettig, C. F. Schelle, R. LeSar, U. V. Waghmare, and N. A. Spaldin. Theoretical prediction of new high-performance lead-free piezoelectrics. Chemistry of Materials, 17(6):1376–1380, 2005.

[35] L. Balents. Spin liquids in frustrated magnets. Nature, 464(7286):199–208, Mar. 2010.

[36] J. Behler and M. Parrinello. Generalized neural-network representation of high- dimensional potential-energy surfaces. Phys. Rev. Lett., 98(14):146401, 2007.

[37] N. A. Benedek and C. J. Fennie. Hybrid improper ferroelectricity: A mecha- nism for controllable polarization-magnetization coupling. Physical Review Letters, 106(10):107204, Mar. 2011.

[38] N. A. Benedek and C. J. Fennie. Hybrid improper ferroelectricity: A mechanism for controllable polarization-magnetization coupling. Phys. Rev. Lett., 106:107204, Mar 2011.

[39] J. W. Bennett. Discovery and Design of Functional Materials: Integration of Database Searching and First Principles Calculations. Physics Procedia, 34:14–23, 2012.

[40] J. W. Bennett, K. F. Garrity, K. M. Rabe, and D. Vanderbilt. Hexagonal ABC semi- conductors as ferroelectrics. Physical Review Letters, 109:167602, 2012.

[41] J. W. Bennett and K. M. Rabe. Integration of ﬁrst-principles methods and crystallo- graphic database searches for new ferroelectrics: Strategies and explorations. J. Solid State Chem., 195:21–31, 2012.

[42] T. C. Berkelbach, M. S. Hybertsen, and D. R. Reichman. Theory of neutral and charged excitons in monolayer transition metal dichalcogenides. Physical Review B, 88(4):045318, 2013. PRB.

[43] G. R. Bhimanapati, Z. Lin, V. Meunier, Y. Jung, J. Cha, S. Das, D. Xiao, Y. Son, M. S. Strano, V. R. Cooper, L. Liang, S. G. Louie, E. Ringe, W. Zhou, S. S. Kim, R. R. Naik, B. G. Sumpter, H. Terrones, F. Xia, Y. Wang, J. Zhu, D. Akinwande, N. Alem, J. A. Schuller, R. E. Schaak, M. Terrones, and J. A. Robinson. Recent advances in two-dimensional materials beyond graphene. ACS Nano, 9(12):11509–11539, 2015.

[44] A. Biﬃn, R. Johnson, I. Kimchi, R. Morris, a. Bombardi, J. Analytis, a. Vish- wanath, and R. Coldea. Noncoplanar and Counterrotating Incommensurate Mag- netic Order Stabilized by Kitaev Interactions in γ-Li2IrO3. Physical Review Letters, 113(19):197201, Nov. 2014. BIBLIOGRAPHY 102

[45] A. Biﬃn, R. D. Johnson, S. Choi, F. Freund, S. Manni, a. Bombardi, P. Manuel, P. Gegenwart, and R. Coldea. Unconventional magnetic order on the hyperhoneycomb Kitaev lattice in β-Li2IrO3. Physical Review B, 90(20):205116, Nov. 2014. [46] P. Bl¨ochl. Projector augmented-wave method. Physical Review B, 50(24), 1994. [47] S. Blundell. Magnetism in Condensed Matter (Oxford Master Series in Physics), chap- ter C.8. Oxford University Press, 2001. [48] S. Blundell. Magnetism in Condensed Matter (Oxford Master Series in Physics), chap- ter 4. Oxford University Press, 2001. [49] S. Blundell. Magnetism in Condensed Matter (Oxford Master Series in Physics), chap- ter 1. Oxford University Press, 2001. [50] P. J. Bonasia, G. P. Mitchell, F. J. Hollander, and J. Arnold. Synthesis and characteri- zation of copper(i) and silver(i) tellurolates and selenolates. the x-ray crystal structures of Cu[SeC(SiMe3)3]PCy32 and the homoleptic silver selenolate ag4[sec(sime3)3]4. In- organic Chemistry, 33(9):1797–1802, 1994. [51] W. Boomsma and J. Frellsen. Spherical convolutions and their application in molecular modelling. In I. Guyon, U. V. Luxburg, S. Bengio, H. Wallach, R. Fergus, S. Vish- wanathan, and R. Garnett, editors, Advances in Neural Information Processing Sys- tems 30, pages 3436–3446. Curran Associates, Inc., 2017. [52] M. Bremholm, S. Dutton, P. Stephens, and R. Cava. NaIrO3A pentavalent post- perovskite. Journal of Solid State Chemistry, 184(3):601–607, Mar. 2011. [53] L. Britnell, R. M. Ribeiro, A. Eckmann, R. Jalil, B. D. Belle, A. Mishchenko, Y. J. Kim, R. V. Gorbachev, T. Georgiou, S. V. Morozov, A. N. Grigorenko, A. K. Geim, C. Casiraghi, A. H. C. Neto, and K. S. Novoselov. Strong light-matter interactions in heterostructures of atomically thin ﬁlms. Science, 340(6138):1311–1314, 2013. [54] S. Z. Butler, S. M. Hollen, L. Cao, Y. Cui, J. A. Gupta, H. R. Gutierrez, T. F. Heinz, S. S. Hong, J. Huang, A. F. Ismach, E. Johnston-Halperin, M. Kuno, V. V. Plashnitsa, R. D. Robinson, R. S. Ruoﬀ, S. Salahuddin, J. Shan, L. Shi, M. G. Spencer, M. Terrones, W. Windl, and J. E. Goldberger. Progress, challenges, and opportunities in two-dimensional materials beyond graphene. Acs Nano, 7(4):2898–2926, 2013. [55] G. Cao, T. F. Qi, L. Li, J. Terzic, V. S. Cao, S. J. Yuan, M. Tovar, G. Murthy, and R. K. Kaul. Evolution of magnetism in the single-crystal honeycomb iridates (Na1−xLix)2IrO3. Physical Review B, 88(22):220414, Dec. 2013. [56] C. Capillas, E. Kroumova, M. I. Aroyo, J. M. Perez-Mato, H. T. Stokes, and D. M. Hatch. SYMMODES: a software package for group-theoretical analysis of structural phase transitions. Journal of Applied Crystallography, 36(3):953–954, may 2003. BIBLIOGRAPHY 103

[57] C. Capillas, E. S. Tasci, G. de la Flor, D. Orobengoa, J. M. Perez-Mato, and M. I. Aroyo. A new computer tool at the Bilbao Crystallographic Server to detect and characterize pseudosymmetry. Zeitschrift f¨urKristallographie, 226(2):186–196, 2011. [58] G. Ceder, Y.-M. Chiang, D. R. Sadoway, M. K. Aydinol, Y.-I. Jang, and B. Huang. Identiﬁcation of cathode materials for lithium batteries guided by ﬁrst-principles cal- culations. Nature, 392(6677):694–696, apr 1998. [59] J. Chaloupka, G. Jackeli, and G. Khaliullin. Kitaev-Heisenberg Model on a Honey- comb Lattice: Possible Exotic Phases in Iridium Oxides A2IrO3. Phys. Rev. Lett., 105:027204, Jul 2010. [60] P. Chandra and P. B. Littlewood. A Landau Primer for Ferroelectrics, pages 69–116. Springer Berlin Heidelberg, Berlin, Heidelberg, 2007. [61] R. Chen, H. C. Po, J. B. Neaton, and A. Vishwanath. Topological materials discovery using electron ﬁlling constraints. Nature Physics, 14(1):55–61, oct 2017. [62] S. Chmiela, A. Tkatchenko, H. E. Sauceda, I. Poltavsky, K. T. Sch¨utt,and K.-R. M¨uller.Machine learning of accurate energy-conserving molecular force ﬁelds. Science Advances, 3(5), 2017. [63] S. K. Choi, R. Coldea, A. N. Kolmogorov, T. Lancaster, I. I. Mazin, S. J. Blundell, P. G. Radaelli, Y. Singh, P. Gegenwart, K. R. Choi, S.-W. Cheong, P. J. Baker, C. Stock, and J. Taylor. Spin Waves and Revised Crystal Structure of Honeycomb Iridate Na 2 IrO 3 . Physical Review Letters, 108(12):127204, Mar. 2012. { } { } [64] S. K. Choi, R. Coldea, a. N. Kolmogorov, T. Lancaster, I. I. Mazin, S. J. Blundell, P. G. Radaelli, Y. Singh, P. Gegenwart, K. R. Choi, S.-W. Cheong, P. J. Baker, C. Stock, and J. Taylor. Spin Waves and Revised Crystal Structure of Honeycomb Iridate Na2IrO3. Physical Review Letters, 108(12):127204, Mar. 2012. [65] T. Cohen, M. Geiger, J. K¨ohler,and M. Welling. Spherical CNNs. International Conference on Learning Representations, 2018. [66] T. Cohen and M. Welling. Group equivariant convolutional networks. In Proceedings of the International Conference on Machine Learning (ICML), 2016. [67] T. Cohen and M. Welling. Steerable CNNs. In International Conference on Learning Representations (ICLR), 2017. [68] J. F. Corrigan, O. Fuhr, and D. Fenske. Metal chalcogenide clusters on the border between molecules and materials. Advanced Materials, 21(18):1867–1871, 2009. [69] H. L. Cuthbert, A. I. Wallbank, N. J. Taylor, and J. F. Corrigan. Synthesis and Struc- tural Characterization of [Cu20Se4(3-SePh)12(PPh3)6] and [Ag(SePh)]∞. Zeitschrift fr anorganische und allgemeine Chemie, 628(11):2483–2488, 2002. BIBLIOGRAPHY 104

[70] I. G. Dance, K. J. Fisher, R. M. H. Banda, and M. L. Scudder. Layered structure of crystalline compounds silver thiolates (agsr). Inorganic Chemistry, 30(2):183–187, 1991. doi: 10.1021/ic00002a008.

[71] M. de Jong, W. Chen, H. Geerlings, M. Asta, and K. A. Persson. A database to enable discovery and design of piezoelectric materials. Scientiﬁc Data, 2:150053, 2015.

[72] K. Deguchi, K. Hasebe, K. Gesi, and T. Asahi. 39A-1 (NH4) 2SO4 [F]. In Inorganic Substances other than Oxides, pages 1–53. Springer.

[73] K. Deguchi, K. Hasebe, K. Gesi, and T. Asahi. 39A-16 K2ZnBr4 [F]. In Inorganic Substances other than Oxides, pages 1–10. Springer.

[74] K. Deguchi, K. Hasebe, K. Gesi, and T. Asahi. 39A-2 K2SeO4 [F]. In Inorganic Substances other than Oxides, pages 1–39. Springer.

[75] K. Deguchi, K. Hasebe, K. Gesi, and T. Asahi. 39A-7 Rb2CoCl4 [F]. In Inorganic Substances other than Oxides, pages 1–15. Springer.

[76] K. Deguchi, K. Hasebe, K. Gesi, and T. Asahi. 39A-9 K2ZnCl4 [F]. In Inorganic Substances other than Oxides, pages 1–32. Springer.

[77] K. Deguchi, K. Hasebe, K. Gesi, and T. Asahi. 39A-10 Rb2ZnCl4 [F]. In Inorganic Substances other than Oxides, pages 1–51. Springer, 2005.

[78] S. Dehnen, A. Eichhfer, and D. Fenske. Chalcogen-bridged copper clusters. European Journal of Inorganic Chemistry, 2002(2):279–317, 2002.

[79] M. Dion, H. Rydberg, E. Schrder, D. C. Langreth, and B. I. Lundqvist. Van der waals density functional for general geometries. Physical Review Letters, 92(24):246401, 2004. PRL.

[80] L. Dou, A. B. Wong, Y. Yu, M. Lai, N. Kornienko, S. W. Eaton, A. Fu, C. G. Bischak, J. Ma, T. Ding, N. S. Ginsberg, L.-W. Wang, A. P. Alivisatos, and P. Yang. Atomically thin two-dimensional organic-inorganic hybrid perovskites. Science, 349(6255):1518– 1521, 2015.

[81] S. L. Dudarev, S. Y. Savrasov, C. J. Humphreys, and a. P. Sutton. Electron-energy- loss spectra and the structural stability of nickel oxide:An LSDA+U study. Physical Review B, 57(3):1505–1509, 1998.

[82] I. Dzyaloshinsky. A thermodynamic theory of weak ferromagnetism of antiferromag- netics. Journal of Physics and Chemistry of Solids, 4(4):241–255, 1958. BIBLIOGRAPHY 105

[83] F. A. Faber, L. Hutchison, B. Huang, J. Gilmer, S. S. Schoenholz, G. E. Dahl, O. Vinyals, S. Kearnes, P. F. Riley, and O. A. von Lilienfeld. Prediction errors of molecular machine learning models lower than hybrid DFT error. Journal of Chemical Theory and Computation.

[84] L. J. Farrugia. W inGX and ORTEP for Windows: an update. Journal of Applied Crystallography, 45(4):849–854, Aug 2012.

[85] A. Fonari and C. Sutton. Eﬀective mass calculator for semiconductors. http:// afonari.com/emc/. [86] K. F. Garrity. High-throughput ﬁrst-principles search for new ferroelectrics. Phys. Rev. B, 97:024115, Jan 2018.

[87] K. F. Garrity, K. M. Rabe, and D. Vanderbilt. Hyperferroelectrics: Proper Ferro- electrics with Persistent Polarization. Phys. Rev. Lett., 112:127601, Mar 2014.

[88] A. K. Geim and I. V. Grigorieva. Van der waals heterostructures. Nature, 499(7459):419–425, 2013.

[89] J. Gilmer, S. S. Schoenholz, P. F. Riley, O. Vinyals, and G. E. Dahl. Neural message passing for quantum chemistry. In D. Precup and Y. W. Teh, editors, Proceedings of the 34th International Conference on Machine Learning, volume 70 of Proceedings of Machine Learning Research, pages 1263–1272, International Convention Centre, Sydney, Australia, 06–11 Aug 2017. PMLR.

[90] R. Gilmore. Lie groups, physics, and geometry: An introduction for physicists, engi- neers and chemists. Cambridge University Press, 2008.

[91] P. A. Goddard, J. Singleton, P. Sengupta, R. D. McDonald, T. Lancaster, S. J. Blundell, F. L. Pratt, S. Cox, N. Harrison, J. L. Manson, H. I. Southerland, and J. A. Schlueter. Experimentally determining the exchange parameters of quasi-two- dimensional heisenberg magnets. New Journal of Physics, 10(8):083025, Aug. 2008.

[92] R. G´omez-Bombarelli, J. N. Wei, D. Duvenaud, J. M. Hern´andez-Lobato,B. S´anchez- Lengeling, D. Sheberla, J. Aguilera-Iparraguirre, T. D. Hirzel, R. P. Adams, and A. Aspuru-Guzik. Automatic chemical design using a data-driven continuous rep- resentation of molecules. ACS Central Science, 0(0):null, 0.

[93] D. M. Gonzalez, M. Volpi, N. Komodakis, and D. Tuia. Rotation equivariant vector ﬁeld networks. CoRR, abs/1612.09346, 2016.

[94] I. Goodfellow, Y. Bengio, and A. Courville. Deep Learning. MIT Press, 2016. http: //www.deeplearningbook.org. BIBLIOGRAPHY 106

[95] R. Goodman and N. R. Wallach. Representations and invariants of the classical groups, volume 68. Cambridge University Press, 1998.

[96] H. Gretarsson, J. P. Clancy, X. Liu, J. P. Hill, E. Bozin, Y. Singh, S. Manni, P. Gegen- wart, J. Kim, A. H. Said, D. Casa, T. Gog, M. H. Upton, H.-S. Kim, J. Yu, V. M. Katukuri, L. Hozoi, J. van den Brink, and Y.-J. Kim. Crystal-Field Splitting and Cor- relation Eﬀect on the Electronic Structure of A2IrO3. Phys. Rev. Lett., 110:076402, Feb 2013.

[97] H. Gretarsson, J. P. Clancy, Y. Singh, P. Gegenwart, J. P. Hill, J. Kim, M. H. Upton, A. H. Said, D. Casa, T. Gog, and Y.-J. Kim. Magnetic excitation spectrum of Na2IrO3 probed with resonant inelastic x-ray scattering. Physical Review B, 87(22):220407, June 2013.

[98] D. J. Griﬃths. Introduction to quantum mechanics. Cambridge University Press, 2017.

[99] S. A. Grigera, R. S. Perry, A. J. Schoﬁeld, M. Chiao, S. R. Julian, G. G. Lonzarich, S. I. Ikeda, Y. Maeno, A. J. Millis, and A. P. Mackenzie. Magnetic ﬁeld-tuned quantum criticality in the metallic ruthenate Sr3Ru2O7. Science, 294(5541):329–332, Oct. 2001. PMID: 11598292.

[100] M. D. Hanwell, D. E. Curtis, D. C. Lonie, T. Vandermeersch, E. Zurek, and G. R. Hutchison. Avogadro: an advanced semantic chemical editor, visualization, and anal- ysis platform. Journal of Cheminformatics, 4(1):17, 2012.

[101] L. Hedin. New method for calculating the one-particle green’s function with application to the electron-gas problem. Physical Review, 139(3A):A796–A823, 1965. PR.

[102] C. H. Hendon, D. Tiana, T. P. Vaid, and A. Walsh. Thermodynamic and electronic properties of tunable II-VI and IV-VI semiconductor based metal-organic frameworks from computational chemistry. Journal of Materials Chemistry C, 1(1):95–100, 2013.

[103] J. Heyd and G. E. Scuseria. Eﬃcient hybrid density functional calculations in solids: Assessment of the heyd–scuseria–ernzerhof screened coulomb hybrid functional. The Journal of Chemical Physics, 121(3):1187–1192, jul 2004.

[104] J. Heyd, G. E. Scuseria, and M. Ernzerhof. Hybrid functionals based on a screened coulomb potential. The Journal of Chemical Physics, 118(18):8207–8215, may 2003.

[105] J. Heyd, G. E. Scuseria, and M. Ernzerhof. Erratum: “hybrid functionals based on a screened coulomb potential” [j. chem. phys. 118, 8207 (2003)]. The Journal of Chemical Physics, 124(21):219906, jun 2006.

[106] T. Hikita. 35A-13 TlTiOPO4 [(F)]. In Inorganic Substances other than Oxides. Part 1: SbSI family... TAAP, pages 1–9. Springer. BIBLIOGRAPHY 107

[107] D. Hobbs and J. Hafner. Ab initio density functional study of phase stability and noncollinear magnetism in Mn. Journal of Physics: Condensed Matter, 13:L681–L688, 2001.

[108] D. Hobbs, G. Kresse, and J. Hafner. Fully unconstrained noncollinear magnetism within the projector augmented-wave method. Physical Review B, 62(17):11556–11570, Nov. 2000.

[109] P. Hohenberg and W. Kohn. Inhomogeneous electron gas. Phys. Rev., 136:B864–B871, Nov 1964.

[110] L. Hu, L. P. de la Rama, M. Y. Efremov, Y. Anahory, F. Schiettekatte, and L. H. Allen. Synthesis and characterization of single-layer silverdecanethiolate lamellar crystals. Journal of the American Chemical Society, 133(12):4367–4376, 2011.

[111] X. Huang, Heulings, V. Le, and J. Li. Inorganicorganic hybrid composites containing mq (iivi) slabs: a new class of nanostructures with strong quantum conﬁnement and periodic arrangement. Chemistry of Materials, 13(10):3754–3759, 2001.

[112] X. Huang and J. Li. From single to multiple atomic layers: a unique approach to the systematic tuning of structures and properties of inorganicorganic hybrid nanostruc- tured semiconductors. Journal of the American Chemical Society, 129(11):3157–3162, 2007.

[113] X. Huang, J. Li, and H. Fu. The ﬁrst covalent organicinorganic networks of hybrid chalcogenides: structures that may lead to a new type of quantum wells. Journal of the American Chemical Society, 122(36):8789–8790, 2000.

[114] J. Hubbard. Electron correlations in narrow energy bands III. an improved solution. 281(1386):401–419, 1964.

[115] S. Hwan Chun, J.-W. Kim, J. Kim, H. Zheng, C. Stoumpos, C. Malliakas, J. Mitchell, K. Mehlawat, Y. Singh, Y. Choi, T. Gog, a. Al-Zein, M. Sala, M. Krisch, J. Chaloupka, G. Jackeli, G. Khaliullin, and B. J. Kim. Direct evidence for dominant bond-directional interactions in a honeycomb lattice iridate Na2IrO3. Nature Physics, 11(May), 2015.

[116] E. S¸a¸sıo˘glu,C. Friedrich, and S. Bl¨ugel. Eﬀective coulomb interaction in transition metals from constrained random-phase approximation. Phys. Rev. B, 83:121101, Mar 2011.

[117] J. M. Igartua, M. I. Aroyo, E. Kroumova, and J. M. Perez-Mato. Search for Pnma materials with high-temperature structural phase transitions. Acta Crystallographica Section B Structural Science, 55(2):177–185, 1999. BIBLIOGRAPHY 108

[118] G. Jackeli and G. Khaliullin. Mott insulators in the strong spin-orbit coupling limit: From heisenberg to a quantum compass and kitaev models. Physical Review Letters, 102(1):017205, Jan. 2009.

[119] G. Jackeli and G. Khaliullin. Mott insulators in the strong spin-orbit coupling limit: From heisenberg to a quantum compass and kitaev models. Phys. Rev. Lett., 102:017205, Jan 2009.

[120] G. Jackeli and G. Khaliullin. Mott Insulators in the Strong Spin-Orbit Coupling Limit: From Heisenberg to a Quantum Compass and Kitaev Models. Physical Review Letters, 102(1):017205, Jan. 2009.

[121] A. Jain, G. Hautier, C. J. Moore, S. Ping Ong, C. C. Fischer, T. Mueller, K. A. Persson, and G. Ceder. A high-throughput infrastructure for density functional theory calculations. Computational Materials Science, 50(8):2295–2310, 2011.

[122] A. Jain, G. Hautier, S. P. Ong, C. J. Moore, C. C. Fischer, K. A. Persson, and G. Ceder. Formation enthalpies by mixing GGA and GGA + U calculations. Physical Review B - Condensed Matter and Materials Physics, 84(4):1–10, 2011.

[123] A. Jain, S. P. Ong, W. Chen, B. Medasani, X. Qu, M. Kocher, M. Brafman, G. Petretto, G.-M. Rignanese, G. Hautier, D. Gunter, and K. A. Persson. FireWorks: a dynamic workﬂow system designed for high-throughput applications. Concurrency Computation Practice and Experience, 27:5037–5059, 2015.

[124] A. Jain, S. P. Ong, G. Hautier, W. Chen, W. D. Richards, S. Dacek, S. Cholia, D. Gunter, D. Skinner, G. Ceder, and K. a. Persson. The Materials Project: A materi- als genome approach to accelerating materials innovation. APL Materials, 1(1):011002, 2013.

[125] H. Kay and P. Vousden. Xcv. symmetry changes in barium titanate at low temperatures and their relation to its ferroelectric properties. The London, Edinburgh, and Dublin Philosophical Magazine and Journal of Science, 40(309):1019–1040, 1949.

[126] S. Kearnes, K. McCloskey, M. Berndl, V. Pande, and P. Riley. Molecular graph con- volutions: moving beyond ﬁngerprints. Journal of Computer-Aided Molecular Design, 30(8):595–608, Aug 2016.

[127] I. Kimchi, J. G. Analytis, and A. Vishwanath. Three dimensional quantum spin liquid in 3d-honeycomb iridate models and phase diagram in an inﬁnite-d approximation. arXiv e-print 1309.1171, Sept. 2013.

[128] R. D. King-Smith and D. Vanderbilt. Theory of polarization of crystalline solids. Phys. Rev. B, 47:1651–1654, Jan 1993. BIBLIOGRAPHY 109

[129] R. D. King-Smith and D. Vanderbilt. Theory of polarization of crystalline solids. Physical Review B, 47(3):1651–1654, jan 1993. [130] A. Kitaev. Anyons in an exactly solved model and beyond. Annals of Physics, 321(1):2– 111, Jan. 2006. [131] R. Kleﬀner, J. Flatten, A. Leaver-Fay, D. Baker, J. B. Siegel, F. Khatib, and S. Cooper. Foldit standalone: a video game-derived protein structure manipulation interface using rosetta. Bioinformatics, 33(17):2765–2767, may 2017. [132] W. Kohn. Nobel lecture: Electronic structure of matter—wave functions and density functionals. Rev. Mod. Phys., 71:1253–1266, Oct 1999. [133] W. Kohn and L. J. Sham. Self-consistent equations including exchange and correlation eﬀects. Phys. Rev., 140:A1133–A1138, Nov 1965. [134] R. Kondor, H. Truong Son, H. Pan, B. Anderson, and S. Trivedi. Covariant composi- tional networks for learning graphs. ArXiv e-prints, Jan. 2018. [135] G. Kresse and J. Furthm¨uller.Eﬃciency of ab-initio total energy calculations for metals and semiconductors using a plane-wave basis set. Computational Materials Science, 6(1):15–50, 1996. [136] G. Kresse and J. Furthm¨uller. Eﬃcient iterative schemes for ab initio total-energy calculations using a plane-wave basis set. Physical Review B, 54(16), 1996. [137] G. Kresse and J. Hafner. Ab initio molecular dynamics for liquid metals. Physical Review B, 47(1):558–561, 1993. [138] G. Kresse and D. Jourbert. From ultrasoft pseudopotentials to the projector augmented-wave method. Physical Review B, 59(3):1758–1775, 1999. [139] E. Kroumova, M. I. Aroyo, and J. M. Perez-Mato. Prediction of new displacive ferroelectrics through systematic pseudosymmetry search. Results for materials with Pba 2 and Pmc 2 1 symmetry. Acta Crystallographica Section B Structural Science, 58(6):921–933, 2002. [140] A. V. Krukau, O. A. Vydrov, A. F. Izmaylov, and G. E. Scuseria. Inﬂuence of the exchange screening parameter on the performance of screened hybrid functionals. The Journal of Chemical Physics, 125(22):224106, dec 2006. [141] A. V. Krukau, O. A. Vydrov, A. F. Izmaylov, and G. E. Scuseria. Inﬂuence of the exchange screening parameter on the performance of screened hybrid functionals. The Journal of Chemical Physics, 125(22):224106, 2006. [142] L. D. Landau and E. M. Lifshitz. Mechanics, volume 1 of Course of Theoretical Physics. Elsevier, 1976. BIBLIOGRAPHY 110

[143] C. Lavenn, N. Guillou, M. Monge, D. Podbevsek, G. Ledoux, A. Fateeva, and A. Demessence. Shedding light on an ultra-bright photoluminescent lamellar gold thiolate coordination polymer [Au(p-SPhCO2Me)]n. Chemical Communications, 52(58):9063–9066, 2016.

[144] A. I. Lebedev. Ferroelectric phase transition in orthorhombic CdTiO3: First-principles studies. Physics of the Solid State, 51(4):802–809, Apr 2009.

[145] D. Lebeugle, D. Colson, A. Forget, and M. Viret. Very large spontaneous electric polarization in BiFeO3 single crystals at room temperature and its evolution under cycling ﬁelds. Applied Physics Letters, 91(2):022907, 2007.

[146] E. K.-H. Lee, R. Schaﬀer, S. Bhattacharjee, and Y. B. Kim. Heisenberg-kitaev model on hyper-honeycomb lattice. arXiv e-print 1308.6592, Aug. 2013.

[147] K. Lee, E. D. Murray, L. Kong, B. I. Lundqvist, and D. C. Langreth. Higher-accuracy van der waals density functional. Physical Review B, 82(8):081101, 2010. PRB.

[148] A. J. Leggett. Cuprate superconductivity: Dependence of t c on the c-axis layering structure. Physical Review Letters, 83(2):392–395, July 1999.{ }

[149] J. Li, Z. Yang, H. Liu, and D. Cai. Deep Rotation Equivariant Network. ArXiv e-prints, May 2017.

[150] Y. Li, K. Foyevtsova, H. O. Jeschke, and R. Valent´ı.Analysis of the optical conductivity for A2IrO3 (A = Na,Li) from ﬁrst principles. Physical Review B, 91(16):161101, 2015. [151] Y.-C. Lin, R. K. Ghosh, R. Addou, N. Lu, S. M. Eichfeld, H. Zhu, M.-Y. Li, X. Peng, M. J. Kim, L.-J. Li, R. M. Wallace, S. Datta, and J. A. Robinson. Atomically thin res- onant tunnel diodes built from synthetic van der waals heterostructures. Nat Commun, 6, 2015.

[152] M. E. Lines and A. M. Glass. Basic Concepts, chapter 1. Oxford University Press, Oxford, 2001.

[153] M. E. Lines and A. M. Glass. Domains, Imperfections, And Polarization Reversal, pages 87–126. Oxford University Press, Feb 2001.

[154] M. E. Lines and A. M. Glass. Principles and Applications of Ferroelectrics and Related Materials. Oxford University Press, Feb 2001.

[155] X. Liu, T. Berlijn, W.-G. Yin, W. Ku, a. Tsvelik, Y.-J. Kim, H. Gretarsson, Y. Singh, P. Gegenwart, and J. P. Hill. Long-range magnetic ordering in Na2IrO3 . Physical Review B, 83(22):220403, June 2011. BIBLIOGRAPHY 111

[156] T. Low, A. Chaves, J. D. Caldwell, A. Kumar, N. X. Fang, P. Avouris, T. F. Heinz, F. Guinea, L. Martin-Moreno, and F. Koppens. Polaritons in layered two-dimensional materials. Nat Mater, 16(2):182–194, 2017.

[157] A. O. Lyakhov, A. R. Oganov, H. T. Stokes, and Q. Zhu. New developments in evolu- tionary structure prediction algorithm USPEX. Computer Physics Communications, 184(4):1172–1182, apr 2013.

[158] P.-W. Ma and S. L. Dudarev. Constrained density functional for noncollinear mag- netism. Physical Review B, 91(5):054420, 2015.

[159] K. F. Mak, C. Lee, J. Hone, J. Shan, and T. F. Heinz. Atomically thin mos2: A new direct-gap semiconductor. Physical Review Letters, 105(13):136805, 2010. PRL.

[160] S. Mandal and N. Surendran. Exactly solvable kitaev model in three dimensions. Physical Review B, 79(2):024426, Jan. 2009.

[161] S. Manni, S. Choi, I. I. Mazin, R. Coldea, M. Altmeyer, H. O. Jeschke, R. Valent´ı,and P. Gegenwart. Eﬀect of isoelectronic doping on the honeycomb-lattice iridate A2IrO3. Physical Review B, 89(24):245113, June 2014.

[162] R. M. Martin. Electronic Structure: Basic Theory and Practical Methods, chapter 3. Cambridge University Press, 2012.

[163] R. M. Martin. Electronic Structure: Basic Theory and Practical Methods, chapter 6-9. Cambridge University Press, 2012.

[164] R. M. Martin. Electronic Structure: Basic Theory and Practical Methods, chapter 8. Cambridge University Press, 2012.

[165] K. Mathew, J. H. Montoya, A. Faghaninia, S. Dwarakanath, M. Aykol, H. Tang, I. heng Chu, T. Smidt, B. Bocklund, M. Horton, J. Dagdelen, B. Wood, Z.-K. Liu, J. Neaton, S. P. Ong, K. Persson, and A. Jain. Atomate: A high-level interface to generate, exe- cute, and analyze computational materials science workﬂows. Computational Materials Science, 139(Supplement C):140 – 152, 2017.

[166] I. I. Mazin, H. O. Jeschke, K. Foyevtsova, R. Valent´ı,and D. I. Khomskii. Na2IrO3 as a Molecular Orbital Crystal. Physical Review Letters, 109(19):197201, Nov. 2012.

[167] I. I. Mazin, S. Manni, K. Foyevtsova, H. O. Jeschke, P. Gegenwart, and R. Valent´ı. Origin of the insulating state in honeycomb iridates and rhodates. Phys. Rev. B, 88:035115, Jul 2013.

[168] I. I. Mazin, S. Manni, K. Foyevtsova, H. O. Jeschke, P. Gegenwart, and R. Valent´ı. Origin of the insulating state in honeycomb iridates and rhodates. Physical Review B, 88(3):035115, July 2013. BIBLIOGRAPHY 112

[169] I. I. Mazin and D. J. Singh. Competitions in layered ruthenates: Ferromagnetism versus antiferromagnetism and triplet versus singlet pairing. Physical Review Letters, 82(21):4324–4327, May 1999. [170] N. D. Mermin and H. Wagner. Absence of ferromagnetism or antiferromagnetism in one- or two-dimensional isotropic heisenberg models. Physical Review Letters, 17(22):1133–1136, Nov. 1966. [171] A. I. Mihut, L. E. Spring, R. I. Bewley, S. J. Blundell, W. Hayes, T. Jestdt, B. W. Lovett, R. McDonald, F. L. Pratt, J. Singleton, P. D. Battle, J. Lago, M. J. Rosseinsky, and J. F. Vente. Physical properties of the n=3 ruddlesden - popper compound. Journal of Physics: Condensed Matter, 10(45):L727, Nov. 1998. [172] K. A. Modic, T. E. Smidt, I. Kimchi, N. P. Breznay, A. Biﬃn, S. Choi, R. D. Johnson, R. Coldea, P. Watkins-Curry, G. T. McCandless, J. Y. Chan, F. Gandara, Z. Islam, A. Vishwanath, A. Shekhter, R. D. McDonald, and J. G. Analytis. Realization of a three-dimensional spin-anisotropic harmonic honeycomb iridate. Nature communica- tions, 5(May):4203, Jan. 2014. [173] K. Momma and F. Izumi. Vesta: a three-dimensional visualization system for electronic and structural analysis. Journal of Applied Crystallography, 41(3):653–658, 2008. [174] K. Momma and F. Izumi. V ESTA3 for three-dimensional visualization of crystal, volumetric and morphology data. Journal of Applied Crystallography, 44(6):1272–1276, Dec 2011. [175] H. J. Monkhorst and J. D. Pack. Special points for brillouin-zone integrations. Phys- ical Review B, 13(12):5188–5192, 1976. Phys. Rev. B ISI Document Delivery No.: BV088 Times Cited: 8161 Cited Reference Count: 6 AMERICAN PHYSICAL SOC COLLEGE PK. [176] T. Moriya. Anisotropic superexchange interaction and weak ferromagnetism. Physical Review, 120(1):91–98, Oct. 1960. [177] P. Muller. Crystal structure reﬁnement: A crystallographer’s guide to shelxl. page 213, Jul 2006. [178] U. M¨uller. Symmetry relations at phase transitions, pages 196–215. Oxford University Press, apr 2013. [179] U. M¨uller. Symmetry Relationships between Crystal Structures. Oxford University Press, apr 2013. [180] J. B. Neaton, C. Ederer, U. V. Waghmare, N. A. Spaldin, and K. M. Rabe. First- principles study of spontaneous polarization in multiferroic BiFeO3. Phys. Rev. B, 71:014113, Jan 2005. BIBLIOGRAPHY 113

[181] A. R. Oganov, A. O. Lyakhov, and M. Valle. How evolutionary crystal structure prediction works—and why. Accounts of Chemical Research, 44(3):227–237, mar 2011.

[182] D. Ohlmann, H. Pritzkow, H. Grutzmacher, M. Anthamatten, and R. Glaser. A hex- anuclear copper arylselenolate: synthesis, structure and proposal for its rearrangement. Journal of the Chemical Society, Chemical Communications, (10):1011–1012, 1995.

[183] E. Ohmichi and T. Osada. Torque magnetometry in pulsed magnetic ﬁelds with use of a commercial microcantilever. Review of Scientiﬁc Instruments, 73(8):3022–3026, Aug. 2002.

[184] Y. Okada, D. Walkup, H. Lin, C. Dhital, T.-R. Chang, S. Khadka, W. Zhou, H.-T. Jeng, M. Paranjape, A. Bansil, Z. Wang, S. D. Wilson, and V. Madhavan. Imaging the evolution of metallic states in a correlated iridate. Nature materials, 12(8):707–13, Aug. 2013.

[185] Y. Okamoto, M. Nohara, H. Aruga-Katori, and H. Takagi. Spin-liquid state in the s=1/2 hyperkagome antiferromagnet na 4 ir 3 o 8 . Physical Review Letters, 99(13):137207, Sept. 2007. { } { } { }

[186] S. P. Ong, S. Cholia, A. Jain, M. Brafman, D. Gunter, G. Ceder, and K. A. Persson. The materials application programming interface (API): A simple, ﬂexible and eﬃcient API for materials data based on REpresentational state transfer (REST) principles. Computational Materials Science, 97:209–215, feb 2015.

[187] S. P. Ong, W. D. Richards, A. Jain, G. Hautier, M. Kocher, S. Cholia, D. Gunter, V. L. Chevrier, K. a. Persson, and G. Ceder. Python Materials Genomics (pymatgen): A robust, open-source python library for materials analysis. Computational Materials Science, 68:314–319, 2013.

[188] S. P. Ong, W. D. Richards, A. Jain, G. Hautier, M. Kocher, S. Cholia, D. Gunter, V. L. Chevrier, K. a. Persson, and G. Ceder. Python Materials Genomics (pymatgen): A robust, open-source python library for materials analysis. Computational Materials Science, 68:314–319, 2013.

[189] M. J. OMalley, H. Verweij, and P. M. Woodward. Structure and properties of ordered Li2IrO3 and Li2PtO3. Journal of Solid State Chemistry, 181(8):1803–1809, Aug. 2008.

[190] M. J. OMalley, H. Verweij, and P. M. Woodward. Structure and properties of ordered Li2IrO3 and Li2PtO3. Journal of Solid State Chemistry, 181(8):1803–1809, Aug. 2008.

[191] A. N. Parikh, S. D. Gillmor, J. D. Beers, K. M. Beardmore, R. W. Cutts, and B. I. Swanson. Characterization of chain molecular assemblies in long-chain, layered silver thiolates: A joint infrared spectroscopy and x-ray diﬀraction study. The Journal of Physical Chemistry B, 103(15):2850–2861, 1999. doi: 10.1021/jp983938b. BIBLIOGRAPHY 114

[192] R. Penrose. Applications of negative dimensional tensors. In Combinatorial Mathe- matics and its Applications. Academic Press, 1971. [193] J. Perdew, K. Burke, and M. Ernzerhof. Generalized Gradient Approximation Made Simple. Physical review letters, 77(18):3865–3868, Oct. 1996. [194] J. M. Perez-Mato, R. L. Withers, A. K. Larsson, D. Orobengoa, and Y. Liu. Distortion modes and related ferroic properties of the stuﬀed tridymite-type compounds SrAl2O4 and BaAl2O4. Physical Review B - Condensed Matter and Materials Physics, 79(6):1– 12, 2009. [195] C. J. Pickard and R. J. Needs. Ab initiorandom structure searching. Journal of Physics: Condensed Matter, 23(5):053201, jan 2011. [196] A. K. Pradhan, K. Zhang, D. Hunter, J. B. Dadson, G. B. Loiutts, P. Bhattacharya, R. Katiyar, J. Zhang, D. J. Sellmyer, U. N. Roy, Y. Cui, and A. Burger. Magnetic and electrical properties of single-phase multiferroic BiFeO3. Journal of Applied Physics, 97(9):093903, 2005. [197] C. R. Qi, H. Su, K. Mo, and L. J. Guibas. PointNet: Deep learning on point sets for 3D classiﬁcation and segmentation. arXiv preprint arXiv:1612.00593, 2016. [198] C. R. Qi, L. Yi, H. Su, and L. J. Guibas. PointNet++: Deep hierarchical feature learning on point sets in a metric space. arXiv preprint arXiv:1706.02413, 2017. [199] D. Y. Qiu, F. H. da Jornada, and S. G. Louie. Optical spectrum of mos2: Many-body eﬀects and diversity of exciton states. Physical Review Letters, 111(21):216805, 2013. PRL. [200] K. M. Rabe. Antiferroelectricity in Oxides: A Reexamination. In Functional Metal Oxides, pages 221–244. Wiley-VCH Verlag GmbH & Co. KGaA, jul 2013. [201] K. M. Rabe, M. Dawber, C. Lichtensteiger, C. H. Ahn, and J.-M. Triscone. Modern physics of ferroelectrics: Essential background. In Physics of Ferroelectrics: A Modern Perspective, pages 1–30. Springer Berlin Heidelberg. [202] R. Ramakrishnan, P. O. Dral, M. Rupp, and O. A. von Lilienfeld. Quantum chemistry structures and properties of 134 kilo molecules. Scientiﬁc Data, 1, 2014. [203] R. Ramakrishnan, P. O. Dral, M. Rupp, and O. A. von Lilienfeld. Quantum chemistry structures and properties of 134 kilo molecules. Scientiﬁc Data, 1, 2014. [204] M. Reisert and H. Burkhardt. Spherical tensor calculus for local adaptive ﬁltering. Tensors in Image Processing and Computer Vision, pages 153–178, 2009. [205] R. Resta. Theory of the electric polarization in crystals. Ferroelectrics, 136(1):51–55, nov 1992. BIBLIOGRAPHY 115

[206] R. Resta. Macroscopic polarization in crystalline dielectrics: the geometric phase approach. Reviews of Modern Physics, 66(3):899–915, jul 1994.

[207] R. Resta. Berry phase in electronic wavefunctions. Troisime Cycle de la Physique en Suisse Romande, pages 899–915, Anne Academique 1995-1996.

[208] R. Resta and D. Vanderbilt. Theory of Polarization: A Modern Approach, pages 31–68. Springer Berlin Heidelberg, Berlin, Heidelberg, 2007.

[209] J. Reuther, R. Thomale, and S. Rachel. Spiral order in the honeycomb iridate Li2IrO3. Physical Review B, 90(10):100405, Sept. 2014.

[210] J. Rodriguez-Carvajal. Recent advances in magnetic structure determination by neu- tron powder diﬀraction. Physica B: Condensed Matter (Amsterdam), 192:55, Oct 1993.

[211] M. Rohlﬁng and S. G. Louie. Electron-hole excitations in semiconductors and insula- tors. Physical Review Letters, 81(11):2312–2315, 1998. PRL.

[212] M. Rohlﬁng and S. G. Louie. Electron-hole excitations and optical spectra from ﬁrst principles. Physical Review B, 62(8):4927–4944, 2000. PRB.

[213] K. Rolfs, S. Toth, E. Pomjakushina, D. Sheptyakov, J. Taylor, and K. Conder. Spiral magnetic phase in Li-doped Na2IrO3. Physical Review B, 91(18):5–8, 2015. [214] G. Rom´an-P´erezand J. M. Soler. Eﬃcient implementation of a van der waals density functional: Application to double-wall carbon nanotubes. Physical Review Letters, 103(9):096102, 2009. PRL.

[215] L. Ruddigkeit, R. van Deursen, L. C. Blum, and J.-L. Reymond. Enumeration of 166 billion organic small molecules in the chemical universe database GDB-17. Journal of Chemical Information and Modeling, 52(11):2864–2875, nov 2012.

[216] A. Sahu, A. Khare, D. D. Deng, and D. J. Norris. Quantum conﬁnement in silver selenide semiconductor nanocrystals. Chemical Communications, 48(44):5458–5460, 2012.

[217] L. M. Sandratskii and J. K¨ubler.Non-collinear magnetism: eﬀects of symmetry and relativity. Modern Physics Letters, 10(189), 1996.

[218] J. Schindelin, I. Arganda-Carreras, E. Frise, V. Kaynig, M. Longair, T. Pietzsch, S. Preibisch, C. Rueden, S. Saalfeld, B. Schmid, J.-Y. Tinevez, D. J. White, V. Harten- stein, K. Eliceiri, P. Tomancak, and A. Cardona. Fiji: an open-source platform for biological-image analysis. Nat Meth, 9(7):676–682, 2012. 10.1038/nmeth.2019.

[219] H. Schmidbaur and A. Schier. Argentophilic interactions. Angewandte Chemie Inter- national Edition, 54(3):746–784, 2015. BIBLIOGRAPHY 116

[220] H. Schmidt, F. Giustiniano, and G. Eda. Electronic transport properties of transition metal dichalcogenide ﬁeld-eﬀect devices: surface and interface eﬀects. Chemical Society Reviews, 44(21):7715–7736, 2015.

[221] K. T. Sch¨utt,F. Arbabzadah, S. Chmiela, K. R. M¨uller,and A. Tkatchenko. Quantum- chemical insights from deep tensor neural networks. 8:13890 EP –, Jan 2017. Article.

[222] K. T. Sch¨utt,P.-J. Kindermans, H. E. Sauceda, S. Chmiela, A. Tkatchenko, and K.- R. M¨uller. SchNet: A continuous-ﬁlter convolutional neural network for modeling quantum interactions. ArXiv e-prints, June 2017.

[223] K. T. Sch¨utt,H. E. Sauceda, P.-J. Kindermans, A. Tkatchenko, and K.-R. M¨uller. SchNet – a deep learning architecture for molecules and materials. The Journal of Chemical Physics, 148(24):241722, jun 2018.

[224] J. F. Scott. Searching for new ferroelectrics and multiferroics: A users point of view. npj Computational Materials, 1(July):15006, 2015.

[225] B. C. Server. Structure relations, 2018. http://www.cryst.ehu.es/cryst/rel.html. [226] Y. Shiozaki and T. Asahi. 50A-1: 1-6 SC (NH2) 2 [F]. In Organic crystals, liquid crystals and polymers, pages 1–48. Springer, 2006.

[227] Y. Shiozaki, E. Nakamura, and T. Mitsui, editors. Ferroelectrics and Related Sub- stances: Oxides Part 1: Perovskite-type Oxides and LiNbO3 Family. Springer-Verlag, 2001.

[228] Y. Shiozaki, E. Nakamura, and T. Mitsui, editors. Ferroelectrics and Related Sub- stances: Oxides Part 2: Oxides other than Perovskite-type and LiNbO3 Family. Springer-Verlag, 2002.

[229] Y. Shiozaki, E. Nakamura, and T. Mitsui, editors. Ferroelectrics and Related Sub- stances: SbSI family ... TAAP. Springer-Verlag, 2004.

[230] Y. Shiozaki, E. Nakamura, and T. Mitsui, editors. Ferroelectrics and Related Sub- stances: Organic crystals, liquid crystals and polymers. Springer Berlin Heidelberg, 2006.

[231] Y. Singh and P. Gegenwart. Antiferromagnetic Mott insulating state in single crystals of the honeycomb lattice material Na2IrO3. Physical Review B, 82(6):064412, Aug. 2010.

[232] Y. Singh and P. Gegenwart. Antiferromagnetic mott insulating state in single crystals of the honeycomb lattice material na 2 IrO 3 . Physical Review B, 82(6):064412, Aug. 2010. { } { } BIBLIOGRAPHY 117

[233] Y. Singh, S. Manni, J. Reuther, T. Berlijn, R. Thomale, W. Ku, S. Trebst, and P. Gegenwart. Relevance of the heisenberg-kitaev model for the honeycomb lattice iridates a2iro3. Phys. Rev. Lett., 108:127203, Mar 2012. [234] R. Skomski. Simple models of magnetism. Oxford University Press, Oxford New York, 2008.

[235] E. H. Smith, N. A. Benedek, and C. J. Fennie. Interplay of Octahedral Rotations and Lone Pair Ferroelectricity in CsPbF3. Inorganic Chemistry, 54(17):8536–8543, 2015. [236] J. S. Smith, O. Isayev, and A. E. Roitberg. ANI-1: An extensible neural network potential with DFT accuracy at force ﬁeld computational cost. Chem. Sci., 8:3192– 3203, 2017.

[237] M. Sofos, J. Goldberger, D. A. Stone, J. E. Allen, Q. Ma, D. J. Herman, W.-W. Tsai, L. J. Lauhon, and S. I. Stupp. A synergistic assembly of nanoscale lamellar photoconductor hybrids. Nature Materials, 8(1):68–75, 2009. 10.1038/nmat2336.

[238] N. A. Spaldin. A beginner’s guide to the modern theory of polarization. Journal of Solid State Chemistry, 195:2–10, 2012.

[239] G. L. Stamokostas and G. A. Fiete. Mixing of t2g-eg orbitals in 4d and 5d transition metal oxides. Physical Review B, 97(8), feb 2018.

[240] H. T. Stokes, D. M. Hatch, and B. J. Campbell. ISOTROPY Software Suite. iso. byu.edu. [241] H. T. Stokes, C. Sadate, D. M. Hatch, L. L. Boyer, and M. J. Mehl. Analysis of the ferroelectric phase transition in BaAl2O4 by group theoretical methods and ﬁrst- principles calculations. Physical Review B, 65(6):064105, 2002.

[242] T. Takayama, a. Kato, R. Dinnebier, J. Nuss, H. Kono, L. Veiga, G. Fabbris, D. Haskel, and H. Takagi. Hyperhoneycomb Iridate β-Li2IrO3 as a Platform for Kitaev Mag- netism. Physical Review Letters, 114(7):2–6, 2015.

[243] E. S. Tasci, G. de la Flor, and M. Aroyo. Obtaining the transformation matrix con- necting two group-subgroup related structures. http://sig9.ecanews.org/pdfs/19% 20Emre%20Tasci%20-%20Structure%20Relations.pdf.

[244] J. R. Teague, R. Gerson, and W. James. Dielectric hysteresis in single crystal BiFeO3. Solid State Communications, 8(13):1073 – 1074, 1970.

[245] H. Terauchi, K. Tanabe, H. Maeda, M. Hida, N. Kamijo, M. Takashige, T. Nakamura, H. Ozawa, and R. Uno. EXAFS Studies on Amorphous PbTiO3. Journal of the Physical Society of Japan, 50(12):3977–3979, 1981. BIBLIOGRAPHY 118

[246] N. Thomas, T. Smidt, S. Kearnes, L. Yang, L. Li, K. Kohlhoﬀ, and P. Riley. Tensor ﬁeld networks: Rotation- and translation-equivariant neural networks for 3d point clouds, 2018.

[247] P. Tol´edanoand M. Guennou. Theory of antiferroelectric phase transitions. Phys. Rev. B, 94:014107, Jul 2016.

[248] S. Tongay, H. Sahin, C. Ko, A. Luce, W. Fan, K. Liu, J. Zhou, Y.-S. Huang, C.-H. Ho, J. Yan, D. F. Ogletree, S. Aloni, J. Ji, S. Li, J. Li, F. M. Peeters, and J. Wu. Monolayer behaviour in bulk res2 due to electronic and vibrational decoupling. Nat Commun, 5, 2014.

[249] W. Torng and R. B. Altman. 3D deep convolutional neural networks for amino acid environment similarity analysis. BMC Bioinformatics, 18(1):302, Jun 2017.

[250] A. Toyo. spglib, 2018. https://atztogo.github.io/spglib/. [251] M.-L. Tsai, S.-H. Su, J.-K. Chang, D.-S. Tsai, C.-H. Chen, C.-I. Wu, L.-J. Li, L.-J. Chen, and J.-H. He. Monolayer mos2 heterojunction solar cells. ACS Nano, 8(8):8317– 8322, 2014.

[252] D. L. Turner, T. P. Vaid, P. W. Stephens, K. H. Stone, A. G. DiPasquale, and A. L. Rheingold. Semiconducting leadsulfurorganic network solids. Journal of the American Chemical Society, 130(1):14–15, 2008.

[253] M. M. Ugeda, A. J. Bradley, S.-F. Shi, F. H. da Jornada, Y. Zhang, D. Y. Qiu, W. Ruan, S.-K. Mo, Z. Hussain, Z.-X. Shen, F. Wang, S. G. Louie, and M. F. Crommie. Giant bandgap renormalization and excitonic eﬀects in a monolayer transition metal dichalcogenide semiconductor. Nat Mater, 13(12):1091–1095, 2014.

[254] D. Vanderbilt and R. D. King-Smith. Electric polarization as a bulk quantity and its relation to surface charge. Physical Review B, 48(7):4442–4455, aug 1993.

[255] P. Villars and K. Cenzual, editors. Crystal Structures of Inorganic Compounds. Springer Berlin Heidelberg, 2009.

[256] A. von Hippel, R. G. Breckenridge, F. G. Chesley, and L. Tisza. High dielectric constant ceramics. Industrial & Engineering Chemistry, 38(11):1097–1109, nov 1946.

[257] R. Wahl, D. Vogtenhuber, and G. Kresse. SrTiO3 and BaTiO3 revisited using the projector augmented wave method: Performance of hybrid and semilocal functionals. Phys. Rev. B, 78:104116, Sep 2008.

[258] I. Wallach, M. Dzamba, and A. Heifets. AtomNet: A deep convolutional neural network for bioactivity prediction in structure-based drug discovery. CoRR, abs/1510.02855, 2015. BIBLIOGRAPHY 119

[259] J. Wang, J. B. Neaton, H. Zheng, V. Nagarajan, S. B. Ogale, B. Liu, D. Viehland, V. Vaithyanathan, D. G. Schlom, U. V. Waghmare, N. A. Spaldin, K. M. Rabe, M. Wuttig, and R. Ramesh. Epitaxial BiFeO3 Multiferroic Thin Film Heterostruc- tures. Science, 299(5613):1719–1722, 2003.

[260] S. Wang and J. Li. Two-dimensional inorganicorganic hybrid semiconductors composed of double-layered ZnS and monoamines with aromatic and heterocyclic aliphatic rings: Syntheses, structures, and properties. Journal of Solid State Chemistry, (0), 2014.

[261] Y. Wang, J. Lv, L. Zhu, and Y. Ma. Crystal structure prediction via particle-swarm optimization. Phys. Rev. B, 82:094116, Sep 2010.

[262] D. Weininger. SMILES, a chemical language and information system. 1. introduction to methodology and encoding rules. Journal of Chemical Information and Modeling, 28(1):31–36, feb 1988.

[263] S. Wemple, M. Didomenico, and I. Camlibel. Dielectric and optical properties of melt- grown batio3. Journal of Physics and Chemistry of Solids, 29(10):1797–1803, 1968.

[264] S. Wemple, M. DiDomenico Jr, and I. Camlibel. Relationship between linear and quadratic electro-optic coeﬃcients in linbo3, litao3, and other oxygen-octahedra fer- roelectrics based on direct measurement of spontaneous polarization. Applied Physics Letters, 12(6):209–211, 1968.

[265] D. E. Worrall, S. J. Garbin, D. Turmukhambetov, and G. J. Brostow. Harmonic networks: Deep translation and rotation equivariance. In The IEEE Conference on Computer Vision and Pattern Recognition (CVPR), July 2017.

[266] B. Wul and J. Goldman. Ferroelectric switching in batio3 ceramics. CR Acad. Sci. URSS, 51:21, 1946.

[267] H. Yan, J. N. Hohman, F. H. Li, C. Jia, D. Solis-Ibarra, B. Wu, J. E. P. Dahl, R. M. K. Carlson, B. A. Tkachenko, A. A. Fokin, P. R. Schreiner, A. Vailionis, T. R. Kim, T. P. Devereaux, Z.-X. Shen, and N. A. Melosh. Hybrid metal–organic chalcogenide nanowires with electrically conductive inorganic core through diamondoid-directed as- sembly. Nature Materials, 16(3):349–355, dec 2016.

[268] Q. Yan, J. Yu, S. K. Suram, L. Zhou, A. Shinde, P. F. Newhouse, W. Chen, G. Li, K. A. Persson, J. M. Gregoire, and J. B. Neaton. Solar fuels photoanode materials discovery by integrating high-throughput theory and experiment. Proceedings of the National Academy of Sciences, 114(12):3040–3043, mar 2017.

[269] Q. Yang, J. X. Cao, Y. Ma, and Y. C. Zhou. First principles study of polarization-strain coupling in SrBi2Ta2O9. AIP Advances, 3(5):052134, 2013. BIBLIOGRAPHY 120

[270] F. Ye, S. Chi, H. Cao, B. C. Chakoumakos, J. a. Fernandez-Baca, R. Custelcean, T. F. Qi, O. B. Korneta, and G. Cao. Direct evidence of a zigzag spin-chain structure in the honeycomb lattice: A neutron and x-ray diﬀraction investigation of single-crystal Na2IrO3. Physical Review B, 85(18):180403, May 2012. [271] B. Yuan, J. P. Clancy, A. M. Cook, C. M. Thompson, J. Greedan, G. Cao, B. C. Jeon, T. W. Noh, M. H. Upton, D. Casa, T. Gog, A. Paramekanti, and Y.-J. Kim. Determination of Hund’s coupling in 5d oxides using resonant inelastic x-ray scattering. Phys. Rev. B, 95:235114, Jun 2017.

[272] M. A. Zeb and H.-Y. Kee. Interplay between spin-orbit coupling and Hubbard interac- tion in SrIrO3 and related Pbnm perovskite oxides. Physical Review B, 86(8):085149, Aug. 2012.

[273] H. Zhang. A theory for structural phase transitions in batio3 single crystal and pbzro3 -xpbtio3 solid solution. AIP Advances, 3(4):042118, 2013.

[274] Y. Zhang, G. M. Dalpian, B. Fluegel, S.-H. Wei, A. Mascarenhas, X. Y. Huang, J. Li, and L. W. Wang. Novel approach to tuning the physical properties of organic-inorganic hybrid semiconductors. Physical Review Letters, 96(2):026405, 2006. PRL.

[275] Y. Zhang, J. Sun, J. P. Perdew, and X. Wu. Comparative ﬁrst-principles studies of prototypical ferroelectric materials by LDA, GGA, and SCAN meta-GGA. Phys. Rev. B, 96:035143, Jul 2017.

[276] Z. Zhao, S. Wang, A. R. Oganov, P. Chen, Z. Liu, and W. L. Mao. Tuning the crystal structure and electronic states of ag2se: Structural transitions and metallization under pressure. Physical Review B, 89(18):180102, 2014. PRB.

[277] L. Zhou, Q. Yan, A. Shinde, D. Guevarra, P. F. Newhouse, N. Becerra-Stasiewicz, S. M. Chatman, J. A. Haber, J. B. Neaton, and J. M. Gregoire. High Throughput Discovery of Solar Fuels Photoanodes in the CuO-V2O5System. Advanced Energy Materials, 5(22):1500968, aug 2015.

[278] Y. Zhou, Q. Ye, Q. Qiu, and J. Jiao. Oriented Response Networks. ArXiv e-prints, Jan. 2017.

[279] N. E. R. Zimmermann, M. K. Horton, A. Jain, and M. Haranczyk. Assessing local structure motifs using order parameters for motif recognition, interstitial identiﬁcation, and diﬀusion path characterization. Frontiers in Materials, 4, nov 2017.

[280] A. Zunger. Inverse design in search of materials with target functionalities. Nature Reviews Chemistry, 2(4):0121, mar 2018. 121

Appendix A

Appendix for Realization of a three-dimensional spin-anisotropic harmonic honeycomb iridate APPENDIX A. APPENDIX FOR REALIZATION OF A THREE-DIMENSIONAL SPIN-ANISOTROPIC HARMONIC HONEYCOMB IRIDATE 122

Figure A.1: X-ray diﬀraction pattern in the (hk0) (top) and (h1l) (bottom) planes. Raw data (AB) is well reproduced by calculations (CD) for the Cccm structure (Table A.1), in contrast an F ddd (hyper-honeycomb) structure (EF) can only explain the existence of less than half of the observed diﬀraction peaks.

Single Crystal Reﬁnement

The very diﬀerent magnetic ordering temperature of our ﬂux-grown single crystals, TN = 38 K, compared to 15 K [231] reported for the so-far-synthesized powders of Li2IrO3 (layered honeycomb crystal structure, monoclinic C2/m unit cell [189]) suggested that the ﬂux-grown samples may realize a polytype of Li2IrO3 with a diﬀerent crystal structure. This was clearly revealed by x-ray diﬀraction measurements performed using a Mo-source Oxford Diﬀraction Supernova diﬀractometer. Several crystals were measured and the diﬀraction patterns were all consistent in terms of the unit cell and selection rules for the observed diﬀraction peaks. Here we report in detail the data on an approximate rhombus-shaped 35 103µm3 ﬂux- grown crystal. ∼ × The lattice parameters of the monoclinic layered honeycomb crystal structure [189] could not account for the positions of over 2000 Bragg peaks measured in our diﬀraction experi- ment, which instead could be indexed with an orthorhombic unit cell with parameters given in Table A.1. Representative diﬀraction patterns are illustrated in Fig. A.1AB, where (h, k, l) APPENDIX A. APPENDIX FOR REALIZATION OF A THREE-DIMENSIONAL SPIN-ANISOTROPIC HARMONIC HONEYCOMB IRIDATE 123

Figure A.2: Observed diﬀraction intensities plotted against those calculated in the reﬁned (A) Cccm (Table A.1) and (B) F ddd structural models. The dashed lines indicate 1:1 agreement between data and model and error bars reﬂect the intensity uncertainties after averaging the observed intensities of reﬂections expected to be equivalent under orthorhombic symmetry. The three families of reﬂections discussed in the text are plotted as diﬀerent symbols/colors (black circles, red squares, and blue triangles). Note that the F ddd model predicts zero intensity at the observed (odd, odd, even) reﬂections and largely overestimates the intensities of (odd, odd, odd) peaks. refer to wavevector components in reciprocal lattice units of the orthorhombic unit cell. The highest-symmetry orthorhombic space groups that can account for all of the observed peaks in the diﬀraction patterns are Cccm (no. 66) and Ccc2 (no. 37). Both have the same selec- tion rule for allowed reﬂections for a general atomic position, (hkl): h + k even, (0kl) : both k and l even, (h0l) : both h and l even. Both have a C-centered unit cell, corresponding to a 1 1 translation of ( 2 , 2 ,0), and Ccc2 is obtained from Cccm by removing a mirror plane normal to the c-axis. In the ﬁnal reﬁnements of the crystal structure reported below, we did not ﬁnd any signiﬁcant atomic displacements and correspondingly no improvement in the goodness of ﬁt when the crystal symmetry was lowered from Cccm to Ccc2, so in the following we discuss only the higher symmetry case. The unit cell volume is approximately 4 the unit cell volume of the layered honeycomb structure (Z = 4), which suggested that the× present polytype has the same mass density, but with Z = 16 formula units per unit cell. Since iridium is by far the dominant x-ray scatterer with 77 electrons (oxygen 8 and lithium 3 electrons), we ﬁrst attempted a preliminary ﬁt to APPENDIX A. APPENDIX FOR REALIZATION OF A THREE-DIMENSIONAL SPIN-ANISOTROPIC HARMONIC HONEYCOMB IRIDATE 124

A Cccm B Fddd

c

b a

Figure A.3: Crystal structure models described in the text, (A) Cccm (Table A.1) and (B) F ddd, large brown balls - Ir, medium light gray balls - Li, small gray balls - O.

the x-ray data assuming a simpliﬁed structural model composed solely of Ir ions located in general positions within the Cccm space group symmetry. The iridium coordinates were set free to reﬁne within the bounds of the orthorhombic unit cell. Remarkably, the reﬁnement easily converged with Ir ions occupying two crystallographic sites with coordinates close to those listed in Table A.1. To test that this solution was reliable, and not an accidental local minimum in the least squares reﬁnement, we employed simulated annealing techniques implemented in FullProf [210] to explore the full parameter space of the structural model against the full data set (treating each observed (h, k, l) reﬂection as an independent data point without imposing any symmetry constraints). By constructing a lattice with the dimensions of the orthorhombic unit cell a b c but with lowered symmetry P 1,¯ and populating it with eight iridium ions with atomic× × fractional coordinates free to vary within the full unit cell according to the annealing process, we found an unconstrained (except for inversion symmetry) yet highly reproducible iridium lattice that corresponded to a global APPENDIX A. APPENDIX FOR REALIZATION OF A THREE-DIMENSIONAL SPIN-ANISOTROPIC HARMONIC HONEYCOMB IRIDATE 125

Figure A.4: Preliminary measurements of the change in the lattice parameters along the crystallographic a, b and c direction on cooling below the magentic transition at TN. We do not observe any changes in the crystallographic symmetry, but the elastic response in each direction is highly anisotropic, with the b-axis changing roughly 10 times more that the a-axis. minimum in the parameter space. This structure was found to be in perfect agreement with the iridium framework of the initial reﬁnement, conﬁrming both the structural model and the space group, Cccm. In addition, the choice of space group symmetry was subjected to more rigorous testing by simulated annealing, which was systematically performed under symmetry constrains corresponding to sub-groups of Cccm and F ddd (see below), all of APPENDIX A. APPENDIX FOR REALIZATION OF A THREE-DIMENSIONAL SPIN-ANISOTROPIC HARMONIC HONEYCOMB IRIDATE 126

2K 15K αab αbc αac 30K 40 40 38K 5 45K -3 60K 90K 120K

) x10 180K

-1 240K T

-1 0 0 0 f.u. B µ ( α

-5 -40 -40

0 45 90 -90 -45 0 45 90 -90 -45 0 45 90

θab (°) θbc (°) θac (°) Figure A.5: The magnetic anisotropy extracted from the low ﬁeld slope of the torque signal τ/µ0H, similar to that shown in Figure 3.4 B, taken for rotations through the three principal crystallographic planes and at diﬀerent temperatures. The anisotropy is shown in units of µB per Ir, for (A) the χa χb, (B) χa χc and (C) χb χc. The only change of sign in the anisotropy is in (A) and an− enlargement− of this scale is− shown in Figure 3D of the main text to emphasize this. which converged to the Cccm solution or failed, respectively. Using the measured Bragg peak intensities, space group symmetry, and the identiﬁed iridium positions, we calculated the electron density maps in the unit cell (using Shelxl [177] and Wingx [84]). This revealed additional electron density pockets, which we identiﬁed as the location of oxygen ions. Lithium ions scatter x-rays very weakly (only 3 electrons) and their positions cannot be reliably identiﬁed using x-ray scattering techniques, especially in the presence of heavy elements such as iridium. However, assuming that the fundamental building blocks of the structure are edge-sharing IrO6 and LiO6 octahedra (as in the honey- comb polytype), one can readily determine idealized lithium positions (listed in Table A.1 and shown in Fig. A.3A) required to achieve this connectivity. Assuming lithium ions to be ﬁxed at the ideal positions, a full structural model was reﬁned against the data set using FullProf [210]. Iridium and oxygen ions were located in the initial positions determined above, and their atomic coordinates were set free to vary within the constraints of Cccm crystal symmetry. It became apparent that the structural model gave an excellent ﬁt to most reﬂections, but over-estimated the diﬀraction intensity of a small subset. Speciﬁcally, the empirically-determined selection rules for observed (h, k, l) reﬂections give three families: (even, even, even) with h + k + l = 4n, n integer, (odd, odd, odd) except l = 3 + 6n, n integer, and (odd, odd, even). The intensities of these families of peaks are plotted in Fig. A.2A against the model calculation. It is clear that the model is in excellent agreement with the (even, even, even) and (odd, odd, odd) reﬂections. The model also explains the presence of the third family of reﬂections, the (odd, odd, even), but the observed intensity is weaker than predicted. In fact those reﬂections showed an asymmetry in the intensity not expected under orthorhombic symmetry, i.e. I(odd, odd, even) = I(-odd, odd, even) (Fig. A.2A only shows the averaged (reduced) intensity of those reﬂections6 with the error APPENDIX A. APPENDIX FOR REALIZATION OF A THREE-DIMENSIONAL SPIN-ANISOTROPIC HARMONIC HONEYCOMB IRIDATE 127

4

2

0 /H (a.u.) -2

-4

0 10 20 30 μ0H (T)

Figure A.6: Torque signal taken at magnetic ﬁelds up to 35 T at the National High magnetic Field Laboratory. The ﬁeld H∗ is extremely clear at all angles. At angles away from the principal axes the torque signal is very clearly linear and follows a sin 2θ dependence described by equation A.4. The larger asymmetry in this data set compared to that measured in the superconducting magnet, is due to the larger ﬁeld gradient experienced by the sample. bars indicating the spread of values). The degrees of both the lowered average intensity and asymmetry were found to vary across a number of diﬀerent samples measured, however, the excellent agreement to the (even, even, even) and (odd, odd, odd) reﬂections was robust and consistent across all samples tested. We propose that the discrepancies in (odd, odd, even) intensities are most likely due to sample-dependent structural stacking faults, as discussed later in this section. A ﬁnal reﬁnement was performed against the (even, even, even) and (odd, odd, odd) reﬂections with excellent reliability factors RF2 = 3.83%, wRF2 = 4.91%, and RF = 2.27% [including also the (odd, odd, even) reﬂections in the reﬁnement resulted only in very small changes in the oxygen positions, which we regard to be below the accuracy that can be reliably determined]. The obtained structural parameters from the ﬁnal reﬁnement are given in Table A.1; essentially the same results are obtained in reﬁnement done using Sir-92 [24] and Shelxl [177]. The above reﬁnement assumed stoichiometric Li2IrO3 with all atomic positions fully occupied. However, we have also tested for the possibility that each of the seven cation sites (Ir1-2, Li1-5) could have a mixed Li/Ir occupancy. In this test we constrain the total site occupancy to unity (i.e. no structural vacancies) with no constraint on the total Li:Ir atomic ratio (i.e. stoichiometry free to vary). Under these constraints a APPENDIX A. APPENDIX FOR REALIZATION OF A THREE-DIMENSIONAL SPIN-ANISOTROPIC HARMONIC HONEYCOMB IRIDATE 128

Figure A.7: (A) The two choices of edge shared bonds give rise to two kinds of links that are locally indistinguishable. These deﬁne two bonding planes (see Figure 3A of the main ◦ text) that are an angle φo 70 apart. (B) Links along the c-axis can either keep the same (S-links) or rotate (R-links)∼ the honeycomb planes. full reﬁnement of Li/Ir occupancies on the cation sites lead to no signiﬁcant improvement in the reﬁnement parameters. Furthermore, the occupancies of the Li and Ir sublattices reﬁned to their nominal values (Li only in Li1-5 sites and Ir only in Ir1-2 sites) within an error of less than 3%, further conﬁrming the stoichiometric composition and the structural model in Table A.1. The obtained crystal structure is illustrated in Fig. A.3A. The full 3D x-ray diﬀraction pattern observed is well accounted for by this model and representative plots are shown in Fig. A.1CD. The reﬁned structure has IrO6 octahedra distorted from ideal cubic with non-equivalent Ir-O distances spanning a range of up to 7% for each octahedron, ∼ comparable to the range of Ir-O distances reported for the IrO6 octahedra in the layered honeycomb polytype [189]. The resulting Ir network show in Fig.1B-C of the main text is a novel arrangement of near-ideal honeycombs in three dimensions not reported before as far as we know in other 3d or 5d oxides. Ir honeycombs form parallel rows that alternate along the two diagonals of the unit cell in the ab plane, namely along a + b at z = 0 and along a b at z = 1/2. This alternation leads to a 3D network of inter-connected honeycomb rows− stacked along the c-axis, where all nearest-neighbor Ir-Ir links are nearly the same length ( c/6) and all Ir-Ir-Ir bond angles are close to 120◦. The Ir positions are indeed very close to∼ such an ideal p lattice realized for Ir1 at 8k (1/4, 1/4, 1/12), Ir2 at 8i (1/2, 1/2, 1/6) and c = 3(a2 + b2), compare with Table A.1 where the latter equation is satisﬁed to within 0.1%. This near- APPENDIX A. APPENDIX FOR REALIZATION OF A THREE-DIMENSIONAL SPIN-ANISOTROPIC HARMONIC HONEYCOMB IRIDATE 129 R

Orthorhombic Monoclinic HHC

Layered HC S

Figure A.8: The harmonic honeycomb family is rich in structural possibilities that tune symmetry (depending on whether the number of NR and NS links is odd or even) and dimensionality (the extent of the NS links). This table summarizes this observation. Note we assume that the IrO6 octahedra have ideal cubic symmetry. Complex distortions may create systems of lower symmetry than that indicated. regularity of the Ir lattice is directly manifested in the observed x-ray diﬀraction pattern by a conspicuous absence of detectable scattering intensity along the c-axis for l = 3 + 6n, n integer as illustrated in Fig. A.1B, this is not due to a general symmetry-imposed selection rule of the space group, but is due to a near cancellation of intensity for a lattice built out of near-ideal honeycomb sections stacked along the c-axis. The obtained iridium lattice can be thought of as being the N = 1 member of a regular series of periodic structures of alternating honeycomb sections of diﬀerent widths (N = 1, 2, 3 ... ) as illustrated in Fig. 5B of the main text, with the layered honeycomb polytype (C2/m) being∞ the N = end member. The N = 1 structure could be “transformed” into the honeycomb polytype∞ by selectively mirror-imaging in the bc plane the iridium honeycomb rows centered at z = 1/2. In this case, iridium ions form inﬁnite honeycomb layers in the (a + b, c) plane and the unit cell along c is halved. It is clear from this construction why the reported repeating unit cell dimension of the layered honeycomb structure along this direction (labelled as bm = 8.9294 A˚ in the standard monoclinic cell notation [189]) is nearly half that of the c-axis repeat of the N = 1 polytype, c = 17.8363(10) A,˚ reported here. For completeness we note that the diﬀerent polytypes in the series plotted in Fig. 3.5B could be easily distinguished experimentally, as they have diﬀerent symmetries and/or diﬀer- ent unit cell sizes, and consequently distinct diﬀraction patterns. For illustration we consider the N = 0 hyper-honeycomb[127, 146] shown in Fig. 3.5B, H 0 . The periodic iridium atomic arrangement can be described by an orthorhombic unit cellh ofi the same size a b c and × × APPENDIX A. APPENDIX FOR REALIZATION OF A THREE-DIMENSIONAL SPIN-ANISOTROPIC HARMONIC HONEYCOMB IRIDATE 130

H Table A.1: Fractional atomic coordinates for 1 -Li2IrO3 extracted from single-crystal x- ray data at 300 K (Cccm space group, a = 5.9119(3)h i A,˚ b = 8.4461(5) A,˚ c = 17.8363(10) A,˚ Z = 16). All sites are fully occupied and Li positions are ﬁxed to nominal values such that edge-sharing IrO6 and LiO6 octahedra form a near-hexagonal arrangement in both (a + b, c) and (a b, c) planes. The isotropic displacement parameter U for Li is also ﬁxed to a value in the range− found for the other atoms. Values in brackets show standard deviations in the ﬁtted parameters.

Atom Site x y z U(A˚2) Ir1 8k 0.25 0.25 0.0836(2) 0.0124(4) Ir2 8i 0.5 0.5 0.1670(3) 0.0206(6) Li1 8j 0 0.5 0.3333 0.01 Li2 8k 0.75 0.25 0.25 0.0 Li3 8k 0.75 0.25 0.91667 0.01 Li4 4c 0.5 0.5 0.5 0.01 Li5 4d 0.5 0 0 0.01 O1 16m 0.77(1) 0.515(3) 0.087(4) 0.02(1) O2 8g 0.72(2) 0.5 0.25 0.04(1) O3 8l 0.00(1) 0.262(8) 0 0.006(9) O4 16m 0.49(1) 0.262(6) 0.163(3) 0.006(9)

orientation of axes as for N = 1, but face-centered and with diamond glide planes. In the corresponding space group, F ddd (no. 70), iridium ions occupy a single crystallographic site, 16g (0, 0, z) (origin choice 1), with z = 1/12 assuming the c-axis Ir-Ir bond length is c/6. Fig. A.1AB and EF show the comparison between data and the calculated diﬀraction pat- tern for a generic hyper-honeycomb structural model constructed such as to have hexagonal ◦ layers of edge-sharing IrO6 and LiO6 octahedra in the (a b, c) planes and 90 O-Ir-O and O-Li-O bonds. The atomic coordinates considered are Li1± 16g (0, 0, 1/4), Li2 16g (0, 0, 5/12), O1 32h(1/4, 0, 1/6), O2 16e (1/4, 0, 0) and the full structure is plotted in Fig. A.3B. As il- lustrated in Fig. A.1EF the F ddd space group has a much more restrictive selection rule for allowed reﬂections compared to Cccm, for example in the (hk0) plane h + k is required to be a multiple of 4 and both h and k to be even, as opposed to the less restrictive h + k even for Cccm, and for (h1l) both h and l odd, as opposed to h odd and l unrestricted for Cccm. The Cccm selection rules can account for all the experimentally observed reﬂections, whereas an F ddd unit cell could not account for the presence of the (odd, odd, even) reﬂections, such as the relatively strong (110), see Fig. A.1AE. Furthermore, reﬁnement of the F ddd structure against the intensities of reﬂections allowed in this symmetry, namely (even, even, even) and (odd, odd, odd), gives a statistically rather poor ﬁt with RF2 = 21.4%, wRF2 = 36.2%, and RF = 13.3%. This becomes clear when comparing the calculated intensities to those APPENDIX A. APPENDIX FOR REALIZATION OF A THREE-DIMENSIONAL SPIN-ANISOTROPIC HARMONIC HONEYCOMB IRIDATE 131 observed, shown in Fig. A.2B. The F ddd model only reproduces the correct intensities for the (even, even, even) reﬂections, whereas the intensities of the (odd, odd, odd) reﬂections are calculated to be approximately double that observed. For completeness, the additional family of (odd, odd, even) reﬂections observed in the experimental data are also shown in Fig. A.2B, wrongly predicted to have exactly zero intensity in the F ddd space group. These results, coupled with the conclusions drawn from the simulated annealing tests, conclusively show that the hyper-honeycomb F ddd structural model (and lower-symmetry structures ob- tained by small distortions of an F ddd parent structure) can be ruled out for the single crystals reported in this study. Finally, we note that in addition to sharp Bragg peaks the x-ray diﬀraction pattern also revealed the presence of weak, but clearly visible diﬀuse scattering in the form of “rods” of scattering intensity in-between Bragg peaks along the l-direction, sharply deﬁned in the h and k directions, as clearly seen in Fig. A.1B with the selection rule h odd and k odd. Whilst a quantitative reﬁnement of the data including the diﬀuse scattering is beyond the scope of this present study, we propose that this diﬀuse scattering most likely originates from occasional structural faults in the nominal Cccm atomic stacking sequence along the c-axis. The presence of diﬀuse scattering takes intensity away from the sharp Bragg peaks, and it is possible that some families of Bragg peaks are aﬀected more than others; this might explain why the intensity of one particular family of reﬂections, namely the (odd, odd, even) peaks located on the diﬀuse scattering rods, appears weaker in experiment than predicted by a structurally-perfect Cccm model considered in our reﬁnement, see Fig. A.2A (blue triangles). We have carried out extensive high-resolution SXD measurements at 8 K to search sig- nature of lowering of structural symmetry due to magnetic transition. These∼ measurements were performed on the 6-ID-B undulator bemaline at Advanced Photon Source using an in- cident photon energy of 11.215 keV and pyrolitic graphite analyzer. Only resolution-limited Bragg peaks allowed by the proposed space group were observed indicated the structure remained three-dimensionally ordered and fully coherent well below TN . Furthermore, these measurements also ruled out any superlattice peaks (e.g. due to structural modulation, or magnetic order) at half-integer reciprocal-lattice points such as (1/2,0,0), (1/2,1/2,0) The temperature dependence of the orthorhombic lattice parameters around the magnetic tran- sition TN = 38 K was measured using θ 2θ scans to determine the 2θ location of strong structural Bragg peaks (-2,0,6), (0,0,12),− and (0,2,14) as a function of temperature between 8.4 - 45.1 K. Preliminary, data in Figure A.4 shows a small change of all orthorhombic lat- tice parameters around the 38 K magnetic transition and relaxation to comparable lattice parameters both below and above the transition. The percent change in lattice parameter appears to be an order of magnitude greater for the b-axis than for a or c, analogous to magnetic anisotropy seen in the susceptibility data. APPENDIX A. APPENDIX FOR REALIZATION OF A THREE-DIMENSIONAL SPIN-ANISOTROPIC HARMONIC HONEYCOMB IRIDATE 132 Magnetic Characterization A magnetically anisotropic material experiences a magnetic torque when its magnetization is not aligned with the applied magnetic ﬁeld; the deﬂection of the cantilever in a uniform magnetic ﬁeld is hence a direct measure of the magnetic anisotropy,

τ = M H. (A.1) × At small ﬁelds, where the magnetic response is linear, the magnetic anisotropy is captured by a susceptibility tensor χij. Mi = χijHj (A.2) The tensor is diagonal in the basis of the principal magnetic axes, which deﬁnes three prin- cipal components of magnetic susceptibility. For an orthorhombic crystal, these magnetic axes naturally coincide with the crystallographic directions, deﬁning χa,b,c. For example, for rotations in the b-c plane, the anisotropic magnetization (Mb,Mc) = (χbHb, χcHc) creates a torque

τa =MbHc McHb = (χb χc)HbHc (A.3) − − Deﬁning θ as the angle between a crystallographic axis (c in this case) and the applied magnetic ﬁeld, the torque can be rewritten as

2 2 (χb χc)H sin2θ τa =(χb χc)H sinθcosθ = − (A.4) − 2 From this expression, the magnetic axes can be precisely identiﬁed from a complete angular dependence of the torque measurements (Figure 4B of the main text), with the amplitude of the sin2θ dependence being proportional to the magnetic anisotropy αbc = (χb χc). In H − 1 -Li2IrO3 the magnetic axes are independent of temperature between room temperature h i and 1.5 K, but unusually, the sign of the anisotropy between the b and c axes, αbc, changes at around 75 K(Figure 4D of the main text). A convenient way to represent magnetization as observed by torque measurements is by plotting τ/H versus H (Figure 4B of the main text). This ﬁgure clearly demonstrates the linear dependence of magnetization at low ﬁelds with a slope that follows a sin2θ dependence with ﬁeld orientation (colored curves). The softer component of magnetization appears to saturate at a ﬁeld H∗, above which the linear response (equation A.4) is no longer valid. The ﬁnite torque at magnetic ﬁelds greater than H∗ indicates the ﬁnite angle between M and H up to the highest measured magnetic ﬁelds. H∗ is strongly dependent on the orientation of the crystal with respect to magnetic ﬁeld. The largest kink ﬁeld along the crystallographic a direction was measured at the NHMFL in Tallahassee. The observed overall negative slope at higher ﬁelds is due to a force component from a ﬁnite magnetic ﬁeld gradient. A nonlinear torque signal was measured below H∗ for magnetic ﬁelds aligned close to the hard susceptibility direction, χa, where the minimal torque condition is an unstable equilibrium (Figure 4B of the main text and Figure A.6). APPENDIX A. APPENDIX FOR REALIZATION OF A THREE-DIMENSIONAL SPIN-ANISOTROPIC HARMONIC HONEYCOMB IRIDATE 133 In the harmonic honeycomb series each iridium atom occupies a local environment with uniaxial g-factor anisotropy that can be captured by a magnetic susceptibility χk, parallel to and χ⊥, perpendicular to the plane deﬁned by its three nearest neighbor iridium atoms — the interlaced honeycomb planes. The measured high temperature magnetic anisotropy, αij, arises from the sum of this local anisotropy of the two honeycomb planes revealing that χk > χ⊥. Notably this is the opposite of the anisotropy χk < χ⊥ observed for the layered H sodium iridate, -Na2IrO3 Ref. [232]. Superposition of both honeycomb planes leads to h∞i φ φ Ma = M⊥cos /2 + Mksin /2 φ φ Mb = M⊥sin /2 Mkcos /2 (A.5) − where the magnetization parallel, Mk, and perpendicular, M⊥, to each of the planes can be written

φ φ M⊥ = χ⊥H⊥ = χ⊥(Ha cos /2 + Hb sin /2) φ φ Mk = χkHk = χk(Ha sin /2 Hb cos /2) (A.6) − Therefore, the geometric relation between the underlying pair of honeycomb planes results in three components of magnetization determined by only two microscopic parameters

2φ 2φ Ma = Ha χ⊥cos /2 + χksin /2 2φ 2φ Mb = Hb χ⊥sin /2 + χkcos /2

Mc = Hcχk (A.7)

Using χ± = (χk χ⊥)/2 the anisotropic susceptibility of this family of structures can be simpliﬁed to ±

χa = χ+ χ−cosφ − χb = χ+ + χ−cosφ

χc = χ+ + χ− (A.8) As a consequence, at high temperatures where g-factor anisotropy dominates, all three principal components of the magnetic susceptibility must order with χc > χb > χa. The geometry of the undistorted, edge-sharing octahedra constrains the angle separating these two planes to φ = arccos(1/3) 70◦ (Figure 3A of the main text). The geometric angle φ = arccos 1/3, which is also reﬂected≈ in the crystal morphology, is directly apparent in the observed high temperature magnetic anisotropy, where χa,b,c are equally spaced,

1 χa = χ+ ( /3) χ− − 1 χb = χ+ + ( /3) χ−

χc = χ+ + χ−. (A.9) This equal separation is observed as the ratios of the high temperature anisotropies saturating 1 1 to the values of αba/αac = /2, αbc/αac = /2, αbc/αab = 1 (see Figure 3.3 B). − APPENDIX A. APPENDIX FOR REALIZATION OF A THREE-DIMENSIONAL SPIN-ANISOTROPIC HARMONIC HONEYCOMB IRIDATE 134 Kitaev quantum spin liquid

Every member of the harmonic honeycomb series is bonded by edge sharing IrO6 octahedra. The edge-sharing geometry of the octahedra preserves the essential ingredients of the Kitaev model and this is universal for this family of structures. All three dimensional arrangements of edge-sharing octahedra maintain the interfering Ir-O2-Ir exchange paths, where each of the three nearest neighbor Ir-Ir interactions predominantly couples a particular orthogonal component of spin (see Figure 4A of the main text). In the idealized limit of symmet- ric octahedra, such changes may compete primarily with the usual rotationally symmetric Heisenberg interactions. In the Kitaev limit where Heisenberg interactions may be set aside, the Hamiltonian becomes a sum of spin-anisotropic exchange terms

c X bˆ bˆ h X aˆ+cˆ aˆ+cˆ h X aˆ−cˆ aˆ−cˆ HK = K S S K S S K S S , (A.10) − i j − i j − i j ˆ hiji∈b⊥ hiji∈(aˆ+cˆ)⊥ hiji∈(aˆ−cˆ)⊥ where Sbˆ and Saˆ±cˆ = (Saˆ Scˆ)/√2 are the spin operators in a set of three orthogonal directions, with aˆ, bˆ, cˆ being± unit vectors along the orthorhombic crystallographic axes. Here we label each bond ij by the axis perpendicular to its Ir-O2-Ir plane; for each bond, h i ˆ ˆ this normal vector lies along one of the directions (aˆ + cˆ), (aˆ cˆ), b . The b⊥ bonds are all oriented along the crystallographic c direction. Thus{ all the nearest− } neighbor Ir-Ir bonds can be divided into three classes, one for each component of spin: the bˆ component from the c-axis bonds, and the aˆ cˆ components from the h bonds deﬁning each honeycomb plane (depicted in red and blue± with corresponding signs in Figure 4A of the main text). The exchange couplings Kh are constrained by the± symmetry of the space group to be the same c bˆ h on the (aˆ cˆ)⊥ bonds, but K , the coeﬃcient of S coupling, is symmetry-distinct from K . The Hamiltonian± in Equation A.10 was studied by Kitaev on the honeycomb lattice and shown to give an exactly solvable quantum spin liquid. The solution relies on the fact that spin algebra can be represented in an enlarged Hilbert space of Majorana fermions χα µ 0 µ (α = 0, 1, 2, 3) by mapping S (i/2)χ χ (where µ = 1, 2, 3) and implementing constraints to project back to the physical→ Hilbert space. As a result, each spin is represented in terms of two degrees of freedom — one a 2 gauge ﬁeld, the other a Majorana fermion moving in this ﬁeld. The three-fold local connectivityZ of the honeycomb lattice together with the orthogonal Ising coupling of the Kitaev Hamiltonian (Equation A.10) freezes the gauge ﬁeld ﬂuctuations associated with the Hilbert space constraint, resulting in static 2 ﬂuxes. The problem then reduces to the motion of non-interacting particles in a ﬁxed ﬁeld.Z The ground state of these non-interacting fermions, expressed in terms of the underlying spins, is a complicated many-body superposition, and in particular is a quantum spin liquid. In 2D the solution is possible because the honeycomb lattice contains the right number of hexagon plaquettes (minimal closed paths linking sites) to host the 2 ﬂuxes. This can be seen via Euler’s theorem — which states that the number of minimalZ plaquettes plus the number of sites equals the number of links, on any 2D lattice. Threefold coordination means there are three bonds per two sites, and hence there is one ﬂux degree of freedom for every two spins, as required by the solution. In 3D, there are too many minimal plaquettes APPENDIX A. APPENDIX FOR REALIZATION OF A THREE-DIMENSIONAL SPIN-ANISOTROPIC HARMONIC HONEYCOMB IRIDATE 135

to host the required number of independent 2 ﬂuxes. However, a similar counting formula shows that the required number of independentZ gauge ﬁeld degrees of freedom is matched by subtracting the number of enclosed volumes from the number of faces. Each enclosed volume gives a constraint; the independent ﬂux constraints in 3D are not individual ﬂuxes but rather unending ﬂux lines, which form closed ﬂux loops. An additional diﬀerence in the 3D lattices is that, unlike the 2D honeycomb where every plaquette has six sites, in the harmonic honeycomb lattice the plaquettes vary in length, H including 6, 10, 14 and so on. In particular, for the 1 -Li2IrO3 member there are two minimal plaquettes, 6 sites long and 14 sites long. Theh producti of spin operators around each such plaquette forms an operator which commutes with the Hamiltonian. However products of such plaquette operators around an enclosed volume are reduced to the identity operation, constraining the ﬂux lines to form closed loops. These gauge ﬁeld ﬂuxes remain static, enabling the spin-liquid solution to be extended to 3D for all members of this family [146, 127]. The ground state of the Hamiltonian described by Eq. A.10 contains no gauge-ﬁeld ﬂuxes. In this zero ﬂux sector, the Hamiltonian is quadratic, diagonal in momentum space. Assum- ing Kc = Kh = K, the dispersion of Majorana Fermions is given by the eight eigenvalues of the tight-binding matrix ∗ ∗ 0 1 0 0 0 0 0 V2 U3 ∗ 1 0 V1 0 0 0 0 0 0 V1 0 1 0 0 0 0 0 0 1 0 V1 0 0 0 K (A.11) 0 0 0 V ∗ 0 1 0 0 1 0 0 0 0 1 0 V ∗ 0 2 0 0 0 0 0 V2 0 1 V2U3 0 0 0 0 0 1 0

where U3 = exp [ik c], V1,2 = 1 + U1,2 and U1,2 = exp [ik (a b)/2] with the +/ sign · · ± − corresponding to U1, U2 respectively. In the symmetric octahedra idealization where the Kitaev Hamiltonian is most likely to be relevant, the crystallographic vectors take the simple form a = (2, 2, 0), b = (0, 0, 4) and c = ( 6, 6, 0) in the Ir-O Euclidean coordinate system, in unis where the Ir-O distance is 1. The tight− binding dispersion above is easily generalized to the other 3D lattices with the same a, b base-centered orthorhombic Bravais lattice vectors and arbitrarily long unit cells along c, by appropriately cycling between V1 and V2 in the alternating oﬀ-diagonal elements of the matrix. The resulting spectrum of the Majorana Fermions is gapless, and remains gapless for the entire region of parameter space with Kc 2Kh [146, 127]. The gapless fermion excitations form a 1D nodal contour within the 3D Brillouin≤ zone, satisﬁed by the two equations k c = 0 and cos (k a/2) + cos (k b/2) = 1/2. For reference, note the BZ boundary satisﬁes· the equations cos· (k c) = 1· or cos (k a/2) + cos (k b/2) = 0. · − · · In the vicinity of the nodal contour the dispersion is linear (ω k⊥ ) in the two directions perpendicular to the nodal contour. Increasing Kc/Kh shrinks the∼ | nodal| contour to a point, APPENDIX A. APPENDIX FOR REALIZATION OF A THREE-DIMENSIONAL SPIN-ANISOTROPIC HARMONIC HONEYCOMB IRIDATE 136 at Kc = 2Kh; for Kc > 2Kh the fermion spectrum is gapped. If ﬂux excitations proliferate, they will conﬁne the fermions excitations in the spin liquid. In 2D, ﬂux excitations are point objects and proliferate at any ﬁnite temperature. But in 3D, the ﬂuxes form closed loop, with an energy cost proportional to the length of the ﬂux loop; large ﬂux loop cost arbitrarily high energy. Thus, in the 3D quantum spin liquid the fermions will survive in the deconﬁned phase until an entropy driven phase transition at ﬁnite temperature, separating the 3D quantum spin liquid and the classical paramagnet. APPENDIX A. APPENDIX FOR REALIZATION OF A THREE-DIMENSIONAL SPIN-ANISOTROPIC HARMONIC HONEYCOMB IRIDATE 137 Other possible structures To facilitate our description of the harmonic honeycomb family we develop a simple language based on their structural building blocks. Given a choice of one shared edge, there are two locally indistinguishable choices for the two remaining bonds, shown in Figure A.7 (A). Each Ir neighbor can then be in one of two planar environments, which we denote as the harmonic honeycomb plane (Figure 3A of the main text). The vertical (c-axis) bonds can then rotate the orientation of the planes (R-links) or keep them the same (S-links), shown in Figure A.7 (B). We emphasize that the Ir is always coordinated by three others in both kinds of bonds, just as in the layered honeycomb. In addition to the harmonic honeycomb family described in the main text, we mention a few other structural possibilities and their consequences here. The main text only describes a family of structures which have N links of the type S but only one R link. We can distinguish members of a more general structural family by diﬀerent numbers of R and S links, and since the stoichiometry is unchanged we H denote them NR,NS -Li2IrO3. For the NR =odd structures, the crystal structures are h i orthorhombic. If NR is even the material is monoclinic, just as Na2IrO3, which has the H ◦ 0, -Li2IrO3 structure. Note that even in this case, the 70 internal bonding geometry h ∞i ∼ is still evident in the angle between the monoclinic crystalline directions am and cm.A H − material containing exclusively R links, , 0 -Li2IrO3, is the ‘hyper-honeycomb,’ so named in analogy with the hyper-Kagome [185,h∞160, i127, 146]. By changing the number of S and R links we can therefore tune the global dimensionality and alternate the symmetry of the materials that are otherwise locally indistinguishable (see Figure A.8). Finally, we note that S and R links diﬀer in another important regard: S links are inversion symmetric while R links are not. For structures containing the latter, this may lead to magnetic components in the Hamiltonian that break inversion symmetry, for example the Dzyaloshinsky-Moriya term [176, 82]. Note this is a local property in that the total space group for the systems may remain inversion symmetric. 138

Appendix B

Appendix for Ab initio Studies of Structural and Energetic Trends in the Harmonic Honeycomb Iridates

H H Table B.1: Lattice parameters for various levels of theory for 1 and Li2IrO3 and H H h i h∞i 1 and Na2IrO3 . All calculations for a given structure type are initalized with identicalh i magnetich∞i order. U = 1.5 eV. The percentage diﬀerence between the relaxed and experimental lattice parameter is indicated by the color of the cell.

H H 1 Li2IrO3 1 Na2IrO3 h i h i Level of Theory a (A)˚ b (A)˚ c (A)˚ a (A)˚ b (A)˚ c (A)˚ Experiment 5.91 8.45 17.84 – – – PBE+SOC+U 5.96 8.53 18.02 6.48 9.10 19.02 PBE+SOC 6.01 8.75 17.17 6.46 9.11 19.13 PBE+U 6.01 8.73 16.99 6.46 9.12 19.10 PBE 6.01 8.76 17.03 6.45 9.13 19.17 Percent error color key: 1% 2% 3% > 3% ≤ ≤ ≤ APPENDIX B. APPENDIX FOR AB INITIO STUDIES OF STRUCTURAL AND ENERGETIC TRENDS IN THE HARMONIC HONEYCOMB IRIDATES 139

Table B.2: Total energy (eV) for constrained collinear magnetic orders on relaxed Li2IrO3 structures.

H Li2IrO3 # h i Mag. Order 0 1 2 ∞ Ferro c -35.199 -35.199 -35.199 -35.199 Ferro b -35.195 -35.195 -35.195 -35.194 Ferro a -35.194 -35.193 -35.194 -35.192 N´eelc -35.190 -35.191 -35.192 -35.193 N´eelb -35.195 -35.195 -35.194 -35.195 N´eela -35.193 -35.194 -35.194 -35.194

Table B.3: Total energy (eV) for constrained collinear magnetic orders on relaxed Na2IrO3 structures.

H Na2IrO3 # h i Mag. Order 0 1 2 ∞ Ferro c -32.923 -32.910 -32.906 -32.908 Ferro b -32.925 -32.911 -32.907 -32.910 Ferro a -32.930 -32.918 -32.915 -32.915 N´eelc -32.927 -32.917 -32.913 -32.916 N´eelb -32.927 -32.917 -32.914 -32.917 N´eela -32.925 -32.917 -32.912 -32.916

Table B.4: Bond lengths and angles for experimental and theoretical structures.

Li2IrO3 Na2IrO3 Exp. Theory Exp. Theory Ir-Ir (A)˚ 2.97 0.01 3.01 0.01 3.13 0.01 3.19 0.01 ± ± ± ± Ir-O-Ir (◦) 94 3 94 1 98.5 0.5 100 1 ± ± ± ± APPENDIX B. APPENDIX FOR AB INITIO STUDIES OF STRUCTURAL AND ENERGETIC TRENDS IN THE HARMONIC HONEYCOMB IRIDATES 140

(a) (b) NON-MAGNETIC (c) Ir Ir (d) FERROMAGNETIC C (e) Ir Ir Li Na Li Na O O O O 10 10 0.5 Total Total 0.5 Total Total

0.0 8 0.0 8 (eV) (eV) f f -0.5 -0.5 E E 6 6 − − E E -1.0 -1.0 (eV) -1.5 4 -1.5 4

-2.0 -2.0 Γ Y T Z Γ X X 1 Y Γ Y T Z Γ X X 1 Y b 2 2 0 0 c a 0.5 0.5 0.0 0.0 -2 -2

T (eV) (eV) f f -0.5 -0.5 X1 E E

− -4 − -4 Z Y E -1.0 E -1.0 Γ X -1.5 -6 -1.5 -6 -2.0 -2.0 X X 1 Γ Y T Z Γ X 1 Y (eV) Γ Y T Z Γ X Y (eV) Density of States (Arbitrary Units) Density of States (Arbitrary Units)

Figure B.1: Non-magnetic and ferromagnetic c band structures of relaxed unit cells of Li2IrO3 H and Na2IrO3 1 with PBE+SOC+U with path through k-space show at the bottom of (a). While the non-magnetich i band structure is metallic (b), a gap opens up between j = 1/2 H states with a magnetic order (d). The density of states for Li2IrO3 and Na2IrO3 1 (and likewise for the entire harmonic honeycomb series) is dominated by oxygen p and iridiumh i d orbitals (c and e).

Table B.5: Table of total energy, Ir-Ir bond lengths, and Ir-O-Ir bond angles for Li2IrO3.

Series Member H 0 H 1 H 2 H h i h i h i h∞i Ir-Ir Bond Lengths (A)˚ Ir1-Ir1 2.99684 Ir1-Ir1 3.00519 Ir1-Ir3 3.00367 Ir1-Ir1 3.01747 Ir1-Ir1 3.00675 Ir1-Ir2 3.00499 Ir2-Ir2 3.00226 Ir1-Ir1 3.01011 Ir2-Ir2 2.99884 Ir3-Ir3 3.00838 Ir-O-Ir Bond Angles (Degrees) Ir1-O1-Ir1 94.73 Ir1-O1-Ir2 94.64 Ir1-O1-Ir3 94.36 Ir1-O1-Ir1 94.63 Ir1-O2-Ir1 93.17 Ir1-O2-Ir2 94.59 Ir1-O2-Ir3 94.57 Ir1-O2-Ir1 94.41 Ir2-O3-Ir2 93.43 Ir3-O3-Ir3 94.06 Ir1-O4-Ir1 93.83 Ir1-O4-Ir2 94.23 Ir2-O5-Ir2 94.26

Table B.6: Table of total energy, Ir-Ir bond lengths, and Ir-O-Ir bond angles for Na2IrO3.

Series Member H 0 H 1 H 2 H h i h i h i h∞i Ir-Ir Bond Lengths (A)˚ Ir1-Ir1 3.18524 Ir1-Ir1 3.19486 Ir1-Ir3 3.20029 Ir1-Ir1 3.18503 Ir1-Ir1 3.19941 Ir1-Ir2 3.20077 Ir2-Ir2 3.20393 Ir1-Ir1 3.17998 Ir2-Ir2 3.18584 Ir3-Ir3 3.18442 Ir-O-Ir Bond Angles (Degrees) Ir1-O1-Ir1 101.30 Ir1-O1-Ir2 101.27 Ir1-O1-Ir3 101.25 Ir1-O1-Ir1 100.38 Ir1-O2-Ir1 100.11 Ir1-O2-Ir2 101.39 Ir1-O2-Ir3 101.40 Ir1-O2-Ir1 99.97 Ir2-O3-Ir2 100.18 Ir3-O3-Ir3 100.08 Ir1-O4-Ir1 100.36 Ir1-O4-Ir2 100.27 Ir2-O5-Ir2 101.39 APPENDIX B. APPENDIX FOR AB INITIO STUDIES OF STRUCTURAL AND ENERGETIC TRENDS IN THE HARMONIC HONEYCOMB IRIDATES 141

Table B.7: Table of total energy, Ir-Ir bond lengths, and Ir-O-Ir bond angles for experimen- tally synthesized harmonic honeycomb iridates.

H H H H Series Member Li2IrO3 Li2IrO3 0 Li2IrO3 1 Na2IrO3 h∞i h i h i h∞i Ir-Ir Bond Lengths (A)˚ Ir1-Ir1 2.97885 Ir1-Ir1 2.96502 Ir1-Ir1 2.98356 Ir1-Ir1 3.13793 Ir1-Ir1 2.97870 Ir1-Ir1 2.96981 Ir1-Ir2 2.97575 Ir1-Ir1 3.12975 Ir2-Ir2 2.96144 Ir-O-Ir Bond Angles (Degrees) Ir1-O1-Ir1 94.74 Ir1-O1-Ir1 95.07 Ir1-O1-Ir2 91.57 Ir1-O1-Ir1 97.97 Ir1-O2-Ir1 95.33 Ir1-O2-Ir1 92.57 Ir2-O2-Ir2 96.89 Ir1-O2-Ir1 99.45 Ir1-O3-Ir2 91.78 Ir1-O4-Ir2 95.90

H Table B.8: 1 Li2IrO3 PBE+SOC+U lattice parameters for varying U. All calculations are initializedh withi the same magnetic order. The ﬁnal magnetizations are not identical to one another. For PBE+SOC+U(0.25 eV) and PBE+SOC, the experimental lithium iridate structure is metallic. The relaxed PBE+SOC+U(0.25 eV) and PBE+SOC structures have gaps and relax to non-magnetic ground states.

Indirect Direct U (eV) a (A)˚ b (A)˚ c (A)˚ Gap Gap (meV) (meV) 1.5 5.96 8.51 18.05 322 373 1.0 5.96 8.53 18.02 230 298 0.5 5.97 8.49 18.03 78 155 0.25 6.01 8.74 17.16 128 128 0 6.01 8.75 17.17 108 108

Table B.9: PBE+SOC+U for various initial magnetizations. All relaxations have a magnetic order. Magnetic orders were initialized with magnetic moments of 1 Bohr magneton on each iridium atom.

Initial magnetic eV per a (A)˚ b (A)˚ c (A)˚ order Li2IrO3 Random order 1 5.96 8.51 18.05 -35.20 Random order 2 5.96 8.51 18.05 -35.20 Ferromagnetic 5.96 8.54 18.01 -35.20 along c Non-magnetic 5.96 8.54 18.03 -35.20 APPENDIX B. APPENDIX FOR AB INITIO STUDIES OF STRUCTURAL AND ENERGETIC TRENDS IN THE HARMONIC HONEYCOMB IRIDATES 142

Table B.10: PBE+U for various initial magnetizations. Calculations initialized with as a non-magnetic state relax to be non-magnetic and have similar lattice parameters to a non spin-polarized calculation.:

Initial Magnetic eV per a (A)˚ b (A)˚ c (A)˚ order Li2IrO3 Random order 1 5.97 8.62 17.50 -34.54 Random order 2 5.97 8.62 17.50 -34.51 Ferromagetic 5.97 8.62 17.50 -34.54 along c Non-magnetic 6.02 8.72 16.99 -34.63 Non 6.01 8.73 16.99 -34.63 spin-polarized 143

Appendix C

Appendix for Silver Benzeneselenolate is a Self-Assembling Direct-Gap Metal-Organic Chalcogenide Assembly APPENDIX C. APPENDIX FOR SILVER BENZENESELENOLATE IS A SELF-ASSEMBLING DIRECT-GAP METAL-ORGANIC CHALCOGENIDE ASSEMBLY144 C.1 General Information

Standard high vacuum, Schlenk line technique was employed for gram scale synthesis under dried nitrogen atmosphere. All reagents were obtained from commercial sources including dry toluene and tetrahydrofuran and were used without further puriﬁcation. The reported yields are for isolated sample. Powder X-Ray diﬀraction studies were performed on a Bruker AXS D8 Discover GADDS X-Ray Diﬀractometer, operated at 35 kV and 40 mA at a wave- length of Co Ka, 1.79 A.˚ Scanning electron microscopy (SEM) images were collected on a Zeiss Gemini Ultra-55 Analytical Field Emission SEM with a secondary electron detector and at an accelerating voltage of 3 keV, and an FEI Phenom G1 Tabletop SEM. Samples of crystalline silver benzeneselenolate specimens were prepared by the drop casting of iso- propanol suspensions onto a silicon wafer, which were allowed to settle followed by drying the surface with a stream of compressed air. Fluorescence spectra were obtained using an Edinburgh FLS980 spectrometer using an excitation wavelength of 380 nm.

C.2 Miscible Gram-Scale Synthesis of [AgSePh] ∞ An oven dried round bottom ﬂask equipped with a stir bar was charged with silver nitrate (1.4 g, 0.008 mol) and triphenylphosphine (4.4 g, 0.017 mol) in 250 mL of dry tetrahydrofuran. The solution was stirred for 16 h under nitrogen at ambient temperature giving a cloudy, white suspension. Diphenyl diselenide (1.3 g, 0.004 mol) in 80 mL of dry tetrahydrofuran was then added slowly to the ﬂask at -50 C. The reaction was stirred while warming slowly to room temperature in which a deep yellow solution resulted. The solution is layered with 75 mL of diethyl ether and stirred rapidly until solution is clear and colorless and bright yellow crystals have precipitated. The solvent is decanted and the solid was puriﬁed by the addition of fresh isopropyl alcohol followed by sonication and centrifugation to separate the crystalline pellet and supernatant. The crystals are then dried under vacuum giving a canary yellow ﬁne powder (2.3 g isolated). An additional SEM images of a typical morphology for the product is shown in Fig. S2.

C.3 Immiscible Interface Synthesis of [AgSePh] . ∞ In a glass scintillation vial, 5 mL of 3 mM diphenyl diselenide in toluene solution was carefully layered over 5 mL of a 3 mM aq. silver nitrate solution and allowed to crystallize at room temperature for 3 days. Crystals are recovered by passing a substrate, glass or silicon, through the liquid interface into the aqueous phase, and then gently pulling the substrate at a 45 degree angle back into the organic phase. The crystals preferentially adhere to the solid substrate. Poor adhesion is noted when hydrophobic substrates are used; pristine silicon wafers gave poor results, as did gold, which becomes rapidly functionalized with benzeneselenolate monolayers on exposure to the organic solution. Gentle drying by forced air is generally acceptable for most analyses, although an absorbent laboratory wipe can be APPENDIX C. APPENDIX FOR SILVER BENZENESELENOLATE IS A SELF-ASSEMBLING DIRECT-GAP METAL-ORGANIC CHALCOGENIDE ASSEMBLY145 used to wick residual liquids from the surface. Alternatively, suspensions of the crystals can be isolated by removing the aqueous layer from their reaction vessel using a glass pipette, and then decanting the toluene layer leaving behind the crystals. The product is then dispersed in isopropanol and sonicated brieﬂy to remove any residual crystals oﬀ the sides of the glassware, and then pelletizes readily from isopropanol under centrifugation. The crystals are stored in the dark under vacuum (¡1 mg isolated per crystallization vial). Additional SEM images of typical morphologies for crystals covered by this method are collected in Figure S3.

C.4 Fluorescence Imaging Methods

Fluorescent images were acquired on a Zeiss LSM 710 confocal microscope with an Axio Ob- server.Z1 (Carl Zeiss Microimaging, Thornwood, NY). Crystalline [AgSePh]∞ was dried on glass coverslips (No. 1.5) and imaged using a 100 oil immersion objective (Plan-Apochromat, 1.40 NA). Confocal scans of the material were obtained using a 405 nm diode laser to excite the sample and a 585 m wide pinhole. The emission spectrum was separated and the inten- sity of light between 400-700 nm (in 10 nm bins) was recorded on 32 detectors using the LSM 710 Linear Unmixing mode. The 32 images were imported to and analyzed using FIJI[218]. Isolated crystals were deﬁned using the tracing tool in FIJI to detect the edges of the single crystal and then used create a region of interest (ROI) around the crystal. For each ROI, the mean intensity, area, width and height was measured and recorded. Data were then exported to Origin 8.5.1 (Originlab, Northampton, MA) for analysis by linear regression and plotting. Atomic Force Microscopy AFM images were captured on a Cypher ES (Oxford Instruments). A budget Sensors TAP150G cantilever with a spring constant of 4.5 N/m was used in the repulsive tapping regime with an amplitude of 1.6 nm and a Asp/A0= 0.08. The z sensor was calibrated using an 18 nm step sample.

C.5 Calculation Methods

Density functional theory (DFT) calculations were performed using a plane-wave basis with the Vienna Ab Initio Simulations Package (VASP) [135, 137, 136]. We used a short-range hy- brid functional of Heyd, Scuseria, and Ernzerhof (HSE) [141, 104, 103, 105] for band structure calculations; we used the local density approximation (LDA), the generalized gradient ap- proximation of Perdew, Burke, and Ernzerhof (PBE) [193], and the vdW-df2 [79, 214, 147] functional to relax the experimental structure. Electron-ion interactions are treated with PAW pseudopotential [46, 138] with a 520 eV plane-wave cutoﬀ; and the Brillouin zone was sampled with a Monkhorst-Pack mesh [175] of 15 15 3 for PBE and df2 relaxations, and a 7 7 1 mesh for the computationally more-demanding× × HSE calculations. × × APPENDIX C. APPENDIX FOR SILVER BENZENESELENOLATE IS A SELF-ASSEMBLING DIRECT-GAP METAL-ORGANIC CHALCOGENIDE ASSEMBLY146 C.6 Calculation Details

Band structures for bulk and single layer [AgSePh]∞ and [AgSePh]∞ replaced with hydrogens are given in Figure C.5. The band structures is nearly identical between bulk and single layer [AgSePh]∞. The inorganic bands still present in [AgSePh]∞ replaced with hydrogens are similar to those of bulk and single layer [AgSePh]∞ with small changes to the band gap and eﬀective masses at the direct gap. Two symmetrically equivalent conﬁgurations of the benzene ligands are possible within the 2/c space group for the given reﬁnement of [AgSePh]∞[69]. We calculated that the two orientations diﬀer in formation energy by 214 meV per formula unit with DFT-PBE and we use the lower energy structure for DFT-HSE calculations. Despite the energy diﬀerence, the band structures of these conﬁgurations are nearly indistinguishable. We calculated the elec- tronic structure for the average of these two conﬁgurations and also observed that the band structure remained largely unaﬀected by change in the ligands orientation. The structural parameters for the conﬁguration used for our DFT calculations is given in Figure C.7. The CIF for the original reﬁnement containing both conﬁgurations as partial occupancies can be found in Cuthbert et. al [69]. DFT calculations were performed for bulk and single-layer [AgSePh]∞ in the lower energy of the two reﬁned conﬁgurations (as described above) and single layer [AgSePh]∞ with the phenyls replaced with hydrogens. The hydrogens positions for the latter case are relaxed with DFT-PBE. The primitive cell was used for all calculations. The structure used for our calculations of the single layer unit cell is simply the conventional unit cell with one of the [AgSePh]∞ layers removed. There is a 14 Adistance˚ between the single layers of [AgSePh]∞ and [AgSeH]∞ layers due to the periodic boundary conditions used in our VASP calculations. To assess DFTs ability to reproduce the experimental structure, we relaxed the experi- mentally reported crystal structure,28 choosing the lower energy of the two possible phenyl conﬁgurations reported in space group 15, with LDA, PBE, and df2 functionals. (All df2 calculations were performed with PBE pseudopotentials.) A summary of the relaxation re- sults, including percentage change in lattice parameters, variables describing the Ag lattice, and the dihedral angle between above and below plane phenyls, is given in Table C.2. The structures were relaxed until the stress on the unit cell was less than 0.5 kBar. LDA gave the best agreement with experiment with isotropic changes in lattice parame- ters of less than 3%. The df2 with PBE pseudopotentials give anisotropic expansion of the b lattice parameters. PBE gave the worst agreement with experiment with 7% increases in a and b lattice parameters lying in the AgSe plane. df2 gives the best agreement with the dihedral angle between above and below layer phenyl ligands. However, the distortion of the Ag lattice shows poor description of the covalently bonded AgSe layer. The relaxations were insensitive to an increase in the basis energy cutoﬀ and adding a U = 3.5 eV to Ag atoms. The dihedral angle for the phenyl groups was determined by ﬁtting Miller planes to a phenyl group from each orientation in VESTA and calculating the angle between the planes normal vector[173]. The band structure of the df2-relaxed structure shows a greater separation between bands of inorganic and organic character, with the bands of organic APPENDIX C. APPENDIX FOR SILVER BENZENESELENOLATE IS A SELF-ASSEMBLING DIRECT-GAP METAL-ORGANIC CHALCOGENIDE ASSEMBLY147

Figure C.1: Powder X-Ray diﬀractogram of [AgSePh]∞ overlapping the diﬀractogram cal- culated from Cuthbert et al. providing positive identiﬁcation for silver benzeneselenolate.28

Figure C.2: Larger [AgSePh]∞ crystal sizes, having dimensions in excess of 20 µm, are observed in the gram-scale-reaction product. character moving away from the Fermi level. Otherwise, the bands remain largely unchanged. The eﬀective masses of [AgSePh]∞ at the direct band gap were calculated using the EMC code[85]. The band structures and densities of state were plotted using a locally modiﬁed version of pymatgen[187]. APPENDIX C. APPENDIX FOR SILVER BENZENESELENOLATE IS A SELF-ASSEMBLING DIRECT-GAP METAL-ORGANIC CHALCOGENIDE ASSEMBLY148

Figure C.3: Additional micrographs of [AgSePh]∞. Detail of step edges of the layered system down to single layer step edges are evident in the SEM micrographs.

Table C.1: Calculated eﬀected masses at the direct gap of bulk, single and hydrogen- truncated [AgSePh]∞ The eﬀective masses at the direct gap are similar for bulk and single layer [AgSePh]∞ and [AgSePh]∞ truncated with hydrogens. Only two principle directions are given for 2D single layer calculations. Structure Principle Principle Principle Direction 1 Direction 2 Direction 3 Bulk a 1.130 b 0.441 c* 18.91 Single Layer a 1.146 b 0.444 – – Truncated a 0.466 b 0.298 – – APPENDIX C. APPENDIX FOR SILVER BENZENESELENOLATE IS A SELF-ASSEMBLING DIRECT-GAP METAL-ORGANIC CHALCOGENIDE ASSEMBLY149

Figure C.4: Single particles of [AgSePh]∞ were selected from confocal microscopy images and their spectra were compared. Color was invariant regardless of size and aspect ratio. Thickness had no discernable eﬀect but the precise thicknesses of crystals can be inferred only from total intensity. 100 isolated crystals were selected for this representation.

Figure C.5: HSE band structures for bulk and single-layer [AgSePh]∞ and single layer [AgSePh]∞ with the phenyls replaced with hydrogens Dashed lines show the Fermi level (at 0 eV) and the HSE band gap for bulk and single-layer [AgSePh]∞. Color of band signi- ﬁes the fraction of band occupations by inorganic atoms (Ag and Se) versus organic atoms (C and H). Bulk and single layer HSE band structures look identical. Single layer and hydrogen truncated AgSe look similar for Ag and Se dominated bands with small changes to the band gap and mobilities. APPENDIX C. APPENDIX FOR SILVER BENZENESELENOLATE IS A SELF-ASSEMBLING DIRECT-GAP METAL-ORGANIC CHALCOGENIDE ASSEMBLY150

Figure C.6: HSE, PBE, and df2 band structures for bulk [AgSePh]∞ Dashed lines show the Fermi level. Color of band signiﬁes the fraction of band occupations by inorganic atoms (Ag and Se) versus organic atoms (C and H). Band occupations and shape remain similar across these three levels of theory. N, N1 and Z are along the primitive lattice vectors a , b and c , respectively. ∗ ∗ ∗

Figure C.7: Parameters of Ag lattice used in relaxation table. APPENDIX C. APPENDIX FOR SILVER BENZENESELENOLATE IS A SELF-ASSEMBLING DIRECT-GAP METAL-ORGANIC CHALCOGENIDE ASSEMBLY151

Table C.2: Relaxation Wyckoﬀ tables:Lattice and Wyckoﬀ position parameters for one phenyl conﬁguration of Cuthberts crystal structure and DFT relaxations of that conﬁgu- ration.

a b c β Function 1 1 1 1 θ1 θ2 = θ3 l1 = l2 l3 Dihedral angle aexp − bexp − cexp − βexp − Experiment – – – – 152 104 3.029 2.911 52 LDA -1.17% -1.97% -2.62% -0.65% 152 104 2.993 2.849 29 PBE 6.18% 7.86% 0.43% -0.65% 170 95 3.132 3.656 28 df2 2.74% 10.54% 1.11% -0.92% 154 103 3.099 3.332 38

Table C.3: Wyckoﬀ table for experimental structure of [AgSePh]∞. Lattice and Wyckoﬀ position parameters for one phenyl conﬁguration of Cuthberts crystal structure. Cuthbert Spacegroup: 15 (C2/c) a b c 5.876 7.299 29.124 α β γ 90 95.79 90 Label x y z Wyckoﬀ letter Ag1 0.5 0.381 0.25 e Ag2 0.5 0.982 0.25 e C1 0.671 0.186 0.141 f C2 0.453 0.258 0.127 f C3 0.369 0.267 0.081 f C4 0.807 0.11 0.108 f C5 0.496 0.191 0.049 f C6 0.716 0.12 0.06 f H1 0.439 0.199 0.018 f H2 0.447 0.555 0.116 f H3 0.802 0.08 0.037 f H4 0.729 0.823 0.072 f H5 0.363 0.3 0.15 f Se1 0.792 0.182 0.205 f APPENDIX C. APPENDIX FOR SILVER BENZENESELENOLATE IS A SELF-ASSEMBLING DIRECT-GAP METAL-ORGANIC CHALCOGENIDE ASSEMBLY152

Table C.4: Wyckoﬀ table for LDA Relaxation of experimental structure of [AgSePh]∞. Lattice and Wyckoﬀ position parameters for one phenyl conﬁguration of Cuthberts crystal structure relaxed with LDA. LDA Spacegroup: 15 (C2/c) a b c 5.807 7.155 28.361 α β γ 90 95.163 90 Label x y z Wyckoﬀ letter Ag1 0.5 0.363 0.75 e Ag2 0 0.262 0.75 e C1 0.277 0.061 0.86 f C2 0.058 0.02 0.873 f C3 0.022 0.021 0.921 f C4 0.457 0.103 0.893 f C5 0.201 0.063 0.955 f C6 0.419 0.104 0.941 f H1 0.171 0.066 0.992 f H2 0.627 0.141 0.882 f H3 0.561 0.141 0.968 f H4 0.351 0.483 0.931 f H5 0.418 0.483 0.846 f Se1 0.338 0.062 0.794 f APPENDIX C. APPENDIX FOR SILVER BENZENESELENOLATE IS A SELF-ASSEMBLING DIRECT-GAP METAL-ORGANIC CHALCOGENIDE ASSEMBLY153

Table C.5: Wyckoﬀ table for PBE Relaxation of experimental structure of [AgSePh]∞. Lat- tice and Wyckoﬀ position parameters for one phenyl conﬁguration of Cuthberts crystal struc- ture relaxed with PBE. PBE Spacegroup: 15 (C2/c) a b c 6.239 7.873 29.248 α β γ 90 95.166 90 Label x y z Wyckoﬀ letter Ag1 0.5 0.328 0.25 e Ag2 0 0.292 0.25 e C1 0.259 0.061 0.356 f C2 0.059 0.025 0.372 f C3 0.036 0.028 0.419 f C4 0.436 0.099 0.387 f C5 0.212 0.066 0.45 f C6 0.411 0.102 0.434 f H1 0.193 0.07 0.487 f H2 0.591 0.129 0.374 f H3 0.549 0.134 0.458 f H4 0.379 0.499 0.431 f H5 0.422 0.494 0.347 f Se1 0.29 0.06 0.29 f APPENDIX C. APPENDIX FOR SILVER BENZENESELENOLATE IS A SELF-ASSEMBLING DIRECT-GAP METAL-ORGANIC CHALCOGENIDE ASSEMBLY154

Table C.6: Wyckoﬀ table for df2 Relaxation of experimental structure of [AgSePh]∞. Lattice and Wyckoﬀ position parameters for one phenyl conﬁguration of Cuthberts crystal structure relaxed with df2. df2 Spacegroup: 15 (C2/c) a b c 6.037 8.068 29.446 α β γ 90 94.904 90 Label x y z Wyckoﬀ letter Ag1 0.5 0.393 0.25 e Ag2 0.5 0.98 0.25 e C1 0.665 0.188 0.139 f C2 0.445 0.237 0.127 f C3 0.365 0.237 0.081 f C4 0.803 0.14 0.105 f C5 0.502 0.188 0.047 f C6 0.721 0.14 0.059 f H1 0.439 0.188 0.011 f H2 0.472 0.6 0.115 f H3 0.829 0.099 0.034 f H4 0.696 0.778 0.071 f H5 0.339 0.278 0.152 f Se1 0.787 0.186 0.204 f 155

Appendix D

A prototypical ferroelectric: BaTiO3

BaTiO3 is the prototypical ferroelectric. Well above room temperature, BaTiO3 has a cubic perovskite structure in space group P m3¯m (221), shown in Figure D.1. As temperature is lowered, BaTiO3 undergoes several phase transitions to lower symmetry space groups that give rise to a spontaneous polarization, see Figure D.2 [273, 125]. BaTiO3 has been known to be ferroelectric since 1946 [256, 266]. In its tetragonal phase, BaTiO3 has a polarization is 2 26 µC/cm [263]. We use BaTiO3 as a prototypical example for explaining how we conduct our automated ferroelectric search in Chapter 6 and Appendix F.

Figure D.1: BaTiO3 is the quintessential ferroelectric. BaTiO3 has a cubic perovskite crystal structure at high temperatures. Both the barium and titanium are octahedrally coordinated by oxygen. Octahedra of similar center element share corners. APPENDIX D. A PROTOTYPICAL FERROELECTRIC: BATIO3 156

Figure D.2: BaTiO3 goes through three phase transition as temperature is lowered: P m3¯ (221) P 4mm (99) Amm2 (38) R3m (160). The red arrows in the diagram indicate the direction→ of the spontaneous→ polarization→ due to the displacement of the titanium atom and associated rearrangement of the oxygen atoms[273, 125]. 157

Appendix E

Appendix for An Automatically Curated First-Principles Database of Ferroelectrics APPENDIX E. APPENDIX FOR AN AUTOMATICALLY CURATED FIRST-PRINCIPLES DATABASE OF FERROELECTRICS 158

Table E.1: Table of calculated versus experimentally measured polarizations as given in the Landolt-B¨ornstein- Group III: Condensed Matter - Ferroelectrics and Related Substances [227, 228, 229]. Workﬂow ID Formula Polarization Change LB number Exp Exp Ref wﬁd 1476040956.832394 O3PbTi 117.2 1A-11 75 [14, 245] wﬁd 1476040982.95148 LiNbO3 84.1 2A-1 71 [264, 11] wﬁd 1484444959.892999 NaNbO3 54.0 1A-1 12 [12] wﬁd 1484444962.722730 KNbO3 51.6 1A-2 41.2 [10] wﬁd 1484444953.778541 BaO3Ti 50.0 1A-10 26 [8] wﬁd 1476040950.744757 KNbO3 47.7 1A-2 41.2 [10] wﬁd 1476040947.794782 BaO3Ti 47.1 1A-10 26 [8] wﬁd 1476040944.53976 BaO3Ti 46.3 1A-10 26 [8] wﬁd 1476041110.265759 Bi2O9SrTa2 38.2 9A-12 5.8 [23] wﬁd 1484444968.854031 Bi2Nb2O9Pb 37.3 9A-10 NA [20] wﬁd 1476040384.215156 CdO3Ti 37.0 1A-9 NA [9] wﬁd 1476041128.167316 Bi2O9SrTa2 37.0 9A-12 5.8 [23] wﬁd 1476040759.946834 CdO3Ti 34.9 1A-9 NA [9] wﬁd 1476040393.450782 NaNbO3 31.9 1A-1 12 [12] wﬁd 1476040403.435688 NaNbO3 31.9 1A-1 12 [12] wﬁd 1476040428.848867 O3PbZr 23.5 1A-15 16 [15] wﬁd 1476040441.814364 O5PTiTl 22.3 35A-13 NA [106] wﬁd 1476040425.250661 HfO3Pb 19.7 1A-16 Antiferroelectric [13] wﬁd 1476040435.561861 NbO4Sb 18.1 5A-2 19.7 [21] wﬁd 1484694826.997820 Bi4O12Ti3 17.1 9A-15 50 [16] wﬁd 1476041077.120822 Bi4O12Ti3 11.5 9A-15 50 [16] wﬁd 1476040374.879552 CH4N2S 4.8 50A-1 3.5 [226] wﬁd 1476040840.841892 O7Sr2Ta2 3.0 8A-6 1.9 [22] wﬁd 1484445017.971658 B7IMn3O13 2.8 18A-20 NA [19] wﬁd 1476040471.728223 Cl4K2Zn 2.2 39A-9 0.135 [76] wﬁd 1476040104.360695 Br4K2Zn 2.0 39A-16 3.0 [73] wﬁd 1484445205.351382 B7ClCr3O13 1.6 18A-2 2.5 [17] wﬁd 1484445029.449720 K2O4Se 0.7 39A-2 0.15 [74] wﬁd 1484445193.941953 Cl4Rb2Zn 0.5 39A-10 0.16 [77] wﬁd 1484445190.110462 Cl4K2Zn 0.5 39A-9 0.135 [76] wﬁd 1484445186.170228 B7ClMg3O13 0.3 18A-1 0.08 [18] wﬁd 1476040478.537387 Cl4Rb2Zn 0.3 39A-10 0.16 [77] wﬁd 1476040475.325951 Cl4CoRb2 0.04 39A-7 0.15 [75] wﬁd 1476040492.518912 H8N2O4S 0.02 39A-1 0.6 [72] APPENDIX E. APPENDIX FOR AN AUTOMATICALLY CURATED FIRST-PRINCIPLES DATABASE OF FERROELECTRICS 159

Table E.2: New high-quality candidates

Formula Workﬂow ID Polarization Energy Distortion Band Energy Subcategory (µC/cm2) Diﬀerence max (A)˚ Gap (eV) Above (eV) Hull (eV) Ag2S wﬁd 1476040932.225218 0.4 0.002 0.127 1.342 0.075 Ag2S wﬁd 1476041128.167316 27.5 -0.077 0.723 0.409 0.156 Ag2S wﬁd 1484444982.346272 45.3 0.089 0.956 1.342 0.075 AgAl11O17 wﬁd 1476041161.431473 2.2 0.000 1.115 3.142 0.005 AgC2O2 wﬁd 1476040384.215156 0.0 -0.002 0.328 0.980 0.016 AlCH2NaO5 wﬁd 1476040789.617210 0.8 -0.001 0.082 5.030 -0.000 AlCl4Hg2Sb wﬁd 1484445042.637068 0.5 -0.000 0.738 0.835 0.030 AlH3O3 wﬁd 1476040304.362065 1.1 0.009 0.398 4.963 0.004 Hydroxyls AlH3O3 wﬁd 1484445287.593799 8.0 0.007 0.667 4.918 0.018 Hydroxyls AuCl4K wﬁd 1484445086.092903 0.3 0.000 0.072 1.451 0.003 B13C2Li wﬁd 1476041173.637876 0.8 -0.000 0.039 2.562 -0.021 B2O6Zn3 wﬁd 1476040456.859630 0.1 -0.000 0.031 2.709 0.049 Ba2F7Y wﬁd 1484445183.339213 0.7 -0.062 1.262 6.501 0.111 BaC2CaO6 wﬁd 1484445190.110462 1.3 -0.018 0.745 4.676 0.026 BaCO3 wﬁd 1484444965.570570 1.0 -0.001 1.299 4.465 0.015 Oxocarbons BaCl5La wﬁd 1476040438.759718 26.3 0.013 1.526 4.150 0.009 BiO3Y wﬁd 1476040851.179557 9.9 0.037 0.650 2.057 0.074 Br3CsGe wﬁd 1476040104.360695 18.4 0.015 0.332 1.461 0.017 C2HO2 wﬁd 1484445250.57163 3.4 -0.003 0.313 2.829 0.001 Oxocarbons C2HgN2S2 wﬁd 1484444959.892999 0.9 -0.002 0.059 2.126 0.021 C6Cu2H10N4S3 wﬁd 1476040837.97019 0.0 -0.007 0.946 2.733 0.035 CCs4O4 wﬁd 1476040059.599818 1.7 -0.003 0.294 1.629 0.030 CH4N2S wﬁd 1476041035.850896 4.8 -0.006 0.770 3.293 0.006 CHO2Tl wﬁd 1476041077.120822 0.7 0.000 0.088 3.516 0.026 Oxocarbons CK4O4 wﬁd 1476040355.151056 2.6 -0.001 0.167 2.232 0.144 CK4O4 wﬁd 1484445253.438371 9.1 0.002 0.289 2.165 0.053 CK4O4 wﬁd 1476040413.044763 14.6 -0.002 0.584 1.946 0.146 CK4O4 wﬁd 1476040390.68687 16.6 0.006 0.608 1.989 0.049 CLi4O4 wﬁd 1476040854.772923 0.1 0.071 0.221 4.738 -0.007 Oxocarbons CLi4O4 wﬁd 1484445317.338075 16.6 0.003 0.236 4.149 0.168 Oxocarbons CLi4O4 wﬁd 1476041081.548433 49.0 0.016 1.157 5.050 -0.023 Oxocarbons CLi4O4 wﬁd 1476040950.744757 49.2 0.058 0.793 5.088 -0.023 Oxocarbons CN2Pb wﬁd 1476040496.278929 10.4 -0.003 0.189 1.728 0.039 CNa4O4 wﬁd 1476040428.848867 3.6 -0.001 0.151 1.903 0.177 Oxocarbons CNa4O4 wﬁd 1476040902.993927 12.5 -0.000 0.670 1.719 0.176 Oxocarbons CNa4O4 wﬁd 1484444968.854031 39.2 0.010 1.277 2.184 -0.002 Oxocarbons CNa4O4 wﬁd 1484445017.971658 39.2 0.026 0.999 2.184 -0.002 Oxocarbons CNa4O4 wﬁd 1476040986.216576 56.3 0.153 1.356 2.162 0.022 Oxocarbons CO4Rb4 wﬁd 1484444962.722730 0.6 -0.001 0.117 1.714 0.082 Oxocarbons CO4Rb4 wﬁd 1484444978.482971 14.4 0.003 0.571 1.397 0.020 Oxocarbons CO4Rb4 wﬁd 1476040478.537387 14.4 -0.004 0.746 1.395 0.020 Oxocarbons Ca5ClO12P3 wﬁd 1476040897.624205 2.1 0.001 0.446 5.353 0.019 CaF2 wﬁd 1476040844.52392 16.3 0.058 0.838 6.227 0.261 Cd2ClP3 wﬁd 1484694771.994384 0.8 0.000 0.052 1.125 0.057 Cl4GaHg2Sb wﬁd 1476041044.880577 0.6 -0.001 0.802 0.754 0.049 ClH3O5 wﬁd 1476040226.929827 5.2 0.047 1.187 5.381 0.007 ClH4NO4 wﬁd 1476041121.199250 2.2 -0.001 0.903 5.255 0.001 ClIn wﬁd 1484445180.530019 3.7 0.000 0.039 1.450 0.081 CrO3 wﬁd 1484445151.553442 0.4 0.021 1.413 1.588 0.039 CrO9P3 wﬁd 1476040974.294686 1.1 0.001 0.276 3.161 0.034 Cs2HgI4 wﬁd 1484445283.158561 0.3 -0.001 0.068 2.050 0.021 Cs2O3Pb wﬁd 1476040245.01667 7.2 0.000 0.288 1.391 0.033 CuI wﬁd 1484445295.230944 0.6 -0.002 0.121 1.099 0.188 Er2F7K wﬁd 1476040368.725338 1.5 0.000 0.183 6.924 0.074 Fluorides F2HRb wﬁd 1484445224.025729 1.5 -0.001 0.082 6.648 0.049 Fluorides F2Pb wﬁd 1476041088.40149 5.4 -0.003 0.098 4.396 0.105 F3Nd wﬁd 1484694880.421050 17.7 0.172 1.143 7.669 0.071 Fluorides F3PbRb wﬁd 1476040279.158189 4.0 0.033 0.776 3.804 0.083 APPENDIX E. APPENDIX FOR AN AUTOMATICALLY CURATED FIRST-PRINCIPLES DATABASE OF FERROELECTRICS 160

Table E.3: New high-quality candidates

Formula Workﬂow ID Polarization Energy Distortion Band Energy Subcategory (µC/cm2) Diﬀerence max (A)˚ Gap (eV) Above (eV) Hull (eV) F5FeK2 wﬁd 1476040966.672844 0.5 -0.000 0.084 3.663 0.087 Fluorides F5V wﬁd 1476040393.450782 30.0 0.022 1.582 3.215 0.125 F6LiV wﬁd 1476040909.718858 1.2 -0.024 1.704 3.154 0.097 FTl wﬁd 1476041001.553476 6.4 0.029 0.498 3.149 0.114 GaLuO3 wﬁd 1484445209.371670 8.2 0.021 0.344 2.894 0.045 Hexagonal manganite- like GaO3Sc wﬁd 1476040875.673476 10.4 0.014 0.416 3.115 0.051 Hexagonal manganite- like H2Mg wﬁd 1484445164.611735 30.9 -0.040 0.849 2.365 0.072 H2MoO4 wﬁd 1476040207.31872 0.6 -0.001 0.381 3.426 -0.067 H2O2Sr wﬁd 1476041124.761330 1.2 0.003 0.257 3.984 0.012 Hydroxyls H2O2Sr wﬁd 1476040759.946834 1.2 -0.001 0.187 3.984 0.012 Hydroxyls H2O4S wﬁd 1476040460.586026 20.4 -0.003 0.983 6.140 0.003 H2O4Sn3 wﬁd 1484445064.70045 1.3 -0.006 0.624 2.479 0.060 H2O4U wﬁd 1476041106.860617 2.9 0.087 1.465 1.909 0.049 Hydroxyls H2O4U wﬁd 1476040156.35457 2.9 -0.004 0.174 1.914 0.049 Hydroxyls H3LaO3 wﬁd 1476040737.27481 17.9 -0.002 0.189 4.002 0.006 Hydroxyls H3O3Pr wﬁd 1476040371.699091 0.3 0.002 0.153 3.676 0.004 Hydroxyls H3O3Y wﬁd 1476040282.74358 7.8 -0.001 0.087 3.889 -0.008 Hydroxyls H4O5S wﬁd 1476041144.098790 0.8 -0.000 0.195 5.643 0.003 HInO2 wﬁd 1476040139.05518 13.2 0.010 0.243 1.771 0.050 Hydroxyls HK2NO6S2 wﬁd 1484445051.753689 3.2 0.006 0.595 5.261 0.009 HNaO wﬁd 1476040452.983312 10.7 0.002 0.198 2.982 -0.001 Hydroxyls HNaO wﬁd 1484445186.170228 10.7 0.001 0.196 2.982 -0.001 Hydroxyls HORb wﬁd 1476040489.133921 10.5 0.007 0.402 3.391 0.010 Hydroxyls ILi6PS5 wﬁd 1476040187.488112 1.4 0.016 0.770 2.290 -0.009 K2O7Zn6 wﬁd 1476040485.585687 2.6 -0.001 0.218 0.808 0.076 K3S4Sb wﬁd 1476040441.814364 1.0 0.008 0.736 2.158 0.019 KLaS4Si wﬁd 1476040464.155093 7.4 0.003 0.285 2.854 0.013 LiO12P3Zr2 wﬁd 1476040894.532948 8.1 0.003 1.225 4.394 -0.020 LiO4PV wﬁd 1476040196.242976 0.0 -0.000 0.066 2.670 0.018 LiO4PV wﬁd 1476041131.850447 0.0 0.000 0.083 2.670 0.018 MoO3 wﬁd 1476040193.378775 5.2 0.072 0.658 2.155 -0.105 NaO11V6 wﬁd 1476040314.446703 2.4 0.010 0.271 0.987 0.050 NbO5P wﬁd 1484694927.058575 4.1 -0.001 0.159 2.249 0.002 O23Rb6Si10 wﬁd 1476040149.329165 0.1 0.013 0.724 4.303 0.004 O23Rb6Si10 wﬁd 1476040869.259479 0.5 0.008 0.653 4.221 0.010 O2Si wﬁd 1476040956.832394 0.0 0.004 0.570 5.606 0.008 O2Si wﬁd 1476040944.53976 0.0 -0.000 0.131 5.527 0.013 O2Si wﬁd 1476040094.757061 0.0 -0.003 0.846 5.388 0.008 O2Si wﬁd 1476040820.373005 0.0 -0.000 0.342 5.388 0.008 O2Si wﬁd 1484694862.160232 0.1 0.008 0.784 5.503 0.003 O2Si wﬁd 1476041095.479946 0.1 0.004 0.736 5.434 0.006 O2Si wﬁd 1484445313.916250 0.2 0.004 0.688 5.673 0.008 O2Si wﬁd 1476041154.194447 0.4 -0.010 1.296 5.592 0.014 O3SbY wﬁd 1476040753.50691 7.4 0.017 0.462 1.485 -0.018 Hexagonal manganite- like O3ScY wﬁd 1476040358.683542 6.5 0.010 0.321 3.152 -0.004 Hexagonal manganite- like O3Te wﬁd 1476041150.764661 0.4 0.002 0.505 0.550 0.679 OPb wﬁd 1484444945.05931 53.7 -0.002 0.531 2.257 0.096 APPENDIX E. APPENDIX FOR AN AUTOMATICALLY CURATED FIRST-PRINCIPLES DATABASE OF FERROELECTRICS 161

Table E.4: Known high-quality candidates

Formula Workﬂow ID Polarization Energy Distortion Band Energy Subcategory (µC/cm2) Diﬀerence max (A)˚ Gap (eV) Above (eV) Hull (eV) Ag3IS wﬁd 1476040471.728223 0.7 0.002 1.022 0.260 0.080 Proposed by Theory Ag3IS wﬁd 1476040762.919897 0.7 0.041 0.772 0.260 0.080 Proposed by Theory Ag3IS wﬁd 1476040109.318651 11.8 0.050 0.627 0.505 0.071 Proposed by Theory Ag3IS wﬁd 1476040331.097043 11.8 0.011 1.158 0.505 0.071 Proposed by Theory Al2BaO4 wﬁd 1476040858.743894 0.3 0.004 0.560 4.079 0.002 Proposed by Theory Al2BaO4 wﬁd 1476041047.628179 0.3 0.004 0.560 4.079 0.002 Proposed by Theory Al2BaO4 wﬁd 1476040992.366616 0.3 0.004 0.559 4.079 0.002 Proposed by Theory Al2CaH4O10Si2 wﬁd 1476040098.062674 4.2 0.005 0.752 5.056 0.004 Al3F19Pb5 wﬁd 1476041165.857604 13.9 0.020 0.762 5.206 0.084 AlBiO3 wﬁd 1476041098.970098 81.1 0.068 0.481 2.876 0.000 Perovskite AlF7MgNa2 wﬁd 1476040117.949518 1.1 -0.000 0.208 6.660 0.063 B2K3Nb3O12 wﬁd 1476040134.799732 0.1 0.004 0.220 2.373 0.005 B3CaH5O8 wﬁd 1476041117.46294 0.6 0.004 0.957 5.591 -0.000 B7ClCr3O13 wﬁd 1476040223.934313 1.6 -0.000 0.093 2.688 0.014 Boracite B7ClMg3O13 wﬁd 1476040840.841892 0.3 0.010 0.491 5.695 0.004 Boracite B7IMn3O13 wﬁd 1476041141.321099 2.8 0.005 0.471 3.696 0.012 Boracite BaNiO3 wﬁd 1476040159.879894 3.7 0.000 0.046 1.480 0.050 BaO3Ti wﬁd 1476040217.741157 46.3 0.011 0.226 1.726 0.022 Perovskite BaO3Ti wﬁd 1484445022.713113 47.1 0.011 0.129 1.731 0.022 Perovskite BaO3Ti wﬁd 1476040190.49918 50.0 0.014 0.241 2.290 0.020 Perovskite BaO5Ti2 wﬁd 1476041157.542583 15.3 0.003 0.168 2.142 0.041 BeF4H8N2 wﬁd 1476040928.68650 0.6 0.011 0.549 6.640 0.022 N2H8SO4 family BeF4H8N2 wﬁd 1484445148.273011 0.6 0.009 0.545 6.641 0.022 N2H8SO4 family Bi2Nb2O9Pb wﬁd 1476040947.794782 37.3 0.041 0.523 2.321 0.010 Perovskite Bi2O9SrTa2 wﬁd 1476040415.883279 37.0 0.028 0.546 2.503 0.006 Perovskite Bi2O9SrTa2 wﬁd 1476040872.620729 38.2 0.019 0.515 2.312 0.015 Perovskite Bi4O12Ti3 wﬁd 1476040291.620895 11.5 0.023 0.487 1.616 0.052 Perovskite Bi4O12Ti3 wﬁd 1476040275.56900 17.1 0.062 0.562 2.447 0.013 Perovskite Bi4O12Ti3 wﬁd 1484445193.941953 58.2 0.062 0.566 2.368 0.014 Perovskite BiCl8F4H3K6 wﬁd 1476040112.283926 0.1 -0.001 0.160 4.194 0.029 BiInO3 wﬁd 1484445014.628732 63.7 0.466 0.817 2.749 0.039 Perovskite BiInO3 wﬁd 1484444953.778541 63.7 0.011 1.400 2.749 0.039 Perovskite BiO3Sc wﬁd 1476040374.879552 6.5 0.323 0.726 2.675 0.029 BiO3Sc wﬁd 1484445145.139977 6.6 0.000 0.089 2.675 0.029 APPENDIX E. APPENDIX FOR AN AUTOMATICALLY CURATED FIRST-PRINCIPLES DATABASE OF FERROELECTRICS 162

Table E.5: Known high-quality candidates

Formula Workﬂow ID Polarization Energy Distortion Band Energy Subcategory (µC/cm2) Diﬀerence max (A)˚ Gap (eV) Above (eV) Hull (eV) Br4K2Zn wﬁd 1476040115.133166 2.0 0.001 0.140 3.656 0.036 N2H8SO4 family C3ClH10NO4 wﬁd 1476040269.225119 0.3 -0.000 0.275 5.608 -0.000 Proposed by Theory Ca3Mn2O7 wﬁd 1476040396.862183 5.6 0.010 0.383 0.294 0.042 Ca3Mn2O7 wﬁd 1484445029.449720 5.9 0.010 0.388 0.300 0.042 CdO3Ti wﬁd 1476040231.867950 34.9 0.003 0.147 2.405 0.092 Perovskite CdO3Ti wﬁd 1476040203.326613 37.0 0.003 0.121 2.458 0.093 Perovskite Cl3CrRb wﬁd 1476040445.577528 0.0 -0.001 0.115 0.502 0.032 Cl3CrRb wﬁd 1476040766.163640 0.0 0.007 0.357 0.502 0.032 Cl3CsPb wﬁd 1476040435.561861 2.3 0.006 0.575 2.418 0.028 Cl4CoRb2 wﬁd 1484445157.56323 0.0 -0.001 0.251 0.831 0.021 N2H8SO4 family Cl4K2Zn wﬁd 1476041169.873380 0.5 0.013 0.698 4.509 0.040 N2H8SO4 family Cl4K2Zn wﬁd 1476041110.265759 2.2 0.000 0.112 4.412 0.053 N2H8SO4 family Cl4Rb2Zn wﬁd 1476040320.922919 0.3 -0.000 0.129 4.450 0.038 N2H8SO4 family Cl4Rb2Zn wﬁd 1476040953.684754 0.5 0.006 0.920 4.514 0.032 N2H8SO4 family ClH wﬁd 1476040295.440338 57.2 0.273 1.132 5.152 0.049 CsF3Pb wﬁd 1476040124.631808 0.7 0.004 0.449 3.383 0.077 Proposed by Theory CsO4PZn wﬁd 1476040056.258909 1.0 0.012 0.678 3.958 0.027 F4MgSr wﬁd 1484694929.994404 10.8 0.035 0.924 6.662 0.079 Proposed by Theory H2KO4P wﬁd 1484445095.317873 0.5 0.003 0.360 5.248 0.010 H2KO4P wﬁd 1476040475.325951 5.2 0.005 0.238 5.421 0.007 H2O wﬁd 1484694826.997820 13.5 -0.001 0.882 5.478 0.035 H2O wﬁd 1484445205.351382 13.5 0.000 0.833 5.478 0.035 H2O4PRb wﬁd 1484445276.419623 5.5 0.006 0.333 5.222 0.004 H8N2O4S wﬁd 1476041147.43703 0.0 0.007 1.267 5.073 0.000 N2H8SO4 family HfO2 wﬁd 1476040425.250661 52.4 0.061 0.859 4.366 0.035 HfO3Pb wﬁd 1484445174.483678 19.7 -0.004 0.605 2.809 0.036 Perovskite HfO3Sr wﬁd 1476040963.135149 15.1 -0.000 0.114 3.744 0.045 K2O4Se wﬁd 1476040982.95148 0.7 0.000 0.404 3.630 0.016 N2H8SO4 family KNbO3 wﬁd 1484445298.485748 47.7 0.011 0.226 1.472 0.013 Perovskite KNbO3 wﬁd 1484444992.013915 50.4 0.013 0.177 2.311 0.010 Perovskite KNbO3 wﬁd 1476040865.547657 51.6 0.013 0.218 2.058 0.011 Perovskite LiNbO3 wﬁd 1476041051.123043 84.1 0.031 1.337 3.396 -0.004 Perovskite LiNiO4P wﬁd 1476040220.723663 0.2 -0.000 0.083 3.397 0.040 MgO3Si wﬁd 1476041102.78923 1.1 -0.005 1.522 4.663 0.025 N6Pb wﬁd 1476040079.687428 0.4 -0.000 0.229 2.303 0.021 NaNbO3 wﬁd 1476040492.518912 31.9 0.021 0.493 2.402 0.002 Perovskite NaNbO3 wﬁd 1484694837.128419 31.9 -0.000 0.683 2.402 0.002 Perovskite NaNbO3 wﬁd 1476040743.679850 54.0 0.015 0.420 2.362 0.002 Perovskite NbO4Sb wﬁd 1476040403.435688 18.1 0.000 0.211 2.461 -0.002 O2Zr wﬁd 1476040756.894491 51.0 0.046 0.828 3.815 -0.065 O3PbTi wﬁd 1476040989.22333 117.2 0.039 0.581 1.861 0.045 Perovskite O3PbZr wﬁd 1476041014.627130 23.5 -0.004 0.356 2.868 -0.024 Perovskite O5PTiTl wﬁd 1484445106.855737 22.3 0.004 0.664 2.674 0.027 O7Sr2Ta2 wﬁd 1476040410.139034 3.0 -0.000 0.088 2.943 0.012 163

Appendix F

Isotropy Subgroups: How to check if two structure are continuously deformable

A nonpolar-polar structure pair are continuously deformable if the polar structure belongs to an isotropy subgroup of the nonpolar structure. Given a nonpolar-polar structure pair, one can determine if the polar structure is related to the nonpolar structure via an isotropy subgroup by checking the following: First, we check that the point group of the polar space group is a subgroup of the point group of the nonpolar space group. An example relating the point groups of the phase transition of BaTiO3 P m3¯m R3m (see Figure F.1a) is given in F.1b. Second, we determine the→ index of the group-subgroup relationship. The index tells us how many types of ferroelectric domains can form [178]. For some intuitive examples, let’s consider the phase transitions of BaTiO3, shown in Figure D.2. The index for the cubic to tetragonal transition is 6, one for each face of a cube. The index for the cubic to orthorhombic transition is 12 one for each edge of a cube. The index for the cubic to rhombohedral transition is 8, one for each corner of the cube. More formally, the deﬁnition of the index i is given by i = it ik where it is the transla- × tionengleiche (same translation) index and ik is the klassengleiche (same symmetry) index [178]. it gives the reduction of point group operations and ik gives the reduction in transla- tion symmetry. For example, if the unit cell volume is doubled due to the transition, ik = 2. If the number of point group operations is reduced by a third, it = 3. For the BaTiO3 examples, ik = 1 because the ratio of the number of formula units per primitive unit cell for the polar to nonpolar structure is 1. it however varies because diﬀerent numbers of symmetry operations are lost when the structure distorts to the polar space group. The table in Figure F.1c gives the indices for the maximal polar subgroups of P m3¯m (221). Third, we ﬁnd chains of maximal subgroups compatible with the index of the group- subgroup relation for the nonpolar-polar structure pair. From these chains, we can determine APPENDIX F. ISOTROPY SUBGROUPS: HOW TO CHECK IF TWO STRUCTURE ARE CONTINUOUSLY DEFORMABLE 164 possible transformation matrices between the nonpolar to polar lattice. Fourth, for each possible transformation matrix we must check whether the Wyckoﬀ positions are compatible between the nonpolar structure in the low-symmetry setting and the polar structure. When a structure is transformed to a lower symmetry setting, the Wyckoﬀ positions are said to “split”, meaning that due to the reduced symmetry, more symmetrically unique positions are required to describe the crystal structure. Fifth, for the transformations that have compatible Wyckoﬀ splitting, we transform the nonpolar lattice to the polar symmetry setting and compare to the polar lattice. If the lattices match within a generous tolerance of 3 Aand˚ 10 degrees, we continue with the symmetry check. Finally, we check the distance each atom has to move during the distortion. If the maximum distortion distance is within our tolerance of 1.5 A,˚ we store the distortion in our distortion database to then be computed with our ﬁrst-principles workﬂow. APPENDIX F. ISOTROPY SUBGROUPS: HOW TO CHECK IF TWO STRUCTURE ARE CONTINUOUSLY DEFORMABLE 165

Figure F.1: Symmetry checks for isotropy subgroups the BaTiO3phase transition P m3¯m (221) R3m (160). a) cubic and rhombohedral BaTiO3 structures. b) The max- imal subgroup→ relations of the of the point group 4/m32¯ /m (abbreviated as m3¯m), mod- iﬁed from Figure 7.1 in [179] and reproduced with permission. The nonpolar point group (4/m32¯ /m) is highlighted in green and the polar point group (3m) is highlighted in red. The point groups highlighted in blue (43¯ m and 32¯ /m) are the maximal subgroups between the nonpolar and polar point groups. c) A table, generated using the BCS tool CELLSUB (http://www.cryst.ehu.es/cryst/cellsub.html)[29], of the indices of the maximal po- lar subgroups of the cubic space group P m3¯m with k-index of 1. We have highlighted those in red that correspond to subgroups shown in Figure D.2 d) A table of the possible transformation matrices for diﬀerent chains of maximal subgroup from the nonpolar (221) to polar space group (160) for a group-subgroup index of 8. This table was generated using the BCS tool (http://www.cryst.ehu.es/cryst/symmodes.html) SYMMODES[56]. This transformation matrix is used to transform the lattice and Wyckoﬀ positions. APPENDIX F. ISOTROPY SUBGROUPS: HOW TO CHECK IF TWO STRUCTURE ARE CONTINUOUSLY DEFORMABLE 166

Figure F.2: Wyckoﬀ splitting for BaTiO3 from the cubic phase to tetragonal phase. While the cubic phase has 3 symmetrically unique positions, the tetragonal phase has 4.

Figure F.3: Once we have possible transformation matrices for the group-subgroup relation of a given index that give the proper Wyckoﬀ splitting, we transform the nonpolar lattice to the polar symmetry setting and compare to the polar lattice. If the lattices match within a generous tolerance of 3 Aand˚ 10 degrees, we then check the distance the atoms have move during the distortion. 167

Appendix G

A brief primer on deep learning

This section serves to give a quick introduction to the basics of deep learning. Deep learning is a subﬁeld of machine learning where multiple layers of neural networks are used to learn complex functions. In Figure G.1 and Chapter7, we use diagrams inspired by Penrose notation [192] to depict neural networks. A neural network or model is a function with learnable parameters. For example, we can represent a model that learns the function y = f(x) as Figure G.1a. Fully-connected networks are commonly used and easy to mathematically write down. A single layer is composed of two components, a linear transformation and a nonlinear function. In this example, we use the hyperbolic tangent function. A one-layer fully-connected network is shown in Figure G.1b and written as:

y = tanh(W x + b) (G.1) where highlighted variables indicate learned parameters. Similarly, a two-layer fully-connected network is shown in Figure G.1c and written as:

y = tanh(W2 tanh(W1x + b1) + b2)) (G.2) In this example, one can see the importance of having the nonlinear function. If it was not present, the two layer network expression could be re-written as a single layer with 0 0 W = W2W1 and b = W2b1 + b2. Networks with multiple layers can learn more complicated functions. Fully-connected networks tend to become cumbersome when the input vector is large or when the input data has additional structure. Convolutional neural networks (CNNs) are extensively used in image processing and computer vision. We build on this type of network in Chapter7. CNNs take advantage of the adjacency information of pixels by scanning over an image with learned ﬁlters that are typically much smaller than the image (commonly 3 3 or 5 5 pixels in size). As the ﬁlter is scanned across the image (across convolution centers),× the ﬁlter× multiplies the portion of the APPENDIX G. A BRIEF PRIMER ON DEEP LEARNING 168

Figure G.1: Diagrams for example neural networks a) Diagram for an arbitrary function f. b) A one-layer fully-connected network. c) A two-layer fully-connected network. d) A diagram for backpropogation through a fully-connected network. image it overlaps. This resulting matrix is summed to produce a pixel of the output image. This reuse of weights makes CNNs very eﬃcient compared to fully-connected networks. To evaluate a model’s performance, we have to deﬁne a cost function, this is also called the error or loss. The cost function is typically evaluated on the output of the model and is used to update learned parameters via a process called backpropogation. Backpropogration requires a model to diﬀerentiable (or at least have gradients deﬁned for each operation). One takes derivatives of the cost function with respect to the learnable parameters (using the chain rule) to obtain that gradients used to update those parameters. How these gradients are used depends on the optimizer used and hyperparameters of the optimizer such as the learning rate. For the most simple form of gradient descent, one simply updates the learned parameter by the gradients multiplied by a learning rate (typically 10−10 to 10−1). More sophisticated optimizers often add in additional “physics” like momentum to better explore the loss surface. For a deeper dive into deep learning, we recommend Ref. [94] and the course materials available at Ref [4]. 169

Appendix H

Appendix for Tensor Field Networks APPENDIX H. APPENDIX FOR TENSOR FIELD NETWORKS 170

H.1 Proofs of general equivariance propositions

For equivariant , the following diagram is commutative for all g G: L ∈ L X Y DX (g) DY (g) L X Y If a function is equivariant with respect to two transformations g and h, then it is equiv- ariant to the composition of those transformations: (DX (gh)x) = DX (g)DX (h)x L L = DY (g) DX (h)x L = DY (gh) (x) L for all g, h G and x ; that is, the following diagram is commutative: ∈ ∈ X L X Y DX (g) DY (g) L X Y DX (h) DY (h) L X Y

Composing equivariant functions 1 : and 2 : yields an equivariant L X → Y L Y → Z function 2 1: L ◦ L X Y 2( 1(D (g)x)) = 2(D (g) 1(x)) L L L Z L = D (g) 2( 1(x)) L L That is, the following is commutative:

L1 L2 X Y Z DX (g) DY (g) DZ (g)

L1 L2 X Y Z H.2 Motivating point convolutions

We can represent input as a continuous function that is non-zero at a ﬁnite set of points (using Dirac δ functions): X V (~t) = Vaδ(~t ~ra) − a∈S APPENDIX H. APPENDIX FOR TENSOR FIELD NETWORKS 171

A point convolution is then equivalent to applying an integral transform with kernel X F (~t ~s) δ(~t ~ra) − − a∈S for some function F . This transform yields Z 3 X X (~t) = d ~sF (~t ~s) δ(~t ~ra) Vbδ(~s ~rb) L − − − a∈S b∈S X X = δ(~t ~ra) F (~ra ~rb)Vb − − a∈S b∈S X = δ(~t ~ra) a − L a∈S where we deﬁne X a := F (~ra ~rb)Vb L − b∈S as in the main text.

H.3 Proof of equivariance of point convolution layer

Figure H.1: Condition for layer rotation equivariance

Under a rotation ~ra (g)~ra, we know that ~rab (g)~rab and 7→ R 7→ R (lf ,li) X (lf ) (lf ,li) Fcm ( (g)~rab) = D 0 (g)F 0 (~rab) (H.1) R mm cm m0

(l) because of the transformation properties of the spherical harmonics Ym . APPENDIX H. APPENDIX FOR TENSOR FIELD NETWORKS 172

Figure H.2: Filter equivariance equation

Then (lO) X (lI ) (lI ) acm (g)~ra, Dm m0 (g)Vacm0 L O R I I I m0 X (l ,m ) = C O O (lF ,mF )(lI ,mI ) mF ,mI

X (lF ,lI ) X (lI ) (lI ) Fcm ( (g)~rab) Dm m0 (g)Vbcm0 × F R I I I b∈S m0 X (l ,m ) = C O O (lF ,mF )(lI ,mI ) mF ,mI

X X (lF ) (lF ,lI ) D 0 (g)F 0 (~rab) mF mF cmF × 0 b∈S mF

X (lI ) (lI ) D 0 (g)V 0 mI mI bcmI × 0 mI 0 X (lO) (lO,mO) X (lF ,lI ) (lI ) = D 0 (g)C Fcm (~rab)V mOmO (lF ,mF )(lI ,mI ) F bcmI 0 mO b∈S

X (lO) (lO) (lI ) = D 0 (g) 0 ~ra,Vacm . mOmO acmO I 0 L mO APPENDIX H. APPENDIX FOR TENSOR FIELD NETWORKS 173

Figure H.3: Equivariance of Clebsch-Gordan coeﬃcients. Note that each D may refer to a diﬀerent irreducible representation.

H.4 Details for gravitational accelerations and moment of inertia tasks

Moment of inertia radial functions We can write the moment of inertia tensor as X Iij := maTij(~ra) a∈S where (0) (2) δij Tij(~r) := R (r)δij + R (r) rˆirˆj − 3 The expression that R(2) is multiplying is the 3D symmetric traceless tensor, which can be constructed from the l = 2 spherical harmonic. To get agreement with the moment of inertia tensor as deﬁned in the main text, we must have 2 R(0)(r) = r2 R(2)(r) = r2 3 − Figure H.5 shows the excellent agreement of our learned radial functions for ﬁlters l = 0 and l = 2 to the analytical solution.

Point generation details and radial hyperparameters The number of points is uniformly randomly selected from 2 through 10. The masses are scalar values that are randomly chosen from a uniform distribution from 0.5 to 2.0. The coordinates of the points are randomly generated from a uniform distribution to be inside a cube with sides of length 4 for gravity and 1 for moment of inertia. We use 30 Gaussian basis functions whose centers are evenly spaced between 0 and 2. We use a Gaussian variance that is one half the distance between the centers. We use a batch size of 1. For the test set, we simply use more randomly generated points from the same distribution. APPENDIX H. APPENDIX FOR TENSOR FIELD NETWORKS 174

Figure H.4: Diagrammatic proof of point convolution rotation equivariance.

We note that 1/r2 diverges as r 0. We choose a cutoﬀ minimum distance at 0.5 distance because it− is easy to generate suﬃcient→ examples at that distance with a few number of points per example. If we wanted to properly sample for closer distances, we would need to change how we generate the random points or use close to 1000 points per example.

H.5 Proof of weighted point-averaging layer equivariance

Let S be the set of points (not including the missing point at M~ ) with locations ~ra. Suppose that the output of the network is a scalar and a vector ~δa at each point in S. We take APPENDIX H. APPENDIX FOR TENSOR FIELD NETWORKS 175

Figure H.5: Radial function learned by l = 0 and l = 2 ﬁlters for moment of inertia toy dataset. The ﬁlters learn the analytical radial functions. For a collection of randomly generated point sets, the mean minimum distance is the average of the minimum distance between points in each point set. Distances smaller than the mean minimum distance might not have been seen by the network enough times to correct the radial ﬁlter.

the softmax of the scalars over S to get a probability pa at each point. Deﬁne the votes as ~va := ~ra + ~δa, so the guessed point is X ~u := pa~va a∈S This is the ﬁrst operation that we have introduced that lacks manifest translation equivari- ance because it uses ~ra by itself instead of only using ~ra ~rb combinations. We can show − that ~ra ~ra + ~t implies 7→ X h i ~u pa(~ra + ~t) + pa~δa = ~u + ~t 7→ a∈S

because the pa sum to 1. This voting scheme is also rotation-equivariant because it is a sum of 3D vectors. The loss function loss = (~u M~ )2 − is translation-invariant because it is a function of the diﬀerence of vectors in 3D space and rotation-invariant because it is a dot product of vectors.

H.6 Missing point task accuracies and MAE by epoch

In Table H.1, we give the prediction accuracy and MAE on distance for the missing point task broken down by atom type. There are 1,000 molecules in each of the train and test APPENDIX H. APPENDIX FOR TENSOR FIELD NETWORKS 176

Table H.1: Performance on missing point task by atom type

Number of Accuracy (%) atoms with Distance Atoms ( 0.5 A˚ given type MAE in A˚ and≤ atom type) in set Hydrogen 5-18 (train) 7207 94.6 0.16 19 10088 93.2 0.16 23 14005 96.7 0.14 25-29 16362 97.7 0.15 Carbon 5-18 (train) 5663 94.3 0.16 19 6751 99.9 0.10 23 7901 100.0 0.11 25-29 8251 99.7 0.17 Nitrogen 5-18 (train) 1407 74.8 0.16 19 616 74.7 0.18 23 37 81.1 0.19 25-29 16 93.8 0.26 Oxygen 5-18 (train) 1536 83.3 0.17 19 1539 80.2 0.21 23 1057 68.0 0.20 25-29 727 60.1 0.21 Fluorine 5-18 (train) 50 0.0 0.18 19 6 0.0 0.07 23 0 25-29 0 sets; however, when comparing results by atom type, the relevant number to compare is the number of examples where a speciﬁc atom type is removed. In Figure H.6 and Figure H.7, we give the accuracy and distance MAE for the missing point task as a function of the number of training epochs (Tables 7.1 and H.1 contain the results after 225 epochs). APPENDIX H. APPENDIX FOR TENSOR FIELD NETWORKS 177

Figure H.6: Accuracy of missing point task by epoch of training

Figure H.7: Distance MAE of missing point task by epoch of training